Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Document related concepts

Density of states wikipedia, lookup

Electrical resistivity and conductivity wikipedia, lookup

Electrostatics wikipedia, lookup

Woodward effect wikipedia, lookup

Aharonov–Bohm effect wikipedia, lookup

Electrical resistance and conductance wikipedia, lookup

Anti-gravity wikipedia, lookup

Monte Carlo methods for electron transport wikipedia, lookup

Transcript

Compound Semiconductor Device Physics (The Open Edition) Sandip Tiwari Original Publisher: ACADEMIC PRESS Originally published by Harcourt Brace Jovanovich, Publishers This open book is made available under the Creative Commons License with Attribution license terms; you are free to share and distribute with attribution. See http://creativecommons.org/licenses/by/3.0/ for license terms. Library of Congress Cataloging in Publication Data Tiwari, Sandip, 1955Compound semiconductor device physics/Sandip Tiwari. p. cm. Bibliography: p. Includes index. ISBN 0-12-691740-X 1. Compound Semiconductors. 2. Semiconductors. I. Title. QC611.8.C64T59 1992 To Kunal, Nachiketa, and Mari From the unreal lead me to the real! From darkness lead me to light! —Brihadaranyaka Upanishad Contents Preface xv 1 Introduction 1.1 Outline of the Book . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Suggested Usage . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3 Comments on Nomenclature . . . . . . . . . . . . . . . . . . . . . 1 2 3 4 2 Review of Semiconductor Physics, Properties, and Device Implications 2.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Electrons, Holes, and Phonons . . . . . . . . . . . . . . . . . . . 2.3 Occupation Statistics . . . . . . . . . . . . . . . . . . . . . . . . . 2.3.1 Occupation of Bands and Discrete Levels . . . . . . . . . 2.3.2 Band Occupation in Semiconductors . . . . . . . . . . . . 2.4 Band Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.5 Phonon Dispersion in Semiconductors . . . . . . . . . . . . . . . 2.6 Scattering of Carriers . . . . . . . . . . . . . . . . . . . . . . . . 2.6.1 Defect Scattering . . . . . . . . . . . . . . . . . . . . . . . 2.6.2 Carrier–Carrier Scattering . . . . . . . . . . . . . . . . . . 2.6.3 Lattice Scattering . . . . . . . . . . . . . . . . . . . . . . 2.6.4 Phonon Scattering Behavior . . . . . . . . . . . . . . . . . 2.7 Carrier Transport . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.7.1 Majority Carrier Transport . . . . . . . . . . . . . . . . . 2.7.2 Two-Dimensional Effects on Transport . . . . . . . . . . . 2.7.3 Minority Carrier Transport . . . . . . . . . . . . . . . . . 2.7.4 Diffusion of Carriers . . . . . . . . . . . . . . . . . . . . . 2.8 Some Effects Related to Energy Bands . . . . . . . . . . . . . . . 2.8.1 Avalanche Breakdown . . . . . . . . . . . . . . . . . . . . 2.8.2 Zener Breakdown . . . . . . . . . . . . . . . . . . . . . . . 2.8.3 Density of States and Related Considerations . . . . . . . 2.8.4 Limiting and Operational Velocities of Transport . . . . . 2.8.5 Tunneling Effects . . . . . . . . . . . . . . . . . . . . . . . 2.9 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . General References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 7 9 24 24 29 32 40 43 45 47 47 48 49 50 63 65 69 71 72 81 84 85 89 92 92 ix x CONTENTS Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Mathematical Treatments 3.1 Introduction . . . . . . . . . . . . . . . . . . . . 3.2 Kinetic Approach . . . . . . . . . . . . . . . . . 3.3 Boltzmann Transport Approach . . . . . . . . . 3.3.1 Relaxation Time Approximation . . . . 3.3.2 Conservation Equations . . . . . . . . . 3.3.3 Limitations . . . . . . . . . . . . . . . . 3.4 Monte Carlo Transport Approach . . . . . . . . 3.5 Drift-Diffusion Transport . . . . . . . . . . . . 3.5.1 Quasi-Static Analysis . . . . . . . . . . 3.5.2 Quasi-Neutrality . . . . . . . . . . . . . 3.5.3 High Frequency Small-Signal Analysis . 3.6 Boundary Conditions . . . . . . . . . . . . . . . 3.6.1 Shockley Boundary Conditions . . . . . 3.6.2 Fletcher Boundary Conditions . . . . . 3.6.3 Misawa Boundary Conditions . . . . . . 3.6.4 Dirichlet Boundary Conditions . . . . . 3.6.5 Neumann Boundary Conditions . . . . . 3.7 Generation and Recombination . . . . . . . . . 3.7.1 Radiative Recombination . . . . . . . . 3.7.2 Hall–Shockley–Read Recombination . . 3.7.3 Auger Recombination . . . . . . . . . . 3.7.4 Surface Recombination . . . . . . . . . . 3.7.5 Surface Recombination with Fermi Level 3.8 Summary . . . . . . . . . . . . . . . . . . . . . General References . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Pinning . . . . . . . . . . . . . . . 4 Transport Across Junctions 4.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Metal–Semiconductor Junctions . . . . . . . . . . . . . 4.2.1 Drift-Diffusion . . . . . . . . . . . . . . . . . . 4.2.2 Thermionic Emission . . . . . . . . . . . . . . . 4.2.3 Field Emission and Thermionic Field Emission 4.2.4 Thermionic Emission-Diffusion theory . . . . . 4.3 Heterojunctions . . . . . . . . . . . . . . . . . . . . . . 4.3.1 Thermionic Emission . . . . . . . . . . . . . . . 4.3.2 Tunneling . . . . . . . . . . . . . . . . . . . . . 4.3.3 Resonant Fowler–Nordheim Tunneling . . . . . 4.4 Ohmic Contacts . . . . . . . . . . . . . . . . . . . . . 4.5 p–n Junctions . . . . . . . . . . . . . . . . . . . . . . . 4.5.1 Depletion Approximation . . . . . . . . . . . . 4.5.2 High-Level Injection . . . . . . . . . . . . . . . 4.5.3 Gummel–Poon Quasi-Static Model . . . . . . . . . . . . . . . . . . . . . . 93 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 97 97 99 104 107 111 117 126 136 140 140 143 148 149 151 153 155 157 157 158 159 164 166 169 173 174 175 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 181 181 182 190 191 195 198 201 205 209 217 218 224 225 229 233 xi CONTENTS 4.5.4 Abrupt and Graded Heterojunction p–n Diodes 4.6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . General References . . . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 253 264 265 265 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 271 271 273 273 275 279 282 295 296 297 297 299 299 308 309 310 316 323 323 329 333 350 354 355 361 362 362 6 Insulator and Heterostructure Field Effect Transistors 6.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2 Heterostructures . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3 Strained Heterostructures . . . . . . . . . . . . . . . . . . . . . 6.4 Band Discontinuities . . . . . . . . . . . . . . . . . . . . . . . . 6.5 Band Bending and Subband Formation . . . . . . . . . . . . . 6.6 Channel Control in HFETs . . . . . . . . . . . . . . . . . . . . 6.7 Quasi-Static MISFET Theory Using Boltzmann Approximation 6.7.1 Capacitance of the MIS Structure . . . . . . . . . . . . 6.7.2 Flat-Band Voltage . . . . . . . . . . . . . . . . . . . . . 6.7.3 MISFET Models Based on Sheet Charge Approximation 6.8 Quasi-Static HFET Theory Using Analytic Approximations . . 6.8.1 Sub-Threshold Currents . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 367 367 369 371 374 376 390 395 408 410 411 440 457 5 Metal–Semiconductor Field Effect Transistors 5.1 Introduction . . . . . . . . . . . . . . . . . . . . . . 5.2 Analytic Quasi-Static Models . . . . . . . . . . . . 5.2.1 Gradual Channel Approximation . . . . . . 5.2.2 Constant Mobility Model . . . . . . . . . . 5.2.3 Constant Velocity Model . . . . . . . . . . 5.3 Constant Mobility with Saturated Velocity Model . 5.3.1 Transconductance . . . . . . . . . . . . . . 5.3.2 Output Conductance . . . . . . . . . . . . . 5.3.3 Gate-to-Source Capacitance . . . . . . . . . 5.3.4 Gate-to-Drain Capacitance . . . . . . . . . 5.3.5 Drain-to-Source Capacitance . . . . . . . . 5.4 Accumulation–Depletion of Carriers . . . . . . . . 5.5 Sub-Threshold and Substrate Injection Effects . . . 5.6 Sidegating Effects . . . . . . . . . . . . . . . . . . . 5.6.1 Injection and Conduction Effects . . . . . . 5.6.2 Bulk-Dominated Behavior . . . . . . . . . . 5.6.3 Surface-Dominated Behavior . . . . . . . . 5.7 Piezoelectric Effects . . . . . . . . . . . . . . . . . 5.8 Signal Delay along the Gate . . . . . . . . . . . . . 5.9 Small-Signal High Frequency Models . . . . . . . . 5.10 Limit Frequencies . . . . . . . . . . . . . . . . . . . 5.11 Transient Analysis . . . . . . . . . . . . . . . . . . 5.12 Off-Equilibrium Effects . . . . . . . . . . . . . . . . 5.13 Summary . . . . . . . . . . . . . . . . . . . . . . . General References . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . xii CONTENTS 6.8.2 Intrinsic Capacitances . . . . . . . . 6.8.3 Transconductance . . . . . . . . . . 6.9 Quasi-Static Equivalent Circuit Refinements 6.10 Small-Signal Analysis . . . . . . . . . . . . 6.11 Transient Analysis . . . . . . . . . . . . . . 6.12 Hot Carrier Injection Effects . . . . . . . . . 6.13 Effects Due to DX Centers . . . . . . . . . . 6.14 Off-Equilibrium Effects . . . . . . . . . . . . 6.15 p-channel Field Effect Transistors . . . . . . 6.16 Summary . . . . . . . . . . . . . . . . . . . General References . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 458 461 462 464 474 474 480 488 493 494 494 495 7 Heterostructure Bipolar Transistors 503 7.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 503 7.2 Quasi-Static Analysis . . . . . . . . . . . . . . . . . . . . . . . . . 505 7.2.1 Extended Gummel–Poon Model . . . . . . . . . . . . . . 509 7.2.2 Ebers–Moll Model . . . . . . . . . . . . . . . . . . . . . . 524 7.3 Implications of Heterostructures and Alloy Grading . . . . . . . . 529 7.3.1 Charge Transport and Storage in the Base–Emitter Junction538 7.3.2 Alloy Grading, Doping Design and Transport at the Base– Emitter Junction . . . . . . . . . . . . . . . . . . . . . . . 539 7.3.3 Base–Emitter Capacitance . . . . . . . . . . . . . . . . . . 544 7.3.4 Electron Quasi-Fields in Single Heterojunction Bipolar Transistors . . . . . . . . . . . . . . . . . . . . . . . . . . 549 7.4 High Current Considerations of the Base–Collector Junction . . . 551 7.4.1 Barriers and their Influence in Heterojunction Collectors . 551 7.4.2 Collector Electron Quasi-Fields . . . . . . . . . . . . . . . 558 7.4.3 Diffusion Capacitances . . . . . . . . . . . . . . . . . . . . 561 7.4.4 Current Gain Effects . . . . . . . . . . . . . . . . . . . . . 561 7.5 Generation and Recombination Effects . . . . . . . . . . . . . . . 563 7.5.1 Bulk Effects . . . . . . . . . . . . . . . . . . . . . . . . . . 564 7.5.2 Surface Effects . . . . . . . . . . . . . . . . . . . . . . . . 568 7.5.3 Current Gain Behavior . . . . . . . . . . . . . . . . . . . . 573 7.6 Small-Signal Analysis . . . . . . . . . . . . . . . . . . . . . . . . 576 7.6.1 Parameter Notation and Assumptions . . . . . . . . . . . 578 7.6.2 Static and Small-Signal Solutions . . . . . . . . . . . . . . 583 7.6.3 Network Parameters and their Approximations . . . . . . 590 7.6.4 Frequency Figures of Merit . . . . . . . . . . . . . . . . . 609 7.7 Small-Signal Effects of Alloy Grading . . . . . . . . . . . . . . . . 616 7.8 Transit Time Resonance Effects . . . . . . . . . . . . . . . . . . . 623 7.9 Transient Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . 626 7.10 Off-Equilibrium Effects . . . . . . . . . . . . . . . . . . . . . . . . 626 7.11 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 640 General References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 641 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 641 xiii CONTENTS 8 Hot Carrier and Tunneling Structures 8.1 Introduction . . . . . . . . . . . . . . . . . . 8.2 Quantum-Mechanical Reflections . . . . . . 8.3 Hot Carrier Structures . . . . . . . . . . . . 8.4 Resonant and Sequential Tunneling . . . . . 8.5 Transistors with Coupled Barrier Tunneling 8.6 Summary . . . . . . . . . . . . . . . . . . . General References . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . 9 Scaling and Operational Limitations 9.1 Introduction . . . . . . . . . . . . . . . . . 9.2 Operational Generalities . . . . . . . . . . 9.3 General Scaling Considerations . . . . . . 9.4 Limits from Operational Considerations . 9.5 Scaling and Operational Considerations of 9.5.1 Limitations from Transport . . . . 9.6 Scaling and Operational Considerations of 9.7 Summary . . . . . . . . . . . . . . . . . . General References . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 645 645 649 653 661 680 683 683 684 . . . . . . . . . . . . . . . . FETs . . . . HBTs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 689 689 690 693 698 699 708 710 712 712 713 . . . . . . . . . . . . . . . . A Network Parameters and Relationships 715 B Properties of Compound Semiconductors 721 C Physical Constants, Units, and Acronyms 731 Glossary 735 Index 746 xiv CONTENTS Preface New books on the use of semiconductors in devices, of the last few years, have been either directed to the practitioner by emphasizing the state of the art or to the university student by using major simplifications in a treatment that achieves analytic and closed-form mathematical solutions. Presumably, a reason for this is the difficulty in describing numerical techniques and their validity in the restricted space of technical publications or the limited time in the classroom. Modern devices, with their small dimensions, however, require an understanding of the physics of reduced dimensions, the use of statistical methods, and the use of one-, two-, and three-dimensional analytic and numerical analysis techniques. These techniques also bring with them alternate approximations and simplifications. An understanding of these is a prerequisite to the appraisal of the results. This book is an attempt at finding the common ground for the above, and the product of a desire to write it the way I advocate the teaching of this subject. The subject is not trivial and I have resisted oversimplifications. It is an intermediate-level text for graduate students interested in learning about compound semiconductor devices and analysis techniques for small dimension devices. It should be appealing to students who have already achieved an understanding of the principles of operation of field effect transistors and bipolar transistors. While the emphasis of the treatment is on compound semiconductor devices, and examples are mostly drawn from them, it should also be useful to those interested in silicon devices. The principles of devices are the same; compound semiconductor devices only bring with them more complications associated with negative differential mobility and stronger quantum-mechanical and off-equilibrium effects. As befitting a textbook, there is very little original material here, and references have been chosen for the inquisitive to find elaborations and complementary treatments. I have included original material only where I have felt a compelling reason to buttress and elaborate an argument whose results were not in doubt. Both one-dimensional classical approximations and numerical procedures of better accuracy have been incorporated in order to clarify device behavior. I have also tried to use consistent device examples for both the analytic and the numerical approaches. This allows both a better appreciation of the approximations and a better feel for cause and effect. Students, I hope, will look at appearances of unusual features carefully and try to recognize their origin either xv xvi Preface in the underlying nature or the approximation of the model. Most problems at the end of the chapters have been designed to emphasize the concepts and to complement arguments or derivations in the chapters. The rest emphasize the nature of approximations by critically evaluating realistic conditions. These rely on the use of numerical techniques by the student. The reward is a deeper feel for the subject; a note of caution though, they require both will and an access to computers. This effort owes its gratitude to many: family, teachers, authors of discerning reviews and books, and my colleagues, who have generously discussed, encouraged, and criticized. I thank J. East, T. N. Jackson, P. McCleer, P. Mooney, P. Solomon, W. Wang, and S. L. Wright for the conversations. M. Fischetti, D. Frank, S. Laux, and J. Tang, premier practitioners of the art and science of numerical techniques and their applications, have influenced this work in countless ways. This book was partly written, revised, and practiced during a sabbatical leave at the University of Michigan. For the delightful and refreshing time, I thank Professors P. Bhattacharya, G. I. Haddad, J. Singh, D. Pavlidis, F. L. Terry, and K. Tomizawa, and the students who attended my courses and provided invaluable feedback. S. Akhtar, J. East, S. Laux, P. Price, J. Singh, F. Stern, and J. Tsang have commented on parts of the manuscript in depth; I am very grateful to them for this and to F. L. Terry for many exchanges on the contents and teaching of semiconductor devices. This book would certainly not have been possible without the active encouragement and support of International Business Machines Corporation, the help of my colleagues, and the influence of the environment at Thomas J. Watson Research Center. As the book has evolved, its many rough edges have worn away, but many remain. I welcome comments and suggestions on the latter. Sandip Tiwari Chapter 1 Introduction Compound semiconductors have been a subject of semiconductor research for nearly as long as elemental semiconductors. Initial discoveries of the late 1940’s and early 1950’s, discoveries that began the use of semiconductors in our everyday life, were in germanium. With time, it has been supplanted by silicon—a more robust, reliable, and technologically well-behaved material with a stable oxide. Compound semiconductors, whose merit of superior transport was recognized as early as 1952 by Welker, have continued to be of interest since these early days although their success has been narrower in scope. The areas of significant applications include light sources (light emitting diodes and light amplification by stimulated emission of radiation), microwave sources (Gunn diodes, Impatt diodes, etc.), microwave detectors (metal–semiconductor diodes, etc.), and infrared detectors. All of these applications have been areas of the semiconductor endeavor to which compound semiconductors are uniquely suited. The success in optical, infrared, and microwave applications resulted from the direct bandgap of most compound semiconductors for the first, the small bandgap of some compound semiconductors for the second, and the hot carrier properties, superior electron transport characteristics, and unique band-structure effects for the last. With the increasing demand placed on voice and data communications, transmitting, receiving, and processing information at high frequencies and high speeds using both microwave and optical means has become another area where compound semiconductor transistors (the field effect transistors and bipolar transistors) have also become increasingly important. This increased usage stems from their higher operating frequencies and speeds as well as from the functional appeal of integration of optical and electronic devices. This expansion in the use of compound semiconductors, in applications requiring the highest performance, is expected to continue even though they still remain difficult materials for electronic manufacturing. 1 2 1.1 1 Introduction Outline of the Book The emphasis of the text is on the operating principles of compound semiconductor transistors: both field effect and bipolar devices. However, a rigorous treatment of the quasi-static, high frequency, and off-equilibrium behavior of small-sized devices requires a careful understanding of the underlying physics of transport and the mathematical methods used in the analysis of devices. While this is better handled as a separate course on semiconductor physics, quite often these courses are not aimed specifically towards understanding of device physics, and hence are difficult to unite with device physics. Additionally, students—the intended audience of this text,—arrive at an advanced course on devices with a very varied training and with one or more of the many diverse ways of analyzing semiconductor devices. Compound semiconductors bring with them their own peculiarities. Effects related to high surface state density that manifest themselves in the form of Fermi level pinning and high surface recombination, negative differential mobility, etc., have been treated to varied levels of sophistication in the older texts. However, the use of compositional changes and heterostructures, and the emphasis on off-equilibrium behavior of small sized device structures, are relatively new developments and have lacked the attention to detail exemplified in the earlier texts. Thus, advanced semiconductor device courses, generally geared towards silicon, leave an insufficient grasp of the techniques and tools needed to understand small-dimension high frequency compound semiconductor devices. A book emphasizing the operation of compound semiconductor devices, however, does still have relevance to silicon devices. The operating principles are similar; the parameters and relative magnitude of effects is different. The examples here are largely chosen from compound semiconductors although the underlying discussion also stresses silicon and germanium. To coherently develop the theory of device operation, especially because of the emphasis on small structures, the book breaks with the traditional treatment of device theory. It begins with a review and general development of semiconductor properties and their general relationship with devices. It then discusses the mathematical treatments that are either traditional or increasingly being employed. The stress here is on their underlying assumptions, their limitations, and how one would employ them in different parts of the device to derive the device characteristics of interest. A thorough discussion of two-terminal junctions has also been undertaken because they constitute building blocks for the transistors of interest, and because they are a very convenient means to develop and emphasize the methodology to be employed in the three-terminal device treatment. This is followed by a development of the operation of transistors based on the use of unipolar transport with metal–semiconductor junctions and heterojunctions and the use of bipolar transport. The second to last chapter of the book is devoted to a discussion of devices where hot carrier transport and tunneling is central to the operation. These are two- and three-terminal device structures using transit of carriers with a limited number of scattering events or externally tunable tunneling, two unique phenomena not conventionally em- 1.2. SUGGESTED USAGE 3 ployed in three-terminal device structures. They are compound semiconductor devices that need non-traditional device physics which ultimately may also be useful in description of the conventional devices as their sizes continue to shrink. The last chapter discusses this from a general perspective in order to show how present understanding of devices may be used to understand both the future development and the future limitations of devices. The bulk of the book is devoted to the treatment of the mainstream compound semiconductor transistors: the metal–semiconductor field effect transistor (MESFET), the heterostructure field effect transistor (HFET), and the heterostructure bipolar transistor (HBT). Our discussion of these devices includes quasi-static behavior and development of the corresponding low frequency models, small-signal high frequency behavior and development of corresponding models useful to higher frequencies, transient behavior, the role of off-equilibrium effects in these devices, and various other phenomena important to the operation and usefulness of the device. Through-out the book, we will use the term “off-equilibrium” phenomenon to describe the local phenomenon resulting from loss of equilibrium between the carrier energy and the local electric field, a phenomenon that results in an overshoot effect in the velocity of carriers. This term should be distinguished from “non-equilibrium” or lack of thermal equilibrium, which always occurs when a bias is applied and results in the flow of current. Examples of the various other phenomena include effects such as sidegating—the effect of a remote terminal other than the three terminals of the device acting as an additional gate electrode with an effect on the channel transport; piezoelectric effect—the influence on device characteristics because of strain-induced piezo-effects; and surface recombination—recombination of electrons and holes at the surfaces of the bipolar transistor—and others. Among the compound semiconductors, the discussion frequently takes GaAs as an example. This is largely because our understanding of GaAs and the technology of GaAs-based devices is more mature than that of the other compound semiconductors. However, many examples are cited from Ga.47In.53 As (the lattice matched composition with InP), InP itself, and InAs. Other compound semiconductors are cited when particular properties are specifically of interest. The discussion has largely been kept general even if referring to GaAs. 1.2 Suggested Usage The text is best suited for a two semester course with the first covering through MESFETs. The development of a feel for a subject is best achieved by a simultaneous development of healthy skepticism. This requires a good understanding of the underlying assumptions and the methods of attack on the problem being analyzed, and an appreciation of the relevant general properties. Chapters 2 and 3 are an untraditional attempt at meeting these requirements, and the discussion of two-terminal diode structures and one example of a three-terminal transistor structure brings these concepts together coherently. The second course, constituting the rest of the book, then builds on this by analyzing HFETs and HBTs 4 1 Introduction and then dwells on the new developments that are of considerable intellectual interest. The last chapter on scaling and operational limitations serves to continue a discussion begun in the previous chapter of the conventional development of devices with time and how one may look at the subject very broadly by going to the roots in electromagnetic and other classical equations. The text could be used for a one semester course with the subject ranging from the treatment of MESFETs through the hot carrier and tunneling structures. I also recommend that small-signal treatment based on the small-signal drift-diffusion equation be excluded from such a course. This treatment is peripheral to the objectives that a one semester course would usually have. The references occur in two places. General references, long articles and books that have extensive breadth and scope, have been placed at the end of chapters. The reader will find these advanced, complementary, and supplementary reading, and the vast reference lists in them useful for further perusal. References have also been placed in figures and footnotes, as part of the main text. These references are more specific; they supplement comments made in the text and are also in many instances sources for the material developed or reproduced in the text. The problems need to be treated with caution. They range from questions that can be answered in one line to questions that require extensive use of computation facilities. The author believes in a balance of the two; success with both is indicative of a systematic and detailed understanding of the subject and of using the knowledge in uncharted regions. The reader should exercise appropriate restraint in what he or she attempts, keeping in mind the available facilities. 1.3 Comments on Nomenclature We will generally use only MESFET, HFET, and HBT as the acronyms for metal–semiconductor field effect transistor, heterostructure field effect transistor, and heterostructure bipolar transistor. These are meant to define a general class of devices which have sufficiently different operational basis. These devices, however, can be implemented in many ways, largely because compound semiconductors can be grown in a variety of heterostructures with many variations in control of the bandgap and doping in the structures. MESFETs, e.g., can be grown with a thin heterostructure underneath the gate or a thick heterostructure underneath the channel—one suppresses gate current while the other suppresses substrate injection current. They, however, all use a doped channel where quantization effects are unimportant and the operational basis is largely unchanged. HFETs similarly can be grown in a variety of ways. In such transistors a large bandgap material abuts a small bandgap material with an abrupt hetero-interface. HFETs exist with a gate made of metal, a gate made of a semiconductor1 , a doped large bandgap semiconductor, 1 A close compound semiconductor analog of the poly-silicon gate silicon MOSFET (metal– oxide–semiconductor field effect transistor) may, more generically, be called a semiconductor– 1.3 Comments on Nomenclature 5 an undoped large bandgap semiconductor, and various heterostructures at the channel-substrate interface. These are all generically HFETs where the abruptness of the hetero-interface between the channel region and the control region is important to the operational basis of the device. HBTs, similarly, also have many variations—two examples being use of one heterostructure (in the emitter) and two heterostructures (in both emitter and collector) in the structure. insulator–semiconductor field effect transistor (SISFET). HFET is a superset of such devices. 6 1 Introduction Chapter 2 Review of Semiconductor Physics, Properties, and Device Implications 2.1 Introduction An adequate description of different semiconductor devices requires an understanding of the physics of the semiconductor ranging all the way from the semiclassical description to the quantum-mechanical description. The nearly-free electron model of a carrier in a semiconductor is a semi-classical description. Along with other semi-classical phenomenology this description has been quite adequate in describing the functioning of several important devices—both the silicon bipolar transistor and the silicon MOSFET. However, this same carrier, when confined in a short space between two ideal abrupt heterostructure interfaces,1 exhibits behavior in which the quantum-mechanical effects are of paramount importance and central to explaining many of the observations on the structure. In this, a particle in a box problem, the momentum of the carrier in the direction orthogonal to the heterostructure interface is no longer continuous. The particle exhibits a behavior in which quantum-mechanical effects are important. The applicability of these descriptions is not mutually exclusive. The quantum-mechanical description can be shown to reduce to the semi-classical in the proper limits. It just so happens that the sophistication and depth of the quantum-mechanical description is not necessary in what we view as the functioning of the devices cited. If we probe deeper, e.g., the silicon MOSFET operating at 77 K or the compound semiconductor HFET operating at 300 K, we find that we need to incorporate the increased sophistication to explain many of the observations, and the rigorous quantum-mechanical treatment also has 1 An abrupt interface between two dissimilar materials that exhibit long range lattice periodicity. 7 8 2 Review the beauty of reducing to the classical description in the classical limits. The HFET provides quite an interesting example of the relationship between the accuracy of results sought and the necessary rigorousness in the description of the problem. This is a device in which a channel is formed for conduction in a small bandgap material by using a large bandgap material for the insulator and/or for providing the carriers. It may be viewed as one of the MOSFET-like implementations of compound semiconductor FETs. If the potential variation in the small bandgap material is rapid, and this rapid potential variation occurs at high carrier concentrations following Gauss’s law, then one would expect quantum-mechanical effects resulting from confinement similar to that for a particle in a box. However, if carrier concentration is small, then the potential variation is slow and the sophisticated description is unnecessary. The device, in different bias regions, requires different levels of description, to explain observations. In fact, different regions of the device at the same bias may require different levels of sophistication. There are more carriers under normal operating conditions at the source end of the device where they are injected than at the drain end where they are collected. So, while quantum-mechanical effects may be necessary in the description of the device at the source end, they may not be at the drain end. Temperature is also important in the evaluation of the acceptable methodology of handling this problem. At room temperature, thermal energy is 25.9 meV; clearly if the confinement leads to energy effects much smaller than this energy, then the inclusion of confinement effects is not necessary. Silicon MOSFET, which also has a large discontinuity at the oxidesemiconductor interface, has a much smaller predicted effect for both electrons and holes at 300 K where the effect is ignored, but at 77 K, thermal energy and energy discretization is comparable, and at least for some problems, the discretization may not be ignored. So for conventional bipolar and field effect transistors, we need to make a judicious choice of the level of description needed. In devices, where the wave nature of the electron is central to their functioning (tunneling, e.g., in tunnel diodes) the quantum-mechanical description is unavoidable. This chapter is a review that connects the basis of semiconductor theory in classical and quantum mechanics to its implications in devices, with an emphasis on examples from compound semiconductors. We discuss the particle-wave duality and the description of electrons in a lattice with the effect of lattice on the electron folded into the effective mass. We discuss lattice vibrations and the concept of phonons. This early description is made with respect to a onedimensional lattice, which allows us to explore the formation of energy bands, the concept of holes, the specification the of energy-momentum relationship for both the electrons and the phonons, and the description of a quasi-continuum of allowed states via the density of states. Using these one-dimensional examples as a basis, we then discuss the behavior of the three-dimensional semiconductor crystals. Since our primary interest is in devices, our discussion of the properties of semiconductor crystal is related to specifically those phenomena that influence electron transport and electron interactions. Transport, e.g., is intimately 9 2.2. ELECTRONS, HOLES, AND PHONONS related to the electron’s interaction with its environment, i.e. scattering. We consider the various mechanisms of scattering and their behavior in the semiconductor crystal. The carrier velocities are also related to the band structure. We discuss this and other band structure-related phenomena as the last part of this chapter. This chapter is written as a general review with an emphasis on mathematics where it has been considered necessary. One example of this emphasis is the occupation of carriers at discrete energy levels, such as donors and acceptors, which brings out the importance of degeneracy; and, together with the description of band occupation, establishes the framework for semiconductor statistics to be developed further in the following chapters. 2.2 Electrons, Holes, and Phonons Consider a free electron in the absence of any other interactions. The timeindependent Schrödinger’s equation characterizing the behavior of this single electron consists of only the kinetic energy term and is h̄2 2 ∇ ψ(r) = Eψ(r). 2m (2.1) Including the time-dependent component, the solution is of the form ψk (r, t) = A exp [j (k.r − ωt)] , (2.2) where A is a normalization pre-factor. This eigenfunction describes a plane wave. This plane wave, whose wave vector is k2 , is associated with an energy whose dispersion relation is a parabolic relationship, E(k) = h̄2 k 2 , 2m (2.3) and whose momentum is given by p = h̄k. (2.4) The wavelength and angular frequency associated with this plane wave are λ= h , p (2.5) and E . (2.6) h̄ This wavelength is the de Broglie wavelength characterizing the wave particle duality. ω= 2 Throughout the book, we employ bold fonts to indicate vectors. The magnitude of these vectors is indicated using the normal font. Readers should refer to the Glossary for the definition of symbols. 10 2 Review For a single plane wave, the probability of finding the electron ψψ∗ is a constant in real space; the electron can be found anywhere with an identical likelihood. To describe a more localized electron, one may construct a wave packet by considering a group of plane waves with a finite amplitude in a narrow range of the wave vector. The function Z ∞ φ(r, t) = A(k) exp [j(kr − ωt)] dk, (2.7) −∞ which is a superposition of plane waves, or equivalently a Fourier expansion in the k-space, describes a wave packet if A(k) is non-zero for a range δ of wave vector k about k0 such that δ k0 . This function now allows us to determine the probability of finding an electron; it is now higher in certain ranges of r and k. Using a Taylor series expansion of the angular frequency ω about k0 , i.e., dω + · · ·, (2.8) ω = ω0 + (k − k0 ) dk k0 we can write φ(r, t) ≈ = Z ∞ dω exp [j(k0 r − ω0 t)] t A(k) exp j(k − k0 ) r − dk −∞ dω t exp [j(k0 r − ω0 t)] , B r− dk dk (2.9) where B(r − (dω/dk)t) is the envelope function of the resultant plane wave. The group velocity of this wave packet, the velocity of the electron, is given by vg = dω , dk (2.10) and the phase velocity, the velocity of the plane wave, is vp = ω0 . k0 (2.11) In doing this we have shown that superposition of plane waves can be used to characterize localization of electrons and hence have related some of the consequences of the quantum-mechanical description with the classical description. We have, until now, considered the free electron as possessing no potential energy, and solved the single body problem whose Hamiltonian contained only the kinetic energy term. In studying semiconductor devices, we are interested in electrons in semiconductors. This is a many-body problem. Even if the behavior of electrons is treated as a single electron problem unaffected by other electrons in the crystal (the one-electron approximation), we must consider several other factors. The Hamiltonian must now include several additional energy terms such as the kinetic energy of nuclei and core electrons (the ion core) that oscillate around a mean position, a movement whose effect is characterized by 2.2 Electrons, Holes, and Phonons 11 phonons; the potential energy of these ion cores; and the potential energy of the electrons due to influence of other electrons and the cores. In addition, the crystal is finite sized, albeit of a large size. There are explicit quantization effects associated with this confinement; there is a large but finite set of allowed values of the wave vector k which are characterized by a finite density of states for the electron. The crystal is also a periodic structure where the ion cores, on average, occupy a lattice with a specific lattice constant. Since the ions are considerably heavier than the electrons, the electron eigenfunction may be treated as being instantly responsive to the ion movement. This is the adiabatic approximation and it allows the decoupling of the Schrödinger equation into an ionic and an electronic equation. The one-electron approximation provides a reasonable description for this problem because both the core electrons and the valence electrons exist in close proximity to the cores and hence screen the interaction, since both the exclusion principle and repulsion cause separation of electrons and because electrons spend very little time near a core due to the large accelerations resulting from large forces. Let V (r) represent the potential energy term for the electron Hamiltonian. It has the periodicity of the lattice R—the direct lattice vector—and V (r) = V (r + R). (2.12) Bloch’s theorem states that for such a periodic potential, the eigenfunction solution of the Hamiltonian for the one-electron problem has a solution of the form ψk (r) = exp(jk.r)uk (r), (2.13) and uk (r) = uk (r + R). (2.14) The consequence of this is that ψk (r + R) = exp(jk.R)ψk (r), (2.15) and it brings us to the concept of reciprocal lattice. The wave vector k has the units of reciprocal length. For values of k = G, such that G.R = 2nπ, (2.16) where n is an integer, the eigenfunction ψG is periodic in R. If the magnitude of the wave vector was equal to the reciprocal lattice vector G, then the eigenfunction would be periodic in real space. That is the important consequence of Equation 2.15. The translating of the wave vector k by the reciprocal lattice vector, i.e., k = G + k0 , (2.17) results in ψk (r + R) = exp(jk0 .R)ψk (r). (2.18) This is a restatement of Bloch’s theorem with a new wave vector k0 , i.e., all wave vectors differing from k by integer multiples of the reciprocal lattice vector 12 2 Review Figure 2.1: The cubic unit cell of the zinc blende structure is shown in the part (a). The open and closed circles denote the sites for the group III and group V atoms. Part (b) shows the corresponding first Brillouin zone—a truncated octahedron. satisfy the requirements of the eigenfunction. We make the wave vector unique by translating all the wave vectors to the first Brillouin zone, the primitive or Wigner–Seitz unit cell in reciprocal space. This brings us to the definition of the reciprocal lattice. In general, the direct lattice vector may be expressed in terms of primitive unit cell vectors ai which are not necessarily orthogonal to each other.3 The primitive unit cell vectors of the reciprocal lattice bi , defining the Brillouin zone, are then given by b1 = 2π a2 × a3 , a1 .(a2 × a3 ) (2.19) b2 = 2π a3 × a1 , a1 .(a2 × a3 ) (2.20) b3 = 2π a1 × a2 . a1 .(a2 × a3 ) (2.21) and Figure 2.1 shows the primitive cell of the zinc blende structure (the common form of occurrence for most compound semiconductors) and the first Brillouin zone of this face-centered cubic crystal. 3 A common method of notation, to describe various planes in the unit cell, is to use the reciprocal of the intercepts in units of the primitive vectors. As an example, if a1 /h, a2 /k, and a3 /l are the three intercepts, then the Miller indices (hkl) identify the plane. The vector perpendicular to this plane hhkli is the direction. 13 2.2 Electrons, Holes, and Phonons The first Brillouin zone is a truncated octahedron. The importance of this first Brillouin zone for the present discussion is that all wave vectors beyond the first Brillouin zone may be folded into the first Brillouin zone using a translation of the reciprocal lattice vector G, which is composed of integer multiples of the primitive vectors of the reciprocal cell. Certain positions in the Brillouin zone are of particular importance because of their symmetry, and the relation to other characteristics that this entails. We will return to a discussion of the significance of the Brillouin zone and of these symmetry points during our discussion of semiconductor properties. We have now considered the form the eigenfunction solution may take for the one-electron approximation in periodic potential. Determination of the actual eigenfunction and the eigenenergy can be considerably more complex. If the kinetic energy of the electrons is much larger than the periodic potential energy resulting from the lattice, then the behavior of the electron can be modelled approximately by a nearly free electron eigenfunction. The effect of the lattice potential is to make the electron respond to externally applied forces as if it has a differing effective mass (m∗ ) instead of the free electron mass. Note that the mass of the electron itself has not changed. To determine the response of the electron in the crystal to an externally applied stimulus such as an electric field, one need not consider the internal forces such as those due to lattice—their influence has already been folded into the effective mass which can be either smaller or larger than the free electron mass. Thus, the behavior of the nearly free electron is similar to that of the free electron discussed earlier; the difference is the change in effective mass. The periodicity of the lattice potential has another significant effect. Standing waves formed due to this periodicity cause a shifting in energy because of the resultant charge movement. This leads to bands of energy that are allowed energies for an electron and an energy gap of disallowed energies. A good example of this that can be solved explicitly is the Kronig–Penney model. Consider Figure 2.2, which shows the periodic potential in a hypothetical one-dimensional crystal. The spatial periodicity is a for a potential barrier whose height and width are V0 and b respectively. We are interested in finding the energies and wave vectors allowed in this periodic structure. Schrödinger equation for the barrier region (a − b < z < a, etc.) is − h̄2 ∂ 2 ψ + V0 = Eψ, 2m ∂z 2 (2.22) whose solution should be of the form ψ1 (z) = A exp(αz) + B exp(−αz), where α= 2m(V0 − E) h̄2 1/2 . (2.23) (2.24) 14 2 Review Figure 2.2: The periodic potential used in Kronig–Penney model. It consists of periodic potential wells in a hypothetical one-dimensional crystal. The spatial periodicity is a, the barrier width is b, and potential barrier height is V0 . The Schrödinger equation for the well region (0 < z < a − b, etc.) is − h̄2 ∂ 2 ψ = Eψ, 2m ∂z 2 (2.25) whose solution should be of the form ψ2 (z) = C exp(jβz) + D exp(−jβz), where (2.26) 1/2 2mE β= . (2.27) h̄2 The constants can be evaluated based on continuity at z = 0 and consequences of Bloch’s theorem. The consequence of the latter is that, for any k, ψk (z + a) = exp(−jka)ψk (z), (2.28) and one could use this to establish continuity at z = −b. Thus the four boundary conditions that are periodic in nature are: and ψ1 (0) ∂ψ1 ∂z z=0 ψ1 (−b) ∂ψ1 ∂z z=−b = = = = ψ2 (0), ∂ψ2 , ∂z z=0 exp(−jka)ψ2 (a − b), ∂ψ2 exp(−jka) . ∂z (2.29) z=0 This is a set of four equations, with four unknowns A, B, C, and D. A solution exists when the determinant of the coefficients of these unknowns vanishes, a condition that can be written as cos(ka) = α2 − β 2 sinh(αb) sin (β(a − b)) + cosh(αb) cos (β(a − b)) . 2αβ (2.30) 15 2.2 Electrons, Holes, and Phonons Figure 2.3: A plot representing Equation 2.32 as a function of the parameter βa for P = 1 (solid line) and P = 10 (dot-dashed line). Allowed bands occur where the function lies in between −1 and +1. For real k, allowing for travelling waves, the left hand side will have a value between −1 and +1. The right hand side is an oscillating function with increasing energy, i.e., also β. Only those values of E that limit the magnitude of the right hand side between −1 and +1 allow for a wave solution or a pass-band in energy. Outside this range lie the values of E that are forbidden; these form the energy gap regions. We will consider the solution using a parameter P which is proportional to the area under the barrier, P = mabV0 . h̄2 (2.31) We now consider, for constant P , barriers of infinitely small thickness, i.e., the condition where b → 0 and the barriers are replaced by delta functions. Since sinh(αb) → αb and cosh(αb) → 1, the constraint of Equation 2.30 reduces to cos(ka) = P sin(βa) + cos(βa). βa (2.32) The constant P representing the area under the potential barrier represents the strength of electron binding in the crystal. A large value of P is the tight binding limit while P = 0 is the free electron limit. Figure 2.3 shows the right hand side of Equation 2.32 plotted as a function of βa for a small and a large value of P . The transition between the allowed and forbidden bands occurs at β = nπ/a where n is an integer. For a one-dimensional crystal, these are the Bragg reflection conditions. At this transition, k = nπ/a and the electron wave 16 2 Review Figure 2.4: Schematic of extended (a) and reduced zone (b) plot of energy E versus wave vector k for the Kronig–Penney model. function is a standing wave. Since β has a direct square-root dependence on the energy of the electron, Figure 2.3 also shows that for small P , the allowed energy bands are larger, together with smaller bandgaps, compared to large values of P . For any P , at higher energies, the allowed bands get broader and bandgaps smaller. So, for tight binding of an electron represented by a large P , the allowed energy bands are smaller, but for high energies in either of the limits, the passband approaches that of a free electron. The energy versus wave vector relationship resulting from this analysis is shown in Figure 2.4. The figure shows, in both extended and reduced zone representation, the formation of allowed bands and their respective energies versus wave vector relationship. The reduced zone, also called folded zone representation, is the more popular form because it completely and succinctly describes the relationship of interest. It can be seen that near the band edge the E versus k relationship is close to parabolic (the second term of a Taylor series expansion). In the case of a free electron, it is exactly parabolic over the whole energy range. The Kronig–Penney is a highly idealized model limited to a one-dimensional crystal; arbitrary potential forms can only be treated via sums of a Fourier series. In a real crystal one would therefore resort to rather intensive numerical techniques using complicated wave functions to determine the energy-band diagram. Some examples of such approaches4 are the plane wave approach suitable for 4 W. A. Harrison, Solid State Theory, Dover, N.Y. (1979) has a rigorous treatment of these 2.2 Electrons, Holes, and Phonons 17 nearly-free electrons, the tightly bound electron approach, the orthogonalized plane wave approach and its specialized application using the pseudopotential approach. Nearly free electron models are quite approximate representations of the real crystals. One problem, e.g., is that near the ion core, the eigenfunction must differ substantially from a plane wave and hence several terms of the Fourier expansion of uk (r) with reciprocal lattice vectors are necessary to obtain any accuracy. The tightly bound electron model takes the opposite approach by assuming that the lattice potential energy is much larger than the kinetic energy. The tighter binding is particularly true for the electrons that are largely bound to the ion cores. The result is that one would expect the wave functions to be closer to the wave functions of the electrons when the atoms are separated from each other. The Bloch electron wave function can then be constructed using a linear combination of atomic orbitals to determine the energy-band structure. In the same vein, one may construct the electron wave functions using a linear combination of molecular orbitals. The necessity of using several terms of the Fourier expansion of uk (r) with reciprocal lattice vector in the plane wave approach is addressed by a suitable modification of the wave function in the orthogonalized plane wave method. This method allows development of a wave function which behaves approximately like a plane wave between ion cores and approximately like an atomic wave function near ion cores with the atomic wave function part orthogonal to the plane wave part. A development from the orthogonalized plane wave method is the use of pseudopotentials, which takes advantage of the reduction in effective potential for a valence electron due to the opposite effect of the real potential V (r) and the atomic orbital effect. The result of these complex calculations is the development of the energyband diagram of the three-dimensional lattice—a description of the relationship between the energy and crystal momentum associated with the electron. While we will discuss these specifically for the semiconductors later in this chapter, it should come as no surprise that they are considerably different from that seen for the Kronig–Penney model. They are different in different directions in the k-space, and the energy minima or maxima of various bands do not have to occur at zone center, i.e., k = 0. The highest normally filled band at absolute zero temperature is the valence band and the lowest normally empty band at absolute zero temperature is the conduction band. We return now for further discussion to the highly idealized Kronig–Penney model whose E–k relationship is shown in Figure 2.4. Let the second band be a valence band and the third band a conduction band. If we expand, for the conduction band, the E–k relationship via a Taylor series expansion, i.e., E = E0 + ak 2 + bk 4 + · · · , (2.33) at small values of k, the relationship is parabolic. So, at small values of k, this is like the free electron case, but has a differing mass m∗ given by 2 −1 2 ∂ E ∗ m = h̄ , (2.34) ∂k 2 approaches. 18 2 Review with the energy relationship given by E − E0 = h̄2 k 2 . 2m∗ (2.35) The electron, in the periodic potential, behaves as if it is moving in a uniform potential whose magnitude is E0 /q and as if it has an effective mass m∗ . The equation for effective mass has a much more general validity than implied above. Mass has the significance of being the proportionality factor between force and acceleration. Thus, for a force F , and a group velocity vg ,5 F = m∗ dvg . dt (2.36) In addition, since F dt = dp = h̄dk, (2.37) dk . dt (2.38) ∂ω , ∂k (2.39) F = h̄ Since the group velocity is given as vg = from the E–k relationship, it follows in one dimension as vg = 1 ∂E , h̄ ∂k (2.40) or more generally in the n-dimension case as vg = 1 ∇k E(k). h̄ (2.41) For one dimension, the time rate of change of the group velocity because of the application of the force F , is 1 d dE 1 d dk dE dvg = = , (2.42) dt h̄ dt dk h̄ dk dt dk and hence, using Equation 2.38 and 2.42, the force is related as 2 −1 d E dvg F = h̄2 , dk 2 dt and therefore the effective mass is given by 1 1 d2 E = 2 . m∗ dk 2 h̄ (2.43) (2.44) 5 Effective mass and momentum will be discussed again when we consider real threedimensional crystal structures. We have not yet stressed the distinction between crystal and electron momentum. Here, p = h̄k is, of course, the electron momentum. 19 2.2 Electrons, Holes, and Phonons For a general three-dimensional situation where it may be different in different directions, it is related, by extension, as 1 1 ∂2E . ∗ = 2 mij h̄ ∂ki ∂kj (2.45) The second and the fourth band of our Kronig–Penney example have maximum in energy at zone center. The energy near these maxima is also expandable in a Taylor series form, and should have a parabolic relationship between E and k at the maximum. However, here, similar arguments as before yield a negative effective mass. An electron occupying one of the states near the band maximum would accelerate in the opposite direction. At normal temperatures the bands are partially occupied or filled, thus allowing movement of an electron from a filled state to an empty state and hence causing the flow of current. If we consider an electric field applied in the negative direction, an electron near the bottom of the conduction band, which has a positive m∗ and a negative charge, feels a force in the positive direction and hence has an associated velocity, the group velocity, given by ∂E vg = , (2.46) ∂k which is also positive. The electron at the bottom of the partially filled conduction band moves in the positive direction. Now, consider the valence band which is only partially empty. Since the current in a filled band is zero, the current in a band with a single unoccupied state is the negative of the current in a band with a single occupied state. Therefore, we may interpret the conduction in the partially empty band in terms of holes, “particles” representing absence of electrons and possessing a positive elementary charge as well as positive mass. Now, we may treat these particles, electrons in the conduction band and holes in the valence band, as having a positive mass but opposite charge. The energy band diagrams describe the relationship between the energy and crystal momentum for electrons in the crystal. If an electron did not undergo scattering, then the effect of an applied field E, assuming −q as the electronic charge,6 is to cause a change in momentum following −qE = h̄ dk , dt (2.47) and the electron, in the reduced-zone approach, would be expected to transit the Brillouin zone, reach the Brillouin zone boundary, re-enter and transit again, an oscillatory phenomenon in k-space, and hence real space, a phenomenon termed Zener–Bloch oscillations. The angular frequency of such an oscillation would be ω= qEa , h̄ (2.48) where a is the unit cell dimension. In reality, there are several phenomena that reduce the likelihood of this happening. We have considered the lattice to 6 We use the notation q to represent the magnitude of elementary charge. The sign of the charge will be included explicitly. 20 2 Review be perfectly periodic with no imperfections. Any disturbance from the idealized picture leads to a perturbation, which can cause the electron to change its state—a process that may or may not conserve energy and momentum. Impurities, defects in crystallinity, etc., can all cause changes in energy and momentum. So can the vibration of ion cores around their mean positions. All these processes, that we call scattering, dampen an unlimited change of momentum because any perturbation introduced by these processes can cause a change in the state of the electron and hence its momentum, and even in the most perfect of crystals, scattering due to lattice vibrations are always present. Our discussion of electrons was based on idealized grounds in a one-dimensional framework. On the basis of this we made comments on how one may go about developing accurate three-dimensional models that mimic real crystals. The results of these will be the subject of discussion in the latter part of this chapter from a device perspective. In a similar vein, we will consider the lattice vibration in one dimension, to understand the behavior of phonons—“particles” that characterize these vibrations. This will establish the conceptual framework for us to discuss phonon dispersion in three dimensions in the latter part of this chapter. Consider Figure 2.5, which shows a one-dimensional lattice consisting of two atoms of differing atomic mass m and M . Since the amplitude of the vibrations of the atoms tends to be small, the force on the atoms can be characterized by the first term of the functional expansion with position. This is the restoring force similar to that of spring models. Denoting the force constant as β, the position as z, we may write the force F for the two species as: F2n = m and F2n+1 = M d2 z2n = β (z2n+1 + z2n−1 − 2z2n ) , dt2 (2.49) d2 z2n+1 = β (z2n+2 + z2n − 2z2n+1 ) . dt2 (2.50) The wave solution is of the form z2n = A exp [j(ω1 t − 2nqa)] , (2.51) z2n+1 = B exp [j (ω2 t − (2n + 1)qa)] , (2.52) and where q, like k for electrons, is the symbol for wave vector. Substituting, and solving for the displacement relationship between z2n+1 and z2n , we get z2n+1 = β [1 + exp (−2jqa)] z2n . 2β − M ω22 (2.53) Since this can only be satisfied if the time dependence of z2n+1 is the same as that of z2n , the angular frequencies must be the same, i.e., ω1 = ω2 = ωq . Following a procedure similar to that for derivation of coefficients for Kronig–Penney model, 2.2 Electrons, Holes, and Phonons 21 Figure 2.5: Mean and instantaneous position of atoms in a diatomic linear lattice is shown in the top part of the figure. The vibration shown corresponds to the acoustic branch. The lower part of the figure shows the dispersion relationship for this problem with m < M as discussed in the text. 22 2 Review we have a unique solution for the constants only if the determinant of coefficients in A and B is zero, i.e., (2β − M ωq2 )(2β − mωq2 ) − 4β 2 cos2 (qa) = 0. (2.54) The dispersion relation for phonons that characterize these vibrations, then, is: E h̄ 2 = ωq2 =β 1 1 + m M ±β " 1 1 + m M 2 4 sin2 (qa) − mM #1/2 . (2.55) This dispersion relationship is shown in Figure 2.5. As with the energy-band behavior in Kronig–Penney model, there exists a forbidden zone of energy, or angular frequency, that the vibrations may not have. The vibrations in this periodic structure have been treated as for harmonic oscillators; they have more fundamental foundation in quantum mechanics akin to the treatment of photons. It is therefore quite useful to introduce the concept of phonons, as indistinguishable “particles” which characterize these vibrations. In many ways, this wave aspect of lattice vibrations in a periodic structure is also similar to that of the wave nature of electrons in the periodic structure. The modes of vibrations are discrete just as the states of the electrons are discrete. Phonons are particles that obey principles of conservation of energy and momentum; however, phonons themselves need not be conserved, since a change in temperature can increase or reduce the number of vibrations, unlike electrons in conduction or valence bands. These phonons, representing vibrations occurring at a frequency ωq , have an energy h̄ωq where h̄ is the reduced Planck’s constant, and have a momentum h̄q. The occupancy probability of the state (nq ) of energy h̄ωq at a temperature T is given by Bose–Einstein statistics: nq = 1 . exp (h̄ωq /kT ) − 1 (2.56) Returning now to the dispersion relationship of phonon modes in the simple one-dimensional diatomic model, Figure 2.5 shows that there are two bands— the higher energy branch is called optical branch, and the lower energy branch is called acoustic branch. Acoustic branch results from in-phase vibration of neighboring atoms, while optical branch results from out-of-phase vibration of neighboring atoms. At the zone edge, however, they show a similar character. Figure 2.6 shows a schematic of the displacement of the atoms at the zone center and at the zone edge for the acoustic and optical branches for the diatomic lattice. Since the acoustic mode has in-phase vibration, it has a smaller frequency and hence smaller energy. The optical branch has a higher frequency and energy because of the out-of-phase vibration. The acoustic phonon is similar to a propagating acoustic wave; hence the use of the adjective. The term optical phonon originates from the excitation of these vibrations by photons in the infrared part of the spectrum. At p the Brillouin zone boundary, the frequency of the optical branch reduces to 2β/m, i.e., that due to the lower mass ions, and, as Figure 2.6 shows the, heavier atoms remain stationary. Similarly, the 2.2 Electrons, Holes, and Phonons 23 Figure 2.6: An instantaneous snap-shot of displacement of atoms during acoustic and optical mode vibrations for the diatomic one-dimensional lattice. Part (a) shows the zone center schematic for the optical branch, part (b) shows the same for the acoustic branch, part (c) shows the zone edge schematic for the optical branch, and part (d) shows the same for the acoustic branch. 24 2 Review p frequency of the acoustic branch reduces to 2β/M , i.e., that due to the higher mass ion with the smaller mass ion stationary. Interaction between phonons and electrons, alluded to in our comments regarding Zener–Bloch oscillations, is among the stronger scattering mechanisms and is crucial to understanding the transport of carriers in semiconductors. We will review this later in the chapter. Interactions can also occur between phonons and other phonons. Since phonons, with their basis in lattice vibrations, are one of the major means for heat transport in the lattice, phonon-phonon interactions are of a large interest in that subject. In semiconductors, this is of interest because heat dissipation has to be transported; however, it is not of primary importance. When two phonons interact with the sum of the momentum still within the first Brillouin zone, then the process, called a normal process, leaves the heat transport unaffected. However, if the resultant phonon wave vector is outside the first Brillouin zone, then the translation by the reciprocal lattice vector G results in a wave vector which is opposite in sign to the sum of the the wave vectors of the two incident phonons. This process is known as the umklapp7 process, and since the equivalent wave vector is negative, it produces a thermal resistance. 2.3 Occupation Statistics The occupation of carriers in the energy bands, as well as the behavior of impurities in the semiconductor, are all related to the statistics of occupation of energy levels by electrons. Electrons are fermions and hence the statistics are non-classical. Limitations placed by Pauli’s exclusion principle should cause a behavior that is dependent on doping. Occupation of bands and discrete impurity energy levels is related to many effects of importance in semiconductor devices, most prominent among which is the behavior of degenerate material due to Fermi–Dirac statistics of occupation. The subject of occupation statistics arises not just in calculating this doping dependence, but also in generationrecombination effects, etc., This section is a review of the general principles of the approach as applied to both energy band states and impurity states. 2.3.1 Occupation of Bands and Discrete Levels Electrons are independent and indistinguishable particles with a spin of ±1/2. Pauli’s exclusion principle restricts the occupation of any state by only one electron. The statistics for this situation are commonly referred to as Fermi– Dirac statistics. Consider a closed system of energy E consisting of n particles that can occupy energy levels · · · Ej · · · each of which has a degeneracy · · · gj · · ·. The number of distinguishable arrangements by which nj particles can occupy a jth state is given by the permutation term Pj : Pj = 7 To gj ! . nj ! (gj − nj )! turn over; from the German word umklappen. (2.57) 25 2.3 Occupation Statistics For the closed system, the total number of such arrangements is the product over all the states of the system. This is given by the permutation term P given by Y Y gj ! . (2.58) P = Pj = nj ! (gj − nj )! j j This permutation term is very large, since, in a usual problem such as electrons in the semiconductor, the number of states and carriers is large. We may use Sterling’s approximation for the natural logarithm of a factorial, given by ln(x!) = x ln(x) − x. (2.59) The system is in thermodynamic equilibrium, i.e., has time-independent macroscopic properties when the P is a maximum. This can be found by setting the derivative of P or equivalently of ln(P ) to zero, with the condition that the number of particles n and the total energy E remain a constant. The total number of particles and the total energy of the system are therefore constrained by X n= nj (2.60) j and E= X nj E j . (2.61) j Therefore, the maximum, using Lagrangian multipliers,8 occurs when X gj 0 = d ln(P ) = −1 − ln(nj ) + ln (gj − nj ) + − g j − nj j nj + A + BEj dnj g j − nj X g j − nj + A + BEj dnj . = ln nj (2.62) j Therefore, nj = gj . exp (−A − BEj ) + 1 (2.63) The ratio of particles to states of this specific problem is referred to as the Fermi–Dirac distribution function, and is given by f(E) = nj 1 1 = = , gj exp (Ej /kT ) + 1 exp [(E − ξf ) /kT ] + 1 (2.64) 8 The method of Lagrangian multipliers allows us to maximize and minimize a dependent variable when the maximization and minimization is performed under the constraint that another set of dependent variables, which are also a function of the same independent variables, remain constant. Let f be the former, and let φ and ψ be the latter; then, df +Adφ+Bdψ = 0. 26 2 Review where we have made the appropriate substitutions for constants A and B from the definition of macroscopic properties of the system. Ej = E − ξf , where E is the energy of the level of interest, and ξf is known as the Fermi energy. Fermi energy, based on the above relationship, has the following meaning: at absolute zero temperature, all the states above the Fermi energy are empty and all the states below it are filled. At any finite temperature the states at the Fermi energy are half filled. Similar to the Fermi–Dirac statistics, the Maxwell–Boltzmann statistics apply to a system of independent particles, but unlike Fermi–Dirac statistics, these are distinguishable particles which are non-interacting. One may employ mathematics similar to the above with the distinction that now the number of n arrangements of the jth particle state are gj j /nj !, and hence the total number of permutations of the system are: ! Y gjnj . (2.65) P = n! nj ! j n Since g1n1 × · · · gj j × · · · is a constant, a similar procedure to the above (see Problem 1) leads the ratio of particles to states for the Maxwell–Boltzmann distribution function as nj Ej E − ξf f(E) = = exp − = exp − . (2.66) gj kT kT This is the probability of the occupation of the state j; the exponential factor is the Maxwell–Boltzmann factor. Both of these statistics are useful in describing the occupation of states in the energy bands. When the number of carriers is small, the number of available states is so much larger than the number of carriers that the Fermi–Dirac distribution reduces to the Maxwell–Boltzmann distribution. This conclusion also follows from the above relationships. If the energy level of interest is higher than the Fermi energy by 3kT , then the exponential term is greater than 20, and use of the much simpler Maxwell–Boltzmann statistics leads to an error of less than 5%. We now consider the statistics of donors, acceptors and traps. Donor and acceptor statistics become considerably important in the limits of degeneracy. Degeneracy implies a Fermi level above the donor level or below the acceptor level since the carrier densities are now close to or higher than the number of states available in the bands. This implies that only a fraction of the donors or acceptors contribute the carriers. The occupation of the donor energy levels is therefore central to the determination of the carrier density given a donor or acceptor impurity density in the high carrier density limit. This problem is actually quite complex. We are implicitly arguing that electrons at the donor levels, or lack of them at the acceptor levels, does not contribute to conduction and hence can not be included in the count of nearly free electrons or holes. In the limit of very high doping, impurity bands form because of energy level 27 2.3 Occupation Statistics splitting caused by impurity–impurity interactions. Such impurity bands may coalesce with the conduction or valence bands. States are now available for change of momentum and hence conduction may take place through these levels. This is the reason that carrier freeze-out, the removal of carriers from conduction processes, does not occur as easily in highly doped material. Here, we will ignore such band formation. Thus, the derivation is strictly useful only in the limits of low degeneracy. + Let ND be the total number of donor centers, ND the ionized donors and + 0 ND the neutral donor centers. ND electrons contributed by the ionized donors are distributed among energy levels · · · j · · · of energy · · · Ej · · · and degeneracy · · · gj · · ·; let these be occupied by · · · nj · · · electrons. In addition to occupying 0 these energy levels in the conduction band, electrons also occupy ND sites at the donor energy level ED . The number of ways that the jth level in the conduction band can be occupied is Qj = Cngjj = gj ! , nj ! (gj − nj )! (2.67) and hence the total number of such arrangements is R= Y j gj ! . nj ! (gj − nj )! (2.68) Since a neutral donor center results from the addition of an electron to an 0 ionized donor, we have ND electrons to be distributed among ND donor centers at an energy ED . In the lattice, the donor usually exists at a substitutional site, and ionizes by giving away an excess electron from its outer shell (see Figure 2.7). Since spin degeneracy is two, this excess electron can have a spin in one of two orientations. So, 0 ND ND Q = CN 0 = 2 D ND ! 0 ! (N − N 0 )! ND D D (2.69) 0 gives the number of arrangements of ND electrons on ND sites. The total number of electrons in the system is X 0 n = ND + nj , (2.70) j and the total energy is 0 E = ND ED + X nj E j . (2.71) j The total number of arrangements for the electrons, both in the bands and at the discrete levels, is 0 P = Q × R = 2ND ND ! 0 ND ! (ND − 0 ND )! Y j gj ! . nj ! (gj − nj )! (2.72) 28 2 Review Figure 2.7: A schematic describing processes that occur during the change in ionization state for most common donors and acceptors in a semiconductor. Our procedure, as before, follows with the use of Lagrangian multipliers and Sterling’s approximation to maximize P . We need to evaluate the differential: X X 0 0 d[ln(P ) + A(n − ND − nj ) + B(E − ND ED − nj Ej )] j = j 0 0 0 d ND ln(2) + ln(ND !) − ln(ND !) − ln[(ND − ND )!]+ X [ln(gj !) − ln(nj !) − ln[(gj − nj )!]] + j 0 An − AND −A X j 0 nj + BE − BND ED − B X j nj E j } . 0 Maximizing with respect to (w.r.t.) ND leads to 0 0 ln 2 − ln ND + ln ND − ND − (A + BED ) = 0, and 0 ND = ND 1+ 1 2 1 . exp (A + BED ) (2.73) (2.74) (2.75) Similarly, maximizing w.r.t. to nj leads to nj 1 = , gj 1 + exp (A + BEj ) (2.76) for the occupation of conduction band states. This we had derived before, but the distribution function for occupation of electrons at the donor levels is the new result. Substituting for the thermodynamic variables as before, we may 29 2.3 Occupation Statistics write the distribution function for electron occupation at the donor level as f (ED ) = 0 ND = ND 1+ 1 2 1 , exp [(ED − ξf ) /kT ] (2.77) and since the total number of donors are divided between those that are neutral + 0 and those that are ionized, i.e., ND = ND + ND , we obtain + ND 1 = . ND 1 + 2 exp [(ξf − ED ) /kT ] (2.78) Occupation statistics for acceptors can be found in a similar manner. Most common acceptors occupy substitutional sites in the lattice and are deficient by one electron in their outer shell. The electron can go in the outer shell of a neutral acceptor in only one way without violating Pauli’s exclusion principle. This electron may, however, come out with either spin and go to one of the two degenerate valence bands that commonly occur for most semiconductors of interest. This leads to (see Problem 3): f (EA) = and NA− 1 = , NA 1 + 4 exp [(EA − ξf ) /kT ] NA0 = NA 1+ 1 4 1 . exp [(ξf − EA ) /kT ] (2.79) (2.80) Most trap or deep levels can be treated in a similar manner as above. The degeneracy of the levels, a term associated with the factors 2 and 4 above (strictly speaking, 2 and 1/4), may be different for a trap level because these need not be from the adjacent columns of the periodic table. An additional feature of the deep level, as a result, is that they may have more than one ionized state within the bandgap. The impurity can be in any of these states, and the equilibrium statistics depend on all the other possible states of the system. Problem 23 of Chapter 3 is an advanced exercise related to this subject. 2.3.2 Band Occupation in Semiconductors We have now discussed the occupation probabilities of carriers in states that arise from many different causes. In a device, the parameter that is of more interest is the number of carriers that are available for conduction. To determine this, in addition to the probability of occupation of a state, we need to know the number of such states. In a three-dimensional crystal, there is a distribution of such states, a quasi-continuum, since the number of states is large. This may be lumped together in a density of state function D(E) which is the number of states in a unit energy range at any energy E. Thus in an energy range dE at the energy E, the total number of states is D(E)dE. The number of carriers, knowing the density of states as a function of energy, can now be determined 30 2 Review as a function of the Fermi energy. If Ec represents the energy of the bottom of the conduction band, then, at thermal equilibrium, Z Emax n= f(E)D(E)dE, (2.81) Ec where D(E) is the density of states available for occupation, and Emax is the maximum energy available in the conduction band. Since the distribution function decreases exponentially, we can replace Emax by ∞ without any significant error. Consider only the simplest approximation of bands, the parabolic band. The density of states (D(E)), i.e., the number of states per unit volume of the crystal per unit energy, can be found by considering arguments based on allowed wave vectors of the crystal. For a one-dimensional crystal, the permitted values of the wave vector k of the wave function exp(jkr) in the periodic lattice are ±2πl/L, where l is an integer and L is the linear dimension. This follows from the requirement that the ends of the crystal be electron nodes. By extension, for a cube of dimension L, the permitted values of the wave vector are ±2πlx /L, ±2πly /L, and ±2πlz /L, corresponding to the three independent directions and with lx , ly , and lz as positive integers. Thus, the magnitude of wave vector k follows as 4π 2 lx2 + ly2 + lz2 4π 2 l2 4π 2 l2 2 = = . (2.82) k = L2 L2 V 2/3 Each permitted value of k corresponds to various combinations of lx , ly , and lz which result in the same l given by l= L V 1/3 k= k. 2π 2π (2.83) All states on a sphere, whose radius is l, result in identical energy, although the carrier may be moving in different directions. For energy varying from 0 to E, or the wave vector varying from 0 to k, the total number of modes allowed is the volume of sphere, i.e., 4πl3 /3 or V k 3 /6π 2 . Thus, the density of states per unit volume and unit energy, taking into account two possible spin orientations, is given as 3 3/2 k 1 2 dk 1 2m∗ d 1/2 D(E) = 2 = 2k = (E − Ec ) . (2.84) dE 6π 2 π dE 2π 2 h̄2 In general, there may be more than one equivalent valley and the masses along the three axes may be unequal. The effective mass in the expression above, by convention, is the density of states effective mass that corresponds to the real density of states. Thus, for unequal, longitudinal (m∗l ) and transverse (m∗t1 and m∗t2 ) masses, and a degeneracy gv of the valleys, the density of states function D(E) is given by the expression 3/2 1 2m∗d 1/2 D(E) = (E − Ec ) , (2.85) 2π 2 h̄2 31 2.3 Occupation Statistics where m∗d = gv2 m∗l m∗t1 m∗t2 1/3 . (2.86) Note the differences between the conduction effective mass and density of states effective mass. Given this density of states, the integral relationship for electron density now becomes 1 n= 2π 2 2m∗d h̄2 3/2 Z (E − Ec)1/2 dE . Ec 1 + exp [(E − ξf ) /kT ] ∞ (2.87) Changing to variable η = (E − Ec)/kT , and denoting ηfc = (ξf − Ec )/kT , the integral relationship takes the form n= 1 2π 2 2m∗d h̄2 3/2 3/2 (kT ) Z ∞ 0 η 1/2 dη ≡ NC F1/2 (ηfc ) , 1 + exp (η − ηfc ) (2.88) where F1/2 is the Fermi integral of the order one-half.9 The parameter NC thus has the value 1 NC = 2 2π 2m∗d h̄2 3/2 3/2 π (kT ) 1/2 2 m∗d kT =2 2πh̄2 3/2 . (2.93) NC is an “effective” conduction band density of states. It may be viewed as an energy integrated density of state which approximates the effect of total density of states in the conduction band, but which appears at the edge of the conduction band. For values of of ηfc smaller than −3, i.e., with non-degenerate statistics dominating, the Fermi integral takes an exponential form, and the expression for electron density reduces to ξf − Ec n = NC exp (ηfc ) = NC exp , (2.94) kT which is the classical Maxwell–Boltzmann relationship. 9 Fermi integrals are related to Γ functions by Fν ηf = 1 Γ (ν + 1) Z ∞ 0 η ν dη 1 + exp η − ηf , (2.89) where ηf is the function ηf c in this instance. It can also be the corresponding valence band function ηf v for the calculations of hole density. Elsewhere, we have also used ηf n and ηf p synonymously for these for convenience. The derivative of F1/2 function w.r.t. ηf is the F−1/2 Fermi function. The Γ functions have the characteristics: Γ (ν + 1) = Γ For integer variables, Z ∞ η ν exp(−η)dη, Γ (ν + 1) = νΓ (ν) , (2.90) = π1/2 , Γ (1) = 1. (2.91) 0 1 2 and Γ (ν + 1) = ν!. (2.92) 32 2 Review Figure 2.8: The Fermi integral (F1/2 (ηf )) as a function of the parameter ηf . A derivation similar to the above leads to the relationship for holes (see Problem 2) as p = NV F1/2 (ηfv ) , (2.95) where ηfv = (Ev − ξf )/kT , and the effective density of states for the valence band is ∗ 3/2 3/2 1/2 md kT 1 2m∗d 3/2 π =2 (kT ) , (2.96) NV = 2 2 2π 2 h̄ 2πh̄2 with m∗d as the effective density of states mass for the valence band. A plot of the Fermi integral as a function of the parameter ηf (ηfc or ηfv ) is shown in Figure 2.8. The product of carrier concentrations in the Maxwell–Boltzmann limit is Eg Ec − Ev np = n2i = NC NV exp − = NC NV exp − , (2.97) kT kT where ni is the intrinsic carrier density. 2.4 Band Structure Our discussion, so far, has already dealt with the central role of band structure in the occupation of carriers in a band and hence their behavior in thermal equilibrium. Band structure is also central to determining the transport characteristics of carriers and many other phenomena because it determines the relationship 2.4 Band Structure 33 Table 2.1: Symmetry points in the first Brillouin zone of face-centered cubic lattice. Symmetry Wave Vector Degeneracy Point k= Γ 0 1 L ±(π/a)h111i, ±(π/a)h1̄11i, ±(π/a)h11̄1i, and ±(π/a)h111̄i 8 X ±(2π/a)h100i, ±(2π/a)h010i, and ±(2π/a)h001i 6 K ±(3π/2a)h110i, ±(3π/2a)h1̄10i, ±(3π/2a)h011i, ±(3π/2a)h01̄1i, ±(3π/2a)h101i, and ±(3π/2a)h101̄i 12 W ±(π/a)h210i, ±(π/a)h021i, ±(π/a)h102i 6 between the energy and the momentum of the carrier. In this section, we will review the band structure relationships in compound semiconductors. The consequences of the band structure in some major and general phenomena will be the subject of subsequent sections. We have noted that the reciprocal space, also called phase space, k-space, Fourier space, and momentum space, is a convenient tool to describe the behavior of both electronic states and vibrational states. The coordinate axes of the reciprocal lattice are the wave vectors of the plane waves corresponding to the Bloch states or the vibration modes. The Wigner–Seitz unit cell in the reciprocal space is the first Brillouin zone. This was shown in Figure 2.1. This is also the first Brillouin zone for single element semiconductors Si and Ge, i.e., for diamond lattice. Let us consider the conventional definitions of the coordinate system and the important points of symmetry in the first Brillouin zone. These positions in the Brillouin zone are of particular importance because of their symmetry, and hence the relation to other characteristics that this entails. Table 2.1 summarizes the wave vectors of some of these symmetry points. Since there is symmetry of rotation around the three axes, and of mirror reflection in the three planes, the irreducible part of this first Brillouin zone is only 1/48th in size. This irreducible part is shown in Figure 2.9. The reduced part shown in Figure 2.9 is the minimum description of wave vectors of carriers and vibrational modes in the zinc blende crystal in order to characterize their effect. In numerical calculations, it is quite often convenient to use the description of band structure only in this irreducible zone and then perform symmetry operations to generate the information as it becomes necessary during the calculations. The task of determining the energy–momentum relationship for a threedimensional lattice is of course a difficult one. It involves the determination of the solutions to Schrödinger equation using the crystal Hamiltonian. This crystal Hamiltonian contains energy terms due to kinetic, potential, and magnetic contributions arising from electrons in a lattice structure of the nuclei. The 34 2 Review Figure 2.9: The irreducible part of the first Brillouin zone of zinc blende crystals is shown as the 1/48th part of the truncated octahedron. The major symmetry points are identified in this irreducible part. solution can be accomplished in a number of ways using perturbation theory: using tight binding approximation, i.e., using functions that are linear combinations of either atomic or molecular orbitals; using pseudopotentials; and using various other functional approaches such as Green’s functions techniques. Perturbation theory allows the determination of final energy solution, by using the smaller Hamiltonian terms as perturbing functions. The basis states for using this perturbation are determined from the major term associated with Coulombic interactions with the nuclei. Since the basis functions, involving calculations based on using atomic orbitals near the cores, are |s > and |p > like, the resulting functions are combinations of these at various important points of the Brillouin zone. Figures 2.10–2.13 show the band structures10 of Si, Ge, GaAs, InP, InAs, AlAs and Ga.47In.53 As, over a large energy range, and Figure 2.14 shows the band structure of both conduction and valence band for GaAs in larger detail. We can make some general observations regarding these band structures. GaAs is a direct bandgap semiconductor with the ordering of minima from low to high energies in the conduction band as Γ, L, and X. All compound semiconductors exhibit a universal feature of a degenerate light and heavy hole 10 These are based on the band structure calculations of M. Fischetti. Some of this information is published in M. Fischetti, “Monte Carlo Simulation of Transport in Technologically Significant Semiconductors of the Diamond and Zinc Blende Structures, Part I: Homogeneous c Transport,” IEEE Trans. on Electron Devices, ED-38, No. 3, p. 634, Mar. 1991 IEEE. 2.4 Band Structure 35 Figure 2.10: Conduction band structure of silicon (a) and germanium (b) over major points and directions in the first Brillouin zone. After M. Fischetti, “Monte Carlo Simulation of Transport in Technologically Significant Semiconductors of the Diamond and Zinc Blende Structures, Part I: Homogeneous c Transport,” IEEE Trans. on Electron Devices, ED-38, No. 3, p. 634, Mar. 1991 IEEE. 36 2 Review Figure 2.11: Conduction band structure of GaAs (a) and InP (b) over major points and directions in the first Brillouin zone. After M. Fischetti, “Monte Carlo Simulation of Transport in Technologically Significant Semiconductors of the Diamond and Zinc Blende Structures, Part I: Homogeneous Transport,” c IEEE Trans. on Electron Devices, ED-38, No. 3, p. 634, Mar. 1991 IEEE. 2.4 Band Structure 37 Figure 2.12: Conduction band structure of InAs (a) and AlAs (b) over major points and directions in the first Brillouin zone. After M. Fischetti, “Monte Carlo Simulation of Transport in Technologically Significant Semiconductors of the Diamond and Zinc Blende Structures, Part I: Homogeneous Transport,” c IEEE Trans. on Electron Devices, ED-38, No. 3, p. 634, Mar. 1991 IEEE. 38 2 Review Figure 2.13: Conduction band structure of Ga.47In.53 As over major points and directions in the first Brillouin zone. After S. Tiwari, M. Fischetti, and S. E. Laux, “Transient and Steady-State Overshoot in GaAs, InP, Ga1−xInx As, and InAs Bipolar Transistors,” Tech. Dig. of International Electron Devices Meeting, c p. 435, Dec. 9–12, 1990 IEEE. Figure 2.14: Details in medium energy region of the band structure of GaAs over major points and directions of the Brillouin zone. 2.4 Band Structure 39 band at zone center, and a split-off band. The split-off band comes about because of the perturbation from the magnetic energy associated with the spin and orbit of the electron. This coupling is generally referred to as spin-orbit coupling or L.S coupling, and the split-off band arising from it is 0.34 eV below the valence band maxima in GaAs. The bandgap of intrinsic GaAs, at 300 K, is 1.42 eV, the L valley is 0.29 eV, and the X valley about 0.48 eV above the Γ minimum. Referring to the earlier band structure figure of silicon (Figure 2.10), Si is an indirect bandgap semiconductor with an intrinsic bandgap of 1.10 eV; the minimum in conduction band energy occurs ≈ 85% of the way to the X point from the Γ point. Constant low energy surfaces around this valley, loosely referred to as the X valley, are 6-fold degenerate and aligned along the Cartesian coordinates. The next lower valley is between the line joining X with the U point, followed by the L point. Again there is the degenerate light and heavy hole band at zone center which is the valence band maximum. Unlike compound semiconductors, silicon does not exhibit a large separation of the split-off band. The origin of this smaller separation is in the spin-orbit energy that gives rise to the formation of the split-off band. Light atoms exhibit small spin-orbit interaction. In silicon, spin-orbit splitting is only 0.044 eV. Spin-orbit energy, however, rises rapidly with atomic mass. Germanium has a spin-orbit splitting of 0.29 eV. Germanium is also an indirect bandgap semiconductor with a bandgap of 0.72 eV for intrinsic material at 300 K. The ordering of the conduction band minima is L, X, and Γ. The constant energy surfaces in the lowest conduction valley, the L valley, are ellipsoids aligned along the h111i direction. These are eight-fold degenerate while the ones in silicon were six-fold degenerate. Both in silicon and germanium, the lowest conduction bands have multiple valleys associated with them. A consequence of this is the availability of a large number of states to scatter into. A large change in momentum is required for this process, and is available through zone edge phonons. The result of this is that, at low energies, both silicon and germanium experience higher scattering than direct bandgap compound semiconductors. Another interesting feature from the band structures is the observation of the lower effective mass for holes of germanium. This gives rise to nearly identical electron and hole mobilities in germanium. InP is a direct bandgap compound semiconductor with similar ordering of conduction band minima as GaAs. Like GaAs, the light and heavy hole bands are degenerate and a split-off band occurs ≈ 0.78 eV below, at the zone center. The bandgap of intrinsic InP is 1.35 eV at 300 K. InAs is a direct bandgap compound semiconductor with a small energy gap of ≈ 0.36 eV at 300 K. Its ordering of conduction band minima is also Γ, L and X. Most compound semiconductor are direct bandgap materials. AlAs and GaP are two of the few compound semiconductors with indirect energy bandgap. In AlAs, the X valley is the minimum conduction energy valley followed by the L valley. It exhibits a behavior similar to silicon, and some of these characteristics may be traced to aluminum, which is a light atom like silicon. 40 2.5 Properties of Semiconductors for Devices Phonon Dispersion in Semiconductors We have considered the conceptual basis for treatment of phonons as part of our discussion of one-dimensional models. To recapitulate, the Bloch function formalism considers the electron in a periodic lattice whose host atoms are stationary. At finite temperatures, atoms vibrate around this mean position. The periodic vibration leads to perturbation of the stationary periodic potential and causes the changes in the electron wave function in time. The lattice vibrations can be described in a framework that is analogous to the description of electrons. Phonons, representing these vibrations occurring at a frequency ωq , have an energy h̄ωq , where h̄ is the reduced Planck’s constant, and have a momentum h̄q. Phonons describe vibrations just as photons describe electromagnetic waves. Two phonon branches result in this idealized one-dimensional system, a high energy branch for optical phonons, and a lower energy branch for acoustic phonons. Scattering resulting from optical and acoustic phonons are commonly referred to as optical phonon scattering and acoustic phonon scattering. Since the energy of the acoustic phonon mode is smaller it produces less perturbation than the optical phonons. Three-dimensional crystals bring with them additional complexity in phonon dispersion. In the diatomic one-dimensional crystal, the atoms could vibrate only along one axis, i.e., along the longitudinal direction. In a three-dimensional crystal, they may have longitudinal oscillations, as well as transverse oscillations in two orthogonal directions. In the primitive cell, if there are N different types of atoms either of differing mass or ordering in space, 3N vibration modes will result. In general, three of these branches, the acoustic branches, will disappear at zone center. The remaining 3N − 3 branches will be optical branches. For the cubic crystals, GaAs or Si, e.g., N = 2, and hence there are three acoustic and three optical branches, each three comprising of one longitudinal and two transverse modes. However, along h100i, h110i, and h111i directions, the two transverse directions are indistinguishable. So, here, in the cubic crystal, the two transverse oscillations are degenerate . Examples of phonon dispersion curves that describe the energy or frequency dependence as a function of wave vector are shown in Figure 2.15 and 2.16 for Si, Ge, GaAs, and InAs. The order of magnitude of the optical phonon energy is between 25 and 50 meV for most semiconductors of interest, in the same order of magnitude as the thermal energy. Heavier ions should be more sluggish; the acoustic branch then should have a lower peak energy. This is reflected in the ascending ordering of peak acoustic energies of InAs, Ge, GaAs, and Si in inverse proportion to the weight of the heaviest element. A similar trend holds for the lowest optical branch energy for these materials. An additional interesting feature of these figures is that, for compound semiconductors, the longitudinal optical phonon is slightly more energetic than the transverse optical phonon at low momenta because of the presence of ionic charge. At high momenta, in certain directions, the optical branches may even cross over because the higher momenta results in a larger reduction in energy of the longitudinal mode due to the effect of the dipole. Phonon Dispersion 41 Figure 2.15: Phonon dispersion curves for Si (a) and Ge (b) as a function of the wave vector in the first Brillouin zone. After Landolt-Börnstein; O. Madelung, M. Schulz, and H. Weiss, Eds., Semiconductors, V 17, Springer-Verlag, Berlin (1982). 42 Properties of Semiconductors for Devices Figure 2.16: Phonon dispersion curves for GaAs (a) and InAs (b) as a function of the wave vector in the first Brillouin zone. After Landolt-Börnstein; O. Madelung, M. Schulz, and H. Weiss, Eds., Semiconductors, V 17, SpringerVerlag, Berlin (1982). 2.6. SCATTERING OF CARRIERS 43 These figures also show that at specific large momenta, in directions differing from the major crystal axis direction h100i, h110i, or h111i, the degenerate transverse modes split because of the breakdown of symmetry. This occurs for both optical and acoustic modes. 2.6 Scattering of Carriers The carrier transport in a medium occurs under the influence of applied forces which accelerate the carriers in the preferred direction, and the carrier interacts with its environment whose general effect is to render the motion random. Scattering is a general term for the interaction of the carrier with the surroundings. Our discussion of scattering is a review, short on detail, but with a view of understanding its general consequences for compound semiconductors. An electron in the crystal, under the influence of an external force, such as due to the electric field, picks up its energy during its acceleration, but changes energy and/or momentum by various scattering mechanisms that come about because of lattice vibrations or other carriers in its surrounding, as well as defects of the lattice. A broad classification of these scattering mechanisms is considered in Figure 2.17 based on their origin. These various scattering mechanisms are events of interaction between the carrier and its surroundings which cause it to change its momentum and/or energy. It therefore represents the individual and aggregate effect of the carrier’s surroundings which influences the carrier’s individual and aggregate transport behavior. The behavior of electrons in a perfect crystal can be described by a wave function. This is the Bloch function, which is the solution of the time independent Schrödinger equation. If the scattering processes were not to occur, the application of an electric field would increase the velocity linearly with time, an occurrence generally described as ballistic motion. In reality, for long sample lengths, it reaches a limiting value. This limiting value is proportional to the field at low fields (v = µE, where v is the velocity, µ the mobility, and E the electric field, a constant mobility region), and saturates to the value vs at high fields (the saturation velocity limit). The electron wave function can be described by the same Bloch function until it scatters, i.e., it interacts with an imperfection. When it interacts with the imperfection, the wave function is affected because of perturbation in the periodic potential. The electron has a new wave function at the end of the interaction, i.e., at the end of interaction the electron has a new wave vector and a new energy (in some scattering processes energy may remain unchanged; such scatterings are called elastic scatterings, an example is scattering by impurities). This new wave function describes the behavior of the electron until another interaction. If the perturbation is small, the effect of this interaction can be analyzed by perturbation theory. Our division of these scattering mechanisms is in three general classes: (a) scatterings that come about due to imperfections in the periodicity of the lattice, which we call defect scattering, (b) carrierrelated scattering due to interactions in between the carriers, a process that becomes important at high carrier concentrations, and that can couple with 44 2 Review Figure 2.17: A schematic of classification of various scattering mechanisms based on their origin. 2.6 Scattering of Carriers 45 other modes of scattering, and (c) scattering due to interaction of carriers with the perturbing potential produced by lattice vibrations. 2.6.1 Defect Scattering Imperfections in the periodic potential of a crystal come about due to crystal defects such as vacancies, dislocations, interstitials, etc. However, this is quite uncommon because, except in highly lattice mismatched structures, devices of interest employ material where the density of these is less than unintentional substitutional impurities. Defect scattering also arises from impurity atoms themselves that are used to dope the crystal—this is generally referred to as impurity scattering—and originates in the deviation of the local potential around an impurity from the local and periodic potential of the atoms of the host crystal. If the impurity atom is ionized (as is almost always the case) it is called ionized impurity scattering and this particular scattering is strong. If the impurity atom is not ionized, i.e., it is neutral, it is referred to as neutral impurity scattering. Neutral impurity scattering is quite weak because of the small perturbation in potential from a neutral atom on a lattice site. Consider the scattering due to impurity atoms in a crystal as a function of temperature. We assume that impurity density is not so large so as to cause formation of an impurity band and its coalescence with the conduction band. Such a material, therefore, shows freeze-out of carriers, i.e., at low temperatures, the carriers do not have sufficient thermal energy to make the transition to the conduction or valence bands. At temperatures below the freeze-out temperature, the impurities are largely neutral, and hence there is a weak impurity scattering. As the temperature is raised, impurities ionize and impurity scattering becomes stronger and hence the carrier mobility decreases. As the temperature is continued to be raised, the thermal energy of the carriers continues to increase, their velocities are larger, and the impurity scattering process becomes weak again. An analogy may be drawn between this and the Rutherford scattering used to analyze the scattering of light atoms by heavier nuclei. A high velocity, and energy of particle, causes both a smaller time of interaction and smaller effect on the velocity of the carrier. Because of the large disparity in masses between the atoms and the moving carriers, this scattering conserves energy and is an example of elastic scattering. At high temperatures, other scattering processes become important and impurity scattering plays an increasingly smaller role. It is generally important in the 77 K (liquid nitrogen temperature) to 300 K (room temperature) range. The third defect scattering that is important occurs in mixed crystals such as Ga.47 In.53 As and Ga.7Al.3 As. Due to the random variation of the atoms either on the cation or the anion sites of the lattice, a non-periodic perturbation occurs naturally in such material even when no defect has been added. The perturbations are sufficiently small that alloy scattering generally becomes important only below 300 K. The last of the defect scattering processes important to devices is related to interactions at the surfaces and interfaces of the lattice. This is generally referred 46 2 Review Figure 2.18: A schematic of interface scattering resulting from steps on the crystal surface. Figure 2.19: Steady-state velocity–field characteristics of electrons, in lightly doped bulk Si at the SiO2 /Si interface, in lightly doped GaAs, and at the Ga.7 Al.3 As/GaAs interface at 300 K. to as interface scattering (see Figure 2.18). This crystal defect scattering process is certainly very important at insulator–semiconductor interfaces. It can be important if interfaces are rough and have steps such as mis-oriented compound semiconductor growth. Since carriers in two-dimensional systems are confined very close to the interface, any surface potential perturbation, e.g., through surface atomic steps leads to a decrease in the mobility. In the velocity–field curves shown in Figure 2.19, e.g., the silicon surface mobility is almost half as much as the corresponding bulk mobility. Steps are not the only way this scattering can cause a net energy or momentum change of the carriers. If there are a number of surface states,11 they may cause perturbation effects of their own even for a perfectly smooth surface. For an ideal interface, an incident carrier goes through a reflection without los11 Surface states result from a number of causes, primarily surface reconstruction and nonterminated bonds at the surface. 2.6 Scattering of Carriers 47 ing its energy. Its momentum parallel to the interface is maintained while its momentum perpendicular to the interface is reversed. An example of this is the Ga1−x Alx As/GaAs interface which can be made atomically smooth with negligible interface state density. A low energy electron that can not penetrate the Ga1−xAlx As/GaAs barrier loses no energy and maintains the momentum parallel to the interface. From the scattering perspective, a non-ideal interface is the SiO2 /Si interface. Quite a large fraction of incident carriers lose energy and momentum at the interface because of interface states and atomic roughness. The result of such scattering, called diffuse scattering, is a thermalization of carrier energy distribution and decrease of mobility. 2.6.2 Carrier–Carrier Scattering Carrier-carrier scattering conserves the total energy and momentum of the interacting particles. This scattering, also sometimes referred to as plasma scattering, does cause redistribution of the energy and momentum among the interacting particles, and hence its primary effect is in influencing the carrier distribution as a function of energy and momentum. Thus, the scattering influences those parameters that depend on the shape of the distribution of carriers with energy and momentum. Relaxation rate of energy and transfers to other valleys or bands that depend strongly on energy tails do therefore get influenced directly by carrier–carrier interactions. An additional important way that carrier–carrier scattering influences transport is through its coupling with other scattering mechanisms—the coupling of plasma scattering together with phonons, referred to as plasmon scattering, is an important scattering mechanism in hot electron devices. 2.6.3 Lattice Scattering Lattice scattering is a broad term used for those scattering mechanisms that arise from the existence of the lattice itself. The lattice is a periodic structure, whose periodicity of the perturbation is incorporated in the nearly-free electron model being employed throughout this text. In this periodic lattice, at any finite temperature, the nuclei vibrate around their central positions, a behavior embodied in the dispersion behavior of the semiconductor. Lattice vibration modes that occur at high frequencies and have associated with them a relatively higher energy of 10s of meV are referred to as optical phonon modes. Those occurring at lower frequency over a wider spectrum of frequencies are known as acoustic modes. Optical modes arise from atoms vibrating out of phase with each other, resulting in their higher frequency. Acoustic modes are long range vibrations where the atoms move in phase. These vibrational modes interact with the free electron in a variety of ways, giving rise to the scattering that we call optical and acoustic phonon scattering. Before reviewing further the phonon scattering processes, we summarize a few other terms that are often employed in the description of scattering. These terms arise from the location of the carrier in the reciprocal space as a result 48 2 Review of the scattering process. Referring to the phonon scattering, an electron that scatters via optical phonon scattering is likely to have a significant change in momentum since optical phonons can have large momentum. Large momentum changes most often occur with changes in the valleys or bands that the carriers occupy. Holes, with their degenerate bands, can easily change bands, e.g., between light hole and heavy hole bands; thus corresponding scattering processes, termed inter-band scattering processes, can occur even at low energies. These inter-band scattering processes are unlikely for electrons at low energies. High energy electrons, such as during an avalanche process, may change bands. All such processes involving changes in bands are called inter-band scattering processes, while if a process occurs within a band it is called intra-band scattering process. Inter-band scattering may occur so that the carrier such as an electron scatters within the same valley, e.g., within the Γ valley for electrons. This is referred to as intra-valley scattering. Scattering may occur between different valleys, e.g., using an optical phonon for the large momentum change; this scattering is then referred to as inter-valley scattering. This discussion becomes semantically more elusive, because many valleys can be degenerate. The L valleys are eight-fold degenerate and the X valleys are six-fold degenerate. These are all examples of inter-valley scattering occurring with a large momentum change and hence quite likely involving optical phonons. These valleys are degenerate in energy; however, the amount of momentum change required to transfer to the different valley locations is different. This leads to a further sub-division of intra-valley scattering to f-scattering and g-scattering. f-scattering is the scattering occurring with the nearest degenerate valley locations, and g-scattering is the farthest. 2.6.4 Phonon Scattering Behavior The optical phonon energy is considerably larger in Si than in Ge or GaAs. This may be traced to the larger average weight of the nuclei in Ge and GaAs and smaller bonding forces. Electrons need approximately this energy ≈ 37 meV in Ge, ≈ 36 meV in GaAs, and ≈ 63 meV in Si before they can emit an optical phonon, i.e., lose energy in an optical scattering process. Also, with lowering of temperature, there is a decrease in the occupation probability as described by Equation 2.56. This is referred to as freeze-out of optical phonons. Corresponding to this smaller likelihood of occurrence of optical phonons, there is a smaller likelihood of absorption of an optical phonon. Hence, at low temperatures there is a reduction in optical phonon scattering. Emission process can still occur, and continues to be leading cause for loss of energy at high electric fields. Both of these factors are important to the observed velocity–field behavior and operation of high mobility and hot electron structures as a function of temperature and bias. Now consider the nature of the perturbing potential in acoustic mode. A change in atomic spacing, i.e., deformation of the lattice, leads to a disturbance in the potential called the deformation potential. The magnitude of the deformation potential is proportional to the strain induced by vibrations, and the 2.7. CARRIER TRANSPORT 49 corresponding scattering is called deformation potential scattering. In addition to this spacing effect, if the atoms are slightly ionic (as in all of the compound semiconductors), then the displacement of the atoms leads to a potential perturbation due to the charge on the ions. This is called the piezoelectric potential, and the resulting scattering process is called piezoelectric scattering. It is important in compound semiconductors at low temperatures in relatively pure materials. Recall that optical scattering is weak at low temperatures and low fields due to optical phonon freeze-out, etc., and impurity scattering is weak because of purity and carrier freeze-out, leaving acoustic phonon scattering as the dominant process. The deformation potential scattering is weaker than the piezoelectric scattering, and hence piezoelectric scattering dominates. Optical vibrations also lead to potential perturbation in two ways similar to the case of acoustic vibrations. The first, a non-polar perturbation effect of strain, leads to a scattering referred to as as non-polar optical scattering. The second, due to the polarization from the ionic charge, is referred to as polar optical scattering. In GaAs, AlAs, etc., both these scattering processes are important. In general, for compound semiconductors, the polar optical phonon scattering is the dominant optical scattering mechanism. 2.7 Carrier Transport We will now discuss the relationship of the various scattering mechanisms reviewed above with the steady-state transport behavior of carriers. The operation of a device is interlinked with the transport behavior of carriers. The velocity– field curves for carriers in a semiconductor describe the steady-state behavior of the carriers for both low fields, where perhaps an equally useful parameter is the mobility, and of high fields. The transport of the carrier is related to the scattering of the carriers. In the discussion above, we implicitly assumed a majority carrier. Minority carrier transport is important in the base of a bipolar transistor. It can be significantly different from a majority carrier device at comparable background doping and identical temperatures. This comes about because of changes in scattering behavior that result from changes in screening effects of the perturbations. Scattering can also change when the band occupation behavior is changed, such as through the quantum-mechanical effects of two-dimensional carrier gas systems. Since scattering involves transition from one state to another, it involves a transition probability embodied in a coupling coefficient that describes the likelihood of such a change taking place—a measure of the overlap function of the two states, and the number of such states that are available. It is proportional to both of these. Consider some examples. The overlap function between valence and conduction bands is small in indirect bandgap semiconductors. There is therefore a very small likelihood of band to band transitions at low and moderate fields. Lifetimes of such materials are therefore large. In direct semiconductors, the overlap is larger, so the lifetime is generally worse. Overlap functions can of course be made large in certain device situations and are the reason for tunneling such as 50 2 Review Figure 2.20: Steady-state phonon scattering rates as a function of energy, at low energies, in GaAs, InP, Ga.47In.53 As, and InAs at 300 K. After S. Tiwari, M. Fischetti, and S. E. Laux, “Transient and Steady-State Overshoot in GaAs, InP, Ga1−x Inx As, and InAs Bipolar Transistors,” Tech. Dig. of International c Electron Devices Meeting, p. 435, Dec. 9–12, 1990 IEEE. in the Zener effect. Zener tunneling is as likely in indirect semiconductors as in direct semiconductors. The number of available states is also directly related to the scattering. More available states increases the likelihood of the scattering event. Two-dimensional effects change the density of state distribution as well as screening and hence may influence the scattering behavior. This section reviews the relationship of the scattering with the transport properties of the carriers. 2.7.1 Majority Carrier Transport We now consider scattering rates of some common compound semiconductors in order to relate them to the transport characteristics of interest in the operation of devices. Figure 2.20 shows some of the scattering rates due to phonon processes, at 300 K and low energies, for GaAs, InP, Ga.47In.53 As, and InAs. The minimum in the scattering rates, occurring at very low energies, is due to acoustic scattering. At the low energy threshold for the optical phonon modes, scattering rises rapidly due to the large rate of optical phonon scattering at 300 K. At 77 K and lower temperatures this rate would be lower. At low energies the scatterings are intra-valley events. At higher energies, comparable to or higher than the secondary valley separation, a large density of states is available for inter-valley scattering. So, these scattering rates show another threshold where the secondary valley occurs in GaAs, InP, and Ga.47In.53 As. InAs has 2.7 Carrier Transport 51 a secondary valley at higher than 1 eV and does not, therefore, show such a threshold. Note that InP has the highest low energy scattering; it has both a higher effective mass that leads to higher density of states to scatter into, and a stronger coupling coefficient for scattering. Both Ga.47In.53 As and InAs show favorable low scattering rate characteristics over the energy range, a behavior partly due to the larger secondary valley separation which inhibits inter-valley scattering over a significant energy range. The two divisions of lattice scattering that we have considered are intervalley and intra-valley scattering. In intra-valley scattering, low momentum phonons are involved. At low fields, this intra-valley scattering is important in materials where the conduction band minima occurs at the Γ point, e.g., GaAs, InP and most other compound semiconductors. Inter-valley scattering involves large momentum phonons and is important at low fields in materials with conduction band minimum at non-zero crystal momentum, i.e., non-Γ minimum semiconductors. Examples are Ge, which exhibits a minimum at h111i (i.e., the L point), and Si where it occurs close to h100i i.e., the X point). The phonons that take part in inter-valley scattering are sometimes referred to as inter-valley phonons even though they may be of either the acoustic or optic type. When fields are high, electrons pick up enough energy in between scattering events, and hence even where the central valley is the minimum energy valley inter-valley scattering becomes important. The negative differential mobility of GaAs, e.g., arises from inter-valley scattering from Γ to L and X valleys. Figure 2.21 shows the velocity–field characteristics for GaAs (≈ mid-1016 cm−3 doping) for various temperatures. This figure serves to compare the temperature dependence of the most dominant scattering processes in GaAs. The decrease in mobility at low fields is due to intra-valley scattering, the decrease in velocity at higher fields is due to inter-valley scattering, and the saturation in velocity at very high fields is due to a balance between the energy gain in between scattering events and the energy loss due to high inter-valley scattering. Both of these processes and the corresponding energy and momentum loss rate are shown as a function of the field at room temperature for GaAs in Figure 2.22. In thermal equilibrium, the energy and momentum exchange in between electrons and the lattice is balanced out by phonon absorption and emission. With an applied electric field, the energy and momentum are lost at a higher rate to the lattice, and at moderate fields the inter-valley optical phonon scattering processes dominate. The momentum loss rate hdp/dti, where p is the magnitude of the momentum, causes randomization of the electron velocity distribution in momentum space and consequently results in a finite mobility. Note that the momentum loss rate is higher than the energy loss rate (also recall that optical phonons involve a loss of ≈ 36 meV of energy per emission event). We will discuss subsequently the fitting of both these loss rates, phenomenologically, by a time constant called the relaxation time. The relaxation times for momentum (τp ) and energy (τw ) are in general approximations—phenomenological fitting parameters. These time constants characterize the driving force of return to 52 2 Review Figure 2.21: Velocity–field characteristics for electrons in lightly doped GaAs as a function of electric field for various temperatures. Figure 2.22: Momentum and energy loss rate in steady-state as a function of electric field for GaAs at 300 K due to inter-valley and intra-valley scattering involving polar optical phonons. 53 2.7 Carrier Transport equilibrium. and dp − dt loss dW − dt loss = = hpi , τp hW i . τw (2.98) Here, W is the energy of mean energy of the carriers and the angled brackets indicate an averaging over all the carriers.12 We may now describe some general features of the relative importance of different scattering mechanisms in the transport of carriers. Since ionized impurity scattering is inefficient at higher carrier energies, it becomes important in the 77 K to 300 K temperature range. Alloy scattering is important for transport in mixed crystals, in the temperature range below 300 K. Carrier–carrier scattering preserves both the energy and the momentum if it is between carriers of the same type. It therefore causes a substantial difference in between the transport of a majority carrier and a minority carrier. Lattice scattering becomes dominant at high temperatures and high carrier energies. Optical phonons, with their large momentum and energy compared to acoustic phonons, are dominant when carriers have large energies and are dominant in inter-valley transfers. Acoustic phonons establish a lower limit in scattering since they can exchange very low energies also. At very low temperatures, therefore, while optical phonon absorption can be frozen out because of their reduced density, acoustic phonons continue to be important. At low temperatures and low fields, both acoustic phonons and the impurity scattering are important. At high fields and very low temperatures, impurity scattering becomes weak because of the higher carrier energy, but optical phonon emission becomes important. Acoustic phonon scattering should also be considered. At high temperatures phonon scattering prevails, and both absorption and emission processes become dominant. Now, let us consider the temperature dependence of the low field and high field behavior in the velocity–field curves of Figure 2.21. At high fields, as we have already discussed, this velocity is dominated by inter-valley scattering processes occurring largely through optical phonons, which are polar in compound semiconductors and non-polar in silicon and germanium. At low fields, other mostly inter-valley scattering processes dominate. The low field behavior is equally well characterized by the mobility or the drift mobility, which relates the velocity with the low electric field. While drift mobility is the real mobility of interest in most electronic devices, one quite often also uses Hall mobility which is a far easier transport parameter to measure accurately. 12 The energy relaxation time τ can not be exact for any scattering process. The exactness w requires the final states of the scattering process to yield a Maxwell–Boltzmann distribution. So, this equation needs to be used with great caution and critical reservations. More on the relaxation time approximation and the appropriateness of the approach in Chapter 3. 54 2 Review Figure 2.23: Theoretical drift and Hall mobility for a compensation ratio of two as a function of background electron density at 300 K and 77 K for GaAs. Drift Mobility At room temperature, ionized impurity scattering and polar phonon scattering dominate the scattering processes in doped samples. As the temperature is lowered, phonon scattering becomes less efficient and the mobility is limited more by ionized impurity and deformation potential acoustic scattering. As temperature is decreased further, the ionized impurity scattering dominates. Thus, for low field regions in doped GaAs, both the ionized impurity scattering and phonon scattering are important over a broad temperature range. The dependence of mobility on carrier and impurity density in GaAs, for 300 K and 77 K, is shown in Figure 2.23. For pure material, impurity scattering is reduced, but most of the other processes remain. Figure 2.24 shows the contribution of the various scattering processes to limiting the mobility of lightly doped GaAs, and their temperature dependence. Drift mobility, as discussed thus far, depends on the carrier scattering embodied in the phenomenological carrier relaxation time. To calculate the mobility, we need to determine this relaxation time, including its functional dependence on energy. The average value of this relaxation time then is obtained by averaging over the energy states that the carrier occupies. For electrons, using a parabolic band approximation, we obtain τµ = τ . (2.99) The averaging is over energy, which is related to the momentum in the parabolic 2.7 Carrier Transport 55 Figure 2.24: Electron mobility in n-type lightly doped GaAs as a function of temperature together with contributions from the various sources of scattering. Curve (a) is for mid-1013 cm−3 doping, curve (b) is for ≈ 1015 cm−3 doping, and curve (c) is for mid-1015 cm−3 doping. After J. S. Blakemore, “Semiconducting and Other Major Properties of Gallium Arsenide,” J. of Appl. Phys., 53, p. R123, Oct., 1982. 56 2 Review approximation through a square law. The relaxation time, therefore, is also often written as hv2 τ i h(E − Ec) τ i = . (2.100) τµ = hE − Ec i hv2 i The time constant for mobility can be calculated knowing what scattering process is dominant. Alternately, if more than one is important, they all have to be evaluated and resultant determined as a geometric mean. The geometric mean comes about because scattering rates add, and the time constant is inversely proportional to this rate. Thus, the time constant τµ is related to the time relating the inverse of scattering rates τ1 , τ2 · · · 1 1 1 = + + ···, τµ τ1 τ2 (2.101) and the drift mobility is related to this time constant through13 µd = q hv2 τ i qτµ . ∗ = m m∗ hv2 i (2.102) If one associates µ1 , µ2 , · · · as the mobilities with the various scattering processes corresponding to τ1 , τ2 , · · ·, then 1 1 1 = + +··· µ µ1 µ2 (2.103) For a given momentum, the velocity of carriers is inversely related to the effective mass. A larger effective mass results in smaller velocity for identical forces on the carrier. Since the velocity of carriers and their mobility is intimately related to the effective mass, we also need to consider the band structure of the crystal. The conduction band minima in both silicon and germanium do not occur at a crystal momentum of zero, i.e., the materials have an indirect bandgap. The group velocity at the minima, which are either near the X-point (about 15 percent away from it) in silicon, or the L-point in germanium, is zero, but the crystal momentum is non-zero. Crystal momentum and particle momentum are two different quantities. Perhaps we should always refer to the reduced wave vector corresponding to the crystal momentum as kc . Usually though, the same notation is used for both reduced wave vectors—k.14 Since in general the effective mass is a tensor, it has a directional dependence. This dependence is quite clear in the differing curvature in different directions of 13 This relationship, Mathiessen’s rule, has limited, not universal, validity since it is based on relaxation time approximation. 14 i.e., we use p = h̄k where the k is the particle reduced wave vector corresponding to the particle momentum. This is related to the band structure and the crystal reduced wave vector through the relationship 1 dE p = m∗ v = m∗ , (2.104) h̄ dkc where kc is the crystal momentum. In this text, we use k to denote the reduced wave vector for both the particle and the crystal. The effective mass m∗ is in general a tensor. The m∗ 57 2.7 Carrier Transport Figure 2.25: Constant low energy surfaces commonly encountered in cubic crystals. Part (a) shows a spherical surface encountered for Γ valley minima in the conduction band, part (b) shows an ellipsoidal surface encountered for L and X valley minima in the conduction band, and part (c) shows a warped surface encountered for the two degenerate valence bands. After C. Jacobani and L. Reggiani, “The Monte Carlo Method for the Solution of Charge Transport in Semiconductors with Applications to Covalent Materials,” Review of Modern Physics, 55, No. 3, July 1983. Figure 2.10 for Si and Ge. Let us now consider how the occupation of the bands, the motion of carriers due to anisotropy of masses, and the occupation of more than one degenerate bands are related. In thermal equilibrium, the carriers occupy bands following Pauli’s exclusion principle. Constant energy surfaces are used to show those momentum values that have constant energy and hence an equal likelihood of occupation in thermal equilibrium. The shapes of such surfaces are dependent on the band anisotropy. In cubic crystals, at thermal equilibrium, three types of constant energy surfaces are usually encountered. These are shown in Figure 2.25 with arbitrary origins of the momentum. A parabolic band has an isotropic mass; its constant energy surface is spherical. The L and X valley minima, however, have a rotational symmetry around the crystallographic directions and show a differing effective mass in the transverse direction to it than in the longitudinal direction. The constant energy surface tensor is not direction dependent while the E(k) relationship is. The form 1 m∗ = 1 ∂ 2E h̄2 ∂ki ∂kj = 1/m∗xx 1/m∗yx 1/m∗zx 1/m∗xy 1/m∗yy 1/m∗zy 1/m∗xz 1/m∗yz 1/m∗zz ! (2.105) is suitable at the band minima where it can be directly related to the first expansion term of the E(k) relationship. During a gradual change in k as the carrier travels, its effective mass undergoes a change. 58 2 Review is an ellipsoid. Valence bands are usually double degenerate at zone center. For any energy in excess of this zone center energy, the constant energy surface is warped. Thus, even for moderate doping, in cases where the band structure is not a simple parabola, where the band minima do not occur at the zone center, and where degenerate bands exist, the effective mass for use in conduction calculations has to be derived as a suitable average that reflects the net effect. We first consider the conduction band. For the lowest conduction band minima in the Γ band, the bands are quite isotropic and we may use the usual mass. At higher energy, however, e.g., when a large field is applied and inter-valley transfer occurs, we may not use this constant isotropic effective mass. Transfer of carriers in GaAs occurs first to the L-valley and then to the X-valley with increasing energy. An L-valley has eight equivalent minima in the eight different directions. However, since the minima always occur at the Brillouin zone edge, only four equivalent complete valleys need to be considered. For X-valleys, the minima occur slightly inside the Brillouin zone, and hence all six equivalent minima and six equivalent valleys should be considered. The L and X minima are ellipsoidal surfaces of constant energy, i.e., a cut along the axis leads to an ellipse represented by E − Ec = h̄2 h̄2 2 (k − k ) + (kt − kot )2 , l ol 2m∗l 2m∗t (2.106) where the subscripts l and t denote longitudinal and transverse directions. This is simply a translation of the axes from our original Cartesian coordinate in the reciprocal space to a new Cartesian coordinate that is aligned along the longitudinal axis, and because of symmetry the transverse variations are identical. In terms of the effective mass, if the transformed x-axis is now aligned with the longitudinal axis, then the new effective mass tensor is 1/m∗l 0 0 1 . = 0 1/m∗t 0 (2.107) m∗ 0 0 1/m∗t If the electric field is applied in the h100i direction, as in Figure 2.26, there are four ellipsoid surfaces for the X minima for whom the transverse effective mass is the relevant mass in the determination of the response of the carrier to the field. Similarly, there are two ellipsoidal surfaces for which the longitudinal mass is relevant. Hence, in the process of approximating into the parabolic band picture, i.e., an expression of E − Ec = h̄2 k 2 /2m∗c , we must use the mass i 1 h 1/2 m∗c = × 2m∗t + 4(m∗l m∗t ) . (2.108) 6 For the L-valley minima (Figure 2.27), with a field in h100i direction, all the valleys are equivalent, with the effective conduction mass being 1/2 1 1 ∗2 2 ∗ ∗ m∗c = × mt + ml mt . (2.109) 4 3 3 2.7 Carrier Transport 59 Figure 2.26: The six equi-energy ellipsoidal surfaces for the X minima shown in the first Brillouin zone. For a field aligned with one of the axes, four ellipsoid surfaces form the first equivalent set and the other two ellipsoid surfaces form the second equivalent set. Figure 2.27: The eight equi-energy half-ellipsoidal surfaces for the L minima shown in the first Brillouin zone. For a field aligned with one of the axes all of these surfaces are equivalent. 60 2 Review Table 2.2: Effective masses in Silicon and Germanium. Material Valence Band Conduction Band Light Hole Heavy Hole Longitudinal Transverse Effective Effective Effective Effective Mass Mass Mass Mass Silicon 0.16m0 0.5m0 0.97m0 0.19m0 Germanium 0.04m0 0.3m0 1.6m0 0.082m0 The valence bands are centered in the Brillouin zone and the light and heavy hole bands are degenerate. The equivalent mass can be derived as 1 ghh (E) glh (E) 1 = + . (2.110) m∗c m∗hh m∗lh ghh (E) + glh (E) where ghh (E) and glh (E) are the heavy hole and light hole density of states. The ratio of densities of states in the expression above represents the probability of finding the hole in a state with that mass. Since the density of states varies as 3/2 power of the mass, the conduction mass for holes is 1 m∗hh 1/2 + m∗lh 1/2 . = m∗c m∗hh 3/2 + m∗lh 3/2 (2.111) The longitudinal and transverse effective masses in silicon and germanium for some of the bands are given in Table 2.2. Hall Mobility Hall mobility is a mobility parameter that results from Hall effect measurement. It is a simple and hence very common measurement to gauge the low field transport characteristic of semiconductors. Our objective here is to emphasize its relationship with the drift mobility which is of more immediate interest from a device perspective. The Hall effect is a phenomenon that results from the application of a magnetic field on a sample. Consider the n-type rectangular semiconductor sample of Figure 2.28 with a magnetic field applied perpendicular to the sample, a voltage bias applied to force a current to flow in plane of the sample, and a voltage being measured perpendicular to this flow of current. A voltage, called the Hall voltage, develops in the perpendicular direction because of the Lorentzian force acting on the charged particle. For the electron, this force is given by F = −q (v × B) . (2.112) In steady-state, carriers accumulate and deplete in the transverse direction, causing a transverse electric field which opposes and cancels the field due to the Lorentzian force, to appear. This allows us to write the electric field in the 61 2.7 Carrier Transport Figure 2.28: A schematic defining directions of current flow, electric field, and magnetic fields for Hall effect in an n-type sample. transverse direction, related to the Hall voltage developed across the transverse direction, in terms of the magnetic field, the current and a parameter called the Hall coefficient. This field is related as Ez = RH Jx By , (2.113) where RH is the Hall constant which is related to the characteristics of the motion and the carrier density and is given by RH = 2 2 r pµdp − nµdn , q (nµdn + pµdp )2 (2.114) for a sample with both electron and hole conduction. The pre-factor r (also called Hall factor) in the Hall constant usually varies between one and two for most common scattering processes. This factor is related to the relaxation time for Hall mobility determination τH (analogous to τµ , the relaxation time for drift mobility determination) given by τH = hτ 2 i . hτ i (2.115) For one carrier conduction, the Hall constant is given by RH = − 1 hτ 2 i qn hτ i2 (2.116) 62 2 Review for n-type material, and RH = 1 hτ 2 i qp hτ i2 (2.117) for p-type material. We will consider the physical basis of these relationships during our discussion of mathematical treatments in Chapter 3. Note the difference between this and the relaxation time associated with the drift mobility. If only acoustic deformation potential scattering dominates, and the conduction and valence bands can be assumed to be parabolic, then r = 3π/8. The motion of carriers in the transverse direction occurs due to the applied magnetic field, and is determined by the velocity in the longitudinal direction. The proportionality constant in the longitudinal direction is the drift mobility, however the proportionality in the transverse direction is a mobility term that depends on the same pre-factor term as does the Hall constant. Hence, the Hall mobility in samples with unipolar conductivity is µH = rµd . (2.118) µH = |RH σ| (2.119) More generally, where σ, the conductivity, is given by σ = qnµdn + qpµdp . (2.120) Because the ratio r varies between one and two, the Hall mobility is always larger than the drift mobility. Its significance and ubiquity is largely a result of the ease of its measurement. The Hall and drift mobility are, of course, related to each other through the characteristics of the dominant scattering processes, i.e. through the ratio r above. Figure 2.23 shows the Hall mobility in GaAs as a function of background electron concentration for 300 K and 77 K. This figure also serves to show the difference between drift and Hall mobility as a function of electron concentration. Saturated Velocity The mobility of carriers decreases as a function of particle energy because the scattering rate continues to increase as a function of the energy. Thus, drift and Hall mobilities become negligible at high energies because carriers move short distances in between scattering events. It is the velocity of carriers that is of direct interest to us. At high energies, even though the mobility becomes negligible, the velocity for a high applied field is still high. At low energies, both the velocity and the mobility are useful parameters because they are directly related to each other. However, mobility is used more commonly, both because of the ease of measurement and because of simplifications in many steady-state drift-diffusion calculations in devices. The saturation of velocity at high fields occurs for the following reason. Carriers drift in the high field in between scattering. Any increase in energy 2.7 Carrier Transport 63 Figure 2.29: Drift velocity in GaAs as a function of temperature at a field of 50 kV.cm−1 . resulting from this transport in high field causes an increase in the scattering rate also. An increase in the electric field, therefore, does not result in a significant additional increase in the velocity, and the mobility becomes negligible. An alternative way of looking at this behavior in high fields, where the carrier is in equilibrium with its local conditions, is to note that the mobility is a function of the carrier energy. In low fields, the average carrier energy increases proportionally with the electric field, the scattering rate increases proportionally, and hence the carrier mobility remains constant and independent of the energy and the electric field. In high fields, however, the carrier energy increase causes the mobility to decrease inversely with the electric field and hence results in velocity saturation. Optical phonon scattering is the principal source of scattering in the high field region. Since, as shown by Equation 2.56, the occupation of the optical modes decreases strongly as the temperature decreases, energy relaxation is not as strong, and hence absorption processes are less likely. The drift velocity at high fields also shows a temperature dependence. An example of this is shown in Figure 2.29 where there is nearly a 20% change in the drift velocity at high fields (approximately the saturated velocity) between 300 K and 77 K. 2.7.2 Two-Dimensional Effects on Transport Now, compare the mobility behavior to that of two-dimensional electron gases in GaAs. Here, scattering, due to ionized impurities, occurs through a remote process because donors and carriers are separated. The perturbation in poten- 64 2 Review Figure 2.30: Separation of two-dimensional electron gas from the ionized donors in a two-dimensional electron gas structure. The larger bandgap material (Ga1−x Alx As), from which the electron transfer occurs, is shown on the left. The right hand side shows the smaller bandgap material (GaAs) to which the transfer occurs. An undoped spacer layer, used to decrease remote Coulombic scattering, is also shown in the figure. tial due to ionized donors (sometimes this is referred to as Coulombic scattering also) is separated from the electron gas as shown in Figure 2.30. Decrease of the ionized impurity scattering, and increase of the carrier screening of the ionized impurities because of large carrier densities in the two-dimensional channel, result in a significantly higher mobility. Now, scattering processes such as the piezoelectric scattering become important, at least in part of the temperature range, as shown in Figure 2.31. At the lowest of the temperatures, the residual background doping at the high mobility interface is still important, although because this is low, the mobility is very high. It is interesting to compare this figure with Figure 2.24 which shows the mobility versus temperature behavior for low doped GaAs. Note that over a fairly broad range of temperature, near and above 77 K, the behavior is very similar. Below that temperature, the improvements due to carrier screening make the mobilities of the two-dimensional electron gas system significantly larger. The added complication in the two-dimensional electron gas structures is that one should also consider the quantization and its effects on scattering, as well as the effect of carrier–carrier interaction, and carrier–dopant interaction. The former leads to a decrease in mobility, the latter tends to screen the perturbation potential associated with the dopant. Thus, there is actually an optimum in carrier concentration in the channel where the two balance and allow the highest mobilities at low temperatures. Note the large increases in low field mobility that can be achieved by a decrease or removal of the ionized impurity scattering. At 300 K, since ionized impurity scattering is only one of the two dominant scattering processes, the increase is not very large. At 77 K, mobilities of greater than 70, 000 cm2 .V−1 .s−1 are quite common. The behavior of two-dimensional electron gases is quite complicated; it has increased carrier–carrier scattering whose effect, as we have discussed, is to change the 2.7 Carrier Transport 65 Figure 2.31: Theoretical maximum mobility in a two-dimensional electron gas at the Ga.7 Al.3 As/GaAs interface as a function of temperature is shown as curved marked b. Curve a shows the mobility in very lightly doped GaAs. The figure also shows components of mobility arising from different scattering mechanisms in bulk GaAs. distribution function but to not affect the energy and momentum. We have not discussed the interaction of carrier–carrier scattering processes with other processes, which are also important in these structures. An example of this is given in Figure 2.32, which shows the coupling in between optical phonons and the carrier plasma, called plasmon, as a function of carrier density in GaAs. Significant deviation, and large energy effects, begin to occur at mid-1017 cm−3 carrier density. Carrier densities higher than this exist in twodimensional electron gases in device structures and therefore mobility is fairly sensitive too carrier scattering. Too low a carrier density leads to reduction of screening of Coulombic scattering from remote and local donors, and too high a density leads to increased carrier–carrier scattering effects. 2.7.3 Minority Carrier Transport The examples, until now, have been those of majority carriers. The electron, as a majority carrier, suffers Coulombic scattering from the donors, other electrons, and any other residual impurities. Usually, the latter two are small; only at high carrier densities, such as at high dopings or in two-dimensional electron gas, do the carrier–carrier interactions also become strong. The electron, as a minority carrier, suffers Coulombic scattering from the acceptors, the holes, other electrons, and any other residual impurities. The last two, as in the case 66 2 Review Figure 2.32: Energy of the phonon modes as a function of square-root of electron density in GaAs. Carrier–phonon coupling results in behavior shown at high carrier densities. of the electron as a majority carrier, are usually small. Holes are the new twist to the environment of the electron. The behavior of the electron as a minority carrier depends on the semiconductor and on any residual field in the semiconductor device. It depends on the semiconductor because any interaction between electron and hole—usually the heavy hole since it is far more common—involving exchange of momentum and energy is a function of their relative effective masses. The screening of acceptors by holes (i.e., reduction of Coulombic perturbation by holes in the vicinity of the ionized acceptor) may allow for an increase in the carrier mobility. Holes, if they are considerably heavier than the electron, may cause scattering very similar to that due to ionized acceptors. A slight residual field in the structure causes motion of carriers in the opposite direction, which may result in a drag effect on each carrier by the other. The magnitude of the effect on each carrier is a function of their effective mass, and the disparity in the effective mass. Scattering is a strong function of temperature, hence, different considerations may apply to different temperatures. Figure 2.33 and Figure 2.34 show plots for minority and majority carrier mobilities for Si and GaAs as a function of background donor and acceptor density. These figures are for mobility at 300 K. Silicon has a comparable mobility for electron as a majority and minority carrier, while GaAs shows a minority carrier mobility that is nearly half the value of the majority carrier mobility. In silicon, the effective masses of electron and hole are relatively 2.7 Carrier Transport 67 Figure 2.33: Minority and majority carrier electron mobility in silicon as a function of impurity concentration for negligible electric field at 300 K. Figure 2.34: Minority and majority carrier electron mobility in GaAs as a function of impurity concentration for negligible electric field at 300 K. The majority mobility is at a compensation ratio of two. After S. Tiwari and S. L. Wright, “Material Properties of p-type GaAs at Large Dopings,” Appl. Phys. Lett., 56, No. 6, p. 563, 1990. 68 2 Review similar. Exchanges involving electrons and holes, and screening of impurities by holes, together contribute to this similarity of mobilities. In GaAs, electrons and heavy holes have widely differing masses. Heavy holes can be considered static for scattering purposes, and lead to Coulombic scattering of a magnitude similar to the ionized acceptor. This behavior may change at a different temperature. At 77 K, e.g., for GaAs in the 1015 cm−3 doping range, the minority carrier mobility for electrons is higher than as a majority carrier. Minority carrier devices usually have fields in regions where the electron transits. In the base of the bipolar, e.g., a small field exists even for uniformly doped base structures. This field is the result of the gradient in the hole distribution established to compensate for the electron distribution. It causes a rapid decrease in mobility with the electric field, even though the mobility at zero field is quite comparable to the majority carrier mobility. The majority carrier mobility, of course, does not vary substantially. This difference in behavior is usually ascribed to the electron-hole drag effects which are quite significant for Si because of comparable effective masses. The carrier–carrier scattering conserves momentum. In the absence of an electric field, the average drift momentum is zero. In the presence of drift field, electrons and holes move in opposite directions. The interacting electrons and holes that are in the vicinity of each other and are, on an average, moving in opposite directions, exert a Coulombic attractive force on each other. This reduces the effect of the drift field, and externally, appears as the lowering of mobility. The effect is strong, and shows up at a low electric field. At higher fields, the drag effect does not remain as important because the Coulombic scattering rate decreases and the electron now has a higher energy. The consequence of such an effect can be strong in devices such as bipolar transistors, even if no electric field is built into the structure. In the presence of current, there exists a gradient of electron density in the base. In order to maintain charge neutrality, hole density also changes as a function of position to compensate for the excess charge due to electrons. The excess hole population is equal to the electron population under quasi-static conditions. The diffusion current due to the gradient in hole density is nearly compensated by the drift current resulting from a small electric field that is established in the base. The magnitude of this electric field can be found approximately, by setting the hole transport current to zero (it is substantially smaller than the electron current for the n–p–n bipolar transistor). The current density equation in the driftdiffusion approximation can be used to model this condition. Here we use the current density equation without proof; it will be the subject of discussion in Chapter 3. Thus, dp ≈ 0, (2.121) Jp = qµn Ep − qDp dz implying kT 1 dp E≈ . (2.122) q p dz Electric field is pointed in the direction of increasing p. To maintain charge neutrality, the hole concentration is higher towards the electron injecting electrode. 69 2.7 Carrier Transport Hence the electric field is pointed towards the electron injecting electrode. This is a very substantial simplification of a considerably complex manybody problem. It has been argued that under certain conditions, this drag effect should be balanced by the effect of majority carrier distribution. Hole current being small, the holes are nearly stationary. Thus, they should not transfer much momentum to electrons. Electrons, however, do transfer momentum to holes, resulting in the space charge and electric field to prevent the resulting hole current. This field aids the motion of electrons, just as in the high injection effect, and hence should compensate. 2.7.4 Diffusion of Carriers The phenomenon of diffusion is one of the very direct consequences of scattering. Net diffusion takes place from regions of high carrier concentrations to regions of low carrier concentrations. Regions of high concentrations have a higher carrier population resulting in a higher number of scattering events. Some of these lead to carrier motion towards the low carrier concentration region. However, it is not completely compensated for by scattering events that lead to the motion of carriers from the low concentration region to the high concentration region. The net result is a flow, or diffusion, of carriers determined by the gradient of the carrier concentration, and characterized by the diffusion coefficient (Dn for electrons and Dp for holes). Diffusion coefficients are related to mobilities because their underlying basis is in scattering. This relationship, the Einstein relationship, was derived for Brownian motion in the Maxwell–Boltzmann distribution limit of classical gases. We will show it in the Fermi–Dirac distribution limit using the drift-diffusion equation. Consider thermal equilibrium in an n-type sample, thus Jn = qnµn E + qDn dn = 0. dz (2.123) Since the carrier concentration is given by n = NC F1/2 (ηfc ) , (2.124) dn dηfc = NC F−1/2 (ηfc ) . dz dz (2.125) In thermal equilibrium (ξf = constant) we have dηfc 1 dEc qE =− =− . dz kT dz kT (2.126) Therefore, we may relate the diffusion coefficient and the mobility as Dn kT F1/2 (ηfc ) = , µn q F−1/2 (ηfc ) (2.127) 70 2 Review Figure 2.35: Diffusion coefficient in the longitudinal and transverse direction as a function of electric field for low-doped GaAs at 300 K. the Einstein relationship for electrons; and, following similar arguments, Dp kT F1/2 (ηfv ) = , µp q F−1/2 (ηfv ) (2.128) the Einstein relationship for holes. In the Maxwell–Boltzmann limit, these can be simplified to Dn Dp kT = = . (2.129) µn µp q The diffusion coefficients of electrons in GaAs and other compound semiconductors are larger than in silicon for the same reason as for mobility—largely due to a smaller effective mass. The high diffusion coefficient leads to a shorter base transit time in bipolar transistors in GaAs and other compound semiconductors for comparable base widths. It also has implications for noise behavior: a larger diffusion coefficient usually results in smaller magnitude of noise. Since, in general, conduction band structure can be anisotropic, scattering processes are anisotropic, and since fields exist along specific directions, the diffusion coefficient shows anisotropy. Examples of magnitude of diffusion coefficient with field are given in Figure 2.35 for the longitudinal and transverse directions of GaAs. The anisotropic nature of polar scattering is a particularly strong contributor to this anisotropy. Since polar scattering occurs across the field range so long as it leads to carrier energies above the optical phonon threshold, the diffusion coefficient also exhibits similar behavior. Anisotropy exists both at low 2.8. SOME EFFECTS RELATED TO ENERGY BANDS 71 and high fields. At high fields, the L and X valleys are mostly occupied, the longitudinal effective mass is large, and hence the longitudinal diffusion coefficient is suppressed. It decreases to very low values compared to the zero field value, just as in the case of mobility. The pinch-off regions of a field effect transistor are regions of high fields where the carrier gradient can become large for large gate length devices. The low diffusion coefficient reduces the diffusive current in such regions even if carriers move with finite velocity (the saturated velocity) due to drift effects. 2.8 Some Effects Related to Energy Bands There are a number of device related phenomena that can be intuitively related to the band structures. One example, that we briefly alluded to is the relationship between scattering rate and density of states. Scattering is proportional to the coupling between the two states connected by a scattering process, and the number of states available for scattering into. Thus, at the onset of secondary valley transfer, i.e., when carriers have kinetic energy approximately equal to the inter-valley separation, a rapid rise in the scattering rate occurs, as seen in Figure 2.20 for GaAs, InP, and Ga.47In.53 As. Also note that at low energies, InP has the highest scattering rate. InP has the highest effective mass of the four semiconductors in the figure, and therefore has the highest density of states. Effective mass, which is inversely proportional to the second derivative of the energy with respect to the wave vector, i.e., related to the band structure, is central to a lot of transport parameters of interest. Mobility is inversely proportional to the effective mass—a lower effective mass usually implies faster low field transport characteristics. A lower effective mass also results in improvement in the diffusion coefficient and higher tunneling probability. A smaller effective mass means lower density of states, carriers have a higher velocity for the same energy, and so long as the scattering rate is lower, the off-equilibrium effects are stronger. The highest velocity that the carriers can attain under the most ideal of circumstances (the maximum group velocity) is also limited by the band structure. Another good example of a strong band structure relationship exists in the phenomenon of avalanche breakdown due to impact ionization. This is a process in which a carrier picks up enough energy in between scattering events to cause an electron to jump from the valence band into the conduction band during a scattering event. The process is both band structure- and scattering processdependent. In this section we will describe some of these relationships in more detail, and develop a comparative understanding of some of these parameters for compound semiconductors. 72 2 Review Figure 2.36: Examples of possible impact ionization processes for electron and hole initiated processes for GaAs. The ionization process initiated by a hot electron is shown using solid lines; it results in the transfer of an electron from the heavy hole band to the conduction band. The ionization process initiated by a hot hole from the split-off band is shown using dashed lines. After T. P. Pearsall, F. Capasso, R. E. Nahory, M. A. Pollack, and J. R. Chelikowsky, “The Band Structure Dependence of Impact Ionization by Hot Carriers in Semiconc ductors: GaAs,” Solid-State Electronics, 21, p. 297, 1978 Pergamon Press plc. 2.8.1 Avalanche Breakdown The breakdown phenomenon of most interest occurs in depletion regions of devices. In bipolar transistors, it is the breakdown in the base-collector junction region. In field effect transistors, it is the breakdown in the drain to substrate depletion region. These occur because a high field exists, due to the reverse bias at the junction, and this high electric field is capable of accelerating the carrier and imparting to it a large kinetic energy. Indeed, this kinetic energy can become sufficiently large to cause an electron, or even more than one electron under the right conditions, to be removed from the valence band and transferred to the conduction band. Take the case of GaAs, where examples of the possible electron and hole initiated transitions are described in the Figure 2.36. The process, involving a single electron–hole pair generation, consists of transfer of energy from the hot carrier to an electron in the valence band, which jumps into the conduction band leaving a hole behind. For small bandgap semiconductors, even multiple such pairs may be generated. With the complicated band structure, electrons can be from different bands, 73 2.8 Energy Band Effects holes can be from different bands, phonons (particularly optical phonons with their large momentum) may be involved, etc. Indeed, since the band structure is orientation dependent, and impact ionization occurs due to large energy of the carrier from rapid acceleration in a field, in the event of insufficient randomization, it may even be orientation dependent.15 We will discuss, briefly, a very simplified model, to see how the role of band structure enters in the impact ionization process. We consider a parabolic model for the conduction band with effective mass m∗e , and a parabolic model for the valence band with effective mass m∗h . Under thermal equilibrium conditions, there may exist carriers that have sufficient energy for impact ionization. These carriers are in the tail of the carrier distribution function with energy, and by detailed balance, impact ionization is balanced by its reverse process—Auger recombination. With an increase in electric field, carriers pick more energy, and hence there may now exist carriers with sufficient energy for electron–hole pair or pairs generation. We consider only one electron–hole pair, one band each for the electrons and holes, no phonon involvement, and a process initiated by electrons. The minimum energy that an electron must have is the bandgap Eg to cause the transfer. If i and f signify initial and final state subscripts for the electron causing the impact ionization, the creation of an electron-hole pair of momentum pe and ph in an electron initiated process (see Figure 2.37) requires, by conservation of energy and momentum, p2f p2e p2h p2i = E + + + , g 2m∗e 2m∗e 2m∗e 2m∗h (2.130) pi = pf + pe + ph . (2.131) and Using the method of the Lagrangian multiplier to minimize the carrier energy under the constraint of momentum conservation, ! p2f p2e p2h + + + Ad (pf + pe + ph ) = 0. (2.132) d Eg + 2m∗e 2m∗e 2m∗h Using partial derivatives with respect to pe , ph , and pf gives pe ph pf = ∗ = ∗ = −A, m∗e mh me giving for the initial momentum pi = m∗ 2 + h∗ pf , me (2.133) (2.134) 15 Impact ionization has continued to be the subject of research in semiconductors since 1960s, since it is a very complicated subject involving hot carriers. Orientation dependence is only one of many examples of this. See, e.g., T. P. Pearsall, F. Capasso, R. E. Nahory, M. A. Pollack, and J. R. Chelikowsky, “The Band Structure Dependence of Impact Ionization by Hot Carriers in Semiconductors: GaAs,” Solid-State Electronics, 21, p. 297, 1978, and H. Shichijo and K. Hess, “Band-Structure-Dependent Transport and Impact Ionization in GaAs,” Phys. Rev. B, 23, No. 8, p. 4197, 15 Apr. 1981. 74 2 Review Figure 2.37: A simple one dimensional parabolic band schematic of electron-hole pair generation by impact ionization involving a hot electron. and for the threshold energy of the initial electron ET p2i m∗e ET = = 1+ ∗ Eg . 2m∗e me + m∗h (2.135) If m∗e = m∗h , this relationship gives the threshold energy for impact ionization as ET = (3/2)Eg . This threshold energy is the minimum energy that an electron must possess to initiate impact ionization in our model that assumes single parabolic bands and no involvement of phonons. We can see the tremendous simplification in applying this relationship to real band structures. GaAs has m∗e = 0.067m0 and m∗hh = 0.5m0 , and hence ET = Eg . However, the bands are not parabolic an energy Eg into the conduction band as can be seen from Figure 2.11. So, the situation in real crystals is considerably more complicated; this threshold relationship may overestimate because it ignores phonons in momentum conservation, and the processes may even be orientation dependent. This ionization process is characterized in a semiconductor by the parameter ionization rate. The ionization rate is the relative increase in carrier density per unit length of carrier travel. Thus, the electron ionization rate (αn ) is the rate of increase in electrons per unit length of the travel of an electron: αn = 1 dn . n dz (2.136) 1 dp . p dz (2.137) For holes, the equivalent expression is αp = For GaAs, the impact ionization occurs largely from carriers that are not in the lowest bands. Electrons cause ionization from higher bands, and holes 75 2.8 Energy Band Effects generally cause it from the split-off band. At low fields, the ionization rate is also orientation dependent because of lack of randomization. Examples of ionization rates as a function of electric field are given in Figures 2.38 and 2.39. For most compound semiconductors with greater than an eV of bandgap, the hole ionization rate is larger than the electron ionization rate. Hole effective mass being larger, for similar velocities in the high field regions it has significantly higher kinetic energy. At lower fields, electrons are more likely to have a higher energy since they usually have a smaller scattering rate than holes. Thus at low fields the electron ionization rate tends to be larger. For smaller bandgap semiconductors, e.g., InAs and Ga.47In.53 As, the hole ionization rate is always low because the threshold energy for ionization is lower. Impact ionization does not necessarily need an electric field to show a large generation rate for electrons and holes. In compound semiconductor heterostructures, there exist many smaller bandgap compounds that can be lattice matched to other semiconductors with a bandgap discontinuity for a conduction or valence band that is larger than the bandgap. Even in the absence of an electric field, high energy carriers injected into the smaller bandgap semiconductor can cause impact ionization. This process is often referred to as Auger generation. When impact ionization occurs in the presence of an electric field, such as in a p–n junction, both electrons and holes get accelerated in opposite directions, and both cause further impact ionization. The process of electron–hole pair creation, acceleration of carriers, and creation of more electron–hole pairs sets up an avalanche, and hence the generation of electron-hole pairs in an electric field is also known as an avalanche process, and the related breakdown of a p-n junction an avalanche breakdown. This is an important limiting phenomenon in the usefulness of the device and hence we will investigate it further. The increase in electron current resulting from the ionization caused by this electron and hole current flow is dJn = αn Jn + αpJp , dz (2.138) where Jn is the electron current density and Jp is the hole current density. Similarly, dJp = − (αn Jn + αp Jp ) , (2.139) dz and the total current is J = Jn + Jp . (2.140) Excess current flows due to the presence of electron-hole pair generation. The electron carries the current to one part of the device while the hole carries the current to another part of the device. We may derive the multiplication factor in the terminal currents, due to electron-hole pair generation, as follows. We will consider an electron initiated avalanche process. Let Jn (−wp ) be the electron current at the p-edge and let Jn (wn ) be the current at the n-edge of the depletion region. The hole current is predominant at the p-edge and the 76 2 Review Figure 2.38: Impact ionization coefficient for electrons and holes for GaAs, InP, and Ga.47 In.53 As as a function of the inverse of the electric field. 2.8 Energy Band Effects 77 Figure 2.39: Impact ionization coefficient for electrons and holes for Si, Ge, Al.48 In.52 As, and InAs. 78 2 Review electron current is predominant at the n-edge, i.e. J ≈ Jn (wn ) ≈ Jp (−wp ). In steady-state, dn 1 dJn = G n − Rn + = 0. (2.141) dt q dz We will ignore recombination since generation processes dominate in the avalanche region. As a result, excess current due to avalanche process dominates any recombination current, and can be ignored, thus simplifying our analysis. Denoting the ratio of electron current at z = wn and z = −wp by the electron multiplication factor Mn , we obtain J = Jn (wn ) = Mn Jn (−wp ). (2.142) We also have dJn = αn Jn + αp Jp = (αn − αp ) Jn + αp J. (2.143) dz The solution of the linear differential equation in Jn as a function of position z is hR i Rz ζ α J exp (α − α ) dη dζ + A p p n 0 0 R z Jn (z) = , (2.144) exp 0 (αp − αn ) dζ where η and ζ are dummy variables for the spatial coordinates. The constant A can be determined from our expression for current continuity as Z −wp 1 A = J exp (αp − αn ) dζ − Mn "0Z # ) Z −wp ζ αp exp 0 0 (αn − αp ) dη dζ . And hence, the electron current is given by hR i Rz ζ (1/Mn ) + −wp αp exp −wp (αp − αn ) dη dζ hR i . Jn (z) = J z exp −wp (αp − αn ) dζ (2.145) (2.146) Evaluating this relationship at z = wn allows us to write the equality: "Z # "Z # Z wn wn ζ 1 exp (αp − αn ) dζ = + αp exp (αp − αn ) dη dζ. Mn −wp −wp −wp (2.147) Although this expression appears to be complicated, it actually can be simplified considerably. Introducing I as the magnitude of the integral on the right hand side, we show "Z # Z wn I = ζ αp exp −wp −wp (αp − αn ) dη dζ 79 2.8 Energy Band Effects = Z wn αn exp −wp Z wn (αn − αp ) exp = wn αn exp −wp exp "Z "Z (αp − αn ) dη dζ − "Z ζ −wp # (αp − αn ) dη dζ ζ −wp # (αp − αn ) dη dζ + # wn −wp # ζ −wp −wp Z "Z (αp − αn ) dη − 1. (2.148) A simple expression for the multiplication factor results from this in the form " Z # Z wn ζ 1 1− = αn exp − (αn − αp ) dη dζ. (2.149) Mn −wp −wp The condition for breakdown caused by electron initiated avalanche is the condition where Mn goes to infinity. This occurs when the integral in this equality goes to unity. Avalanche breakdown, therefore, occurs when " Z # Z wn −wp ζ αn exp − −wp (αn − αp) dη dζ = 1. (2.150) The condition for breakdown with a hole initiated process can be found following a similar treatment (see Problem 4). The expression for the hole multiplication factor Mp is given as 1− 1 = Mp Z wn −wp Z αp exp − ζ wn (αp − αn ) dη dζ, and hence breakdown is said to have occured when Z wn Z wn αp exp − (αp − αn ) dη dζ = 1. −wp (2.151) (2.152) ζ Figure 2.40 shows the avalanche breakdown voltages as a function of doping for some of the common semiconductors for an abrupt p+ –n junction using the above criterion and the ionization rates described previously in Figure 2.38 and 2.39. While generally, at the high fields that dominate avalanche process, the hole ionization coefficient dominates, this is not true for small bandgap semiconductors such as Ga.47In.53 As and InAs. Here, hole initiated processes are less likely, so even though they are more likely to avalanche by virtue of a smaller bandgap, due to suppression of hole avalanching, the decrease in breakdown voltage is not as pronounced. 80 2 Review Figure 2.40: Breakdown voltages limited by avalanche process for some of the common compound and elemental semiconductors. Quite often, the integral on the right of the previous equations for multipliν cation factors is approximated by the relationship (V /BV ) where BV is the breakdown voltage, i.e., 1 . (2.153) M= 1 − (V /BV )ν This relationship, depending on the magnitude of the power ν, shows a soft breakdown or a hard breakdown. Soft breakdown is meant to imply a slow and gradual increase in the multiplication factor with increasing bias. It occurs when the ionization rates are slowly varying functions of the electric field. A hard breakdown, with ν ≥ 4, leads to a rapid change in the multiplication factor and comes about when the ionization rate changes rapidly with electric field. Small bandgap materials usually have a higher magnitude of the ionization rate, and the ionization rate changes slowly with the electric field. They therefore exhibit relatively softer breakdown characteristics. A relative comparison of breakdown voltage due to avalanche processes and its relationship with the bandgap is shown in Table 2.3. These breakdown voltages are at a donor doping of 1 × 1017 cm−3 in a p+ –n abrupt junction. This doping is quite typical of the dopings encountered in the collector region of bipolar transistors at the base-collector junction. The doping of the small bandgap semiconductors is too small to be useful at this doping or this temperature. Small bandgap semiconductors can be safely used only at low temperatures, or if the device allows a sufficiently low doping to employed to have an acceptable breakdown voltage. 2.8 Energy Band Effects 81 Table 2.3: Bandgap and the breakdown voltage of a one-sided junction at a doping of 1 × 1017 cm−3 for some semiconductors. Material Bandgap Breakdown Voltage (eV) (V) InAs 0.36 2.0 Ge 0.66 5.0 Ga.47 In.53 As 0.75 6.0 Si 1.12 11.0 InP 1.35 14.5 GaAs 1.42 15.8 GaP 2.27 31.4 SiC 2.99 47.8 The length scale over which the carriers accelerate to pick up the energy from the electric field is a few mean free path (λ). The carrier can usually continue to pick up a substantial amount of energy at these high fields because polar optical phonon scattering—the dominant scattering process—leads to only a small loss of the energy (Ep ), and because it causes a small angle scattering, thus maintaining its direction of drift. We have commented that our simplified parabolic model is quite inadequate for predicting the threshold energy of impact ionization. To obtain it more accurately, the complete momentum-energy relationship and phonon effects should be included. The mean free path, the phonon energy, and the threshold energy are all important parameters in the avalanche process. Table 2.4 summarizes some approximate values of these related data. The mean free path is that for a hot carrier. 2.8.2 Zener Breakdown In the context of breakdown mechanisms, it is also instructive to discuss Zener breakdown. Zener breakdown is not really a breakdown in the traditional sense of breakdown’s meaning. Zener breakdown is a form of internal emission which takes place by tunneling. We will discuss tunneling and the mechanism by which the Zener process occurs in the Chapter 4. Here we describe it to show the relationship between tunneling effects and band structure. Figure 2.41 shows schematically the band transition involved in Zener tunneling and breakdown. Tunneling is a manifestation of the wave nature of electrons. If an overlap between the states in the valence band and the conduction band is large, then electron can tunnel from the valence band to the conduction band in the junction. This is simply to state that one may treat the forbidden gap as a potential barrier of the classical barrier tunneling problem. Zener tunneling will be substantial whenever the potential barrier height is small, the potential barrier width is short, or the effective mass is small. Any of these allow for a large overlap of the electron and hole wave function. For 82 2 Review Table 2.4: Mean free path of energetic carriers, optical phonon energy, and the threshold energy for impact ionization for some semiconductors. Material Mean Free Path Phonon Energy Threshold Energy λ (Å) Ep (eV) ET (eV) AlP 71.0 0.0621 3.14 AlAs 54.4 0.0501 2.80 AlSb 45.3 0.0421 2.00 GaP 32.5 0.0500 2.94 GaAs 39.3 0.0354 1.72 GaSb 48.5 0.0242 0.0848 Ge 78.0 0.037 0.67 InP 38.9 0.0428 1.69 InAs 62.9 0.0296 0.392 InSb 100.2 0.0223 0.187 Si 68.0 0.063 1.15 Figure 2.41: Schematic figure representing the emission of a carrier involved in Zener tunneling in p–n junction. The process results in tunneling between the conduction and the valence bands. 2.8 Energy Band Effects 83 Figure 2.42: Schematic representation of the phonon-assisted tunneling process in real and k-space. This process may, e.g., occur during the Zener tunneling process discussed in the previous figure. Tunneling occurs between states with differing wave vectors and involves emission or absorption of a phonon. a given band structure, the potential barrier height and width, related as the electric field, are conducive to tunneling at large dopings. Small bandgap semiconductors have intrinsically a smaller potential barrier, leading to larger Zener tunneling probabilities, even at low doping. Thus, the process, has an effect on breakdown voltages for both highly doped semiconductors and small bandgap semiconductors. The breakdown voltages can be obtained by determination of the transmission function and the source function, the two characterizing the probability of tunneling and the availability of carriers for tunneling. Like processes leading to avalanche breakdown, Zener processes may involve phonon processes. In the classical problem of tunneling through a barrier, we ignore it, i.e., we consider only energy conserving elastic processes. However, phonon assisted tunneling, an inelastic process, can be quite strong. During such a process, a longitudinal or transverse optical or acoustic phonon is emitted or absorbed in order to conserve momentum. In fact, for indirect semiconductors this is the dominant form of tunneling because it can accommodate the large differences in momenta at the bottom of conduction band and the top of valence band. Figure 2.42 shows an example of phonon assisted tunneling process in real and k-space. Tunneling, as we will see later, is a complex phenomenon. Like phonons, photons may also assist in tunneling. This phenomenon is usually referred to as the Franz–Keldysh effect. 84 2 Review Figure 2.43: Electron concentration as a function of Fermi energy with respect to the bottom of the conduction band for GaAs at 300 K and 77 K. After M. Fischetti, “Monte Carlo Simulation of Transport in Technologically Significant Semiconductors of the Diamond and Zinc Blende Structures, Part I: Homogeneous Transport,” IEEE Trans. on Electron Devices, ED-38, No. 3, p. 634, c Mar. 1991 IEEE. 2.8.3 Density of States and Related Considerations We have discussed the role density of states plays in scattering processes. It also is intimately involved in several other ways, the most important of which is its effect on occupation of bands, and the role of degeneracy at high doping. A larger density of states implies larger carrier density before the Boltzmann approximation breaks down and the conduction electrons begin occupying higher and higher energy states in the band. Figure 2.43 shows electron density in GaAs at 300 K and 77 K as a function of the Fermi energy position with respect to the conduction band edge. This includes the changes in the density of states as a function of energy. Note that at negative Fermi energy with respect to the conduction band edge energy, the Boltzmann approximation is valid, i.e., an exponential variation occurs. However, for positive values, considerably complicated density of states effects occur. The Fermi energy of the carriers is increased by introducing more donors in the semiconductor. Large doping implies smaller spacing between the donors. In the section on occupation statistics, we treated the donor levels as discrete and degenerate levels whose density was equal to the donor density. Close proximity of the donors causes overlap interaction between the carriers confined to them, leading to energy splitting and formation of impurity bands. One may get an 2.8 Energy Band Effects 85 estimate of the doping condition for this by determining the Bohr radius (a) in the crystal s m0 a= a0 , (2.154) 0 m∗ where s is the permittivity of the semiconductor, 0 is the permittivity of vacuum, and a0 is the free space Bohr radius whose magnitude is .529 Å. For semiconductors with a large effective mass, such as Si, this occurs at larger dopings, while for semiconductors with a low effective mass this occurs at a lower doping (see Problem 6). If the doping is continued to be increased, impurity bands coalesce with the conduction band and conduction may now take place through the impurity states. Consequently the semiconductor does not exhibit carrier freeze-out. The doping at which this transition takes place, leading to metallic conduction through the impurity levels, is called the Mott transition. Similar to the degeneracy condition above, Mott transition is small in GaAs (low-1016 cm−3 , and large in Si (mid-1018 cm−3 ). These impurity level effects, related to the band structure, should be considered in the treatment of occupation statistics. Generally, though, we use the simple relationship using effective density of states, which is a delta function of the density of states at the band edge, and in our derivation we assume a parabolic band. This ad hoc treatment can be extended and we may treat the effective density of states as a function of carrier density and use the Fermi– Dirac integral. Figure 2.44 shows the variation of the effective density of states for the electrons with carrier density as a function of temperature for GaAs. The effect of heavy doping, or the lack thereof, can be very significant in device operation at low temperatures. Mott transition and freeze-out effects are central to the design of field effect transistors and bipolar transistors in silicon for 77 K operation. Low doping in the substrate, the base, and the collector, and consequent freeze-out, can lead to large threshold voltage changes and high resistances. On the other hand, in GaAs this is not usually a consideration since freeze-out occurs at low dopings. Increase in density of states, merging of impurity bands, etc., occurs with a decrease in effective bandgap and an increase in effective intrinsic carrier concentration. Bandgap shrinkage, e.g., in the base of the heterojunction bipolar transistor, decreases the barrier to the conducting carrier, e.g., the electron in an n–p–n device. Devices with heavy doping in the base, thus, have a higher current density for identical bias. If this bandgap shrinkage takes place in the emitter because the emitter is higher doped (e.g., in the conventional homojunction bipolar transistor), then the injection efficiency degrades. 2.8.4 Limiting and Operational Velocities of Transport The occupation of higher energy states in the conduction band by the electrons also results in an increase in the magnitude of the average velocity with which the individual carriers move from the thermal velocity (vθ ) to the Fermi velocity 86 2 Review Figure 2.44: Normalized effective density of states, including heavy doping effects, as a function of electron density for GaAs at 300 K. The normalization constant is 3.99×1017 cm−3 . After J. S. Blakemore, “Semiconducting and Other Major Properties of Gallium Arsenide,” J. of Appl. Phys., 53, p. R123, Oct., 1982. (vF ). These are really average speeds of the carriers since the average velocities, at thermal equilibrium, are zero, but the average speeds, which ignore the directional dependence, are not. But, by convention, we call them velocities. For low doping conditions, where Maxwell–Boltzmann statistics are valid, the thermal velocity may be approximately obtained from equal partition of energy, i.e., 3 1 ∗ 2 m vθ = kT, (2.155) 2 2 giving p vθ = 3kT /m∗ . (2.156) We can also find it from the distribution of the carrier velocity from the Maxwell– Boltzmann distribution function. The average velocity is defined from the average value of the square of velocity as 1/2 vθ = hv2 i = "R∞ 2 #1/2 1/2 2 ∗ 2 v exp −m v /2kT v dv 8kT 0R = , (2.157) ∞ πm∗ exp (−m∗ v2 /2kT ) v2 dv 0 slightly different from the value found from arguments based on a non-degenerate classical gas which assigns equal weight to all particles independent of the probability of occurrence. 87 2.8 Energy Band Effects Table 2.5: Thermal and Fermi velocity in GaAs at various temperatures for non-degenerate and degenerate dopings. Temperature vθ vF at n = 1 × 1016 cm−3 at n = 1 × 1018 cm−3 K (cm.s−1 ) (cm.s−1 ) 300 77 4 4.5 × 107 2.3 × 107 5.2 × 106 ≈ 5.4 × 107 ≈ 5.4 × 107 ≈ 5.4 × 107 When doping is large, so that the Fermi energy is in the conduction band, the average energy of the carriers can be larger, and they also move with larger speed. Now, we need to include the effect of the exclusion principle in determining the averages. A consequence of Pauli’s exclusion principle is that the number of independent states in a unit volume in the momentum space for a unit volume in real 3 space is given by 1/(2π) . Let kF be the wave vector at the Fermi energy. Since n is the electron concentration in real space, n = 2 = 1 3 (2π) kF3 , 3π 2 Z kF 4πk 2 dk 0 (2.158) where the first factor of 2 is from spin.16 This gives kF 3 = m∗ vF h̄ 3 = 3π 2 n, (2.159) and hence the Fermi velocity vF vF = 1/3 h̄ 3π 2 n . m∗ (2.160) Here, again, m∗ is the density of states effective mass in view of our parabolic band approximations. This velocity, called the Fermi velocity, characterizes the average speed with which the carriers move under degenerate conditions. For the example of GaAs (m∗ = 0.067m0 at the bottom of the conduction band), Table 2.5 summarizes the relevant velocities for two different doping levels at various temperatures. Fermi velocity is relatively insensitive to temperature, and hence diffusion constants, etc., do not not decrease significantly with temperature, unlike in 16 This is exact at T = 0 K. At any other temperature, it is approximate since carriers will occupy states with k > kF . 88 2 Review Table 2.6: Maximum group velocities in some semiconductors. Material Group Velocity cm.s−1 GaAs Si Ge InP InAs AlAs 1 × 108 6 × 107 1.3 × 108 9.5 × 107 1.3 × 108 6.2 × 107 non-degenerate semiconductors. So heavy doping and lower density of states allow some of the devices to function better at lower temperatures. Another band structure related carrier velocity effect that should be considered is the highest group velocity that the carrier can have given the band structure relationship of energy and momentum. The group velocity (vg ) can be found from the energy-momentum relationship, vg = 1 ∂E , h̄ ∂k (2.161) as discussed earlier. The maximum group velocities for some semiconductors, determined from their band structures, are given in Table 2.6. In this table, the maximum group velocity for Ge occurs in the Γ valley towards h100i. The Γ valley is very sparsely populated—L valley is the one most occupied—and hence it is highly unlikely that structures taking advantage of this could be designed. The maximum group velocities are high in the compound semiconductors, almost twice those of silicon. AlAs is one of the exceptions in these compound semiconductors. It band structure is quite similar to that of silicon. Also, these are theoretically predicted maximum velocities, which could conceptually occur only in the absence of scattering and without inter-valley transfer, both of which will occur. When scattering dominates, we have discussed various velocity–field behaviors for different materials. A generalized plot of maximum steady state velocities, based on simplistic theoretical arguments,17 is shown in Figure 2.45 for various pure semiconductors. Many of the data in this figure are experimental. The horizontal scale in this figure is a good approximation for a velocity when it is limited by non-polar optical phonons (the case with elemental semiconductors but not with compound semiconductors). Other scattering mechanisms do not change the functional form substantially and hence the approximate straight line relationship of this figure. 17 See D. K. Ferry, in W. Paul, Ed., Handbook of Semiconductors, Vol. 1, North-Holland, Amsterdam, p. 584, 1982. 2.8 Energy Band Effects 89 Figure 2.45: Theoretical maximum velocities, saturated or peak, for various semiconductors with respect to an energy function involving optical phonons. After D. K. Ferry, in W. Paul, Ed., Handbook of Semiconductors, Vol. 1, NorthHolland, Amsterdam, p. 584, 1982. Many of these velocity-related features can be seen to be inversely related to the effective mass. The larger the mass, smaller the representative velocity. This is true for group velocity, thermal velocity, Fermi velocity, peak velocity for GaAs, InP, Ga.47In.53 As, InAs, Si, Ge, etc. The effective mass also correlates with the bandgap in compound semiconductors. Lower electron effective mass occurs with smaller bandgaps in compound semiconductors as shown in Figure 2.46. 2.8.5 Tunneling Effects We have discussed tunneling, in a phenomenological way, in our discussion of Zener breakdown. Tunneling is the important example of the wave-particle duality. An estimate of the importance of wave aspect can be obtained by comparing the de Broglie wavelength with the critical device dimension. At device dimensions smaller than or comparable to the de Broglie wavelength, it is more appropriate to discuss electrons in crystals as a wave, and the classical picture that assumes negligible time scale of scattering, drift and diffusion averaged from a number of scattering events, etc., is increasingly poor. Tunneling, e.g., cannot be explained in the particle description, it requires the wave description. The de Broglie wavelength is related to the effective mass, and is shown in Figure 2.47. Smaller effective mass leads to large de Broglie wavelength and 90 2 Review Figure 2.46: The variation of effective mass at Γ minimum and light hole band maximum as a function of the direct bandgap for some compound semiconductors. After H. L. Grubin, in H. L. Grubin, D. K. Ferry, and C. Jacobani, Eds., “The Physics of Submicron Semiconductor Devices”, NATO ASI Series, B180, c 1988 Plenum Publishing Corp., New York. 2.8 Energy Band Effects 91 Figure 2.47: Thermal de Broglie wavelength for an electron at the bottom of the conduction band for various semiconductors. After H. L. Grubin, in H. L. Grubin, D. K. Ferry, and C. Jacobani, Eds., “The Physics of Submicron c Semiconductor Devices”, NATO ASI Series, B180, 1988 Plenum Publishing Corp., New York. 92 Properties of Semiconductors for Devices increasing wave effects, tunneling being the most prominent of them. 2.9 Summary In this chapter we have reviewed the underlying concepts of quantum mechanics and considered their implications for semiconductor physics by considering one-dimensional models. The ideas include the wave–particle duality, the use of plane waves in describing wave packets representing localized particles, and the derivation of quantized states in energy and momentum for carriers or phonons caused by confinement or periodic boundary conditions. We showed that a large crystal, and therefore confinement in a large box, leads to quasi-continuum of these states which has a finite density of states. The electrons in a crystal of periodic potential can, at their simplest, be modelled as having a differing effective mass. The periodicity, a condition where Bloch’s theorem and the concept of reciprocal lattice are particularly useful, leads to the formation of forbidden bands, called the bandgap, and multiple bands; the valence bands are filled and the conduction bands are empty at absolute zero. At finite temperature valence bands are partially empty, and conduction of electrons in valence bands can be modelled by “particles” that we call holes, while conduction in the conduction band can be modelled by electrons. Electrons and holes obey Fermi–Dirac statistics, while phonons, the modes of lattice vibrations, obey Bose-Einstein statistics. Subsequently, we analyzed the consequences of perturbation from our idealized behavior that leads to scattering. Using the band structure and phonon dispersion characteristics of the three-dimensional crystals of interest to us, we discussed some of the band to band processes involving electrons, holes, and phonons, and studied the general consequences of the behavior of these materials to the operation of some of the semiconductor devices of interest. The transport of carriers in the three-dimensional lattice with the constraints of band structure and scattering processes was considered in a general way to understand the behavior of carriers at low energies and at high energies. We also reviewed the behavior of this transport for minority carriers where a gradient in carrier concentration can lead to large diffusive effects, and compared the behavior of minority carriers with majority carriers. Finally, we reviewed effects that are intimately related to band structure: impact ionization and breakdown, limiting velocities, and tunneling. General References 1. B. K. Ridley, Quantum Processes in Semiconductors, Clarendon Press, Oxford (1988). 2. B. R. Nag, Electron Transport in Compound Semiconductors, SpringerVerlag, Berlin (1980). 93 Problems 3. C. M. Wolfe, N. Holonyak Jr., and G. E. Stillman, Physical Properties of Semiconductors, Prentice-Hall, Englewood Cliffs, N.J. (1989). 4. K. Seeger, Semiconductor Physics: An Introduction, Springer-Verlag, Berlin (1985). 5. N. W. Ashcroft and N. D. Mermin, Solid State Physics, Holt, Rinehart and Winston, Philadelphia, PA (1976). 6. C. Kittel, Introduction to Solid State Physics, John Wiley, N.Y., (1968). 7. W. A. Harrison, Solid State Theory, Dover, N.Y. (1979). 8. J. S. Blakemore, Solid State Physics, Cambridge University Press, Cambridge (1985). 9. J. S. Blakemore, “Semiconducting and Other Major Properties of Gallium Arsenide,” J. of Appl. Phys., 53, No. 10, Oct. R123 (1982). 10. I. M. Tsidilkovsky, Band Structure of Semiconductors, Pergamon Press, Oxford (1982). 11. M. Jaros, “Electronic Properties of Semiconductor Alloy Systems,” Rep. Prog. Phys., 48, p. 1091, 1985. 12. F. Capasso, “Physics of Avalanche Photodiodes,” in W. T. Tsang, Ed., Semiconductors and Semimetals, 22, Part D, Academic Press, San Diego, CA (1985). Problems 1. Consider a system of independent and distinguishable particles. Show that for this system, the ratio of the number of occupied particles in the state j to its degeneracy is the Maxwell–Boltzmann distribution function given by nj Ej E − ξf f(E) = = exp − = exp − . (2.162) gj kT kT 2. Show that, as in the case of electrons, the hole occupation following Fermi– Dirac statistics leads to p = NV F1/2 (ηfv ) , (2.163) where ηfv = (Ev − ξf )/kT . For GaAs, draw the electron and hole density, at 300 K, for the functions ηfc and ηfv within 5kT of the conduction and valence band. 94 Properties of Semiconductors for Devices 3. For the most common type of acceptors in semiconductors, show that the degeneracy is 4, and also show that f (EA) = and NA− 1 = , NA 1 + 4 exp [(EA − ξf ) /kT ] NA0 = NA 1+ 1 4 1 . exp [(ξf − EA ) /kT ] (2.164) (2.165) 4. Show that when holes initiate and dominate the avalanche process, the avalanche integral of interest is related by Z wn Z wn 1 = 1− αp exp − (αp − αn ) dη dζ, (2.166) Mp −wp ζ following arguments based on hole generation. 5. For bipolar transport, i.e., with both electrons and holes contributing to conduction, show that the Hall coefficient RH is related to the carrier densities and drift mobilities by " # pµ2dp − nµ2dn r RH = . (2.167) q (nµdn + pµdp )2 6. Estimate the Bohr radius, and the impurity density corresponding to an average distance between impurities equal to the Bohr radius, for n-type GaAs, Si, Ge, InP, Ga.47In.53 As, InAs, GaSb, and InAs. The Bohr radius also gives an indication of the binding energy of the donor, assuming a hydrogenic model for binding of the electron to the donor. Estimate this for these semiconductors, and compare with the observed energies. 7. What is the shape of the constant-energy surface for a semiconductor whose conduction band edge energy changes as the fourth power of the reduced wave vector? Also find the density of states with energy and the effective mass with energy assuming that the coefficient of the E–k relationship is α. 8. What is the relationship, in the previous problem, between the carrier concentration and the Fermi energy? 9. Plot the Maxwell–Boltzmann distribution function and Fermi–Dirac distribution function (assuming ξf − Ec = 3kT ) at 300 K and 77 K as a function of the square of the velocity of carriers assuming m∗ = 0.067m0 for the effective mass of GaAs. What is the width in energy at half of the maximum for the two distributions? At what velocity do the distributions drop to 10% of the magnitude at zero velocity? Problems 95 10. We will consider, simplistically, how one may obtain the phonon behavior in a three-dimensional lattice such as that of GaAs—a zinc blende lattice. To keep the problem tractable, we will consider the oscillations in h111i direction for (111) planes. Alternating planes contain atoms of Ga and As. If a is the linear dimension of the unit cell, the planes alternate with a spacing of a/4 and a/12. One bond to the atoms extends perpendicular to these planes and three bonds extend at an angle of 70.53 degrees in the opposite half. The resulting strength of either is the same. (a) Derive and plot the longitudinal energy-momentum relationship by considering the differential equation that governs the displacement and the force for the two species of atoms. (b) Now consider the same problem for a diamond lattice, i.e., with only one type of atom. How is this result different from the previous? What is its significance? 11. Why are there differences in the variation with wave vector, including a reversal of order, for the energies of the LO and TO phonons? 12. For a semiconductor with isotropic spherical constant energy surfaces in conduction, and two valence bands, find the Hall coefficient. Let τn , τp1 , and τp2 be the momentum relaxation times for the carrier whose densities are n, p1 , and p2 in the respective bands. 96 Properties of Semiconductors for Devices Chapter 3 Mathematical Treatments 3.1 Introduction In using semiconductor devices, our principal interest is in knowing the behavior of currents and voltages at the device terminals due to an applied stimulus, a voltage, or a current, as a function of time. To obtain this knowledge, we need to describe the behavior of the carriers in the device. We need information related to how the carriers move and how they stay stationary. The ensemble of carriers moves in most semiconductor devices as a result of an electric field (we are not considering any magnetic field-based devices in this text), and it stays stationary because there exists no net external force on the ensemble. A stationary ensemble has carriers moving randomly as a result of scattering, a Brownian motion, while a moving ensemble exhibits a net response to the applied force. Both of these are important in studying device behavior. Another important aspect, interrelated with these in the device, is the effect of a rapidly changing electric field during a time transient. The current in the device, at any cross-section, results from moving charged particles (the particle current) and from changing displacement field (the displacement current, d(s E)/dt). These currents have to be related to the applied currents or voltages. We may also use different levels of sophistication in modelling the different regions of the device, depending on how critical they are to the overall device behavior, and the level of accuracy and hence sophistication that is acceptable. These sections of the device, their interfacing with each other, and their interfacing with the device terminals (the contacts that we access) and device surfaces where there are no contacts, have to be modelled accurately to reflect the overall behavior. So, to analyze the device, our mathematical models must include behavior of carriers in semiconductors, boundary conditions between semiconductor sections, time-dependent and time-independent behavior, and carrier behavior at semiconductor contacts and surfaces. Our aim in this chapter is to review and discuss some of the more important general approaches for the analysis so that we may develop the tools necessary to understand the 97 98 3 Mathematical Treatments operation of devices. In trying to describe the behavior of transport in semiconductors, the principal problem to be tackled is that of determining current in the presence of the electric field that moves the carriers, and scattering that limits the unlimited increase in momentum and energy of the particles as a result of the applied field. The most common formulations for describing this behavior are classical. They treat electrons and holes as particles, of certain position, momentum, and energy. The energy that these carrier can possess can be treated as being continuous, except in the bandgap, because the energy level separations are much less than kT for the macroscopic sample sizes employed. We call this methodology the kinetic approach since it uses the kinetics of an average particle with a simple treatment of collisions (scattering) to describe its equation of motion. The approach is quite successful in describing macroscopic properties of the semiconductors in which off-equilibrium effects are not important. A more common approach than the kinetic approach is the use of the Boltzmann Transport Equation (BTE) for describing carrier kinetics. The formulation considers the equation of motion for the distribution function of the particles f(r, p; t). This distribution function f is the probability of finding a particle with the momentum p at the position r at the time t. We will discuss this and simplifications resulting from it (drift-diffusion follows from the the BTE following many approximations) since they have become increasingly popular in describing the hot carrier phenomenon. One additional advantage of BTE is that it leads to a methodology which is not very computationally intensive. Instead of considering the distribution function, we may consider individual particles themselves, selected at random, and collect enough information about them to determine the average ensemble behavior. So, one follows individual particles under the influence of the governing equations and allows them to scatter with probability of scattering determined by the randomness and the relative frequency of occurrence of the specific scattering event. By calculating over several scattering events and/or over behavior of several particles (usually many thousands), one can determine the statistical average behavior of the transport. The Monte Carlo approach is not restricted to many of the assumptions inherent in the simplified BTE approaches, such as simplified treatments of the band structure and distribution functions, in order to obtain the solution. However, these advantages may be offset by a lack of information or simplifications in implementations. An example of the former are the impact ionization processes, whose microscopic features and hence means of implementation are still open to debate. An example of the latter are coupling coefficients for scattering where not enough may be known of the underlying characteristics of the semiconductor itself. The Monte Carlo approach, in spite of these inadequacies, has been highly successful. The reason for this has been that the simplifying assumptions of BTE become questionable well before the inadequacies of a well-implemented Monte Carlo code become suspect. Examples of these successes include description of high field transport and transport involving situations where simplified distribution functions do not exist, such as in very short dimension structures. 99 3.2. KINETIC APPROACH The next level in sophistication has been broadly covered in the Quantum Transport approach, which describes behavior in situations where the quantum nature of states and kinetics is included. This becomes necessary in problems where spatial and temporal extents are similar to the de Broglie wavelength and the duration of scattering events, etc. The kinetic, BTE, and Monte Carlo approaches now become unacceptably inaccurate. Examples of problems where this is true are those involving size quantization, e.g., calculations related to tunneling in coupled barrier structures where the momentum is quantized along one direction. A common Quantum Transport approach is the density matrix approach based on the Liouville equation. The Liouville equation employs the statistical density operator or the density matrix, representing the ensemble of the states of the system, together with the Hamiltonian to describe the state of the system. This approach has shown some success in modelling the coupled barrier problem. All variations of the quantum transport approaches are very complex, and are presently needed in only some of the devices of interest. Hence, in the following few sections, we will restrict ourselves to the discussion of the kinetic approach, the BTE approach, and the Monte Carlo approach. Our objective is to appreciate the methodology, to understand the limits of these approaches, and to relate these to the physical meaning of the results derived. 3.2 Kinetic Approach The simplest of the classical formulations is the particle kinetic approach, which models the kinetics of the motion of an average particle in the presence of a force with a simple treatment of collisions. It provides useful insights and is quite intuitive for many of the standard problems of semiconductor transport. To describe the behavior of the system we need the equation of motion and the relationship between this motion and the current. These, following classical mechanics, can be written as the following for an applied electric field (E), magnetic field (B), and current density (J): and dp dt v J = q (E + v × B) − = = g(p), nq hvi , p , τ (3.1) where q is the charge of the carriers, n is the carrier density, and hvi the average velocity of the carriers. Here, τ is a time constant representing a linear damping term representing the loss of momentum due to scattering. In this set of equations, an ad hoc model is employed to describe the effect of applied fields with an energy dependent time constant τ , but the quantum nature of the problem is accounted for by an effective mass in the functional relationship of the second equation. Quite often groups of particles may be encountered. Some examples of this are different charge of particles such as in ambipolar transport consisting of both electrons and holes, and two valley transport such as with light holes and heavy holes in p-type material or electrons in two valleys 100 3 Mathematical Treatments under high field conditions. In these situations, the groups of particles may be represented by suitable modifications of the previous equations to a set of equations representing each group of particles. Let us now consider some simple examples of application of the kinetic approach, as well as of its limitations. In its simplest form, the semiconductor band structure can be considered parabolic, leading to a constant effective mass; and particles can be considered non-interacting at low concentrations, leading to a Maxwell–Boltzmann distribution of carriers with most particles at the bottom of the band. This leads to a closed-form solution which is useful in the calculation of average properties at low concentrations and negligible fields. For this semiconductor with the spherical constant energy surface, assuming an energy independent scattering, and only electrons as the carriers, Equation 3.1 reduces to and dp dt = v = J = q (E + v × B) − p , m∗ nqv, p , τ (3.2) giving τ dJ + J − µJ × B = nqµE, dt where µ= qτ m∗ (3.3) (3.4) is the mobility of the particle. In our discussion of drift mobility in Chapter 2, this relationship was used implicitly. It shows the approximations related to band structure, and the degeneracy involved. There is an additional approximation of steady-state implicit in this too. We can estimate the time constant— consider GaAs with a mobility of 4000 cm2 .V−1 .s−1 , typical for a donor density of 1×1017 cm−3 at 300 K. The time constant is 0.15 ps. Transient effects related to the relaxation of momentum take place during a time period extending over many time constants. This is not included in the description, and hence may not be expected to be reproduced. Thus, the set of equations should be used for time-varying parameters whose time variation is parameterized at higher than this time constant. Let us consider another example, the response to a sinusoidally varying field with radial frequency ω in an isotropic material with the field along the coordinate axis. The electric field has a magnitude which is the real part of E = Ê exp (jωt) , (3.5) and whose response is a particle current, J = Jˆ exp (jωt) . (3.6) 101 3.2 Kinetic Approach We will discuss the methodology of small-signal analysis later in this chapter. The phasor Jˆ follows from the earlier analysis as nqµωτ nqµ Ê − j Ê. (3.7) Jˆ = 2 2 1+ω τ 1 + ω2 τ 2 The term nqµ is the static conductivity of the material σ. From the Maxwell equations,1 we can derive the wave equation as ∇2 E = − s ω 2 ω E+ J, 2 0 c 0 c2 (3.8) where c is the speed of light in free space, and hence 1/0 c2 is the permeability of free space. Since we are looking at the frequency-dependent response, whose time period is still larger than the relaxation time, we use the frequency dependence of the semiconductor permittivity s : s = s1 − jωs2 , (3.9) and obtain τσ σ 1 2 ∇ Ê = −ω s1 − + jω ωs2 + Ê. 0 c2 1 + ω2 τ 2 1 + ω2 τ 2 2 (3.10) The real part of this response, the response to a sinusoidal signal, goes through a phase change when the effective permittivity eff = s1 − τσ = 0. 1 + ω2 τ 2 (3.11) The effective permittivity is dependent on the carrier density and the low frequency permittivity, which can be approximated to s1 . We also introduce a frequency parameter parameter ωp , the plasma radial frequency; the interrelationships of these are: ! ωp2 τ 2 qnµτ eff = s1 − = s1 1 − , (3.12) 1 + ω2 τ 2 1 + ω2 τ 2 and 1 , (3.13) τ τd where τd is the dielectric relaxation time s1 τd = . (3.14) σ The significance of the real part of the wave equation going negative is that the sinusoidal signal is attenuated, and the frequency at which this occurs is defined by 1/2 1/2 1 1 1 ω = ωp2 − 2 = − 2 . (3.15) τ τ τd τ ωp2 = 1 Discussed in Chapter 9. 102 3 Mathematical Treatments For our example of GaAs, of mobility 4000 cm2 .V−1 .s−1 , donor density of 1 × 1017 cm−3 , time constant 0.15 ps, and s1 = 12.90, the plasma frequency ωp /2π is 3.1 THz, dielectric relaxation time τd is 1.79 fs, and the frequency at which this reversal occurs is 9.7 THz. We can extend the mobility relationship from the case of a single carrier and single time constant to that of two carriers and two time constants (see Problem 1), and show a similar relationship for current for the ambipolar situation (see Problem 2). We can also extend it to multiple time constants in the same general way. Here we give two examples of the calculation of the time constants for electrons, by relating them to the scattering mechanisms for a density of states g(E) in the conduction band and an occupation probability related by the distribution function f. For the average of any transport parameter ϕ(E), following translation of the energy axis to the bottom of the conduction band, changing the primary variable from velocity to energy, and using approximations similar to that employed for occupation statistics in Chapter 2, we obtain (see Problem 3), R∞ 2 0 ϕ(E)g(E) (∂f(E)/∂E) EdE R∞ . (3.16) hϕi = − 3 0 g(E)f(E)dE For parabolic band density of states, the density of states has a square-root dependence on energy, and for non-degenerate conditions the Maxwell–Boltzmann relationship gives an exponential energy dependence for the distribution function, hence, R∞ 2 0 ϕ(E)E 3/2 exp (−E/kT ) dE R∞ hϕi = 3kT 0 E 1/2 exp (−E/kT ) dE R∞ ϕ(E)E 3/2 exp (−E/kT ) dE 0R = . (3.17) ∞ 3/2 E exp (−E/kT ) dE 0 If the variable ϕ(E) has a power law dependence on the energy E, i.e., ϕ(E) = AE ν , then the integral can be related through the Γ functions ν hϕi = A(kT ) Γ (ν + 2.5) , Γ (2.5) (3.18) where the Γ functions satisfy the properties described in our discussion of the Fermi integrals. The average for relaxation time for the mobility, with a momentum relaxation time τp , is R∞ 2 0 τp (E)g(E) (∂f(E)/∂E) EdE hv2 τ i R∞ . (3.19) τµ = hτp i = − = hv2 i 3 0 g(E)f(E)dE Here, the integral was transformed over velocity instead of energy in order to express it in the previously expressed form of Chapter 2. For speed, the rela- 103 3.2 Kinetic Approach 1/2 tionship of the variable is ϕ = v = (2/m∗ ) vθ = 2 m∗ 1/2 (kT )1/2 Γ(3) = Γ(2.5) 2kT m∗ E 1/2 , and hence 1/2 2×1 = 1.5 × π 1/2 8kT πm∗ 1/2 . (3.20) For scattering, by ionized impurity scattering, the Conwell-Weisskopf relationship is τII = AE 3/2 , (3.21) where A is a coupling constant. Hence, the momentum relaxation time for ionized impurity scattering follows as 3/2 τµ = A(kT ) 3/2 Γ(4) (kT ) = 4A 1/2 . Γ(2.5) π (3.22) For acoustic scattering, τac = BE −1/2 , (3.23) and hence the momentum relaxation time is given by −1/2 Γ(1.5) τµ = B(kT ) Γ(2.5) = 2B 1/2 3(kT ) . (3.24) Now let us consider the relaxation time of interest in Hall effect measurements. When a magnetic field B is present, the current, in steady-state may be derived as (see Problem 4) q 2 nτ q 3 nτ 2 J = E− E ×B+ m∗ (1 + ωc2 τ 2 ) m∗2 (1 + ωc2 τ 2 ) q 4 nτ 3 (E.B) B, (3.25) m∗3 (1 + ωc2 τ 2 ) where ωc = qB/m∗ is the cyclotron resonance frequency. If the magnetic field is small, then 2 3 2 q nτ q nτ J= E − E × B. (3.26) ∗ m m∗2 Hall effect measurements involve, as discussed before, a magnetic field orthogonal to the plane of the semiconductor, i.e., orthogonal to the electric field. Let z be the orthogonal direction of the magnetic field, and let x be the direction of the applied field. In steady-state, no current flows perpendicular to this either in the y direction or the z direction. Then, 2 3 2 q nτ q nτ Jx = E − Ey Bz , x m∗ m∗2 2 3 2 q nτ q nτ Jy = E + Ex Bz = 0, y m∗ m∗2 2 q nτ and Jz = Ez = 0. (3.27) m∗ 104 3 Mathematical Treatments The current flow and the the in-plane orthogonal electric fields, ignoring second order terms, are related by Ey = − Jx = − qBz hτ 2 i Ex m∗ hτ i 2 and qn hτ i Ey . Bz hτ 2 i (3.28) This shows that the Hall constant and Hall factors that we applied earlier are related as: and RH = r = Ey 1 hτ 2 i =− , JxBz qn hτ i2 hτ 2 i 2 Ey . hτ i (3.29) We can now show that the Hall pre-factor r, when acoustic deformation potential scattering dominates (see Problem 5), is r= 3π , 8 (3.30) and that the Hall mobility is associated with the Hall relaxation time τH = hτ 2 i . hτ i (3.31) This treatment can thus be extended over several complicated situations, all leading to complicated mathematical relationships even with the assumption of the Maxwell–Boltzmann relationship and explicit energy dependence. Many of the restrictions are violated in practical situations, e.g., degenerate semiconductors, presence of hot carriers, etc. Indeed, the problem rapidly becomes intractable and more sophisticated approaches have to be utilized. 3.3 Boltzmann Transport Approach In the kinetic approach, we introduced classical kinetics to describe the motion of a group of particles with common characteristics described by the relaxation time, charge, and the relationship between momentum and velocity. The BTE2 describes the kinetics using the equation of motion for the distribution function of the particles f(r, p; t). The distribution function f is the probability of finding a particle with a crystal momentum p at a position r at a time t. In thermal 2 For an extended discussion of the BTE and its application in semiconductor transport theory, see E. M. Conwell, “Transport: The Boltzmann Equation,” in W. Paul, Ed., Handbook on Semiconductors, Vol. 1, North-Holland, Amsterdam (1982). 3.3 Boltzmann Transport Approach 105 equilibrium, the probability of finding a carrier in a state with energy E(p) is given by the Fermi–Dirac distribution function f0 f0 [E (p)] = 1 , 1 + exp {[E (p) − ξf ] /kT } (3.32) where ξf is the Fermi energy. When the energy of the electrons is larger than the Fermi energy by a few kT s, the distribution function can be approximated by f0 [E (p)] ≈ exp {[ξf − E (p)] /kT } , (3.33) the Maxwell–Boltzmann distribution function, or Boltzmann distribution function in short. For heavy doping, however, the Fermi–Dirac distribution function should be considered. The effect of the band structure on the distribution function is included in the relationship between energy and momentum. For a spherical constant energy surface with parabolic bands whose minimum is at the zone center, this relationship takes the form p2 E= , (3.34) 2m∗ while for more complex forms of parabolic bands, with different energy-momentum relationships in different directions, it still has the square dependence on the momentum but in a more complex form, E= p2y p2x p2z + + . 2m∗x 2m∗y 2m∗z (3.35) The constant energy surface is now an ellipsoid. The momentum p has an equivalence with the crystal wave vector k through the reduced Planck’s constant. In the rest of our discussion of the BTE, we will use the momentum as p, although using k is just as common and is even employed elsewhere in this book. Degenerate minima, such as for the light hole and heavy hole valence bands, may be included by using their energy–momentum relationship and their degeneracy. Close to thermal equilibrium, for many problems, it may be sufficient to treat these as two independent constant energy surfaces of equal energy (e.g., in unstrained materials spheres at very low energies). The force F on the particle in an electric field and magnetic field causes a change in drift momentum related by F= dp = q(E + v × B), dt (3.36) between scattering events. Let the distribution in real and phase space at any instant of time under general conditions be given by f(r, p; t). For the changes that occur between time instants t and t+∆t, consider the effect of drift. The carriers which had the momentum p − ∆tdp/dt ∆t time interval earlier, drift to have the momentum p after the elapsing of time ∆t. Therefore, the effect of drift in time interval ∆t 106 3 Mathematical Treatments is to cause a change in the distribution function of f(r, p − ∆tdp/dt) − f(r, p). Hence, the rate of change of the distribution function with time due to drift is given by ∂f ∂f dp ∆t = − . ∆t, (3.37) ∂t drift ∂p r,t dt i.e., ∂f = −ṗ.∇p f. ∂t drift (3.38) The rate of change due to diffusion, e.g., resulting from concentration or temperature gradients, can be found similarly. The carriers which were at the position r − ∆tdr/dt ∆t time interval earlier, diffuse to the position r after the elapsing of time ∆t. Therefore, the effect of diffusion in time interval ∆t is to cause a change in the distribution function of f(r − ∆tdr/dt, p) − f(r, p). Hence, in a similar manner as above, the rate of change of the distribution function with time due to diffusion is given by ∂f = −v.∇r f. (3.39) ∂t diff These are the changes in the distribution function due to drift and diffusion. Changes in the distribution function also occur due to scattering. Carriers may be scattered into and out of the elemental volume at (r, p; t). Treating these as independent processes, the total rate of change in the distribution function f can be written as ∂f ∂f ∂f ∂f = + + ∂t ∂t drift ∂t diff ∂t scatt ∂f . (3.40) = −ṗ.∇p f − v.∇r f + ∂t scatt This long argument establishing the change of distribution function in the sixdimensional (r, p) space can be derived directly by application of Liouville’s theorem for semi-classical equation of motion. A consequence of this theorem is the conservation of (r, p)-space volume.3 Thus, ∂f f(r + ∆r, p + ∆p; t + ∆t) − f(r, p; t) = lim ∂t scatt ∆t ∆r,∆p;∆t→0 = ṗ.∇p f + v.∇r f + ∂f , ∂t (3.41) an equivalent result. The BTE incorporates effects taking place in time. Thus, should it be possible to make appropriate analytic expressions, the BTE will describe the time 3 For arguments leading to this, see N. W. Ashcroft and N. D. Mermin, Solid State Physics, Holt, Rinehart and Winston, Philadelphia, PA (1976). 3.3 Boltzmann Transport Approach 107 transient effects too if the scattering relationship can be characterized. The expression is also valid for steady-state; the distribution function does not change in steady-state, giving ∂f = q(E + v × B).∇p f + v.∇r f. (3.42) ∂t scatt Both of the above are convenient forms for the BTE. For multiple bands (e.g., two valleys) we have two distribution functions and two equations as a generalization of the one band treatment. The same is true for degenerate bands such as those due to holes. The scattering term in these cases must include effects on the distribution function due to scattering events taking place within the band, into the band, and out of the band. A similar generalization procedure could be used for more valleys. 3.3.1 Relaxation Time Approximation One of the most important parameters to be introduced as part of the discussion on scattering is the relaxation time. In the kinetic approach, we introduced it in an ad hoc manner to incorporate the loss term in the momentum. In our following discussion, we will establish it on a firmer basis, and also establish limits of the validity of using a relaxation time. It is a very justifiable time constant for certain scattering processes, where it can be established as a single valued function of momentum or energy. However, scattering processes do exist where this may be unjustified, e.g., in polar optical scattering. In such cases it is an engineering approximation, or a fitting parameter, used to allow simplification of calculation using the distribution function approach. In interpreting results of such a calculation, these approximations should be considered in understanding the limits of validity. 0 Let S(p, p ) be the probability per unit time of a transition from an initial 0 0 state p to a final state p in unit volume of the momentum space at p . The term S, thus, incorporates the effect of selection rules of transitions, etc. The 0 distribution function at p describes the probability of finding the electron in that momentum state. The probability of a scattering occurring into this state is proportional to the likelihood of this state being empty, which is given by 0 the number of carriers scattered from p per unit time is R1 − f(p ). Thus, 0 0 0 0 f(p)S(p, p )(1 − f(p ))d3 p with the integral over the entire p volume to cover all such scattering events. Similarly, the number scattered into p from the 0 0 entire p volume is proportional to the distribution function at p , the scattering probability, andRthe probability of there being an empty state at p. This is given 0 0 0 by the integral f(p )S(p , p)(1 − f(p))d3 p . The total rate of change of the distribution function f due to scattering can be found from the difference of these two integrals as: Z h i ∂f 0 0 0 0 = f(p )S(p , p) − f(p)S(p, p ) d3 p , (3.43) ∂t scatt 108 3 Mathematical Treatments provided we assume non-degenerate conditions and hence neglect the effect of exclusion principle. This condition also implies that f 1. The relaxation time approximation implies that this integral can be simplified, under certain conditions, to the expression ∂f f(p) − f0 (p) =− , (3.44) ∂t scatt τ (p) where f0 (p) is the unperturbed Maxwell–Boltzmann distribution function. We now consider the conditions and the scattering processes for which this is clearly justified. Let us consider the effect of a small perturbation in the thermal equilibrium distribution function. Such a perturbation may occur from small changes in field, temperature, or external optical excitation. Let this perturbation cause a new distribution function f = f0 + ∆f, (3.45) where the perturbation ∆f in the distribution function is much smaller than the thermal distribution function f0 . Since the distribution function remains unchanged in thermal equilibrium, we have Z h i ∂f0 0 0 0 0 = f (p )S(p , p) − f (p)S(p, p ) d3 p = 0. (3.46) 0 0 ∂t scatt Then, in the presence of the perturbation, our scattering equation reduces to Z Z ∂f 0 0 0 0 3 0 = ∆f(p )S(p , p)d p − ∆f(p) S(p, p )d3 p . (3.47) ∂t scatt This perturbation causes a current flow because any disturbance in equilibrium causes motion of the charged particles. Since this current is proportional to the velocity, it is an odd function of the velocity. Hence, the perturbation in the distribution function ∆f is also an odd function of the velocity. Clearly, if the first term in the scattering equation vanishes, then Z ∂f 0 0 = −∆f(p) S(p, p )d3 p ∂t scatt ∆f(p) = − . (3.48) τ (p) where τ (p) = R 1 0 S(p, p )d3 p 0 . (3.49) Thus, a sufficient condition for the validity of relaxation time approximation is that the first term in the scattering equation above vanish, i.e., Z 0 0 0 ∆f(p )S(p , p)d3 p = 0. (3.50) 3.3 Boltzmann Transport Approach 109 Figure 3.1: A schematic for the discussion of scattering processes in momentum space under the influence of a force F for a semiconductor with ellipsoidal constant energy surfaces. After E. Conwell, in W. Paul, Ed., Handbook of Semiconductors, Vol. 1, North-Holland, Amsterdam (1982). We now discuss the conditions and the scattering processes for which this is true. 0 If ∆f(p ) is an odd function of momentum (or velocity) then this integral 0 vanishes if S(p , p) is an even function of momentum (or velocity). For the scattering probability to be an even function, the scattering probability is equal for all combinations involving the momenta and their conjugates, i.e., 0 0 0 0 S p, p = S(p, p ∗ ) = S(p∗ , p ) = S(p∗ , p ∗ ). (3.51) The momentum p∗ is in exactly the opposite direction of the momentum p. Scattering processes that randomize the momentum (or velocity) fulfill this condition. Intuitively, this makes sense since random processes can not result in 0 any net scattering into either p or p . Let us consider the ellipsoidal surfaces, 0 i.e., consider the anisotropic mass of energy E and E as shown in Figure 3.1. 0 In the presence of the force F , the states at p ∗ have an increase in popula0 tion of the carriers, and the ones at p , its complex conjugate, have a decrease in the population of the carriers. Thus, we have the change in distribution func0 0 0 0 tions, ∆f(p ∗ ) > 0 and ∆f(p ) = −∆f(p ∗ ). If the momentum p ∗ has more carriers, it results in an increase in transition of carriers from the momentum 0 p ∗ to the momentum p, with an equal decrease in transition from momen0 tum p and momentum p. This occurs because the scattering probability to 0 0 the momentum p from the momentum p and its conjugate p ∗ are equal, i.e., 110 3 Mathematical Treatments 0 0 0 S(p , p) = S(p ∗ , p). So, the sum of the two transition rates from momentum p 0 and momentum p ∗ into p remains unchanged in presence of small applied force F . In this same manner, we may pair all the states in the same valley. So the 0 total rate of transition from the momentum p to the momentum p remains the same as it was before (i.e., when it was in thermal equilibrium with distribution function f0 ), and is balanced by the rate of transition from the states of momenta p, again with the distribution function f0 . The remaining small change ∆f(p) is caused only by the scattering out of the momentum p, independent of 0 the momentum p , and hence the change in scattering can be defined in terms of the initial state in accordance with the relaxation time. So, for scattering processes that involve randomization of the momenta or velocity, ∂f f(p) − f0 (p) ∆f(p) =− = , (3.52) ∂t scatt τ (p) τ (p) where Z 1 0 0 = S(p, p )d3 p . (3.53) τ (p) In addition to scatterings that randomize the momentum, the relaxation time is also justified if (a) scattering is elastic (i.e., scattering involves a negligible loss of energy) and (b) the scattering probability depends on the momentum p and 0 0 the momentum p only through the angle θ between them. The consequence 0 0 of the first, with no loss of energy, is that SA (p , p) = SA (p, p ) where the additional subscript A refers to the scattering probability normalized to unit 0 area of the constant energy surface at p . These terms are proportional to the power crossing the cross-section which should be the same for elastic processes. If this is the case, then Z h o ∂f0 0 0 0 0 = 0 = f0 (p )SA (p , p) − f0 (p)SA (p, p ) d2 p , (3.54) ∂t scatt and because this integral is evaluated on a constant energy surface, 0 f0 (p ) = f0 (p). (3.55) The appropriateness of the use of relaxation time follows. Now consider the presence of electric field E. Since the change in distribution is proportional to the energy supplied by the field, f = f0 + gE.v, (3.56) where g is a constant which is a function of the carrier mass, etc. From this, we can write the rate of change in the distribution function due to scattering as Z ∂f 0 0 0 = gE.v − gE.v SA (θ )d2 p . (3.57) ∂t scatt We choose the z-axis in the direction of the velocity v and the cylindrical 0 coordinate system. The elemental area at the momentum p is given by 0 0 0 d2 p = (p dθ ).(p sin θ dϕ ) = p 2 sin(θ )dθ dϕ , 0 0 0 0 0 0 0 (3.58) 3.3 Boltzmann Transport Approach and hence Z h i 0 0 0 ∂f = gE.v 1 − cos(θ ) SA (θ )d2 p . ∂t scatt 111 (3.59) This equation follows from the fact that the only the z-component of the velocity 0 0 0 v contributes to the above integral, i.e., the term v cos(θ ) represents the difference contribution. The rest integrate to zero because they are functions of 0 ϕ . The relaxation time follows, then, as Z h i 1 0 0 0 = 1 − cos(θ ) SA (θ )d2 p . (3.60) τ (p) Since the mean free time between collisions (τc ) is Z 1 0 0 = SA (θ )d2 p , τc the relaxation time is τc E, τ = D 0 1 − cos(θ ) (3.61) (3.62) where the denominator is averaged over all the collisions. If all final directions 0 are equally likely, i.e., they are random, hcos(θ )i = 0 and τ = τc . If they involve 0 small angle scattering, then hcos(θ )i would be closer to unity and τ τc , and the time constant will only be a function of energy. Consider now if it is meaningful to talk about relaxation time in its strict sense for various scattering processes. For spherical constant energy surfaces, relaxation time, which is a function of energy only, exists both for acoustic and ionized impurity scattering. For non-polar semiconductors, optical scattering is randomizing, so it also can be treated by a relaxation time which is a function of energy. Multiple valleys, inter-valley scattering, and optical intra-valley scattering also allow the relaxation time approximation in non-polar semiconductors; however, acoustic mode relaxation time approximation is justified only for highly isotropic energy surfaces. For non-polar semiconductors, only for ionized impurity scattering for elliposidal energy surfaces does the use of relaxation time approximation turn out to be poor. For polar semiconductors, polar optical scattering is among the more important scattering mechanisms. The relaxation time approximation is incorrect in this case. However, in practice, a proper Monte Carlo calculation is performed to generate a relevant engineering fitting parameter for the relaxation time. This technique allows, then, the use of a simpler and less intensive BTE approach to analyze a problem, while still maintaining accuracy because it uses Monte Carlo results for the fitting parameter of relaxation time. 3.3.2 Conservation Equations We have now discussed procedures that allow us to determine the distribution function, provided the scattering can be described mathematically either 112 3 Mathematical Treatments through the relaxation time approximation or the transition probability S. The distribution function, for some problems, can be determined in an analytical form, and for some by iterative techniques. However, application of these procedures is still limited to the simplest of the problems of interest. We will discuss, in the next section, one such problem in order to compare the BTE approach with the Monte Carlo approach. A more common technique than these is to use numerical procedures to compute the distribution functions by methods similar to those used in the Monte Carlo approach. This technique also removes the restrictions on using the simplest of distribution functions or simplified dependence on energy alone by restricting the spatial extent of the analysis. By relaxing these requirements on the distribution function, it also allows application of the BTE approach to problems with more complex distribution functions and scattering processes. An example of the latter is the problem of hot carrier transport. But, in the study of devices, we are interested in the carrier density, the current carried by the carriers, the energy of the carriers, etc.; not the probability of finding a carrier at a certain position, with a certain momentum, at a certain time. A set of conservation equations can be generated from the BTE that directly determine these parameters, without having to determine the distribution function. The principle is very similar to, and a simple extension of, the method of determining current in the kinetic approach. For a multi-valley semiconductor, the current, in the kinetic approach, can be written as X X J= qf(p)v(p). (3.63) valleys p To derive the conservation equations, consider the BTE: ∂f ∂f = −ṗ.∇pf − v.∇r f + . ∂t ∂t scatt (3.64) If we wish to determine the expectation of the variable ϕ, we multiply the BTE by ϕ and integrate over the momentum space. This allows us to determine the following conservation equation for ϕ: ∂ ∂ < ϕ >= − hṗ.∇pϕi − ∇r . hvϕi + ϕ , (3.65) ∂t ∂t scatt where we have used and ∇r .v = 0 v.∇r f = ∇r .(vf), (3.66) because the velocity v is a function of momentum p alone. We now have an equation that describes the dependence of hϕi on position and time. Different choices of ϕ(p) lead to different equations of conservation for the parameter. These are referred to as moment equations; the method, method of moments; because of the way they are derived from the BTE. 3.3 Boltzmann Transport Approach 113 The parameters that are of interest to us, such as the carrier concentration and the current, are related to the distribution function f(r, p; t) and the choice of the variable ϕ(p). As an example, consider hϕi for ϕ(p) = 1, then Z hϕi = f(r, p; t)d3p, (3.67) which is the carrier concentration n(r, t). If we choose the variable ϕ(p) = −qp/m∗ , i.e., charge times the velocity of a carrier: current due to a carrier, then Z qp hϕi = − ∗ f(r, p; t)d3 p. (3.68) m This is the equation of charge flux, i.e., the current density J(r, t). If we choose ϕ(p) = p2 /2m∗ , i.e., the kinetic energy of the individual particle, then Z 2 p f(r, p; t)d3 p, (3.69) hϕi = 2m∗ the kinetic energy W (r, t) of the carrier ensemble. When divided by the number of carriers that this represents, it is the average kinetic energy per carrier (w) in the specific ensemble. With this as the meaning of the various moments, Equation 3.65 assumes the conventional meaning of conservation of particle and conservation of current, and extends it further to energy, etc. Note that if recombination effects are important, scattering between bands representing the recombination processes should also be included in the BTE. The meaning of the various moment equations is now quite explicit. These moment equations are to be seen as describing the balancing of the averaged quantities they represent. If one could employ the scattering relationship, ∂f f − f0 =− , (3.70) ∂t scatt τ an approximation for some of the scattering processes, but exact for others, then we can write ∂ ∂ϕ hϕi − hϕi0 ∂ hϕi = − ṗ. − − . hvϕi . (3.71) ∂t ∂p τϕ ∂r This equation is similar in its functional form to the continuity equation. The left hand side is the rate of change of hϕi, the first term is a generation term of hϕi by forces that cause changes in the particle momentum p, the second term is a loss term such as a recombination term of hϕi due to scattering, and the last term is a gradient of the flux of hϕi. When ϕ = 1, the last term is proportional to the gradient of the current carried by particles. For ϕ = 1, τϕ → ∞ (no particles are lost in scattering, unless we consider the inter-band scattering term represented by generation and recombination), and ∂ 1 ∂ . hvϕi = .J. ∂r q ∂r (3.72) 114 3 Mathematical Treatments So, in the absence of generation and recombination, this yields ∂n 1 = ∇.J. ∂t q (3.73) With the interband terms included, it is ∂n 1 = G − R + ∇.J. ∂t q (3.74) where G and R are the generation and recombination terms due to interaction between holes and electrons. This is the first moment equation, the particle conservation equation, and has the same form as used in drift diffusion analysis. For ϕ = −qp/m∗ , we have hϕi hϕi0 and ∂ hϕi ∂r ∂ϕ ṗ. ∂p = J, = 0, = − = 2q ∂ W, m∗ ∂r qn − ∗ F, m (3.75) giving ∂J qn J 2q = ∗F − + ∗ ∇r W. ∂t m hτp i m (3.76) This is the second moment equation, the current conservation equation. In this equation, on the right hand side, the first term represents the effect of the applied force, the second represents the effect of scattering, and the third represents the effect on change in energy of the particles which results in a change in their velocity. For ϕ = p2 /2m∗ , the kinetic energy, and giving hϕi hϕi 0 ∂ϕ ∂p ∂ϕ ṗ. ∂p = = = = W, W0 , p , m∗ F −m∗ 1 J = − F .J, ∗. m q q ∂W 1 W − W0 p2 = F .J − − ∇r . v . ∂t q τw 2m∗ (3.77) (3.78) This is the third moment equation, the energy conservation equation. In this equation, on the right hand side, the first term represents energy gain from the effect of force, the second term represents the energy loss due to scattering, and 3.3 Boltzmann Transport Approach 115 the last term is the equivalent in energy of the last term of the current conservation equation. The equation is based on averages; this term represents the ensemble effect of carrier energy change due to ensemble motion. For symmetric distribution functions, such as the displaced Maxwell–Boltzmann distribution, this last term vanishes. Note that we put in a relaxation time constant approximation in these relations, and we have not included heat conductivity of electron gas q.4 In the absence of the time constant approximation, this set of equations is ∂n 1 ∂n = ∇.J + , ∂t q ∂t scatt ∂J q 2q ∂J = nF + ∗ ∇W + , ∂t m∗ m ∂t scatt ∂W 1 ∂W = F .J − ∇r . (vW ) − ∇r .q + and . (3.79) ∂t q ∂t scatt Let us now see how these equations may be extended to a more complex situation of two valleys, a problem that occurs when considering the effect of the Γ and L valleys in hot carrier transport in GaAs. We will also consider additional simplifications to make the problem more tractable. We will have two sets of equations corresponding to the distribution functions in the two valleys. Identifying each of the individual valleys by the subscripts j and k, and the averages by an overline (this was included in the averaging in our earlier equations), we can write mean momentum and energies as pj and Wj = m∗j nj v j , 3 1 = nj kTj + m∗j nj vj 2 2 2 (3.80) for each of the valleys. We introduce the lower case w for the energy of a single carrier, i.e., Wj wj = . (3.81) nj In the Equation 3.80 we have included an additional term of 3nj kTj /2, which is the mean energy in the Boltzmann approximation even in thermal equilibrium when v j = 0. The temperature of the carriers in the valleys may be different, and is either Tj or Tk . Writing for the jth valley, ∂nj ∂nj = −∇r . (nj v j ) + G j − Rj + , ∂t ∂t scatt ∂v j F 2 1 1 1 = − ∗ − v j .∇vj − ∇nj wj + ∇nj v j 2 + ∗ ∂t mj 3 mj nj 3 nj 4 This should be distinguished from fundamental charge q. 116 3 Mathematical Treatments and ∂w j ∂t ∂v j , ∂t scatt = −v j .F − v j .∇w j − κj 1 2 1 ∇. nj v j − ∇ w j − m∗j vj 2 + 3 nj k 2 ∂w j . ∂t scatt (3.82) Here, the terms G j − Rj represent generation and recombination terms in the jth valley. Energy can also be transferred in the form of heat, i.e., through phonons. Such a term due to heat flux, (∇qj ) has been included in these equations using the thermal conductivity κj and the carrier temperature Tj , 1 2 κj ∇ w j − m∗j vj 2 . (3.83) qj = κj ∇Tj = 3 k 2 For two valleys, inter-valley processes may now be included in the scattering term. Consider with relaxation time approximation, one can write for two valleys5 (this can be generalized for more than two valleys in a similar way) ∂nj nj nk = − + , ∂t scatt τn,jk τn,kj ∂v j 1 1 1 nk 1 + − + = −v , j ∂t scatt τp,jj τp,jk τn,jk nj τn,kj w j − w j0 1 1 ∂w j = − − w + j ∂t scatt τw,jj τw,jk τn,jk ! nk wk wj − . (3.84) nj τw0 ,kj τn,kj where in the relaxation times, following our earlier notation in the BTE, the n subscript denotes carrier relaxation, the p subscript denotes momentum relaxation (not holes, which are not included here), the w subscript denotes energy relaxation, and we distinguish the relaxation time constants τw,jk and τw0 ,kj due to energy exchange with phonons and differences in the references for kinetic energy in the two valleys. They differ by the potential energy of the conduction band minima. The various terms of Equation 3.84 can be given specific meaning in line with the earlier description. In the particle conservation equation, the two terms describe the transfer of particles from one valley to the other. In the 5 See the discussions in K. Bløtekjær, “Transport Equations for Electrons in Two-Valley Semiconductors,” IEEE Trans. on Electron Devices, ED -17, No. 1, p. 38, Jan. 1970 and P. A. Sandborn, A. Rao, and P. A. Blakey, “An Assessment of Approximate Non-Stationary Charge Transport Models Used for GaAs Device Modelling,” IEEE Trans. on Electron Devices, ED-36, p. 1244, Jul., 1989. 3.3 Boltzmann Transport Approach 117 current conservation equation, the four terms describe the transfer of momentum within a valley and from one valley to the other. In the energy conservation equation, the first term describes the relaxation towards lattice temperature in intra-valley and inter-valley scattering, the second term describes the energy loss from the jth valley to the kth valley by inter-valley scattering, and the last term describes the energy gained by the jth valley from the kth valley. We distinguish the relaxation time constants τw,jk and τw0 ,kj due to the differences described above. 3.3.3 Limitations In view of the way we derived this formulation, we should recognize some of its limitations. It assumes Maxwell–Boltzmann or displaced Maxwell–Boltzmann distribution. By the latter we mean that the distribution in energy of electrons is still of the same form that the Maxwell–Boltzmann distribution has in thermal equilibrium (i.e., the effect of the exclusion principle is not important), but that it shifts in energy to have excess mean finite energy and velocity. It continues to be a symmetric function in momentum. In the process of using the relaxation times, polar optical scattering is not well modelled because it is neither elastic nor randomizing nor dependent on the cosine of the angle between the initial and final momentum. The relaxation time constants are, therefore, fitting parameters. Polar optical scattering favors smaller angles as shown in Figure 3.2. This figure shows the relative probability of scattering of an electron at various angles in GaAs due to polar optical scattering. Since polar scattering favors small angle scattering, the momentum of electrons is not destroyed. The higher the energy of the electron, the more favorable is the tendency of the electron to continue in close to the same direction. While this tendency leads to favoring of carrier transit at higher velocities in specific situations, this lack of randomization and the approximation involved in the use of Maxwell–Boltzmann-like statistics lead to errors in specific modelling situations. We make an engineering approximation for the polar-optical scattering by forcing a relaxation time fitted to a more accurate Monte Carlo calculation, but the use of the displaced Maxwell–Boltzmann approximation is not correctable because of the way it is implemented. Figures 3.3 shows the scattering rate due to phonons and for impact ionization in GaAs and Si. The scattering rate variations are somewhat complicated due to the nature of the band structures. We discuss this for phonon processes in silicon (see Figure 3.4). Consider the inter-valley scattering rates from an X valley to another X valley as in silicon. The constant energy surfaces are ellipsoids with two different degeneracies. There are four equivalent ellipsoids (see Figure 2.26) for scattering whose major axis is in the plane perpendicular to the major axis of the ellipsoid that the scattering occurs from, and there is one ellipsoid along the same major axis. So, inter-valley scattering, in silicon, is of two different types, one to the four equivalent ellipsoids that are closest (called f-scattering), and one to the ellipsoid that is farthest away (called g- 118 3 Mathematical Treatments Figure 3.2: Angular scattering probability as a function of scattering angle for polar optical scattering in GaAs at 300 K. The two curves are for electron energies of 0.1 eV and 0.3 eV. scattering). The scattering process requires either the emission or absorption of a phonon to conserve the large change in the momentum. Note that the g-emission involving release of a phonon is the strongest. While this distinction is not of concern for an electron in the Γ band of GaAs, it is related to the inter-valley scattering effect of a hot electron in the L valley. An electron undergoing a scattering from one ellipsoid to another ellipsoid sees six equivalent ellipsoids in the perpendicular plane and one ellipsoid along the axis. Like fand g-scattering, the probability of absorption of the phonons will be different since different momentum changes are involved. The low and moderate energy scatterings are lower in GaAs than in silicon. There are specific energies where the scattering rates show the onset of additional processes, such as the X-L scattering process in silicon, or the Γ-L or Γ-X processes in GaAs. At the lowest energy, the scattering in GaAs is limited by the acoustical mode scattering and optical phonon scattering involving absorption of optical phonons as shown in Figure 3.5. At an energy equal to the optical phonon energy (≈ 36 meV for GaAs), optical phonon emission also occurs, resulting in a sudden increase in the scattering rate at this energy. We commented that at the lowest energies, ionized impurity scattering processes are important for useful dopings. Figure 3.6 shows the scattering rate for GaAs, noting the effect of compensation. The scattering rate is comparable to the polar optical phonon scattering rate at low energies and decreases with energy, as expected. 3.3 Boltzmann Transport Approach 119 Figure 3.3: Scattering rate in GaAs and Si at 300 K as a function of electron energy due to phonon scattering and impact ionization. On the GaAs curve, 1 identifies the onset of optical phonon scattering. The last section of the curves correspond to impact ionization processes. The rest of the identified points of rapid changes occur due to effects related to density of states. 120 3 Mathematical Treatments Figure 3.4: Scattering rate at 300 K as a function of energy due to the two different types of inter-valley scattering in Si from the X valley. For a carrier in any valley, f-scattering denotes scattering involving the nearest 4 valleys and g-scattering denotes scattering involving the opposite valley. The total for both emission and absorption process is also shown. 3.3 Boltzmann Transport Approach 121 Figure 3.5: Scattering rate as a function of energy in GaAs at 300 K showing the dependence on acoustical processes and optical absorption (marked a), and optical (marked b) emission. The curve marked c shows the total scattering rate due to phonons. Figure 3.6: Ionized impurity scattering rate for GaAs at 300 K, for compensated (marked a) and uncompensated (marked b, compensation ratio of 2) 1 × 1017 cm−3 doping levels. 122 3 Mathematical Treatments Figure 3.7: Electron scattering rate due to optical phonon and coupled mode scattering in the presence of holes in GaAs at 300 K. The background doping is 5 × 1018 cm−3 typical of bipolar transistors. Note the large effect of screening. While discussing these scattering mechanisms, we should comment on carrier– carrier scattering. In bipolar transistors, e.g., the electron is a minority carrier in the midst of a lot of holes in the base. In the case of a two-dimensional electron gas there exists a very high local density of electrons. In the former, electron–hole scattering will be important, while in the latter, electron–electron scattering will be important. This scattering, which we have also referred to as plasma scattering, can occur coupled with other scattering modes (e.g., together with optical phonons), and its effect can be very strong on optical phonon scattering at high hole density (see Figure 3.7). The phonon scattering rate is reduced because the holes screen the potential perturbations that are caused by the optical mode vibrations. However, now electron–hole scattering becomes important and has to be included in scattering calculations. We have looked at these various processes to show that one can at least fit the time constant τw to a scattering process as a function of energy. This time constant, then, can be used phenomenologically in the moment equations approach. The last set of equations, Equation 3.84, were non-stationary equations. So, knowing all the necessary parameters involved (i.e., the τ s) and assuming a displaced Maxwell–Boltzmann distribution, allow us to determine the ns, the v j s, and the w j s, and hence to characterize the temporal and spatial response of a semiconductor device. These equations, in spite of the approximations, are still quite complicated. However, knowing the τ s, they are computationally much less intensive than the Monte Carlo approach. In addition, they can be 123 3.3 Boltzmann Transport Approach simplified for certain situations even from this form. An example of this simplification, for the transit in a spatially homogenous sample under the influence of a force F in a single valley semiconductor, ignoring recombination effects, is the set of equations ∂nj ∂nj = = 0, ∂t ∂t scatt F ∂v j ∂v j = − ∗ + , ∂t mj ∂t scatt ∂w j ∂w j and = −v j .F + . (3.85) ∂t ∂t scatt Because of the assumption of spatial homogeneity, these equations do not account for diffusive effects which are included in the spatial gradient terms of the BTE. For a two-valley problem (e.g., in GaAs considering the Γ and the L valleys), we may define, with the subscript l for the lower valley and u for the upper valley, the following for carrier density, average velocity, and average energy per carrier, n = and v = w = m∗ = nl + nu , nl nu vl + vu , nl + nu nl + nu nl nu wl + wu , nl + nu nl + nu nl nu m∗l + m∗ , nl + nu nl + nu u (3.86) leading to the following equations in relaxation time approximation for a spatially homogenous but two-valley semiconductor: ∂n ∂t ∂v ∂t ∂w ∂t and = 0, = − = F v − , m∗ τp w − w0 −v.F − , τw (3.87) where τp and τw lump the effects of related time constants. These time constants could be fitted from a steady-state solution of the Monte Carlo calculation of this same problem of transit in the presence of the force F . The time constants, from the steady-state solution, could be found as and τp = τw = m∗ v F w − w0 − . v.F − (3.88) 124 3 Mathematical Treatments Figure 3.8: The momentum and energy relaxation times (τp and τw ) as a function of energy fitted for undoped GaAs at 300 K and 77 K. Figure 3.8 shows, for 300 K and 77 K, these relaxation times for undoped GaAs. The temporal evolution follows as a solution of our control equations. For example, Figure 3.9 shows the average energy w and the drift velocity v for GaAs at 300 K due to an electric field of 10 kV/cm applied at t = 0 s. These curves are from a Monte Carlo solution. The behavior shows a substantial overshoot in velocity and energy in the first few ps. The response eventually settles to the steady-state characteristics. The overshoot occurs because the momentum relaxation time is lower than the energy relaxation time, leading to a rapid response in the momentum with little initial effect on the energy. It is the nonrandomizing nature of the polar-optical scattering that makes this BTE solution a large approximation for GaAs. Figure 3.10 shows the angular distribution in energy associated with the parallel and perpendicular velocity to the field. In its formulation, the BTE implicitly assumed that the distribution was more like what it is at 2.5 ps where it is quite well randomized. So, during the transient, it does not determine the solution accurately. These approximations can be circumvented quite explicitly with the Monte Carlo approach since all the transitional probability relationships can be explicitly included as one follows the response of individual carriers. 3.3 Boltzmann Transport Approach 125 Figure 3.9: Evolution of kinetic energy and velocity as a function of time following a step change of 10 kV/cm in electric field applied at t = 0 in GaAs. Figure 3.10: Energy associated with parallel and perpendicular components of velocity following application of an electric field of 10 kV/cm along the abscissa. Different time snapshots are shown. 126 3.4 3 Mathematical Treatments Monte Carlo Transport Approach The Monte Carlo approach is a probabilistic approach based on sampling of the parameter distributions of the semiconductor transport problem using a random distribution. Parameters of the problem are governed by probability distributions. Whether a carrier undergoes lattice scattering or defect scattering, and, extending that, the particular types of these scatterings depends on possible occurrences of these events as represented by their probability. Therefore, if a random distribution is used to sample these events in a transport problem and sufficient statistics are collected, one should obtain realistic distributions of parameters of interest. Examples of these parameters may be carrier distribution as a function of energy, momentum, and position in a sample (i.e., the function f of the BTE approach). In general, this function need not be a Maxwell–Boltzmann distribution or displaced Maxwell–Boltzmann distribution in energy and the Monte Carlo approach can determine what it is. Additionally, the significance of Monte Carlo techniques goes beyond this. Small-signal analysis as derived from the drift-diffusion equation (itself a simplification of the BTE) uses superposition in the linear differential equation. This is an additional approximation for both transient and large analog signal operating conditions. A representative solution to such conditions is quite unlikely using either of the previous approaches. Monte Carlo, as a statistical method, is a natural for obtaining solutions to such problems. As with any technique, inaccurate solutions can be obtained if the problem is described incompletely. Our discussion here is a general introduction of how problems are handled in the Monte Carlo approach.6 It should become clear that it is highly numerically intensive; requires extensive computation; a large accumulation of data on energy, momentum, space, and time; and, as in other approaches, a proper description of boundary conditions. The technique involves evaluation of the trajectories of a sufficient number of carriers inside the semiconductor to evaluate a statistically meaningful description of the transport. These trajectories occur under the influence of applied and built-in forces in the semiconductor, and due to scattering events; all of which can lead to a change in energy and momentum of the carrier. Examples of applied and built-in forces are those due to an applied or built-in electric field of a p–n junction, and examples of scattering events are the numerous mechanisms of defect and lattice scattering. The technique evaluates both the scattering event and the time between scattering events, a period during which the carrier moves ballistically. These events are accounted for stochastically according to the relative probability of their occurrence. Consider what this methodology means to the evaluation of the time between scattering events. If p(ϕ) is the probability density of the occurrence of a variable ϕ (e.g., energy of a carrier) and if p(η) is the probability density of 6 For an intuitive discussion of the application of Monte Carlo techniques to analyzing semiconductor problems, see A. D. Boardman, “Computer Simulation of Hot Electron Behavior in Semiconductors using Monte Carlo Methods,” in A. D. Boardman, Ed., Physics Programs: Applied Physics, John Wiley, Chichester (1980). 127 3.4 Monte Carlo Transport Approach the occurrence in a pseudo-random distribution (e.g., a uniform distribution), then Z ϕ Z η 0 0 0 0 p(ϕ )dϕ = p(η )dη . (3.89) 0 0 For a uniform distribution, this means that Z ϕ 0 0 η= p(ϕ )dϕ . (3.90) 0 Inversion of this equation gives a random value of ϕ as a function of the random distribution function η. As an example, consider scattering with a constant total scattering rate S = 1/τ . The probability of the scattering event occuring after time interval t, following a scattering event at t = 0, is the exponential function p(t) = S exp (−St), and hence, following integration, η = 1 − exp (−St) , (3.91) whose inversion gives the corresponding time between scattering as t=− 1 1 ln (1 − η) ≡ t = − ln (η) , S S (3.92) since η has a uniform distribution. Thus, physically, in the process of selection of time for uniform scattering rate, we calculate the cumulative probability function with respect to time, and then use a uniform random number generator to select the corresponding time. This calculation and mapping has to be performed for all the processes to be accounted for. These include further complications, e.g., angle of motion for the carrier following the scattering has to be included since it determines the new direction of the particle. The selection of this angle involves an additional procedure involving probability distribution. Determination of the time during which free flight occurs is actually a fairly difficult problem for the more general case. For a particle of wave vector k corresponding to the momentum p, the probability that a scattering occurs in the time interval dt at time t is p [k (t)] dt. Thus, the probability of no scattering in the time interval 0 to t following a scattering at t = 0 is Z t exp − p [k (τ )] dτ . (3.93) 0 Therefore, the probability that this particle, which has not suffered a scattering in the time interval 0 to t, will suffer a scattering during the time dt at time t is Z t P (t)dt = p [k(t)] exp − p [k (τ )] dτ dt. (3.94) 0 This is not straightforward in a general problem where p(ϕ) is not a constant. In such cases, the calculations are greatly simplified by introducing an additional scattering process, a virtual scattering process, that leaves the particle in the 128 3 Mathematical Treatments Figure 3.11: An example of a carrier motion and scattering as it drifts in an electric field (−z direction) in momentum (a) and real (b) space. same state that it was before but which makes p(ϕ) a constant and equal to its maximum value, thus allowing us to continue the procedure described. This fictitious process is referred to as “self-scattering.” Now that p(ϕ) is a constant, the uniform random number generation can be used, and a “self-scattering” event is treated to leave the particle state unchanged. To summarize, the procedure at its simplest consists of starting from a random position, allowing free flight (also called ballistic flight) of the carrier, until a scattering process is identified to occur by a Monte Carlo procedure. In addition to the energy, momentum determination requires an additional Monte Carlo procedure to evaluate the angle, and then the carrier can proceed in free flight again. Following several such scattering events the final carrier parameters lose their dependence on the initial conditions. For a steady-state homogenous problem, the behavior of the motion of the particle in this large scattering events limit would be representative of the behavior of the particle gas. This conclusion also follows from ergodicity. Let us clarify by considering the example shown in Figure 3.11. This example is for a two-dimensional system, and we study the motion of an electron in real space and k-space (or equivalently momentum space) as it undergoes scattering and drift in time in an electric field in the −z direction. Free flight is shown as a solid line and scattering as a dashed line. Corresponding to each scattering event, a change in momentum is shown via the dashed line in the k-space, and the particle moves again under the influence of the electric field in the −z direction. If this simulation was continued for many more scattering events and hence in time, the final z-position of the particle as a function of time would vary nearly linearly with time for constant effective mass, i.e., the velocity would be a constant. 129 3.4 Monte Carlo Transport Approach The equation of motion of this particle follows from our description of particle motion. The momentum of the particle is h̄k and its energy is h̄2 k 2 /2m∗ for the simple free particle. Under the influence of electric field E, the equation of motion of the particle is ∂ (h̄k) = −qE. (3.95) ∂t If its initial momentum corresponds to a wave vector ki , the momentum at an instant in time t during free flight corresponds to a wave vector k, where k(t) = ki − qE t. h̄ (3.96) Since the motion is by drift, momentum only changes in the direction of the electric field, i.e., in the z direction. For a transient problem, where one is interested in the behavior of a particle gas on a time scale during which too few scattering events occur, as well as for a spatially non-homogenous problem such as transport in the channel of a short gate-length FET or the base-collector space charge region of a bipolar transistor, many more particles have to be considered under the influence of the forces that exist in the channel or the base-collector space charge region in order to obtain meaningful results. The test of the latter is the standard deviation of the parameter of interest in order to determine its uncertainty. This test is usually accomplished by dividing the accumulated information into sufficiently large equal time intervals and determining the parameter of interest (e.g., the velocity). The average of this information is the mean of interest and its standard deviation is a measure of the uncertainty. Real semiconductor problems are usually of significantly higher complexity. Poisson’s equation, which relates the charge density and the displacement vector, should be satisfied together with the charged carrier contributions as they move in a finite sized sample. Additional complexity arises because of changing effective mass, numerous scattering processes, avalanche processes that create additional electrons and holes, momentum quantization in two-dimensional structures, the multiple bands and valleys of real band structures, and the significant deviation of these bands from parabolic approximation. For electrons in many compound semiconductors, e.g., at the least two valleys—the Γ and the L valley—should be considered for problems involving any significant heating of carriers. Quite often, X should be considered too, and neither the X nor the L valleys can be approximated as being parabolic for more than a few fractions of eV. One can make some adjustments by introducing the non-parabolicity factor α which relates the energy and momentum through E (1 + αE) = h̄2 k2 , 2m∗ (3.97) so that the energy E is " 1/2 # 1 h̄2 k2 E (k) = −1 + 1 + 4α , 2α 2m∗ (3.98) 130 3 Mathematical Treatments the velocity of the particle v (k) is v (k) = 1 ∂E h̄k = ∗ , h̄ ∂k m (1 + 2αE) (3.99) and the conductivity effective mass mc is mc = m∗ (1 + 2αE) . (3.100) These approximations do allow extension of the technique of using equations to describe some of the parameters of the problem. However, for small bandgap semiconductors which are both highly non-parabolic and have significant offequilibrium effects, this inaccuracy of analytic description becomes a major limitation. Also, quite often, problems of interest are related to heterostructures with alloy grading and hence position-dependent band structure. For such problems, information could be stored as a look-up table. Monte Carlo methods thus become both numerical and storage intensive. The boundary influences the behavior of a system. The boundary conditions, therefore, should ideally represent the true behavior of the boundary, and failing that should be selected in such a way that the final result of interest is intuitively independent of it. Thus, the initial position of the particle should be irrelevant to the final result of interest above, which was the velocity. This is an initial boundary value problem. Spatially, the device sizes and regions to be analyzed are limited, and the boundaries have to be suitably described. In a surface oriented device, carriers incident at the surface either get reflected or recombine. If it is a majority carrier device, then the second is irrelevant if the population of the minority carrier is low. It may be irrelevant for a minority carrier device if other effects in the system are larger. In both devices, however, careful consideration must be given to what happens at the surface to the carrier as it is reflected spatially. Electron surface mobility in silicon is nearly half of its bulk value at similar carrier densities. This lowering of mobility must arise due to the partial randomization of carrier momentum of particles incident at the surface. This effect may be included by considering the scattering at the surface as partially randomizing. In heterostructures, where crystallinity is maintained between semiconductors (e.g., Ga1−xAlx As/GaAs), there is a lack of surface states as well as non-planarity. These, if present, lead to potential perturbations and hence to scattering. Therefore, in a heterostructure system with low surface states and a planar interface, mobilities are maintained and true reflections occur. Thus, carriers, incident from GaAs into Ga1−xAlx As at the surface, only go through a sign reversal in the momentum normal to the surface if they go through a reflection. The carrier does not always have to reflect back. It may have the requisite momentum and energy to transfer into Ga1−x Alx As. The Monte Carlo procedure must check and allow for such an event to take place. Two boundaries of import that are often encountered are an ohmic contact and a metal–semiconductor rectifying contact. An ideal ohmic contact, unless it is intentionally a part of the intrinsic device devised to affect the operation of the 3.4 Monte Carlo Transport Approach 131 device, is meant to be only a means for providing carriers to the semiconductor without a voltage drop across it. Thus, a Monte Carlo procedure may simulate this process by trying to maintain the particle density at its equilibrium value at the contact in accord with Fermi–Dirac distribution. A lost carrier may thus be replaced by a carrier whose momentum is chosen randomly for a Fermi–Dirac distribution. A metal–semiconductor contact, a rectifying contact, is considerably more complex. Particles that do not have sufficient momentum or energy to cross into the metal get reflected, and, because of the non-planarity and interface states, may be thermalized. Carriers that have sufficient momentum and energy will traverse into the metal. Since for rectifying metal–semiconductor contacts the barrier for injection from the metal to the semiconductor is very large and scattering lengths very short, very few carriers traverse from the metal to the semiconductor, and we may ignore them in the procedure. This question is discussed in further detail in Chapter 4. Let us now consider areas where the complexities associated with the Monte Carlo technique are unavoidable if one is to obtain a reasoned understanding. In our discussion of devices we will look at this question in significantly more detail. Here, we discuss two examples where the utility of the technique becomes quite obvious. When carriers traverse a region where there is a significant gradient in the electric field, they undergo a velocity overshoot in parts of the region. Velocity overshoot is a term that implies that the local velocity v at a local field E becomes higher than what it would reach for a slowly varying field E of the same magnitude. A local off-equilibrium occurs. It arises because the carrier energy and the local electric field are no longer in equilibrium with each other. An example of this local equilibrium at high fields is the existence of velocity saturation. The mobility of carriers is a function of energy, as our earlier treatment shows. Because of the parallel between the energy and the electric field, the mobility can be written as a function of electric field. When the electric field becomes large, higher carrier energy results. Higher carrier energy causes larger amount of scattering, which reduces the mobility. Thus, velocity, a product of mobility and electric field with mobility varying inversely with field, becomes a constant. When a large gradient of electric field exists, the carrier does not immediately achieve the energy that corresponds to the local field if the field is rapidly varying. It actually has a lower energy and hence suffers less scattering, and yet it is accelerated by the high field. The carrier, therefore, is said to have a velocity overshoot. This large velocity occurs in spite of the fact that it has a lower energy. Another way of saying this same thing is that the relaxation rate for momentum is larger than that for energy. A second example is related to distributions that can be determined using the Monte Carlo approach. A very instructive problem in transport is that of transport across p–n junctions. The drift-diffusion theory incorporates a mobility, and a diffusion coefficient that is proportional to the mobility, both of which are a function of the local electric field. In constant mobility approximation, this electric field dependence is ignored, and a solution such as the triode equation of the field effect transistor is found. In a p–n junction and many other 132 3 Mathematical Treatments junctions, large built-in fields occur because of their built-in voltages. The local electric field is high. Should the mobility for such a problem be the mobility corresponding to the local electric field? We have noted above that mobility is a parameter that can be directly related to the energy of the particle. So, while the local electric field, due to built-in considerations, is large, is the energy of the particles also correspondingly large? It is not. Particles, e.g., holes and electrons in a p–n junction, diffuse against the local field. The field can not increase the energy of these particles as it does when the particle is accelerated by the field during drift. Note that the diffusion that occurs in this problem, as elsewhere, is due to scattering that favors the direction towards regions of lower carrier density. Drift, on the other hand, causes the particles to move away from the junction. Intuition suggests that thermal-equilibrium distributions should exist everywhere, i.e., the distribution function should be a Fermi–Dirac distribution, and since this is a non-degenerate case it simplifies to Maxwell–Boltzmann distribution. Now, if we apply a forward bias to the junction, the local electric field is perturbed. Electrons and holes in the process of carrying the current receive excess energy between scatterings from the acceleration in the local field. Can one predict the electron distribution, its energy, and, if it is a Maxwell– Boltzmann type distribution, its temperature; and would that tell us what mobility to employ? The Monte Carlo procedure is suitable for analyzing this problem since it can simulate all the necessary processes that lead to the transport. Figures 3.12 shows at thermal equilibrium and under forward bias, for a silicon p–n junction, the spatial position of the conduction and valence band edges and the distribution of carriers as a function of the kinetic energy. The average energy and the tail for the distribution for both holes and electrons in the region of quasi-neutrality still show thermal distribution corresponding to the 300 K lattice temperature. However, in the space charge region, electrons show higher average energies corresponding to a higher temperature, and extended tails corresponding to a higher temperature hot carrier tail. The distributions have been normalized to show a proper comparison of energy dependence. This heating occurred in spite of a decrease in the electric field in the junction. The distributions can be quite reasonably fitted with the exponential tail, so at least in this case, a displaced Maxwell–Boltzmann distribution (but with a changed temperature) is a good approximation to the behavior of the carriers. Since the carriers do have different temperatures, a different mobility can be argued to be necessary in the drift-diffusion approach. In this example, the electron temperature rises by approximately 15 K in the space charge region; the mobility should correspond to that energy. In reality, this mobility is smaller, but much larger than that corresponding to the high local electric field, which certainly would give erroneous results. Quite often, what helps in obtaining reasonably accurate results by the drift-diffusion approach is that errors in mobility and diffusion, which track each other, give rise to an opposing polarity of errors in the drift and diffusion currents, and hence the result is significantly more accurate. What this example does point out, however, is that applied and built-in electric fields must be treated differently. 3.4 Monte Carlo Transport Approach 133 Figure 3.12: Part (a) shows the band edges for a 2×1017 cm−3 doped silicon p–n junction under thermal equilibrium (solid lines) and a forward bias of 0.87 V (dashed lines) at 300 K. Part (b) shows the electron and hole distribution for the forward bias as a function of kinetic energy for a spatial position outside (dashed lines) and inside the space charge region (solid lines) of the p–n junction. 134 3 Mathematical Treatments It is also useful to consider this problem using the BTE approach.7 Consider a problem with a built-in field of Ebi due to impurity gradient. If f0 is the distribution function in thermal equilibrium corresponding to this condition, then from the BTE, qEbi .∇pf0 + v.∇r f0 = 0. (3.101) With a field Ebi + ∆E, the distribution function changes to f0 + ∆f, and the BTE gives qEbi .∇p f0 + v.∇r f0 + q∆E.∇p ∆f + v.∇r ∆f+ ∂(f0 + ∆f) qEbi .∇p ∆f + q∆E.∇p f0 + ∂t scatt = 0. (3.102) The last term represents the effect of scattering and is the cause of diffusion; the second to last term is negligible, being the product of two perturbations; and the first two terms have a vanishing sum according to the BTE at thermal equilibrium. Current conservation requires that Z ∇r . v∆fd3 p = 0. (3.103) We consider only the case when the electric field Ebi +∆E does not change with position, implying that ∇r ∆f does not change with position. Then, the BTE can be written as ∂ (f0 + ∆f) = −q∆E.∇p f0 . (3.104) qEbi .∇p∆f + ∂t scatt For a built-in field of magnitude E0 , this gives ∂ (f0 + ∆f) qE0 .∇p ∆f + = −q∆E.∇pf0 . ∂t scatt (3.105) To understand the difference between the effects of built-in versus applied fields, consider the case of the same semiconductor with constant doping and identical distribution function f0 at any point chosen in the previous situation. If a field of Eex = Ebi = E0 is applied to it by external means, then the change 0 in the distribution function ∆f satisfies 0 ∂ f + ∆f 0 0 qE0 .∇p∆f + = −qE0 .∇pf0 . (3.106) ∂t scatt If the transition probability is linear and independent of the distribution function (implying negligible carrier induced scattering effects and perturbations), then using S as the scattering rate, we obtain for the built-in and the 7 For detailed arguments on this subject see J. B. Gunn, “Transport of Electrons in a Strong Built-in Electric Field,” J. of Appl. Phys., 39, No. 10, p. 4602, 1968. 135 3.4 Monte Carlo Transport Approach applied field cases qE0 .∇p∆f + S∆f and 0 qE0 .∇p∆f + S∆f 0 = = −q∆E.∇pf0 −qE0 .∇pf0 . (3.107) For a change in electric field ∆E co-directional with E 0 , the distribution functions in the two cases are related through ∆f = 0 ∆E ∆f . E0 (3.108) For bias changes from thermal equilibrium for a non-homogenous semiconductor with a built-in field, the change in the distribution function is a product of a fraction equal to the relative perturbation of the field multiplied by what the distribution function change would have been had the built-in field been an externally applied field. The influence of fields in the case of a built-in field is small, and at thermal equilibrium there is no effect. Monte Carlo calculations confirm this, as follows from the distribution functions in Figure 3.12. Since the drift velocity is given by R vfdp , (3.109) hvi = R fdp we obtain in the presence of the perturbation ∆E velocities in the two cases, 0 vd and vd, that are related by the same ratios (this follows from the above integrals, see Problem 9), ∆E 0 vd = v . (3.110) E0 d So, the effective mobility is also scaled by this factor. This derivation made several approximations for simplifying our effort. In particular, the semiconductor was assumed to be non-degenerate and isotropic, and carrier induced perturbation of scattering was neglected. A Monte Carlo procedure can account for these in a straightforward manner. We had remarked about the particular utility of the Monte Carlo approach towards modelling of transient phenomena. We exemplify this by showing how the transient in the p–n junction takes place when the forward bias is applied. Figure 3.13 shows the turn-on transient of the junction. Note that upon application of the bias, a field is established in the quasi-neutral region. The drift field in the quasi-neutral region vanishes rapidly as the junction charges. The junction depletion region edge can only move as rapidly as the carriers can, which is limited by the maximum group velocity of the carriers. This figure serves to demonstrate that even a simple problem such as that of a p–n junction is, in detail, quite complicated, if we are interested in understanding phenomena that take place on time scales of a few scattering events to a few pico-seconds. The steady-state result from such a calculation would be quite similar to results derived from a quasi-static analysis using the drift-diffusion equation, except 136 3 Mathematical Treatments Figure 3.13: The changes in conduction and valence band edges of 2×1017 cm−3 doped silicon p–n junction when forward biased from thermal equilibrium (dashed lines) at 300 K. The band edges are shown at various instances in time. where overshoot occurs due to large gradients in electric fields. The transient results, if one is only interested in time scales by which time the fields in the quasi-neutral region have died down, will also be accurate. However, in any of the cases, very short times, of the order of few pico-seconds, or in situations where velocity overshoot dominates, erroneous results will occur in the drift-diffusion approach. We will discuss this further in the chapters on devices. Analytic formulations are appealing for two reasons: they allow a simple and rapid understanding of a problem, and they provide an appealing intuitive understanding of the problem. The drift-diffusion approach, derived from the BTE, is the most common analytical tool with these characteristics. It will be used extensively in the rest of the text, and in context we will also discuss its limitations. Here, we summarize some of its characteristics. 3.5 Drift-Diffusion Transport The current transport equation, sometimes called the drift-diffusion equation, can be derived from the BTE equations under several assumptions. This section, therefore, actually belongs with our discussion of the BTE; it has been separated for convenience and because it is going to be the principal approach in our analysis of devices. 137 3.5 Drift-Diffusion Transport The second moment of the BTE yielded an equation which we may write as q J 2q 3 ∂J = ∗ nF − + ∇r nkT, ∂t m hτ i 3m∗ 2 (3.111) for electrons and holes. Among the assumptions inherent in this derivation are all those related to the BTE, an isotropic and parabolic single band, relaxation time approximation, and the assumption that the energy of carriers is due to thermal contributions only (non-degeneracy and no hot carrier effects). The relaxation time, τp = hτ i, is related to the effective carrier mobility by µ= qτp . m∗ (3.112) For transport in an electric field E, this gives the transport equation as: τp ∂J = qµnE − J + µ∇r nkT. ∂t (3.113) The scattering time τp is significantly smaller than the time scales of interest. The perturbation term embodied in the left hand side of the equation is negligible for most of the situations of interest where the time dependent change of interest occurs over many scattering events. Assuming this, and the Einstein relationship, we obtain the current transport equation J = qµnE + qD∇r n, (3.114) where we now drop the subscript r since only spatial gradients will be considered. We derived this equation by considering the BTE for electrons; we may do the same for holes with their opposite charge. The subscripted result for electrons and holes of the drift-diffusion equations are and Jn = qnµn E + qDn ∇n Jp = qpµp E − qDp ∇p. (3.115) The major assumptions that allowed the derivation of the above are those related to relaxation time approximation, single parabolic band structure with homogenous collision time, non-degenerate material, constant temperature of lattice and carriers, several collision events and hence neglect of any off-equilibrium effects, and that the length scale for spatial variation of field, collision time, impurity concentrations, etc. are longer than the mean free path. We introduce quasi-Fermi levels, artificial energy and potential levels akin to the Fermi level used in thermal equilibrium, to define the electron and hole densities as ξn − Ei n = ni exp (βψ − βφn ) = ni exp (3.116) kT and p = ni exp (βφp − βψ) = ni exp Ei − ξp kT . (3.117) 138 3 Mathematical Treatments Here, β = q/kT , ψ is the potential of the intrinsic level, and φn is the potential of the electron quasi-Fermi level. φp is defined as the potential of the hole quasiFermi level. The reference for these can be arbitrary: the intrinsic level, the vacuum level, etc., at some point in the crystal. The last term in these equalities is written using energies.8 Hence, and Jn = Jp = −qnµn ∇φn = nµn ∇ξn qpµp ∇φp = −pµp ∇ξp . (3.118) We can also extend this equation phenomenologically for a material whose composition is slowly changing, i.e., a material with a position dependent band structure.9 Similar treatment implies the existence of an additional force on the carrier resulting from the varying affinity of the carrier. For a slowly varying composition, this may be incorporated in quite a straightforward manner. We can write the carrier concentration as a function of the quasi-Fermi level with the coordinate system chosen as in Figure 3.14. n = NC exp (βψ + βφC − βφn ) (3.119) where φC is the conduction band edge potential with respect to the vacuum level reference and NC is the effective density of states in the conduction band. Then, Jn = = = −qnµn ∇φn n 1 −qnµn ∇ ψ + φC − ln β NC 1 qnµn −∇ψ − ∇ φC + ln(NC ) + qDn ∇n, β (3.120) and similarly, 1 Jp = qpµp −∇ψ − ∇ φV − ln(NV ) − qDp ∇p. β (3.121) 8 Our convention is to write potentials and energies w.r.t. electrons. Potential is higher downwards while energy is higher upwards. The reader should carefully look at these conventions and their reference levels, here and in the rest of the text. The reference levels are changed depending on the problem being analyzed in order to ease the appearance of the mathematics. 9 Due to heavy doping effects the treatment of position dependent band structure is important in homostructure devices also. Early treatment, suitable for both heterostructures and homostructures, was related to this. See J. E. Sutherland and J. R. Hauser, “A Computer Analysis of Heterojunction and Graded Composition Solar Cells,” IEEE Trans. on Electron Devices, ED-24, p. 363, 1972; A. H. Marshak and K. M. Van Vliet, “Carrier Densities and Emitter Efficiency in Degenerate Materials with Position-Dependent Band Structure,” SolidState Electronics, 21, p. 429, 1978; M. S. Lundstrom and R. J. Schuelke, “Numerical Analysis of Heterostructure Semiconductor Devices,” IEEE Trans. on Electron Devices, ED-30, No. 9, p. 1151, Sep. 1983; and A. H. Marshak and C. M. Van Vliet, “Electrical Current and Carrier Density in Degenerate Materials with Non-Uniform Band Structure,” Proc. of IEEE, 72, No. 2, p. 148, 1984. 139 3.5 Drift-Diffusion Transport Figure 3.14: Choice of the reference coordinate system for calculations for an arbitrary slow grading. By defining and φCn = φV p = 1 ln(NC ) β 1 φV − ln(NV ), β φC + (3.122) we account for variations in electron/hole affinity, effective mass, etc. This term can also include degeneracy effects related to high doping by addition of a term of (kT /q) ln F1/2 (ηfn )/ exp (ηfn ) for n-type or a term of (kT /q) ln F1/2 (ηfp )/ exp (ηfp ) for p-type, the terms following directly from the differences in band occupation statistics in Fermi–Dirac and Maxwell–Boltzmann distribution functions. So, for degenerate conditions φCn and φV p 1 1 ln(NC ) + ln F1/2 (ηfn )/ exp (ηfn ) β β 1 1 = φV − ln(NV ) − ln F1/2 (ηfp )/ exp (ηfp ) . β β = φC + (3.123) From this, the current transport equation for slowly graded heterostructures is and Jn Jp = qnµn {−∇ψ − ∇φCn } + qDn ∇n = qpµp {−∇ψ − ∇φV p } − qDp ∇p, (3.124) 140 3 Mathematical Treatments which, along with Poisson’s equation and the current continuity equation, allows us to solve many interesting problems. Quite often, we actually ignore the ∇NC and the ∇NV terms of ∇φCn and ∇φV p because they tend to be small. 3.5.1 Quasi-Static Analysis To gain physical understanding of a device, we are initially interested in the behavior of the device and its response in near-static conditions. We are interested in how the device behaves given a certain bias applied at the device terminals. What we want to know is how the current, e.g., in the device changes if we change the bias of the device under very slowly varying conditions, so that frequency-dependent effects per se are not important. This requires us to find the quasi-static solution to the problem, the simplest and the most popular example of device analysis. Quasi-static solutions can be found by all the approaches and their approximations that we have described. A time-independent Monte Carlo solution, or results from the static BTE equation, or its approximation the drift-diffusion equation, will all give a quasi-static solution. In the p–n junction problem that we discussed, the carrier distributions were under quasi-static conditions. We assumed steady-state (i.e., the device response had completely settled) and no further time dependence in the applied bias. The carrier distributions, etc., during the time the switching occurred could be considerably different than during the quasi-static condition, as it would appear from Figure 3.13 since the device has large time-dependent displacement and particle current effects. All the techniques that we have discussed can also give transient, small-signal, and quasi-static solutions since many of the time-dependent phenomena are incorporated in them. Often, the quasi-static solution is valid up to quite high frequencies. This allows simple predictive modelling to be applied in computer aided design of circuits. However, for both very high frequency and high speed, quite often, this solution is not sufficient. We will discuss the differences, in the context of devices, by finding the quasi-static solution as well as the small-signal frequency dependent solution within the limitations of the techniques used. 3.5.2 Quasi-Neutrality We now apply the drift-diffusion equation, derived above, to establish some procedures that will be used repeatedly in the rest of the book. This also gives us an opportunity to describe some of the assumptions and conditions under which some of the analysis becomes invalid. First, consider the question of when a semiconductor should be considered space charge “neutral” or quasi-neutral. In the non-uniformly doped semiconductor shown in Figure 3.15, carriers separate and generate an electric field. At thermal equilibrium, one may derive this field using the current continuity equation as E=− kT ∇n kT ∇p = . q n q p (3.125) 141 3.5 Drift-Diffusion Transport Figure 3.15: Non-uniformly doped semiconductor (a) and associated band bending (b). (b) also shows the electrostatic potential as a function of position. This implies the existence of a space charge given by ρ = s ∇.E. (3.126) The question we wish to answer is when we should include the effect of this space charge. A semiconductor is quasi-neutral, and the space charge effect can be ignored when the space charge density is small compared to dopants placed in the material, i.e., ρ q |ND − NA | . (3.127) Consider a compositionally homogenous semiconductor. Employing the Maxwell– Boltzmann approximation, dψ kT 1 dn = −E = , dz q n dz and hence ρ d2 ψ kT − = = s dz 2 q " 1 − 2 n dn dz 2 (3.128) # 1 d2 n + . n dz 2 For a quasi-neutral n-type material, n ≈ ND , and hence " # 2 s kT 1 dN 1 d2 n ρ≈− − 2 + . q N dz N dz 2 The condition for quasi-neutrality, then, is 2 s kT 1 dN 1 d2 n + − qN, q N 2 dz N dz 2 (3.129) (3.130) (3.131) 142 3 Mathematical Treatments Figure 3.16: Electron concentration as a function of position resulting from the placement of planes of doping varying in sheet density from 1 × 1011 cm−2 to 3.3 × 1012 cm−2 in lightly doped GaAs. i.e., #−1 " 1 dN 2 1 d2 n s kT 2 = λD − 2 + . N q2 N dz N dz 2 (3.132) The parameter λD , the extrinsic Debye length, is a characteristic length for space charge screening. The mobile charge screens the disturbance created by the fixed charge over the Debye length scale. An interesting example of this is shown in Figure 3.16 which shows the movement of mobile charge resulting from the placement of a plane of doping in the semiconductor. The characteristic length of the electron tail is approximately the Debye length. The figure points out the severe consequences of rapid change in doping. So long as the rate of change in doping is slow enough on the Debye length scale, the material can be considered quasi-neutral. Debye lengths for various dopings in GaAs are summarized in Table 3.1. A rapid change in doping can break down the condition of charge neutrality in a semiconductor, and associated space charge effects must be considered. Only when the Debye length scale is larger than the length scale of doping change, as described in Equation 3.132, should one consider the material charge neutral. A lower doping makes the Debye length large, and hence maintaining charge neutrality easier. Likewise, high doping with a high rate of change in it has the opposite effect. An interesting aside is that exponential profiles are always quasi-neutral; for N (z) = N0 exp (−z/λ) 3.5 Drift-Diffusion Transport 143 Table 3.1: Debye lengths in GaAs at 300 K. Doping Debye Length cm−3 cm Intrinsic 2.3 1 × 1015 1.35 × 10−4 1 × 1016 0.43 × 10−4 1 × 1017 0.14 × 10−4 1 × 1018 0.04 × 10−4 because 1 dN 2 1 d2 n 1 N02 1 N0 + = − + = 0. − 2 2 2 2 N dz N dz N0 λ N0 λ2 (3.133) We can also derive the condition for a varying composition structure. Intuitively, a rapid rate of change in composition should lead to breakdown of quasi-neutrality. An abrupt interface, e.g., should have a large interface charge and a significant accumulation or depletion of charge at it. On the other hand, a linearly varying φCn should leave the material quasi-neutral, with the only effect being that of a quasi-electric field. Application of the same approach of compositionally homogenous material to this compositionally heterogeneous case leads to the following inequality for maintaining quasi-neutrality (see Problem 10): #−1 " 1 dN 2 1 d2 n q 2 d2 φCn 2 λD − 2 + + . (3.134) N dz N dz 2 kT dz 2 As expected, a linearly varying φCn , while satisfying the homogenous case conditions, leads to quasi-neutrality. The effect here is the same as an exponentially changing doping. An interesting aside is that for any condition under which a compositionally homogenous material is not quasi-neutral, there exists, theoretically, a specific compositional profile where it would be quasi-neutral in a compositionally heterogeneous material. 3.5.3 High Frequency Small-Signal Analysis While a detailed understanding of the quasi-static behavior of a device is extremely useful, both in understanding the specifics of the functioning of the device and in its correlation and verification using practical and easier quasi-static measurements, it is not, and can not be, a complete predictor of the behavior of the devices at high frequencies. High frequencies bring with them dispersive effects. The transport and storage of carriers is affected by the frequency more strongly than is predicted by quasi-static modelling, and the signal attenuates more strongly due to losses associated with frequency-dependent phase 144 3 Mathematical Treatments Figure 3.17: A schematic distributed transmission-line representation for modelling the time-varying dependence of channel control by the gate. (a) shows the effect in a MESFET and (b) in an HFET. and amplitude effects. A reason for this is that rapid changes in signal, associated with high frequencies or fast transients, cause a large time-dependent displacement current. The effect of this is only partly included in quasi-static models where capacitors are included to model charge modulation and storage effects. Current transport is an aggregate of particle current and displacement current. Thus, current response at high frequencies is different from that under quasi-static conditions and hence the device behavior is too. Therefore, for high frequency and high speed devices, in order to understand their behavior at those frequencies, we need to model the physics of the devices at those frequencies. Specific examples, pertaining to both the field effect transistor and the bipolar transistor, clarify this importance of modelling at the frequency conditions of interest. Consider the generic field effect transistor first. When a fast timevarying signal is applied at the gate of the transistor, as the control region underneath the gate also varies, the time-varying channel current responds to these changes. In the case of a MESFET or a junction FET (JFET), the control mechanism is the movement of the edge of the gate depletion region which occurs together with the charging and discharging at region’s edge; in the case of insulating gate field effect transistors (examples: MOSFET, MISFET, SISFET), this is build-up or build-down of the charge in the channel. This charging and discharging occurs through both the displacement and particle current flowing in the channel, and mostly or entirely displacement current flowing in the space charge or the insulator region. The conductance in the channel region is dependent both on time and position while the control region responds. The response of the control region is, therefore, not identical at the different positions along the gate, and a simple description of this phenomenon would be to model it as a distributed transmission line of conductances and capacitances as shown in Figure 3.17. The response, in amplitude and phase, of such distributed transmission lines is frequency-dependent. In a bipolar transistor, displacement currents are particularly important in the base-collector space charge regions. For a moving charge packet in a depleted region, the termination of the electric field (an opposite polarity charge) associated with the charge moves from one edge of the depleted transit region 3.5 Drift-Diffusion Transport 145 Figure 3.18: Schematic of the response in minority carrier density in the base of a n–p–n bipolar transistor with a signal of cycle time equal to twice the base transit time. The dashed lines represent the electron concentration distribution under quasi-static conditions. to the other. The transit of the charge causes a displacement current since the electric field changes during transit of this charge. Quasi-static arguments would ignore this current, but, at high frequencies, its effect is substantial, and the effect of transport delay can not be ignored. Simplistically thinking, one would expect the effect of this carrier transit to correspond to a time delay equal to the time it takes to transit this space charge region. The delay in current response, however, does not correspond to the transit time, and about half its value is a better approximation if the carriers transit at a constant velocity throughout this space charge region. We will discuss this further in our treatment of bipolar transistors; it is a consequence of both displacement and particle current being present. We generally ignore the amount of time it takes for a signal to cause a change in the carrier concentration at the base-emitter junction. It is taken to be instantaneous. Similar to the delay in the base-collector space charge region, it should be incorporated if it becomes a significant factor in the operation of the high frequency device. Fortunately, for useful bias conditions of the bipolar transistor, the time it takes to store the charge in the base-emitter space charge region, which occurs at the same time as this transit of carriers, is significantly larger and hence we may ignore the latter. A third example in the bipolar transistor that clarifies the frequency dispersion is shown in Figure 3.18. Assume that the particle density at the base-emitter junction instantaneously responds to an applied signal, i.e., transit 146 3 Mathematical Treatments through base-emitter space charge region and the storage in the space charge region is not limiting. If, now, one applies a high frequency signal of a cycletime twice the amount of time it takes for the carrier to transit the quasi-neutral base region (no displacement current here since it is quasi-neutral), how would the particle density respond? The input signal goes through half a cycle in the amount of time it takes for carriers injected at the base-emitter junction to reach the base-collector junction. So, carriers reaching the base-collector junction are out of phase with the signal at the injecting junction. Quasi-static analysis assumes that they are in phase. Dissipation occurs as a result of this phase lag, and is important to the high frequency operation, and especially operation at a fraction of the ultimate figures of merit that are of interest to us. So, a small-signal analysis attempts to incorporate such effects. For such problems, within approximations of the drift-diffusion approach, this may be done by taking the current continuity equation and incorporating the frequencydependent terms in the equation. The current continuity equation is a linear differential equation, and hence, for small-signals, linear superposition techniques can be applied. For the problem, this would mean that as a function of position z, time t, and a sinusoidal signal of frequency ω (implicitly understood as the real part a complex signal varying as exp(jωt) for the sake of simplicity) applied, the current densities and voltages may be written as ˜ ω, t) = J(z) + J(z, ˆ ω) exp (jωt) , J(z, ω, t) = J(z) + J(z, (3.135) V (z, ω, t) = V (z) + Ṽ (z, ω, t) = V (z) + V̂ (z, ω) exp (jωt) . (3.136) and The overline indicates the quasi-static current; the hat indicates the phasor of the complex signal. The sinusoidal signal is the real part of the complex signal. Electron densities, hole densities, and other parameters vary with frequency in a similar fashion, because of the superposition principle. The one-dimensional current density, and current continuity equations, with these substitutions, are J n (z) + Jˆn (z, ω) exp (jωt) = −q [n(z) + n̂(z, ω) exp (jωt)] µn × ∂ ∂ V (z) + V̂ (z, ω) exp (jωt) + ∂z ∂z ∂ ∂ qDn n(z) + n̂(z, ω) exp (jωt) , ∂z ∂z (3.137) J p (z) + Jˆp (z, ω) exp (jωt) = −q [p(z) + p̂(z, ω) exp (jωt)] µp × ∂ ∂ V (z) + V̂ (z, ω) exp (jωt) − ∂z ∂z ∂ ∂ p(z) + p̂(z, ω) exp (jωt) , qDp ∂z ∂z (3.138) 147 3.5 Drift-Diffusion Transport ∂ [n(z) + n̂(z, ω) exp (jωt)] = ∂t G n + Ĝn exp (jωt) − Rn − R̂n exp (jωt) + i 1 ∂ h J n (z) + Jˆn (z, ω) exp (jωt) , q ∂z (3.139) and ∂ [p(z) + p̂(z, ω) exp (jωt)] = ∂t G p + Ĝp exp (jωt) − Rp − R̂p exp (jωt) − i 1 ∂ h J p (z) + Jˆp (z, ω) exp (jωt) . q ∂z (3.140) These set of equations can be rewritten separately for the time independent and and time-dependent part (varying with exp (jωt), i.e., only the fundamental terms) as ∂ ∂ J n (z) = −qn(z)µn V (z) + qDn n(z), (3.141) ∂z ∂z ∂ ∂ J p (z) = −qp(z)µp V (z) − qDp p(z), (3.142) ∂z ∂z 1 ∂ J n (z), (3.143) 0 = G n − Rn + q ∂z and 0 = G p − Rp − 1 ∂ J p (z), q ∂z for the steady-state terms, and ∂ ∂ ∂ ˆ Jn (z, ω) = −q n(z) V̂ (z, ω) + n̂(z, ω) V (z) + qDn n̂(z, ω), ∂z ∂z ∂z ∂ ∂ ∂ Jˆp (z, ω) = −q p(z) V̂ (z, ω) + p̂(z, ω) V (z) − qDp p̂(z, ω), ∂z ∂z ∂z and (3.144) (3.145) (3.146) ∂ 1 ∂ ˆ n̂(z, ω) = Ĝn − R̂n + Jn (z, ω), ∂t q ∂z (3.147) ∂ 1 ∂ ˆ p̂(z, ω) = Ĝp − R̂p − Jp (z, ω), ∂t q ∂z (3.148) for the time-varying terms. 148 3 Mathematical Treatments Network parameters can be determined from these, the most common one in theoretical analysis being being y-parameters, because we directly determine current as a function of voltage. From experiments, S-parameters are more common since they are directly available from the apparatus, while equivalent circuits are best described using h-parameters because of the high output conductance and hence current source nature of both field effect transistors and bipolar transistors. Network parameters are treated separately in the Appendix A. These network parameters serve several useful purposes. Microwave circuit design and small-signal equivalent circuit modelling can be conveniently performed using them. Device stability can be evaluated because stability factors (e.g., the Linvill stability factor) can be easily determined. Similarly, the ultimate limits of the device both in gain (such as the unilateral gain or the maximum available gain) and frequency figures of merit (such as short-circuit unity current gain frequency and maximum frequency of oscillation) can be directly determined. The network parameters, thus, serve several useful purposes. This analysis is still within the limits of drift-diffusion approximation. It does not include the off-equilibrium effects that occur at small dimensions and which allow achievement of the next level of accuracy. In the case of our FET example, the movement of the depletion region occurs with velocities not limited by the steady-state mobility-field relationship that is incorporated in the transport equation, but at higher velocities, because significant off-equilibrium effects occur due to the gradient in the electric field at the edge of the space charge region. This was shown in the example of p-n junction in our discussion of Monte Carlo approach. Transient and high frequency large signal conditions are two other places where the quasi-static modelling is inadequate. We will discuss transient operation as part of the treatment on devices; large signal operation will not be covered in the text. 3.6 Boundary Conditions Device analysis requires us to describe the operation in a chosen part. This part defines the section that we may be capable of describing mathematically, and that is of interest to us. However, we must be able to describe the couplings of this section at all its boundaries. These couplings, the boundary conditions, must be physically representative and must not cause a change in the result from what it would have been in the absence of this sectioning. For example, in a bipolar transistor, we may wish to describe the behavior in the semiconductor region through some representative equations. But the coupling of the current supplied from the power supplies, and carried in the device by the charged carriers, electrons and holes, requires us to suitably interface the two in the form of some mathematical model. And this holds true for voltages, etc., too. We may wish to describe the transport as a one-dimensional simplification in the quasi-neutral part of a base, in which case we must be able to mathematically model the two ends, the base-emitter junction and the base-collector junction, 3.6 Boundary Conditions 149 Figure 3.19: Band edges and the quasi-Fermi levels of a symmetrically doped n–p junction of GaAs in forward bias. and these must account for the behavior of the emitter and the collector. Thus, boundary conditions, if chosen properly, allow us to simplify the analysis of a problem and give us a better physical insight by isolating the problem. In this section, we will discuss some of the commonly employed boundary conditions in device analysis by a variety of techniques. As a consequence of the discussion, we should also get insight into the simplifications and the underlying behavior that leads to the choice of these boundary conditions. We discuss the more commonly used boundary conditions for drift-diffusion analysis first.10 Most devices of interest to us incorporate p–n junctions: in bipolar transistors for injection and collection, and in n-channel field effect transistors for isolation of the device from the substrate. Many of these devices also incorporate ohmic contacts, metal–semiconductor contacts, or heterojunctions to contact and modulate the carriers. Our discussion is related to these device structures, and we will create mathematical models that can be easily introduced for drift-diffusion analysis first. 3.6.1 Shockley Boundary Conditions Let us first look at the common approximation of the constant quasi-Fermi level in the space charge region of a homogenous p–n junction (see Figure 3.19). Since the current carried by each carrier can be expressed in terms of the quasi-Fermi 10 For an extended discussion of these, see R. M. Warner and B. L. Grung, Transistors: Fundamentals for the Integrated-Circuit Engineer, John Wiley, N.Y. (1983). 150 3 Mathematical Treatments levels for the carrier, we can derive the quasi-Fermi level change from the edge of the depletion region of p and n sides as Z wn ξn ξn Jn exp (Ei /kT ) exp − exp = dz, (3.149) kT z=wn kT z=−wp qni kT µn −wp for electrons. Hence the change in the electron quasi-Fermi level is ∆ξn = = ξn |z=wn − ξn |z=−wp Z wp h i 1 kT ln 1 + |Jn | exp Ei − ξn |z=−wp /kT . qni kT µn −wn (3.150) The change in the quasi-Fermi level is logarithmically related to the integral; a large current flow may cause a significant drop in the quasi-Fermi levels. To check the validity, let us assume that a significant current density is flowing through the structure to cause the variation in quasi-Fermi level position. Since a large current flows, a near flat band condition occurs. The width of the space charge region, under these conditions, is small—certainly less than 1000 Å for typical junction conditions involving current densities of 104 A.cm−2 . Therefore, we may calculate the approximate magnitude of this integral; for GaAs, an approximate magnitude of this is 10−2 eV assuming a mobility of 4000 cm2 .V−1 .s−1 . Thus, our assumption of flat quasi-Fermi level is well justified for this example. Also, given this, the amount of current across this junction is determined by the amount of current being extracted from it by the other regions of the device, e.g., the base of the bipolar or the base of the p–n junction (the quasi-neutral region). This does not always have to be so. If the mobility of the material is extremely poor, or a very high current density is attempted to be extracted, or the temperature is low, the quasi-Fermi levels may change by substantially more than the thermal voltage, since it directly affects the integral. Devices based on p–n junctions, operating with small changes in the quasi-Fermi levels in any region, are said to be operating with low level injection in those regions. Analysis of transport in the quasi-neutral regions can be simplified in driftdiffusion analysis because of the above. In a p–n junction, under these low level injection conditions, where the quasi-Fermi level is flat, the carrier concentrations on the n-side and p-side are related through the difference in the electrostatic potential. Under thermal equilibrium, this electrostatic potential is the junction built-in voltage ψj0 , the contact potential of the junction. This is given by: ND NA kT nn0 pp0 kT ln = ln , (3.151) ψj0 = q ni 2 q ni 2 where ND and NA are the donor and acceptor densities, and nn0 and pp0 are the majority carrier densities in the n-side and p-side at thermal equilibrium. From the law of mass action, the minority carrier densities in either regions, pn0 151 3.6 Boundary Conditions and np0 , also satisfy pn0 nn0 = np0 pp0 = ni 2 , (3.152) for homogenous junctions. With application of a bias of V , the electrostatic potential change at the junction is ∆ψ = ψj0 − V , so that ψj0 − V np (−wp ) = nn0 exp −q kT ψj0 − V . (3.153) and pn (wn ) = pp0 exp −q kT Under bias, the majority and minority carrier concentrations both change. In low level injection, the percent change in majority carrier concentration is insignificant compared to that in minority carrier concentration. Consequently electron and hole majority carrier population change can be ignored and Equation 3.153 still remains valid. This allows us to write the equations qV np (−wp ) = np0 exp kT qV and pn (wn ) = pn0 exp . (3.154) kT These equations are commonly referred to as the law of the junction or Shockley boundary conditions. In the rest of the book, we will refer to these as Shockley boundary conditions. The use of the term “law of the junction” implies a broad validity; these equations are valid for only low level injection conditions in homogenous junctions. In compound semiconductor devices, quite often, we deal with heterogeneous junctions, where this relationship is quite often inappropriate. Shockley boundary conditions describe an exponential relationship between carrier densities at both edges of the depletion region. This exponential factor is sometimes referred to as the Boltzmann factor; its derivation depends on low level injection and Boltzmann approximation being valid. In the derivation of the Shockley boundary conditions, we made two principal assumptions. The first is that we extract a very insignificant fraction of the current that the junction is capable of supplying, i.e., the current is much smaller than either the diffusion or drift current carried by either of the carriers at the junction. We may estimate the latter. If the junction has a doping density of 1 × 1018 cm−3 and the carriers moved at a velocity of 107 cm.s−1 , then the maximum current density can be nearly 1.6 × 106 A.cm−2 . The second assumption in the derivation was related to there being an insignificant change in the majority carrier concentration at either side of the junction. 3.6.2 Fletcher Boundary Conditions Quite often, the latter assumption is the first one to breakdown under bias in actual devices, and it happens in the lower doped side of the junction, e.g., in 152 3 Mathematical Treatments the base of a p–n junction or a bipolar transistor. Under these conditions, the quasi-Fermi level is still be flat within the junction region, but the majority carrier density in one of the regions is affected by the minority carrier injection. Boundary conditions formulated by Fletcher and Misawa are more useful under these conditions. We consider the Fletcher boundary conditions first. We have derived the relationship between the carrier concentrations at the edges of the depletion region (Equation 3.153). Rewriting these equations using Vj for the voltage across the junction, qψj0 qVj p(wn ) = p(−wp ) exp − exp kT kT qψj0 qVj and n(−wp ) = n(wn ) exp − exp . (3.155) kT kT Since qψj0 exp − kT = pn0 np0 = pp0 nn0 from the thermal equilibrium, we may rewrite these as pn0 qVj p(wn ) = p(−wp ) exp , pp0 kT np0 qVj and n(−wp ) = n(wn ) exp . nn0 kT (3.156) (3.157) The increase in majority carrier concentration at the edge of the depletion region, which we ignored in the Shockley boundary condition, occurs in order to maintain charge neutrality. Its increase therefore is equal to the increase in the minority carrier charge at the edge of the depletion region, i.e., and p(−wp ) − pp0 n(wn ) − nn0 = = n(−wp ) − np0 , n(wn ) − nn0 . (3.158) These four equations describe the carrier concentrations at the edge of the depletion region under high injection conditions but still assume flat quasi-Fermi levels in the junction region (we ascribe the potential Vj to the change in the junction potential). By elimination, they can be written in a more appropriate form relating to the thermal equilibrium concentrations (see Problem 11) as p(wn ) = −1 2qVj × kT qVj (pp0 − np0 ) nn0 pn0 exp + kT 2qVj (nn0 − pn0 ) np0 pn0 exp kT nn0 pp0 − np0 pn0 exp 153 3.6 Boundary Conditions n(−wp ) = p(−wp ) = n(wn ) = −1 2qVj × nn0 pp0 − np0 pn0 exp kT qVj (nn0 − pn0 ) np0 pp0 exp + kT 2qVj (pp0 − np0 ) np0 pn0 exp kT −1 2qVj × nn0 pp0 − np0 pn0 exp kT qVj (pp0 − np0 ) nn0 pp0 + (nn0 − pn0 ) np0 pp0 exp kT −1 2qVj × nn0 pp0 − np0 pn0 exp kT qVj (nn0 − pn0 ) nn0 pp0 + (pp0 − np0 ) nn0 pn0 exp . kT (3.159) These are the Fletcher boundary conditions. They relate the electrostatic potential change at the junction Vj , assuming no change in the quasi-Fermi levels in the junction depletion region, with the carrier densities at the edge of the depletion region. In the above relationships, changes in the quasi-Fermi levels may take place in the rest of the quasi-neutral region; their effect is included. 3.6.3 Misawa Boundary Conditions Figure 3.20 shows the quasi-Fermi levels and the electrostatic potential at a p–n diode under high level injection conditions. Any applied bias at the ohmic contact can drop at the ohmic contacts, in the quasi-neutral regions, and at the junctions. The potential Vj used in the Fletcher boundary condition equations above is the part of the applied bias voltage that dropped at the junction. We considered only the junction part in our analysis, and need to relate it to the electrostatic potential changes across the device itself. As Figure 3.20 shows, this involves knowing the changes that occur at the ohmic contacts and in the quasi-neutral regions. We can find the other potential drops as a continuation of our analysis, and another reason for doing this is that the Fletcher boundary conditions are also somewhat cumbersome in appearance. A simpler form results if we write these as products of carrier densities, and as functions of the quasiFermi level splitting. This leads to a form known as the Misawa boundary conditions. As an extension of the discussion of Figure 3.20 consider the quasi-Fermi level splitting and voltage drops across the junction. Excess potential drop occurs in both the n-doped and the p-doped side. Of the applied terminal voltage V, only part of it (Vj ) drops across the junction, and the rest of it drops across in the quasi-neutral regions. The quasi-Fermi level splitting at the junction is less than 154 3 Mathematical Treatments Figure 3.20: Band edges and the quasi-Fermi levels at a GaAs n–p junction in high level injection. the applied voltage. The relationship in the voltage across the junction and the quasi-Fermi level splitting, again assuming Maxwell–Boltzmann relationship, is kT p(−wp ) kT n(wn ) Vj = φp − φn + ln + ln . (3.160) q pp0 q nn0 This relationship follows from the definition of an ohmic contact as a junction where the quasi-Fermi levels merge and the carrier concentrations are equal to their thermal equilibrium values. Misawa conditions can then be derived, and these state (see Problem 12) φp − φn [n(−wp ) + NA ] n(−wp ) = pp0 np0 exp q kT φp − φn . (3.161) and p(wn ) [p(wn ) + ND ] = pn0 nn0 exp q kT The significance of the Misawa boundary conditions is in their simplicity. They are a restatement of the Fletcher boundary conditions, having been derived from them together with the charge neutrality equations. The approximations made in deriving Fletcher boundary conditions are also the approximations for Misawa boundary conditions. The equations can also be recast in another form in terms of only the carrier concentrations. The product of the carrier concentrations at the edges of the depletion region can be written from above using the charge neutrality conditions 155 3.6 Boundary Conditions as (see Problem 13) n(−wp )p(−wp ) = and 3.6.4 n(wn )p(wn ) = φn − φp pp0 np0 exp q kT φn − φp . pn0 nn0 exp q kT (3.162) Dirichlet Boundary Conditions We stated earlier that we may model the ohmic contact as a junction where the carrier concentrations are equal to their values at the thermal equilibrium. This has the physical meaning that the surface recombination velocity at the contact is so large that any excess carrier concentration disappears due to recombination. In reality, of course, ohmic contacts may have smaller recombination velocities. It is also possible to have a method of ohmic contact formation that allows efficient ohmic flow of carriers of only one type as in the graded bandgap contacts. Ga1−xInx As (n-type) and Ga1−xSbx As (p-type) are two examples of such contacts to n-type and p-type GaAs, and we will discuss these examples in Chapter 4. The former has a barrier to hole flow and the latter a barrier to electron flow. So, ohmic contacts may be based on different principles, but they serve one purpose: efficient supply and gathering of carriers. A good ohmic contact provides any requisite amount of carriers with negligible voltage drop across it, so as to not limit the device operation. The most common types of ohmic contacts are based on the use of heavy doping at an interface between a metal and a semiconductor with tunneling as the physical basis for ohmicity. Most allow one of the carrier types to tunnel. Near the surface region, carrier concentrations are determined by the characteristics of this flow which we may embody in the surface recombination velocity S of the contact. For a minority carrier in p-type material, the current is Jn = qS(n − n0 ). (3.163) For a p–n junction problem, this will now have to be solved self-consistently with the the other transport parameters (see Problem 29 of Chapter 4). If the surface recombination were infinite in the above, the carrier concentration would be its thermal equilibrium value and the contact would be ohmic for the minority carrier. If it is low, it may represent an emission velocity for minority carrier into the metal, which may, for some problems, be an adequate representation for metal–semiconductor contact. These various conditions at interfaces bring out some common features employed in drift-diffusion modelling in accord with the behavior of these interfaces. Mathematically, these features can be represented in the form of an identity on the electrostatic potential or the carrier concentration, and is referred to as a Dirichlet boundary condition. As an example, consider the ohmic contact. There could actually be excess immobile charge qN at the interface. The behavior of the parameters would 156 3 Mathematical Treatments follow the following mathematical equalities: ψ − ψj0 − V = 0 (3.164) for the electrostatic potential in a voltage controlled contact, and Z J.dA − I = 0 (3.165) for current. Here, dA is the vector normal to the elemental area with the magnitude of the elemental area. At thermal equilibrium, the carrier densities can be found by using the law of mass action and the equation for charge neutrality. Let the excess immobile charge at the interface be qN . The carrier density equations at the contact are: and np = n−p = ni 2 N. (3.166) The last two equations for carrier densities at the contact may also be written as p 1 n = N + N 2 + 4ni 2 2 p 1 and p = (3.167) −N + N 2 + 4ni 2 . 2 These constitute the Dirichlet boundary conditions for ohmic contacts. Similar boundary conditions may also be written for rectifying metal–semiconductor contacts, although many of the diverse behaviors of various metal–semiconductor contacts can not be written as simply. If the barrier height for injection from the metal to the semiconductor is φB , the contact potential is ψj0 , the surface recombination velocity for the contact is Sn and Sp for electrons and holes, then the Dirichlet boundary conditions can be derived as follows in a somewhat simplified form. The potential follows the relationship ψ − ψj0 + φB − V = 0. (3.168) Using the definition of recombination velocity and the charge relationships, we obtain the current and carrier densities are p 1 2 2 Jn = qSn n − N + N + 4ni 2 p 1 2 2 and Jp = qSp p − −N + N + 4ni . (3.169) 2 These equations constitute one form of Dirichlet boundary conditions for a metal and semiconductor interface with surface recombination velocities of Sn and Sp . 3.7. GENERATION AND RECOMBINATION 3.6.5 157 Neumann Boundary Conditions Besides ohmic and rectifying interfaces, boundaries between semiconductors and insulators are also encountered in practice. No or negligible current flows through the insulators. Gauss’s law requires that for the electric fields normal to the interface E n in the semiconductor and in the insulator, s E n |sem. − insE n |ins. = Qsurf , (3.170) where Qsurf is the interface charge density. If the insulator can be assumed to be infinitely thick, the field in the insulator can be ignored and one has s E n |sem. = Qsurf . (3.171) If one further assumes that the surface is charge-free, then E n |sem. = 0, (3.172) which is often referred to as the Neumann boundary condition. In compound semiconductors, there is significant surface state density and hence quite often a significant surface charge. The Neumann boundary condition is rarely valid. Fermi level pinning at the surface, which results from this surface charge, may be incorporated in two ways. We may make the ad hoc assumption that the surface potential is pinned due to this Fermi level pinning; this is akin to an electrostatic potential Dirichlet boundary condition. Alternately, we may consider a large surface state density of donor and acceptor traps that do not allow Fermi level excursion because of charge imbalance. In this case we may use charge neutrality including these interface charges, as well as Gauss’s law at the interface. 3.7 Generation and Recombination In our discussion of the BTE, we emphasized the scattering events that lead to carriers changing momentum and energy within the conduction bands or the valence bands. In our derivation of the drift-diffusion equations from the BTE, processes in between the conduction bands and the valence bands, described as generation and recombination processes since they involved creation or annihilation of electron–hole pairs, were introduced as another form of scattering event. Such interactions between carriers of opposite types are particularly important in compound semiconductors because most of them are direct bandgap semiconductors. Additional interactions between electrons and holes through levels within the bandgap, due to traps, are also important in compound semiconductors. So, several forms of excitation processes can result in either the recombination of electron and hole pairs or their generation. Radiative recombination, usually involving band to band transitions with the energy released as photons, is the basis of light-emitting diodes and lasers. Radiative recombination can also occur sometimes through discrete levels, e.g., in the Zn-O center 158 3 Mathematical Treatments combination in GaP. This is a unique example where one Zn-O pair forms an isoelectronic recombination center by replacing a Ga-P pair with an energy level in the bandgap. Recombination can also occur without the involvement of radiative processes, such as through traps, through other processes where momentum conservation involves phonons, and through Auger processes where excess energy of annihilation or creation of an electron–hole pair is associated with a third carrier. All these processes are important under different conditions in devices. In order to understand the statistics of these processes and their significance, we use the principle of detailed balance which states that, for a system in thermal equilibrium, the rate of any process and its inverse balance each other. The adjective “detailed” emphasizes that this balance occurs in all details of the process. Consider radiative recombination in thermal equilibrium. The detailed balance requires that, in thermal equilibrium, the same fraction of electron–hole recombination be radiative as is the electron–hole pair generation, and with the same spectral characteristics as the radiation that occurs with electron–hole pair recombination. The principle of detailed balance is a statistical principle, whose manifestations include the principle of microscopic reversibility for probabilities instead of rates, or Kirchoff’s law. The principle of detailed balance was used implicitly in setting the net of scattering rates for all the scattering processes to zero, in thermal equilibrium, in our discussion of the BTE. 3.7.1 Radiative Recombination Let ν be the photon frequency; the principle of detailed balance allows us to write the radiation rate in the band of dν, at the frequency ν, as R(ν)dν = P(ν)%(ν)dν, (3.173) where R is the emission rate, P the net probability per unit time of absorbing a photon, and % is the photon density at the frequency ν given by %(ν)dν = 8πν 2 ϑ3 dν , c3 exp (hν/kT ) − 1 (3.174) where ϑ is the index of refraction. The total number of recombinations can now be derived by integrating over the frequency as 8πϑ2 (kT ) R= c3 h 3 3 Z 0 ∞ 1 η2 dη, τ (ν) exp (η) − 1 (3.175) where τ (ν) is the mean lifetime of the photon in the semiconductor and η = hν/kT . This is the van Roosbroeck-Shockley relationship for radiative recombination rate, valid in thermal equilibrium, and useful in calculating the shape of the luminescence spectrum given by Equation 3.173 if the photon lifetime or alternately the absorption coefficient α(ν) = ϑ/cτ (ν) is known. 159 3.7 Generation and Recombination The radiative recombination rate is proportional to electron and hole densities that are recombining, i.e., Rr = cr np, (3.176) Rr = cr n0 p0 = cr ni 2 , (3.177) and in thermal equilibrium, so that Rr = Rr np . ni 2 Away from thermal equilibrium, the change in recombination rate is 0 0 n0 + n p0 + p 0 Re = Re − Re = Re − Re , n0 p0 0 (3.178) (3.179) 0 where p and n are incremental deviations in carrier concentrations. For small deviations, this gives ! 0 0 0 p n + Re = Re . (3.180) n0 p0 The radiative lifetime then follows, since excess populations of either carriers are the same and given by 0 τr = n ni 2 1 . 0 = n0 + p0 Re Re (3.181) The capture rate cr is usually denoted by the factor B, the probability of radiative recombination, and given by B= Re , ni 2 (3.182) using the thermal equilibrium condition. The radiative lifetime follows as τr = 1 . B (n0 + p0 ) (3.183) The constant B for various compound semiconductors is included in the Appendix B. This description is quite pertinent for moderate doping conditions. It breaks down at very large doping conditions—both experiments and detailed theory indicate that τr saturates in the limit of very high doping. 3.7.2 Hall–Shockley–Read Recombination Traps, because they can exist in more than one charge state, have the ability to act as recombination-generation centers. This ability comes about because 160 3 Mathematical Treatments Figure 3.21: Capture and emission processes for electrons and holes and involving a donor-like trap in n-type semiconductor. these centers can capture an electron and/or a hole from the bands as well as emit one to the bands. Thus, electrons and holes can recombine or lead to a generation process at these traps. The statistics for this were first analyzed by Hall, Shockley, and Read, and are known as Hall–Shockley–Read (HSR) recombination. We will consider a donor-like trap, of density NT , in an n-type crystal. Being a donor-like trap, it exists either in a positively charged state, where we consider a donor that exists only as a singly ionized donor of density NT+ , or in a neutral state with density NT0 . The singly ionized state of the trap exists in the bandgap at an energy ET . In thermal equilibrium, the distribution of these densities is + 0 NT = N T + N T , (3.184) and away from thermal equilibrium conditions, NT = NT+ + NT0 . (3.185) The different processes taking place between the trap and the bands are shown in Figure 3.21. Mathematically, these processes may be represented by and NT0 NT0 + h+ * ) NT+ + e− * ) NT+ , (3.186) where the first is the emission and capture process between the conduction band and the trap, and the second describes the capture and emission process between the valence band and the trap. The rate of capture of electrons from the conduction band is proportional to the number of positively-charged centers NT0 and the number of carriers available for capture n. Thus, Rce = ce nNT+ . (3.187) 161 3.7 Generation and Recombination The rate of emission of electrons to the conduction band is proportional to the number of neutral centers and the available states for capture in the conduction band, i.e., G ce = ee NT0 (NC − n) . (3.188) In thermal equilibrium, the rate of capture and emission are the same so, Rce + ce n 0 N T = = G ce 0 ee N T (NC − n0 ) . (3.189) Similarly, the two processes associated with the valence band yield Rvh = ch pNT0 (3.190) G vh = eh NT+ (NV − p) (3.191) for capture rate of holes, and for emission rate of holes, and in thermal equilibrium Rvh 0 ch p 0 N T = G vh + = eh N T (NV − p0 ) . (3.192) The capture rates of the traps are equal to the product of the capture crosssection of the trap, the thermal velocity, and the density of such traps that can capture. The capture cross-section multiplied by the thermal velocity is a volume associated with each trap per unit time. Any carrier—and carriers move with thermal velocities—incident within this volume gets captured. The capture cross-section is thus a parameter which defines an area in which the trap captures efficiently. The total volume associated with the number of traps, then, determines the capture rate. Thus capture rate of electrons by the ionized trap level gives ce = σvθ NT+ . (3.193) We evaluate the statistics under conditions in which the Boltzmann approximation is valid. This also implies that the effective density of states is much larger than the carrier concentrations in the band. Our thermal equilibrium equations, using the principle of detailed balance, allow us to evaluate some of the constants. The constants for emission are related to the constants for capture as above by + ee = ce and n0 N T , NC N 0 T (3.194) 0 p0 N T eh = ch . NV N + T (3.195) 162 3 Mathematical Treatments Here, we have assumed that the carrier concentration is less than the corresponding effective density of states. In thermal equilibrium, we have ξf − Ec n0 = NC exp kT Ev − ξf ni 2 and p0 = NV exp = . (3.196) kT n0 0 The rate of decrease of an excess carrier concentration n is given by the difference between capture and emission processes 0 − dn dt = Rce − G ce + nNT+ = ce = ce − n0 NT0 NT 0 ! NT Ec − ET + 0 NT . nNT − NC exp − kT (3.197) Similarly, from recombination and emission processes for holes, we have: 0 − dp dt = = = Rvh − G vh pNT0 ch ch pNT0 0 NT − p0 NT+ + NT ! ET − Ev + − NV exp − NT . kT (3.198) In steady-state conditions away from thermal equilibrium conditions, the rate of change of excess electron and hole densities are identical since they only interact with each other during generation and recombination, i.e., 0 0 dp dn = , dt dt (3.199) allowing us to write the positively and neutrally charged trap densities as Ec − ET + NT = NT ce NC exp − + ch p × kT Ec − ET n + NC exp − ce + kT −1 ET − Ev p + NV exp − ch , (3.200) kT and NT0 = ET − Ev NT ce n + ch NV exp − × kT 163 3.7 Generation and Recombination Ec − ET n + NC exp − ce + kT −1 ET − Ev p + NV exp − ch . kT (3.201) This allows us to write the net rate of decrease of excess density as 0 0 dn dp − =− dt dt np − ni 2 × 1 Ec − ET + n + NC exp − kT ch NT −1 ET − Ev 1 p + NV exp − . kT ce NT = (3.202) This expression relates the net rate of change in carrier concentration with 0 0 time, i.e., −U = G − R = dp /dt = dn /dt. Usually, one defines parameters τp0 and τn0 as and τp0 = τn0 = 1 ch NT 1 . ce NT (3.203) and hence the minority carrier lifetime for the n-type semiconductor, for a donor-like trap with a single state, is 0 τp = = p − 0 dp /dt 0 p Ec − ET × n + NC exp − τp0 + np − ni 2 kT ET − Ev p + NV exp − τn0 , kT (3.204) and majority carrier lifetime is 0 τn = − n dn0 /dt 0 = n × np − ni 2 Ec − ET n + NC exp − τp0 + kT ET − Ev p + NV exp − τn0 . kT (3.205) 164 3 Mathematical Treatments In deriving the above equations we considered a single level donor-like trap in the limit of Maxwell–Boltzmann approximation. Traps can be acceptor-like; the equations have the same form as above. A considerably more complex situation occurs when a trap has multiple levels in the band, e.g., transition metals with incomplete d-orbitals usually have several levels associated with different states of ionization. Chromium, e.g., has three levels within the bandgap of GaAs, and it is among the impurities used to obtain semi-insulating GaAs. Statistics in such situations can be quite complicated, because the presence of one state excludes the other. The method of grand partition function to obtain the statistics, summarized in the previous chapter for the statistics of discrete levels, is particularly useful in such situations. Problem 23 discusses such a complicated problem, and its implication on lifetimes. 3.7.3 Auger Recombination Electrons and holes can recombine, without the HSR type interaction at a trap or the involvement of photon emission, by releasing the excess energy to another carrier. Such processes involving more than two carriers are usually referred to as Auger processes. Impact ionization, discussed earlier, is actually one example of an Auger process, a generation process that involves the creation of an additional electron–hole pair due to the excess energy of a hot carrier. The number of Auger recombination processes is large. Auger transitions may take place through band-to-band, band-to-shallow levels, shallow levels-toshallow levels transitions involving excitons, etc. In all these cases the excess energy released in the transition is picked up by a mobile carrier. Because of the involvement of carriers, shallow levels, and transition across much of the bandgap, the process becomes stronger both with increase in doping and by reduction in bandgap. In small bandgap materials, it is also strongly temperaturedependent. Electrons are also more easily likely to get energetic since they usually have a lighter mass. Light holes are also likely to pick up excess energy; however, most holes exist as heavy holes because of the larger density of states for heavy hole band. Band structure is therefore very central to how and which Auger recombination processes are important, as it is for its inverse, the Auger generation process. We can derive the statistics for this process in a similar manner to those for HSR recombination. When the excess energy is received by an electron in the conduction band, we have interaction taking place between two electrons and one hole. Thus, RAe ∝ n2 p, (3.206) and in thermal equilibrium RAe ∝ n20 p0 . (3.207) The generation process depends only on the electron concentration G Ae ∝ n, (3.208) 165 3.7 Generation and Recombination and in thermal equilibrium, G Ae ∝ n0 . (3.209) Relating the rates using the principle of detailed balance, in thermal equilibrium, G Ae = RAe , (3.210) so, away from thermal equilibrium, RAe = RAe n2 p , n20 p0 (3.211) n , n0 (3.212) and G Ae = G Ae and RAe − G Ae = G Ae n2 p n − 2 n0 p0 n0 where γn = G Ae = γn n np − ni 2 , 1 n20 p0 (3.213) (3.214) is an Auger constant. An equivalent expression for holes is RAh − G Ah = γp p np − ni 2 . (3.215) Consequently, the net Auger recombination rate due to electrons and holes is given by: U A = RAe − G Ae + RAh − G Ah = (γn n + γp p) np − ni 2 . (3.216) We can show that under low level injection these expressions reduce to a form where the net recombination rate is proportional to the excess carrier concentration (see Problem 14). For p-type material, such as the base of a bipolar transistor, the net recombination rate is 0 U A = γp NA 2 n , (3.217) 0 where n is the excess carrier concentration. Using this, in a way similar to that of HSR recombination, an Auger lifetime can be defined whose magnitude is τA = 1 . γp NA 2 (3.218) For most semiconductors, where the band to band Auger processes dominate, in the limit of heavy doping the lifetime does appear to follow an inverse dependence with the square root of the doping. 166 3.7.4 3 Mathematical Treatments Surface Recombination In this discussion of the behavior of excess carriers, a particularly important one both at surfaces and in treatments of certain boundary conditions, is that of recombination at surfaces11 and also by extension at interfaces. Compound semiconductor surfaces usually occur with considerable numbers of states in the forbidden gap. Generally, there is a distribution of states and the surface is quite often pinned because of the large number of states. Sometimes this pinning may occur in the bands, e.g., in InAs it occurs in conduction band while for GaSb it occurs in the valence band. When these states occur in the forbidden gap, recombination transitions occur through the non-radiative HSR process at the surface. Carriers within a few diffusion lengths can readily recombine, leading to a net flow of current to the surface that we will call surface recombination current. The treatment of surface recombination is actually quite complex. Simple relations, however, can be derived for low level injection conditions. When excess carriers exist in the bulk, we can derive the diffusive current towards the surface for a uniformly doped sample. It is this diffusive flux that supplies the surface recombination current under low level injection conditions. We will treat this first in a simple way, to show the simplified equations that are used in the Dirichlet boundary conditions and that readily lead to the concept of surface recombination velocity. Following that, we will discuss where this simplified treatment will break down. Let %s be the reflection coefficient at the surface representing the probability that a particle returns to the bulk without recombining at the surface. Similarly, let %b be the reflection coefficient representing the probability that a carrier headed towards the bulk will show up at the surface. We assume, for the simple analysis, that these are independent of current density and carrier concentrations. Following Figure 3.22, the total flux Fs to the surface from the bulk is given by Fs = Fi + %b Fb , (3.219) where Fi is the incident flux and Fb is the total reverse flux. Likewise, we may write the total flux from the surface to the bulk as Fb = Gs + %s Fs , (3.220) where Gs is the generation rate at the surface. The total fluxes, in terms of the reflection parameters, generation rate, and the incident flux, are and Fs = Fb = Fi + %b Gs 1 − %s %b Gs + %s Fi . 1 − %s %b (3.221) 11 Our comments here closely follow the discussion in J. P. McKelvey, Solid State and Semiconductor Physics, Krieger, Malabar, FL (1982). 167 3.7 Generation and Recombination Figure 3.22: Fluxes of carriers representing transport processes taking place in the surface region of semiconductors during surface recombination. After J. P. McKelvey, Solid State and Semiconductor Physics, Krieger, Malabar, FL (1982). For a classical gas distribution, i.e., for non-degenerate materials, the fluxes Fs and Fb are related to the thermal velocity and the free carrier concentration as ≈ nvθ /4, which reduces to ≈ n0 vθ /4 in thermal equilibrium. This follows from the argument that, at any given instant of time, half of the carriers are directed towards the surface, and since their direction is random they have an average velocity of ≈ vθ /2 in the orthogonal direction. This allows us to write the generation rate and the incident flux F i , at thermal equilibrium, at the surface, as n0 vθ (1 − %s ) 4 n0 vθ and Fi = (1 − %b ) . (3.222) 4 Note that the generation rate remains constant; this follows using similar arguments as with the HSR recombination mechanism. Departure from equilibrium results in a disparity between the net flux to and from the surface, the difference of which is the recombination flux. The method applied here is similar to that sometimes used in discussion of metal–semiconductor junctions. The flux directed towards the surface originates from a distance on average equal to the mean free path. Thus, the fluxes to and from the surface at any position are vθ dn Fs = n−γ 4 dz Gs = 168 3 Mathematical Treatments and Fb vθ 4 = dn n+γ , dz (3.223) where γ is a proportionality constant. The sum of the surface and bulk fluxes is ns vθ /4 at the surface. Our equations may now be used to determine the incident flux as Fi = ns vθ 1 − %s %b n0 vθ 1 − %s − (1 + %b ) , 2 1 + %s 4 1 + %s (3.224) and hence the net flux of carriers, assuming only diffusive transport of carriers is 0 ns − n0 1 − %s dn F |surf = Fs − Fb = vθ = −Dn . (3.225) 2 1 + %s dz surf This is simply written as 0 dn −Dn dz = S ∆n|s , (3.226) s with S, the surface recombination velocity, as S= vθ 1 − %s . 2 1 + %s (3.227) Note that if all carriers incident at the surface recombine, then the surface recombination velocity is vθ /2, its largest value. Assuming an infinite surface recombination velocity, as is common for many boundaries encountered in device modelling, is tantamount to assuming that the excess carrier concentration at the surface is zero. For many practical cases, this assumption is justified. The function %s represents the statistics of recombination at the surface, because it represents the probability that a carrier will return. Thus, 1 − %s is proportional to the recombination rate at the surface. We have discussed the statistics of HSR recombination; these also hold for most surfaces, because the recombination occurs through deep traps. The recombination rate at the surface can be represented by similar expressions to those used for a single level. Assuming that there exists a single dominating trap level, the surface recombination rate is ns ps − ni 2 R = σn σp vθ NT s , (3.228) (ns + nT s ) σn + (ps + pT s ) σp where ns and ps are the surface carrier concentrations, and nT s and pT s are the surface carrier concentrations if the Fermi level were at the trap level. Consider an example that is a simplification of this. For a trap with equal hole and electron capture cross-section, if the electron is a minority carrier hence if hole concentrations are large, then the recombination rate is Rs ≈ σvθ NT s ns . (3.229) 169 3.7 Generation and Recombination The rate of recombination of electrons, per unit time, per unit area, is given by the above expression. The reflection coefficient is related to this rate since it expresses the probability of not recombining (see Problem 15). The recombination rate is proportional to the carrier concentration; it is provided by the difference of incident and reflected flux, and the constant of proportionality σvθ NT s is the surface recombination velocity in the absence of any surface space charge, with identical conditions at the surface as in the bulk. For low interface state density oxide-silicon interfaces, σ ≈ 10−16 cm2 and NT s ≈ 1010 cm−2 , resulting in a surface recombination velocity on the order of ≈ 10 cm.s−1 . In compound semiconductors such as GaAs, even if we ignore the effect of surface space charge and other effects which we will soon discuss, NT s ≈ 1014 cm−2 , σ ≈ 10−15 cm−2 , and hence surface recombination velocity is of the order of 106 cm.s−1 . Strictly speaking, recombination rate characterizes the surface effectively for most purposes. Surface recombination velocity is a concept introduced because it characterizes a meaningful constant in some situations. If, in an ad hoc manner, we defined it as a parameter that related the recombination rate to the excess carrier concentration, then it would vary as a function of biasing condition, etc., because the above is only a simple derivation from the more complicated HSR expression. 3.7.5 Surface Recombination with Fermi Level Pinning In the presence of a charge region at the surface, the surface recombination velocity takes an even more complicated form. It now depends on the surface state density, the characteristics of the surface states, surface charge, etc.— parameters which determine the surface carrier concentrations. We can see from the relationships above that it will actually go through a maximum when σn (ns + nT s ) + σp (ps + pT s ) goes through a minimum. This will occur when both electron capture and hole capture processes are equally active, i.e., when the quasi-Fermi levels straddle the trap level. Since the surface space charge situation is important to most compound semiconductors, we will look at it in more detail. We consider variations introduced on our simple model due to the presence of band bending from Fermi level pinning. For low level injection (see Figure 3.23), we may again derive a relationship that relates surface carrier concentrations to the bulk. The presence of surface depletion changes the thermal equilibrium concentration at the surface—in the case of Figure 3.23 this would mean changing from the bulk thermal equilibrium magnitude by the Boltzmann exponential related to the total band bending at the surface. The total recombination rate is a more general case of the above, where we again ignore the nT s and pT s terms and the intinsic carrier density terms, as Rs = σn σp vθn vθp NT s ns ps . ns σn vθn + ps σp vθp (3.230) Let the bulk value of carrier concentrations be n0 and p0 under thermal equilibrium, and let n and p be the bulk values under the low level injection condition. 170 3 Mathematical Treatments Figure 3.23: Band diagram for estimating surface recombination at a trap, in the presence of Fermi level pinning, at (a) thermal equilibrium, and (b) low level injection conditions. If the recombination is the rate-limiting step, then the low level injection condition implies flat quasi-Fermi levels between the bulk and the surface. If the total band bending is ∆ψS from the bulk, the carrier concentration at the surface is q∆ψS ns = n exp − kT q∆ψS , (3.231) and ps = p exp kT with 2 np = ni exp ξn − ξp kT , (3.232) at both the surface and in the bulk. The surface recombination rate can, then, be written as 1/2 Rs = (σn σp vθn vθp ) 1/2 (ns σn vθn /ps σp vθp ) 1/2 NT s (ns ps ) 1/2 + (ps σp vθp /ns σn vθn ) . (3.233) The occupation probability f of the trap NT s at the surface is given by f= σn vθn ns + σpvθp pT s . σn vθn (ns + nT s ) + σp vθp (p + pT s ) (3.234) 171 3.7 Generation and Recombination Since, at thermal equilibrium, the Fermi level is pinned at the trap level ET , the occupation probability is very close to 1/2 (see Problem 16). Away from thermal equilibrium, the resultant surface charge density is given by qNT s σn vθn ns − σp vθp ps 1 = , (3.235) Qs = qNT s f − 2 2 σn vθn ns + σp vθp ps where we again ignore the insignificant terms away from thermal equilibrium. For large trap densities that lead to Fermi level pinning, this charge is insignificant compared to the charge qNT s if all the traps were ionized, or equivalently only a very small deviation from the 1/2 occupation probability occurs. This, however, implies that ns σp vθp = . (3.236) ps σn vθn The ratio of carrier concentrations at the surface is a constant, and in a large trap density, and low level injection limit, the recombination rate is 1/2 Rs = (σn σp vθn vθp ) 2 NT s (ns ps ) 1/2 . (3.237) The recombination rate is not proportional to the minority carrier concentration any more; it is proportional to the square root of the electron and hole concentration at the surface, and since the quasi-Fermi levels are flat, it is also proportional to the square root of the electron and hole concentration in the bulk. A consequence of this is an exp (qV /2kT ) dependence of surface recombination current for low level injection bias conditions where this analysis applies. This square root dependence also appears for recombination in a p-n junction space charge region, and is responsible for similar exp (qV /2kT ) dependence there. Surface recombination velocity, defined as a pre-factor to excess minority concentration during recombination calculations, is no longer a constant but a function of bias conditions. Arguments have been forwarded that we should define surface recombination velocity in an alternate form that preserves a constancy.12 In the above, one may introduce s0 as an intrinsic surface recombination velocity that follows the recombination relation √ Rs = S0 ns ps . (3.238) This intrinsic recombination velocity is related to the conventional definition of surface recombination velocity in terms of excess carrier concentration (e.g., one useful in Dirichlet boundary conditions) via r ns S = S0 . (3.239) ps 12 See the discussion in G. J. Rees, “Surface Recombination Velocity—a Useful Concept?” Solid-State Electronics, 28, No. 5, p. 517, 1985, and P. De Visschere, “Comment on G. J. Rees ‘Surface Recombination Velocity—a Useful Concept?’ ” Solid-State Electronics, 29, No. 11, p. 1161, 1986. 172 3 Mathematical Treatments Figure 3.24: The quasi-Fermi levels and conduction and valence band edges in the presence of a high surface recombination rate. Intrinsic surface recombination velocity is the surface recombination velocity that occurs when the electron and hole densities at the surface are equal. Rigorous calculations of these parameters show that significant deviations occur at high level injection conditions, where our theory does not appear valid. Differences also occur when the surface recombination rate is the rate-limiting step. Under these conditions, the band diagram and the quasi-Fermi levels look as in Figure 3.24, indicating that the carrier flux needed for recombination occurs via both drift and diffusion at the surface. We will continue discussion for the more complicated cases of this subject in Chapter 7 on bipolar transistors. Here, we have only considered the onedimensional situation and have assumed the quasi-Fermi levels to be constant. The trap recombination statistics have to be self-consistently analyzed with the ability of the semiconductor to provide the carriers for recombination at the surface. A changing quasi-Fermi level implies that supply of carriers becomes a rate-limiting step. The recombination rate is now limited by supply of carriers from the bulk and does not necessarily follow this analysis. Additionally, in real devices, two-dimensional considerations predominate under certain bias conditions, i.e., carriers injected along the channel occurring due to Fermi level pinning must also be considered in our analysis. 3.8. SUMMARY 3.8 173 Summary This chapter reviewed and developed methods of analysis that will be used in the rest of the book. In particular, we have emphasized the approximations of various approaches, and how one may isolate sections of a larger problem in order to analyze related behavior. To do this we use appropriate boundary conditions, which mimic the behavior at the interface where a section is isolated, and the appropriate model to describe the events taking place within the section. The first method of analysis considered is based on a simple treatment of the kinetics of particles treated as an ensemble. This was the particle kinetic approach and allowed us to develop meaningful methods for analysis of information related to low-field mobility, etc. The second method is the Boltzmann Transport Equation, which considers the use of distribution functions describing the phase space behavior of particles. The development of this distribution function, or the moments of it (statistical averages corresponding to macroscopic properties) in time allows us to describe the behavior of the system. However, in order to obtain results conveniently, while still maintaining the basis in distribution functions, we had to limit the methodology to displaced Maxwell–Boltzmann distributions and we had to approximate scattering effects by relaxation time approximations. The method, thus, deserves to be used with extreme caution. These limitations are avoided, at the expense of demanding numerical computation, in the Monte Carlo approach where statistics are developed either for an individual particle or an ensemble of particles. The limitations of the Monte Carlo approach are related to the adequacy of the description of the processes taking place in the semiconductor. The collection of a vast amount of statistics on particles avoids the need to assume certain distribution functions for the particles as required in the Boltzmann Transport Approach. Conventional semiconductor devices are usually analyzed within the driftdiffusion approximation. We derived the relevant semiconductor transport equations from the Boltzmann Transport Equation and discussed the limitations and approximations in making the simplification to drift-diffusion equation. We also showed how one may derive small-signal solutions to transport problems of interest based on this approach by considering the frequency dependence in the drift-diffusion equation. In the rest of the book, although this approach is stressed the most, we will also resort to Monte Carlo approach where the application of drift-diffusion is clearly inadequate. In analyzing device problems with any of these approaches, we still need to consider models for the boundaries of the system. Many p–n junction problems can be analyzed adequately with the use of Shockley and Fletcher or Misawa boundary conditions. These boundary conditions allow one to determine the carrier densities over a range of biases in device structures where such junctions exist, one example being the bipolar transistor. We also considered Dirichlet boundary conditions that can be applied at many semiconductor interfaces— metal–semiconductor junctions, ohmic contacts, and high recombination surfaces being some examples. Finally we considered the use of Neumann boundary conditions at semiconductor surfaces. Recombination is a particularly strong 174 Mathematical Treatments and important attribute of compound semiconductors; they are largely direct bandgap materials and hence exhibit radiative recombination. In addition, they have a large trap density and therefore a large non-radiative recombination. In addition, the smaller bandgap semiconductors can have significant Auger recombination. The necessary underlying mathematical basis of all these processes was discussed together with that for surface recombination. General References 1. B. K. Ridley, Quantum Processes in Semiconductors, Clarendon Press, Oxford (1988). 2. P. J. Price, “Monte Carlo Calculation of Electron Transport in Solids,” in R. K. Willardson and A. C. Beer, Eds., Semiconductors and Semimetals, 14, Academic Press, N.Y. (1979). 3. C. Jacobani and L. Reggiani, “The Monte Carlo Method for the Solution of Charge Transport in Semiconductors with Applications to Covalent Materials,” Review of Modern Physics, 55, No. 3, p. 645, July 1983. 4. P. J. Price, “Calculation of Hot Electron Phenomena,” Solid-State Electronics, 21, p. 9, 1978. 5. S. Datta, Quantum Phenomena, Addison-Wesley, MA (1989). 6. E. M. Conwell, High Field Transport in Semiconductors, in Solid State Physics, Suppl. 9, Academic Press, N.Y. (1967). 7. A. C. Smith, J. F. Janak, and R. B. Adler, Electronic Conduction in Solids, McGraw-Hill, N.Y. (1967). 8. R. W. Hockney and J. W. Eastwood,Computer Simulation Using Particles, McGraw-Hill, N.Y. (1981). 9. C. Jacobani and P. Lugli, The Monte Carlo Method for Semiconductor Device Simulation, Springer-Verlag, Wien (1989). 10. W. Paul, Ed., Handbook on Semiconductors, Vol. 1, North-Holland, Amsterdam (1982). 11. J. P. McKelvey, Solid State and Semiconductor Physics, Krieger, Malabar, FL (1982). 12. S. Selberherr, Analysis and Simulation of Semiconductor Devices, SpringerVerlag, Wien (1984). 13. K. Hess, Advanced Theory of Semiconductor Devices, Prentice Hall, Englewood Cliffs, N.J. (1988). 14. J. S. Blakemore, Semiconductor Statistics, Dover, N.Y. (1986). Problems 175 15. J. Pankove, Optical Processes in Semiconductors, Dover, N.Y. (1971). 16. M. V. Fischetti and S. E. Laux, “Monte Carlo Analysis of Electron Transport in Small Semiconductor Devices Including Band Structures and Space Charge Effects,” Phys. Rev. B, 38, No. 14, p. 9721, 1988. 17. L. Reggiani, Ed., Hot-Electron Transport in Semiconductors, SpringerVerlag, Berlin (1985). 18. M. Kurata, Numerical Analysis of Semiconductor Devices, D. C. Heath, MA (1982). 19. C. M. Snowden, Semiconductor Device Modeling, Peter Peregrinus, London (1988). 20. T. H. Glisson, C. K. Williams, J. R. Hauser, and M. A. Littlejohn, “Transient Response of Electron Transport in GaAs Using the Monte Carlo Method,” in VLSI Electronics: Microstructure Science, 4, Academic Press, FL (1982). 21. K. Hess, “Aspects of High-field Transport in Semiconductor Heterolayers and Semiconductor Devices,” in Advances in Electronics and Electron Physics, 59, Academic Press, N.Y. (1982). Problems 1. We have derived the low field mobility relationship as a function of a single time constant; this is an idealization of a single valley semiconductor. At higher fields, though, more than one valley may contribute to conduction. GaAs, e.g., at fields of ≈ 3.0 × 103 V.cm−1 , also exhibits conduction in the L valley and to a lesser extent in the X valley. Consider the problem of conduction in two valleys and derive the mobility relationship assuming that a single time constant characterizes momentum relaxation in each of these valleys. 2. An important problem encountered in minority carrier devices using low dopings or high injection—such as p–i–n diodes, thyristors, and bipolar transistors—is the problem of conduction when both minority carriers and majority carriers are present in sufficient numbers to be strong contributors to current. The problem is usually encountered only at small electric fields. Derive the mobility relationship important in such conditions, expressing it in terms of single time constant approximations for both electrons and holes. This mobility is commonly referred to as the ambipolar mobility. 176 Mathematical Treatments 3. For a parameter ϕ(E) related to transport, show that the weighted average over all carriers is given by the relationship R∞ 2 ϕ(E)g(E) (∂f(E)/∂E) EdE R∞ hϕi = − 0 (3.240) 3 0 g(E)f(E)dE which reduces to R∞ ϕ(E)E 3/2 exp (−E/kT ) dE hϕi = 0 R ∞ 3/2 exp (−E/kT ) dE 0 E (3.241) in the Boltzmann approximation for semiconductors with parabolic bands. 4. Show, using the kinetic approach, that the current obeys the relationship in Equation 3.25 in the presence of a small electric and magnetic field. 5. Show that the Hall pre-factor r for acoustic deformation potential scattering is given as 3π r= . (3.242) 8 p 6. The thermal velocity vθ = 8kT /πm∗ is the root mean square speed or the root mean square of the magnitude of velocity. What is the most probable speed or magnitude of velocity in the Boltzmann approximation? 7. For a carrier density of n, show that the flux of carriers in any direction is given by nvθ /4. 8. The internal energy per unit volume, following our discussion of thermal velocity, etc., is Z ∞ W = Ef(E)D(E)dE. (3.243) 0 Show that, for the Maxwell–Boltzmann approximation, this leads to W = 3nkT /2, where n is the carrier density. At absolute zero, show that the energy is W = 3nξf /5. 9. Consider the problem of transport in external and built-in fields. Using the relationship between the perturbation in the distribution function and the isotropy of the semiconductor, and assuming randomizing scattering processes, show that the drift velocities are related as vd = ∆E 0 v . E0 d (3.244) 177 Problems 10. Show that a non-homogenous semiconductor can be treated as quasineutral provided λD 2 #−1 " 1 dN 2 1 d2 n q 2 d2 φCn − 2 + + . N dz N dz 2 kT dz 2 (3.245) 11. Derive the Fletcher boundary conditions (Equation 3.159) from the relationships between carrier concentrations at the edge of the depletion region and the condition of charge neutrality. 12. Show, mathematically, that the Fletcher boundary conditions (Equation 3.159) and the Misawa boundary conditions (Equation 3.161) are equivalent. 13. Show that the Misawa boundary conditions stated in Equation 3.161 and Equation 3.162 are equivalent. 14. Show that under low level injection, the expression for the Auger recombination rate reduces to a direct proportionality to the excess carrier concentration with the proportionality constant dependent on the square of dopant concentration. 15. Argue how the recombination rate at the surface is related to the reflection coefficient at the surface. Cast the relationship in a mathematical form. 16. Show that if the Fermi level is pinned at the surface, i.e., if the sheet density of traps substantially exceeds the sheet charge density in the surface depletion region, then the occupation probability of a trap level is close to 1/2. Under what conditions may this break down? 17. Is it possible for the momentum relaxation time to be larger than the energy relaxation time? Explain how, and if true what would the consequences be? 18. Assuming Boltzmann and relaxation time approximation, and small departure from thermal equilibrium, show, using the BTE approach, that a gradient of carrier density leads to diffusion whose diffusion coefficient is λvθ /3 where λ is the mean free path. 19. Consider a semi-infinite n-type sample of GaAs doped to 1016 cm−3 and with a mid-gap trap that has identical electron and hole capture crosssections of 10−15 cm−2 . Derive, using justifiable simplifications, the expression for decay of excess carriers in both the low injection limit and the high injection limit. What are the short time and long time limits if 1015 cm−3 carriers were created? What are the short and long time limits if 1017 cm−3 carriers were created? 178 Mathematical Treatments 20. If τn0 = τp0 = τ0 , show that the maximum lifetime occurs when the intrinsic and Fermi energy coincide. Show that this lifetime is ET − Ei τ = τ0 1 + cosh . (3.246) kT 21. If the flux of carriers in any direction is given as nvθ /4, how can the surface recombination velocity exceed vθ /4? 22. In this problem, we will evaluate statistics of trap energy levels arising from independent defects. Consider a semiconductor with two defects associated with energy levels E1 and E2 . (a) What is the occupation probability of the two levels? (b) If the Fermi energy is between the two levels with E2 − ξf kT , what do the occupation probabilities reduce to? 23. We now extend the previous problem to analysis of recombination in a semiconductor when the energy levels arise from the same impurity. A technologically relevant example of this is gold, a transition element, as a substitutional impurity in silicon. In GaAs, multiple levels occur due to chromium, and will be discussed in Chapter 5. For gold, a closed d-shell is inert. A positively charged state can accept an electron, a negatively charged state can donate an electron. The higher negatively charged states occur in the valence band. So, the substitutional impurity in Si causes a lower energy level ED , a donor level, and a higher energy level EA , an acceptor level. (a) Calculate the equilibrium density of Au atoms in the positively charged state (NT+ ), the density of Au atoms in the neutral charge state (NT0 ), the density of Au atoms in the negatively charged state (NT− ), and the total charge density on Au. Consider the degeneracies as ga , and gd . (b) What are the rate equations? Let σn+ represent the capture crosssection for the electron capture process on the donor site leading to 0 a capture rate of c+ n . Let σn represent the capture cross-section for the capture of an electron on an acceptor leading to the capture rate of c0n . Let σp0 represent the capture cross-section for the hole capture process on the donor site leading to a capture rate of c0p . Let σp− represent the capture cross-section for the capture of a hole on an 0 − + 0 acceptor leading to the capture rate of c− p . Let en , en , ep , and ep identify the electron and hole emission rates from donor and acceptor sites. (c) Invoke the principle of detailed balance to evaluate the emission rates in terms of the capture rates at thermal equilibrium. (d) What is the low level neutral region recombination rate? Problems 179 (e) Calculate the low level neutral region minority carrier lifetime for trap concentrations significantly smaller than the shallow donor concentration. (f) In high level injection conditions, what is the the limiting form of the lifetime? (g) Capture cross-sections for Au in Si, at 300 K, are as follows: σn+ = 3.5 × 10−15 cm2 , σn0 = 5.0 × 10−16 cm2 , σp− = 1.0 × 10−15 cm2 , and σp0 = 3.0 × 10−16 cm2 . Assuming that recombination occurs only due to Au in Si, what are the low-level and majority carrier lifetimes for 1016 cm−3 Au-doped Si at 300 K for intrinsic material, 1016 cm−3 n-type material, and 1016 cm−3 p-type material? 24. Let ED and gd be the donor energy in a semiconductor sample that is n-type but compensated. Show that the carrier concentration is related as n2 NC n2 Ec − ED n n + NA − i = ND − NA − n + i exp − . n gd n kT (3.247) How does the activation energy behave in a plot of carrier concentration with temperature in different temperature ranges? 180 Mathematical Treatments Chapter 4 Transport Across Junctions 4.1 Introduction We begin our analysis of devices by first studying two-terminal structures. The theory and understanding of these are important to the understanding of transistors, since junctions are natural parts of these devices. For example, metal–semiconductor junctions are used to control the channel of a metal– semiconductor field effect transistor, p–n junctions are the basis for both injection and isolation in bipolar transistors, and heterojunctions are applicable to both field effect transistors and bipolar transistors. This discussion serves another useful purpose: it allows us to discuss applications of the methods of analysis of the previous chapter in simpler structures, even as they have the richness and diversity that clearly exemplify the approximations of our analysis techniques. This chapter discusses transport at junctions formed between metals and semiconductors, and semiconductors and semiconductors. Drift-diffusion, thermionic emission, and thermionic field emission theories are developed for the metal– semiconductor junctions exemplifying assumptions of equilibrium between the electrons in metal and semiconductor in the drift-diffusion theory, or the lack thereof with significant hot carrier effects in the other theories. The driftdiffusion and the thermionic emission theories are then serially combined to show a theory that still assumes a classical drift-diffusion equation and hence its assumptions of distribution functions. We have discussed transport in builtin and applied fields in p–n junctions when discussing the relative merits of the Monte Carlo and the BTE approaches and have pointed out their effects on the distribution function. That discussion, however, did not bring out a particularly severe approximation in the distribution function at the metal–semiconductor junction itself because of the negligible flow of carriers from the metal into the semiconductor and because almost all carriers entering the metal are lost. Thus, this discussion of metal–semiconductor transport theories brings out the breadth of the problem quite well. 181 182 4 Transport Across Junctions The discussion of metal–semiconductor junctions is naturally amenable to extensions involving transport across heterojunction discontinuities. In transport across heterojunctions, processes encountered in metal–semiconductor junctions are still equally important, but with some additional complications. Now, the transport across the abrupt barrier from one semiconductor to the other can not be dealt with as simplistically as in the metal–semiconductor case, because the barriers are smaller and the scattering rates and energy losses in the semiconductors are much smaller than in a metal. The latter additionally leads to a fair fraction of injected carriers being capable of returning, should their momentum change direction. The lower barrier heights of heterojunctions also results in an increased importance of tunneling, with energy conservation (elastic) and without energy conservation (inelastic), and a particularly interesting example of resonance transmission in the form of resonant Fowler–Nordheim tunneling. This is therefore discussed in the context of heterojunctions. The p–n junction transport in quasi-static approximation is discussed next, to develop examples in high injection, to point out some of its assumptions, and to develop a general charge control approach that is commonly known as the Gummel–Poon analysis after its originators. This analysis will be extended, like the earlier discussions of other junctions, in our discussion of three-terminal device structures. The p–n junctions can also be formed with heterojunctions and are the basis of heterostructure bipolar transistors; the discussion ends with this subject. The chapter concludes with a discussion of ohmic contacts, the most general forms of which are based on tunneling between metals and semiconductors. 4.2 Metal–Semiconductor Junctions We start with a preliminary discussion of contacts. Consider two metals far away. The metals are neutral, they have differing Fermi energies, which characterize the average energy of carriers with respect to the vacuum. When these metals are brought together with a return path for the flow of carriers, as shown in Figure 4.1, carriers move from one to the other until the electrochemical potential is identical. Carriers move from higher energy to lower energy, so that, in thermal equilibrium, the equilibrium Fermi energy lies in between. The charge transfer results in formation of an electric dipole at the interface that also allows the discontinuous change in the vacuum level. The electrostatic potential differences in the bulk, when the metals are separated, are and µ1 = µ2 = Evac − qφ1 Evac − qφ2 , and in contact, in thermal equilibrium, and µ1 µ2 = = Evac − qφ1 − qψ10 Evac − qφ2 − qψ20 , (4.1) 183 4.2 Metal–Semiconductor Junctions Figure 4.1: The vacuum level and the Fermi level of two metals separated is shown in (a), and in (b) the levels are shown when the two metals are brought together in contact with a path for current flow. The lower part of (b) shows the electric dipole formed at the interface due to charge transfer. (4.2) and the two chemical potentials are equal, µ1 = µ2 , (4.3) ψ20 − ψ10 = φ1 − φ2 . (4.4) so that The differences in electrostatic potential balance differences in chemical potential when the two metals are brought in contact and are in thermal equilibrium. Now let us extend this picture to an idealized metal–semiconductor junction as shown in Figure 4.2. Here, we have assumed that interface effects play no role, an assumption that is often incorrect. For now, this serves as a simplified example. When the contact is formed, electrons at the Fermi level in the metal see a barrier of height qφB ,1 and the electrons at the conduction band edge in the semiconductor see a barrier of height qψj0 . In thermal equilibrium, for this idealized situation, these barrier heights from the metal to the semiconductor and from the semiconductor to the metal are related by and 1 We qφB qψj0 = = q (φm − χ) q (φm − χ) − qVn , also use qφM to denote this barrier height elsewhere in this text. (4.5) 184 4 Transport Across Junctions Figure 4.2: Formation of an idealized metal–semiconductor diode; (a) shows the vacuum levels, band edges, work functions, and electron affinities, and (b) shows these in contact in thermal equilibrium with a current path for electron transfer. where qVn = Ec − ξf is evaluated in the bulk. The approximation in the above is the neglect of interface effects. Usually, semiconductors have a significant number of interface states, quite often in the bandgap. Interface states also occur due to surface reconstruction when a metal is placed in intimate contact on a nascent semiconductor surface. The metal–semiconductor barrier height, therefore, is never quite in accord with the above. Silicon comes close, but most compound semiconductors do not. In practice, therefore, we replace the metal–semiconductor barrier height by the experimentally measured values. When we forward or reverse bias this junction (see Figure 4.3), the barrier for injection from the semiconductor to the metal is either reduced or increased. In the forward direction, a reduced barrier results in an increase in injection into the metal of electrons from the semiconductor, while in the reverse direction, an increased barrier results in a decrease in injection into the metal of electrons from the semiconductor. The injection of electrons from the metal to the semiconductor remains essentially the same since the metal is highly conducting and, in this simple picture, the barrier is constant. Therefore the diode conducts a large current in the forward direction and a small current in the reverse direction. The interesting aspects of rectification were recognized very early, and some of the earliest work in hot electron transport was actually related to rectification properties. Many of these theories of the 1930’s and Bethe’s thermionic emission model of the 1940’s have gone through significant modifications as our understanding of the hot electron phenomenon has improved. Before discussing the transport, though, we will discuss some of the modifications that we must include in the above description to make it consistent with real structures. 4.2 Metal–Semiconductor Junctions 185 Figure 4.3: Metal-semiconductor diode with (a) a forward bias and (b) a reverse bias applied to the diode. Barrier heights in compound semiconductors are strongly influenced by chemical interactions and other interface phenomena. Even for ideal systems such as vacuum cleaved surfaces, surfaces behave in different ways, in different orientations, at different temperatures, with different metals, because surfaces do not maintain a physical structure that is identical to that of the bulk. This is a result of the drive to lower energy, and different metals influence it differently, causing different interface states to appear in the bandgap. The surface recombination velocity, which described the surface recombination and was used in modelling the Dirichlet boundary conditions, was one of the consequences of these interface states. These interface states, if they exist in sufficient numbers, cause Fermi level pinning, because a large charge dipole can exist at the interface without any deviation in the Fermi level. In practice, therefore, barrier heights in compound semiconductors are best determined experimentally. This data is sufficiently reproducible, and it adequately describes the required parameter of the interface modelling problem. There are effects on this barrier height which are unrelated to the existence or absence of interface states. One such effect is caused by image force, and it results in a lowering of barrier height that is called image force lowering. A charge in close proximity to a highly conducting surface has a lowering of its energy. This follows directly from the solution of Laplace’s equation describing this problem, with the boundary condition that the conducting plane be treated as an equi-potential surface. Intuitively, this can be described via an image charge of equal and opposite magnitude, that the charge sees behind the 186 4 Transport Across Junctions Figure 4.4: Energy of an electron (solid line) as a function of position in the presence of image charge effect near the metal–semiconductor interface. conducting plane, with the plane being the mirror. An electron and the metal follow this description with the metal as the equi-potential conducting plane. The electron feels an image charge of the opposite type in the metal at an equal distance from the interface. The force on the electron in the semiconductor is given by q2 F= (4.6) 2, 4πs (2z) where z is its distance from the interface, which corresponds to a potential energy of −q 2 /16πs z. In the presence of the electric field E, at the interface, the potential energy due to Coulombic interactions (following Figure 4.4) is E=− q2 − qEz. 16πs z (4.7) Several assumptions have clearly been made in the act of writing this equation. A primary one is that we have assumed that our band structure model holds all the way to the interface. The electric field is assumed constant in the above; in a depleted semiconductor with a uniform charge concentration, it varies linearly with distance. However, close to the interface in a very short region where we utilize this equation, it can be treated as a constant. The maximum in this energy occurs at r q z = zm = , (4.8) 16πs E 187 4.2 Metal–Semiconductor Junctions with a maximum in energy of E = Em q =− 2 r qE . πs (4.9) So, actual metal–semiconductor barrier height is a function of the electric field at the interface and hence of bias applied; it differs from the low field value by the amount of the maximum energy given by Equation 4.9. The effect is most important in reverse bias where E is large because of a larger amount of charge in the semiconductor. Typical barrier heights for GaAs vary between 0.65 eV and 0.85 eV for n-semiconductors and 0.5 eV and 0.6 eV for p-semiconductors. For GaAs again, if an electric field of 100 kV.cm−1 were present, it would lead to a lowering of barrier height by 0.36 eV. Such large fields usually occur either in large reverse bias for moderately doped junctions, or near zero bias conditions for highly doped junctions. Effective barrier height therefore can decrease substantially with doping. In our discussion of the different approaches to modelling transport, we concluded that, for a p–n junction, the drift-diffusion approach models transport adequately because the distribution function remains a displaced-Maxwell– Boltzmann function, and because any errors of drift or diffusion compensate. Away from the metal–semiconductor interface by a few scattering lengths, this should still be an adequate description of the transport in the semiconductor. Near the metal–semiconductor interface, the situation is unlike the p–n junction problem because carriers that get injected into the metal are quite unlikely to return because of a rapid loss in carrier energy in a very short distance. Thus, the random orientation of velocities of the Maxwell–Boltzmann distribution is lost. Within a scattering length of the interface, due to the lack of any returning electrons from the metal, the velocities are all pointed in a hemisphere directed towards the metal, and the distribution function is actually more like a hemi-Maxwell–Boltzmann distribution function. But away from the interface by a number of scattering lengths, transport in the semiconductor region is by drift-diffusion, as usual. The transport at the interface is governed by two considerations. Carriers that have sufficient energy to surmount the barrier, that have velocity pointed towards the metal, and that do not lose these properties during a collision as they reach the metal–semiconductor interface will emit into the metal. This is the thermionic emission process. Due to the small barrier that has to be traversed by the carriers that are close to the interface, and due to the short distance, some carriers may tunnel through into the metal. This is known as field emission, and when thermionic emission is combined together with this, the process is called thermionic field emission. All of these transport processes take place in the metal–semiconductor diode, with current conservation being maintained, and the current magnitude being determined by whichever limits the current to a lower value. In case they are comparable, one may have to include all if one is interested in knowing the magnitude. Often, when combining all these processes, field emission is ignored, and the thermionic–drift-diffusion formulation adopted. 188 4 Transport Across Junctions Figure 4.5: Energy band diagram under an applied bias at a metal– semiconductor junction for (a) drift-diffusion and (b) thermionic and thermionic field emission theory. Early theories assumed that the transport was being limited by the rate at which carriers became available at the metal–semiconductor interfaces, i.e., these theories considered drift-diffusion as the rate-limiting step. The carriers in the semiconductor and the metal at the interface are, then, in equilibrium. For the moment, we ignore the consequences of hemi-Maxwell–Boltzmann distribution to the concept of quasi-Fermi level defined with respect to Maxwell– Boltzmann distribution and modified appropriately for the Fermi–Dirac distribution, since the problem of dealing with this question arises over distances of the order of a few scattering lengths. This assumption of drift-diffusion limited transport means that the quasi-Fermi level is no longer flat in the semiconductor, since it limits the transport, and since carriers are in equilibrium with each other on either side of the interface (see Figure 4.5). In fact, since the transport to the metal–semiconductor interface is the rate-limiting step, the density of carriers at the interface is unaltered by bias, i.e., the quasi-Fermi level at the interface continues to coincide with the metal Fermi level. Electrons are emitted into the metal at the interface at an energy in excess of the metal Fermi energy. These electrons rapidly lose their energy over few 10s of Ås. In thermionic emission theory and its variations, the drift-diffusion in the depletion region is not the rate limiting step, i.e., like the p–n junction in the low-level injection condition, the quasi-Fermi level remains flat, and the current in the structure is substantially smaller than either the drift or the diffusion current flowing at any cross-section in the semiconductor depletion region. The quasi-Fermi level, therefore, remains flat up to the interface, and then discontinuously drops to the metal Fermi level. Strictly speaking, the quasi-Fermi level concept was introduced for the Boltzmann distribution, which is not necessarily valid in the metal. The existence of thermionically limited transport implies that the electrostatic potential change in the semiconductor over a region whose width is smaller than the mean free path of the carrier should be larger than a couple of thermal voltages. This is known as the Bethe condition, and we will show its validity in our derivations. 4.2 Metal–Semiconductor Junctions 189 Figure 4.6: A schematic of drift (bottom half), diffusion (top half), and net currents as a function of position in the depletion region in thermal equilibrium (V = 0), forward bias (V > 0), and reverse bias (V < 0) of a metal– semiconductor junction. After H. K. Henisch, Semiconductor Contacts—An Approach to Ideas and Models, Clarendon Press, Oxford (1984). We can find metal–semiconductor combinations where either of these theories are better approximations. Materials with extremely poor mobilities, such as some of the p-type structures or some of the n-type II-VI materials, show transport limited by drift-diffusion in the semiconductor depletion region. Differing temperatures also affect the limiting mechanism. In this section, we will first derive the simple form of the drift-diffusion theory, then the thermionic emission theory and its modification including field emission, and finally we will unify these two theories to extend the validity to both limits of transport. The dominating component of the drift-diffusion mechanism, drift or diffusion, is dependent on the bias applied and is the cause of the rectification ability. Drift and diffusion at the rectifying junction lead to current in opposite directions. In forward bias, as seen in Figure 4.6, the drift component decreases because of a decrease in drift field, and hence the diffusion component predominates. In reverse bias, the drift current increases because of an increase in the field, and therefore, it determines the reverse current, unless generation effects predominate. 190 4 Transport Across Junctions 4.2.1 Drift-Diffusion We first consider transport assuming that the net current is limited by driftdiffusion transport in the depletion region. We will also assume that diffusivity and mobility are related by the Einstein relationship, i.e., the field strength is low enough for the non-degenerate junction. Consider a forward bias of V on a metal–semiconductor junction whose resultant depletion width is zd . Let J be the current flowing in the metal–semiconductor diode, and let us ignore generation–recombination effects. In terms of ψ, the electrostatic potential, integration of the current continuity equation following multiplication by the exponential factor exp (−qψ/kT ) yields Z zd qψ J exp − dz = kT 0 Z zd qψ qn exp − dψ+ qDn − kT kT 0 qψ exp − dn kT Z zd qψ qψ = qDn nd exp − + exp − dn kT kT 0 zd qψ . (4.10) = qDn n exp − kT 0 If recombination current is absent, current is constant, and we obtain z=z n exp (−qψ/kT )|z=0d J = qDn R zd . exp (−qψ/kT ) dz 0 (4.11) If we assume for convention that the electrostatic potential at the junction is the reference, we have and where ψ(0) = 0 ψ (zd ) qVn = = φB − Vn − V Ec − ξf (4.12) in the bulk. The carrier concentration at the junction and the junction depletion region edge are qφB n(0) = NC exp − , kT qVn and n (zd ) = NC exp − , (4.13) kT and hence Dn qφB qV J = q R zd NC exp − exp −1 . kT kT exp (−qψ/kT ) dz 0 (4.14) 4.2 Metal–Semiconductor Junctions 191 The exponential factor in bias voltage gives rectification character to the current. The second factor in this equation has units of velocity, and is sometimes called a drift-diffusion velocity because it indicates the average velocity with which carriers move via drift-diffusion in the depletion region. The use of the specific carrier concentration relationships above assumes the form of behavior of the quasi-Fermi level shown in part (a) of Figure 4.5. We may simplify this result in reverse and moderate forward bias, where depletion approximation holds. Specifically, the electrostatic potential then follows q 2 ND 2 q 2 ND qψ 2 = z − (zd − z) . kT 2s kT d 2s kT (4.15) Denoting the first term in the above as a2 and the second as η 2 , Z zd Z zd qψ exp − dz = exp −a2 exp η 2 dz kT 0 0 s Z a 2s kT 2 = exp −a exp η 2 dη 2 q ND 0 ≈ s kT , q 2 ND zd (4.16) where we have used the maximum magnitude of 1/2a of the error-function integral. This lets us write, for moderate bias conditions, s q 2 Dn NC 2q (ψj0 − V ) ND qφB qV exp − J= exp −1 . (4.17) kT s kT kT The pre-factor of the current–voltage relationship has a small voltage dependence. It can be ignored in the forward direction where the exponential term dominates, but in the reverse direction, where the exponential is small, it is this term, and the image force barrier lowering, that give rise to bias dependence. Also recall that we ignored generation and recombination in the derivation. In the reverse direction, where drift-diffusion current is small, the generation processes can predominate for materials with low lifetime. 4.2.2 Thermionic Emission In order for drift-diffusion to be a limiting step, the transport of carriers has to be considerably slow. The drift-diffusion approach assumes that the transport to the barrier is a rate-limiting step. More often, though, the transport is limited by injection over the barrier. A simple schematic of this is shown in Figure 4.7, which shows the Bethe condition for transport to be limited by the emission process at the metal–semiconductor junction. The Bethe condition states that for the transport at the metal–semiconductor junction to be limited by the interface, the width of the layer at the interface in the semiconductor 192 4 Transport Across Junctions Figure 4.7: Schematic showing the Bethe condition for transport to be limited by thermionic emission. The width of the region over which a kT drop in potential energy occurs at the barrier (zc ), should be much smaller than the the mean free path λ. zd is the depletion region width of the junction. across which a kT change in electrostatic energy occurs should be significantly less than the mean free path of the semiconductor.2 Let zc be the width of this region over which the kT change in energy occurs. zc λ (4.18) for emission at the metal–semiconductor interface to dominate. We will call this width the collision-less width to indicate its intent. The basis of this condition is that by ensuring it, one assures that the carrier distribution function at z = zc is independent of the current.3 If the carrier distribution function at zc and beyond is independent of the current, then it follows that the quasi-Fermi level in the region beyond is constant and the current is limited by the interface transport and not by the drift-diffusion transport in the bulk. Clearly, an implication of the above condition is that under large forward biases, where the region zc gets broad, the condition should be expected to break down. Thus, there are limitations to the bias conditions up to which we may apply the following analysis. At some high bias point, most semiconductors would require a unified thermionic emission and drift-diffusion description. From the semiconductor, the carriers emitted into the metal are the ones with sufficient energy and appropriate velocity in the collision-less region. Likewise 2 Our discussion here follows the arguments forwarded in F. Berz, “The Bethe Condition for Thermionic Emission Near an Absorbing Boundary,” Solid-State Electronics, 28, No. 10, p. 1007, Oct. 1985. Also, see discussion in G. Baccarani, “Current Transport in Schottky-barrier Diodes,” J. of Appl. Phys., 47, No. 9, p. 4122, Sep. 1976. 3 Strictly speaking, the electrostatic energy change should be more than kT to ensure sufficient change; more on this condition in the thermionic–drift-diffusion section. 193 4.2 Metal–Semiconductor Junctions from the metal, except that the large barrier height and large scattering rate of metals makes such a current small. Our analysis here follows a standard and intuitive approach. Later, in our discussion of thermionic–drift-diffusion transport, we will follow a more exact analysis that relaxes the approximation adopted here related to the distribution function being Maxwell–Boltzmann even at the metal–semiconductor interface. The total current density is the difference in the current flow from the semiconductor into the metal Jsm and the current flow from the metal into the semiconductor Jms . The former is the integral Z ∞ Jsm = qvz dn (4.19) ξn,sem +q(φB −V ) at the interface. This equation states that only those particles with sufficient energy to cross the barrier, and moving in the −z direction, actually cross the barrier. Assuming Boltzmann and parabolic band approximation, dn = 3/2 E − ξn,sem (2m∗ ) p E − E exp dE. c kT 2π 2 h̄3 (4.20) If we further assume that any excess energy is kinetic in nature, i.e., 1 ∗ 2 m v , 2 (4.21) Ec − ξn,sem m∗ v2 exp − exp − 4πv2 dv, kT 2kT (4.22) E − Ec = we get dn = 2 m∗ 2πh̄ 3 and Jsm 3 Z ∞ m∗ Ec − ξn,sem m∗ vx2 = 2q exp − exp − dvx × 2πh̄ kT kT −∞ ! Z ∞ m∗ vy2 exp − dvy × kT −∞ Z ∞ m∗ vz2 v exp − dvz , √ z ∗ kT − 2q(ψj0 −V )/m qφB qV ∗ 2 = A T exp − exp , (4.23) kT kT where A∗ = qm∗ k 2 2π 2 h̄3 (4.24) is known as the effective Richardson’s constant (120 A.cm−2 .K−2 for free electrons). The carriers in the metal in the very tail of the energy should be expected 194 4 Transport Across Junctions to have an exponential tail, even though they do not obey Maxwell–Boltzmann statistics. So, one should expect a similar exponential relationship qφB ∗0 2 , (4.25) Jms = A T exp − kT 0 where the constant A∗ does not necessarily have the same meaning or interpretation as in a semiconductor because of the differences in statistics of the two materials. However, at zero bias, since the two currents are equal, we obtain 0 A∗ = A∗ in this model. The resulting thermionic current can be written, as a function of applied bias of V , as the difference of these two currents qφB qV ∗ 2 J = A T exp − exp −1 . (4.26) kT kT Note that the functional form of this equation is the same as in the drift-diffusion theory. We know the effective mass for an isotropic (spherical constant energy surface) single valley semiconductor. However, what should it be for other semiconductors? For anisotropic constant energy surfaces, such as at L or X minima, or for degenerate bands such as light and heavy hole bands, the appropriate mass is obtained by summing over the relevant masses in the direction of injection, weighted by the probability of the occurrence of a carrier with that mass, i.e., the masses are weighted by the density of states. Problem 1 deals with this question. The effective mass, for arbitrary orientations, appropriate to the calculation of Richardson’s constant is 1/2 , (4.27) m∗ = mx my lz2 + my mz lx2 + mz mx ly2 where lx , ly , and lz are the direction cosines. For X-like minimas, this reduces to 1/2 m∗ = 2m∗t + 4(m∗l m∗t ) (4.28) for injection in h100i direction, and √ 1/2 m∗ = 2 3 m∗t 2 + 2m∗l m∗t (4.29) for injection in h111i direction. Similarly, for L-valleys, 1/2 4 m∗ = √ m∗t 2 + 2m∗l m∗t 3 (4.30) for injection in h100i direction, and m∗ = m∗t + m∗t 2 + 8m∗l m∗t for injection in h111i direction. 1/2 (4.31) 4.2 Metal–Semiconductor Junctions 195 Figure 4.8: The different components of injection at a metal–semiconductor barrier shown in forward (a) and reverse (b) bias. 4.2.3 Field Emission and Thermionic Field Emission Our discussion above has ignored quantum mechanical effects. Carriers that have the velocity and the energy to inject over the barrier may suffer quantummechanical reflections because of the abrupt barrier. Carriers that do not have the requisite energy or velocity to inject over the barrier may still cross into the metal by tunneling through the thin barrier. This finite non-zero probability of penetration can make a substantial difference in the magnitude of current at low temperatures where the thermionic current reduces due to lower density of carriers in the tails, as well as high dopings where the barriers are thinner. This emission behavior is often referred to as field emission, and its inclusion in the thermionic emission model leads to the thermionic field emission model. The field emission probability (see Figure 4.8) increases with temperature because electrons at higher energies see a thinner barrier with a lower barrier height. Since the field emission current over any energy range is proportional to the source function, the carrier concentration, and the characteristics of the barrier, at high energies it decreases again because of the decrease of carrier density at those energies. Thus, it peaks at a certain energy. For very high temperatures, the carrier density is high with high enough energy for crossing the barrier and most current is thermionic. Thermionic field emission current is thus important at low and intermediate temperatures, and high dopings. Simple calculations of tunneling probability usually invoke the WKB approximation (so named after Wentzel, Kramers, and Brillouin)4 that we will discuss later in the context of tunneling in heterostructures. It relates the elastic tun4 The WKB approximation allows us to determine the transmission probability accurately when the change in barrier is continuous. For discontinuous changes, the pre-factor changes and hence one can only determine the proportional dependence on the exponential term of WKB approximation. 196 4 Transport Across Junctions neling transmission probability Tt with the carrier momentum (or, equivalently, the reduced wave vector) through Z Tt ∝ exp −2 |kz | dz , (4.32) where tunneling is assumed to take place in the direction z. The larger the evanescent effect of the carrier momentum in a barrier or the longer the tunneling distance, the smaller the probability. The WKB approximation, for a triangular barrier, gives the result of probability for elastic tunneling transition as " √ # 4 2m∗ 3/2 (qφB ) . (4.33) Tt ∝ exp − 3h̄qE The maximum field at a metal–semiconductor junction is related to the junction potential (the diffusion potential), doping, and the permittivity through r 2qND ψj0 E max = , (4.34) s and hence we may write # 3/2 2(qφB ) p Tt ∝ exp − , 3E00 qψj0 " where E00 qh̄ = 2 r ND . m∗ s (4.35) (4.36) E00 is a characteristic energy parameter which determines, by virtue of its magnitude vis-a-vis the thermal energy, the temperature below which field emission becomes important.5 Figure 4.9 shows this parameter for some of the compound semiconductors. The lower density of states of most of the compound semiconductors and the smaller electron effective mass lead to smaller barriers that are easier to penetrate. Thus, field emission is relatively more important in compound semiconductors than in silicon. Thus, an accurate description of transport in metal– semiconductor junctions in compound semiconductors requires inclusion of both thermionic and field emission. The thermionic field current is given by a relation quite similar to the thermionic emission relationship, although it is relatively more complex to derive (see Problem 2). The current due to thermionic field emission is given by qV qV J = Js exp 1 − exp − , (4.37) E00 coth (E00 /kT ) kT 5 See F. A. Padovani and R. Stratton, “Field and Thermionic Field Emission in Schottky Barriers,” Solid-State Electronics, 9, p. 695, 1966. 4.2 Metal–Semiconductor Junctions 197 Figure 4.9: The characteristic energy E00 as a function of donor concentration for some of the semiconductors. The curve a identifies InAs, the curve b identifies GaAs, and the curve c identifies InP. where Js is related through p q πE00q (φB − V − Vn ) −q(φB + Vn ) exp Js = Jm , kT cosh (E00 /kT ) E00 coth (E00 /kT ) and Jm is the current density under flat band conditions, i.e., qVn Jm = A∗ T 2 exp − . kT (4.38) (4.39) Here qVn is the energy difference between the conduction band edge and the quasi-Fermi level in the bulk. In this relationship, with increasing temperature, the transition from field emission-dominated characteristics to thermionic emission-dominated characteristics occurs naturally through the property of the coth function. Note that the denominator of the voltage exponential asymptotically reaches either E00 in the low temperature limit or kT in the high temperature limit, again consistent with field emission-dominated behavior in the low temperature limit, and thermionic emission-dominated behavior in the high temperature limit. We had alluded to the importance of image force lowering, as well as quantummechanical reflections, to the transport. Image force lowering can be directly included by an appropriate change in the barrier heights. Since image force lowering also affects the shape of the barrier at the interface, it also subtly influences the field emission current of the above. Image force lowering also leads 198 4 Transport Across Junctions to a broadening of the barrier at the interface and hence leads to lower reflection problems, all of which increase the magnitude of the current. The image force effect and the effect of emission from the metal become stronger in reverse bias, which leads to thinner barriers for injection from the metal. In reverse bias, as shown in Figure 4.8, the current from the metal into the semiconductor increases while the current component from the semiconductor into the metal continues to decrease unless effects due to inversion occur at the interface. Increasing image force lowering, due to the increased field at the interfaces, continuously changes the apparent barrier height of the metal–semiconductor junction. Additionally, field emission and tunneling also increase with reverse bias, as does generation current. Hence, there is a continuous increase of the current with reverse bias which is much stronger than in p–n junctions. The current equation for thermionic field emission, where image force lowering was not included explicitly, continues to hold for reverse bias, except for the neglect of generation current. An approximation of it, for reverse bias V larger than a few thermal voltages, is qV E00 E00 − tanh J = −Js exp , (4.40) E00 kT kT where the approximation for Js is Js = √ 1/2 πE00 qφB A T × q (V − Vn ) + k cosh2 (E00 /kT ) qφB exp − . E00 coth (E00 /kT ) ∗ (4.41) In reverse bias, field emission occurs from the metal into the semiconductor through an approximately triangular barrier. Its low temperature limit is given by (see Problem 3) ! 3/2 2 E φ − V − V (2qφ ) 00 B n B √ J = A∗ 2 exp − . (4.42) k φB 3E00 qφB + qV − qVn We have discussed the implication of this field emission from the metal in increasing the reverse bias current; it is also the reason for ohmicity for the large number of ohmic contacts based on heavily doped metal–semiconductor interfaces. 4.2.4 Thermionic Emission-Diffusion theory We have now developed a description for transport across a metal-semiconductor junction based on thermionic emission and with tunneling effects incorporated in it to describe thermionic field emission. We have also developed the description based on drift-diffusion limited transport in the semiconductor depletion region. 199 4.2 Metal–Semiconductor Junctions The objective of a more general theory, that encompasses both thermionic emission and drift-diffusion, is to be applicable to metal–semiconductor junctions in both the limits, over wider bias range, for any semiconductor. A general theory also allows us to understand the relative importance of the two components of transport for any given semiconductor. Thus, a high mobility semiconductor would show a flat quasi-Fermi level to the metal–semiconductor interface, indicating that the drift-diffusion transport in the semiconductor is not ratelimiting. For a low mobility semiconductor, on the other hand, the quasi-Fermi level should change with position in the depletion region and reach the metal Fermi level at the metal–semiconductor interface, indicating that it is the ratelimiting step. To develop such an analysis, we need to express these currents—drift-diffusion in the bulk part of the depletion region, and thermionic emission in the interface part of the depletion region—in terms of the semiconductor parameters and the bias, and then we need to force them to be continuous, thus maintaining the required self-consistency. This requires us to obtain the quasi-Fermi level in the bulk, or equivalently the electron distribution function in the bulk as well as at the interface. The analysis follows, assuming as before a perfectly absorbing boundary condition at the metal–semiconductor junction, i.e., no quantum mechanical reflections, etc. Figure 4.7 showed a schematic description of the problem, broken up into the collision-less region of width zc at the interface responsible for thermionic emission, and the rest of the depletion region from zc to zd responsible for the drift-diffusion. First, we wish to obtain the carrier distribution as a function of the velocity distribution at the interface. All the carriers at the interface z = 0 with velocity in the direction of the metal cross the interface. Hence, at z = 0 the distribution function is hemi-Maxwellian, while at z = zc the distribution is Maxwellian for carriers. The current is given by Z ∞ J=q vf(v, z)dv (4.43) −∞ at any position z in the depletion region, where v is the velocity. Here we are expressing the distribution function as a function of velocity, which is equivalent to describing it in terms of momentum. Consider the forms of the distribution functions. For carriers beginning with velocity vc pointing towards the metal at the edge of the collision-less region zc , the velocity in the collision-less region evolves as 2 v(z) = vc2 − 2q [ψ(zc ) − ψ(z)] m∗ for 0 ≤ z ≤ zc . (4.44) At the interface, carriers with positive v(0) return back while those that are still negative cross the barrier. The carriers that return back to z = zc have velocity identical to when they started but of opposite sign. Therefore, at z = 0 carriers have velocities that p are less than zero only, and at z = zc the carriers have velocities less than 2q∆ψ/m∗ , where ∆ψ is the change in electrostatic 200 4 Transport Across Junctions potential in the collision-less region. In the absence of collision, the distribution function f(v, z) remains the same in the collision-less region, i.e., f(v, z) = f(vc , zc ) for 0 ≤ z ≤ zc . The distribution of carriers of interest at z = zc is m∗ v2 f(v, zc ) = B exp − 2kT p for v < 2q∆ψ/m∗ and zero otherwise. Likewise, at z = 0, m∗ v2 q∆ψ f(v, 0) = B exp − − 2kT kT (4.45) (4.46) (4.47) for v < 0 and zero otherwise. This distribution function is usually referred to as a hemi-Maxwellian distribution function since it is one of the hemispheres of the constant energy spheres in momentum space. By integrating the distribution function over all possible velocities, the carrier density at z = zc and z = 0 follow as r q∆ψ πkT 1 + erf , n(zc ) = B 2m∗ kT r πkT q∆ψ n(0) = B exp − , (4.48) 2m∗ kT and hence q∆ψ n(zc ) exp − . n(0) = 1 + erf (q∆ψ/kT ) kT (4.49) Recall the Bethe condition, which stems from the requirement that the carrier distribution function at z = zc be unaffected by the current, or equivalently that the carrier concentration at z = 0 be significantly smaller than that at z = zc . We may assure this by requiring the electrostatic energy change in the collision-less region to be 2kT or more. This will assure a large change in carrier concentration (see Problem 4). Since ∆ψ is factor of two or larger than the thermal voltage, the error function term is approximately unity and we obtain n(zc ) q∆ψ n(0) ≈ exp − . (4.50) 2 kT Note that the carrier concentration change is larger than what a flat quasi-Fermi level would have implied in this region (see Problem 5). The current follows from Equation 4.43 as r 2kT J = qn(0) , (4.51) πm∗ and one can define an effective velocity veff of transport across the interface as r 2kT veff = . (4.52) πm∗ 201 4.3. HETEROJUNCTIONS Recall our discussion of thermionic emission; this is half of the thermal velocity of the carriers. It averages the velocity in the hemisphere. In terms of carrier density at z = zc , the current can be expressed as r kT q∆ψ J = qn(zc ) exp − . (4.53) 2πm∗ kT We can now invoke the drift-diffusion effect on transport by considering the transport in the rest of the depletion region. If we assume a flat quasi-Fermi level, i.e., no drift-diffusion limitation on transport, then ψ(zc ) − ψ(zd ) n(zc ) = n(zd ) exp q (4.54) kT describes the relationship from the edge of the depletion region to the edge of the collision-less region. Hence, in the absence of drift-diffusion transport limitations, r kT q∆ψ ψ(zc ) − ψ(zd ) exp − J=q exp q , (4.55) 2πm∗ kT kT which is J = = r kT ψ(0) − ψ(zd ) exp q 2πm∗ kT qφB qV A∗ T 2 exp − exp . kT kT qNC (4.56) This is the expression for pure thermionic emission transport. However, if the quasi-Fermi level is not flat, i.e., drift diffusion to the interface is also important, then we must utilize the form similar to Equation 4.14 to relate the band bending, i.e., we relate the carrier concentration at z = zc with z = zd by considering the drift-diffusion current, and then force this current to be the same as the thermionic emission current in order to maintain current continuity. This allows us to write (see Problem 6) 1/2 J= qNC (kT /2πm∗ ) exp (−qφB /kT ) [exp (qV /kT ) − 1] . Rz 1 + (q/µkT ) (kT /2πm ) exp (−qφB /kT ) 0 d exp (qψ/kT ) dz ∗ 1/2 (4.57) This equation takes into account the hemi-Maxwellian distribution of carriers at the metal–semiconductor interface, the lack of collisions in a region of width zc λ over which the electrostatic energy changes by 2kT , as well as the supply of carriers by drift-diffusion across the depletion region. Problem 7 considers the thermionic emission and drift-diffusion limit of this expression. 4.3 Heterojunctions Heterojunctions are formed when two dissimilar materials are joined together at a junction using one of the materials growth techniques. Any arbitrary combination of semiconductors or semiconductors and insulators, or growth technique, 202 4 Transport Across Junctions does not necessarily result in a interface that can be of benefit in devices. Unique combinations, such as SiO2 /Si, or many of the lattice matched semiconductors (to be discussed in the context of heterostructure field effect transistors), result in interfaces with low interface density, and low interface scattering. These heterojunctions are the basis for field effect and bipolar devices. It is the transport properties, both perpendicular and parallel to the interface, that we utilize to advantage in these devices. The effect of low interface states is to allow us to control, in a very reproducible way, both perpendicular and parallel transport. For insulators, such as SiO2 , the perpendicular transport is of little concern since it is negligible (displacement current may still flow) except in breakdown conditions. For semiconductors, both are of interest. Semiconductor heterojunctions are the most popular form for compound semiconductors. This section follows a similar description as before in considering perpendicular transport through the junctions; parallel transport will be considered in our discussion of heterostructure field effect transistors. An additional complication, unlike the SiO2 /Si interface, for semiconductor heterojunctions is the effect of alloy grading, i.e., a changing of the composition of the semiconductor at the interface over a short distance. Such an arrangement is practiced in bipolar transport, its use in field effect transistors is largely to allow ohmic access to the channel of the device, since abrupt discontinuities lead to rectification. The abrupt discontinuities in these heterojunctions can appear both in the conduction band edge energy (∆Ec), and the valence band (∆Ev ), whose origin is the strong inter-atomic Coulombic effects that take place at the interface. Figure 4.10 shows three common forms (Type I, II, and III) of heterojunctions encountered. There is thus a variety of behavior that occurs in realistic semiconductor heterostructures; type I being the form that has been most extensively exploited in devices. Our discussion, throughout this text is principally with this type of heterostructure. This figure showed the discontinuities at an abrupt heterojunction. In general, these discontinuities are not related by differences in electron affinity, and hence throughout this text, following our earlier discussion of this subject, we use these as experimentally obtained parameters. Clearly, since compositional mixing can be achieved in semiconductor heterojunctions over short length scales, variations in discontinuities can also be achieved. Figure 4.11 shows, for an n-type Ga.7 Al.3 As/GaAs heterojunction, the conduction band edge and electron density for abrupt and linearly graded junctions. This is an idealization. We assume that one can obtain an abrupt change to linearly varying composition. However, the conclusion that the barrier height and the discontinuity can be varied in short grading regions is correct. Recalling our discussion of quasi-neutrality, the appearance of a discontinuity in band edges at a heterojunction clearly leads to a breakdown in quasi-neutrality as seen in Figure 4.11. However, following this earlier discussion, a long grading distance at a heterojunction leads to a decrease of the alloy field, an effect of the changing material characteristics, and the quasi-neutrality may be restored provided the Debye length criterion is satisfied. An effect of changing composition over a distance is that in this region the quasi-field for an electron may 4.3 Heterojunctions 203 Figure 4.10: Cases (a), (b), and (c) show schematically the band edges for the three common forms (Type I, II, and III) of semiconductor heterojunctions encountered. The lower half of these cases show the band diagrams with doping conditions commonly encountered. An example for case (a) is GaAs/Ga1−xAlx As, for case (b) is InAs/AlSb, and for case (c) is InAs/GaSb. 204 4 Transport Across Junctions Figure 4.11: The conduction band edge and electron quasi-Fermi level at abrupt and graded Ga1−xAlx As/GaAs heterojunctions. The background doping is assumed to be 1 × 1016 cm−3 and the grading distances for linear grading are 250 Å, 500 Å, and 1000 Å. 4.3 Heterojunctions 205 be different than the quasi-field for a hole, since the change in bandgap as a function of position results in differing changes in the conduction band edge and the valence band edge. We will consider this further in the discussion on heterostructure bipolar transistors. In this section, we consider transport across isotype interfaces, i.e., interfaces of the same polarity. Anisotype interfaces will be considered in our discussion of p–n junctions in the next section. 4.3.1 Thermionic Emission Conduction in heterojunctions should be expected to be similar in nature to the metal–semiconductor junction, except for some additional complexities. The behavior of electrons in the metal was characterized by a free electron mass, and a negligibly short distance over which the carrier injected from the semiconductor thermalized. The injection of carriers from the metal depended on the barrier formed with the semiconductor; no changes occurred in the injection as function of bias, since the barrier and the metal were left relatively undisturbed by the bias. When considering a semiconductor–semiconductor heterojunction, we have to consider changes in the distribution function on both sides of the junction. As an example, any applied bias is partitioned between the two semiconductors in a semiconductor–semiconductor heterojunction, while in a metal–semiconductor junction, the high conductivity of the metal forces the potential drop to occur in the semiconductor alone. We will consider the p–n heterojunction later; here we will consider an isotype heterojunction. Problem 8 considers the transport across the interface using the same procedure as in the thermionic–drift-diffusion theory of a metal–semiconductor junction. As we have discussed, usually, for electrons in the compound semiconductors, thermionic emission theory is adequate for a variety of conditions. Semiconductor heterojunctions, unlike the metal–semiconductor junctions, exhibit much larger field emission and other tunneling effects. This is a result of their smaller barrier height. Our analysis is, therefore, a simplified treatment of the problem of emission using the Maxwell–Boltzmann distribution approximation at the interface. Following Figure 4.12, we may determine the current components if we assume a Boltzmann distribution. Let ND1 and 1 be the doping and the dielectric constant of the large bandgap semiconductor and let ND2 and 2 be the corresponding values for the small bandgap semiconductor. The current flowing from 1 to 2, evaluated at the interface in the first semiconductor, is the product of the charge of the carriers, the number of carriers available for transmission to the second semiconductor, a transmission probability T12 for transmission into the second semiconductor, and the carrier velocity in the z-direction. The transmission probability T12 depends on the availability of states in the second semiconductor for the transmission. Since most of the states are empty in the high energy tail region, the transmission probability is close to unity for transmission in both directions. However, it is not identical. In our discussion of Richardson’s constant and maintaining zero net current at thermal equilibrium in the derivation of the 206 4 Transport Across Junctions Figure 4.12: An isotype n–n heterojunction between a large bandgap and a small bandgap material. The figure shows those carriers that can cross over the barrier if they have the minimum velocity required to cross the barrier. Note the potential drops on each side of the junction in this heterojunction case, in contrast to the case of metal–semiconductor junction. thermionic current in the metal–semiconductor junction, we invoked an argument based on equality of flux in the two directions to obtain the desired result. A Richardson’s constant–based approach will naturally fall out of a discussion of thermionic emission at a semiconductor heterojunction from both sides of the interface. Detailed balance requires that, at thermal equilibrium, these be identical. We will show based on arguments of momentum conservation that the two are related and result in the desired zero net current at thermal equilibrium. This current from semiconductor 1 to 2 (J12 ), due to thermionic emission, obtained by integrating over all possible velocities, and assuming a Maxwell– Boltzmann distribution function at the interface, is given by the integral R∞ R∞ R∞ qT12 ND1 vz exp −m∗1 vx2 + vy2 + vz2 /2kT dvxdvy dvz vzmin −∞ −∞ R∞ R∞ R∞ . (4.58) exp −m∗1 /2kT vx2 + vy2 + vz2 /2kT dvx dvy dvz −∞ −∞ −∞ This integral has the following basis. If we assume drift-diffusion as not being a limitation on transport and assume a Maxwell–Boltzmann distribution function, then the carrier distribution function at the metal–semiconductor interface can be related to that at the edge of the depletion region. This argument is similar to that used in reducing to the thermionic emission limit in our thermionic–driftdiffusion analysis of a metal–semiconductor junction. The limit of integration is appropriately shifted to account for this, and, as we shall show later, to account for conservation of momentum and energy during the emission. The expression above is written as a function of ND1 , the donor and carrier concentration, at the edge of the depletion region. vzmin is related to the emission barrier, which 207 4.3 Heterojunctions is related to the barrier height and the electrostatic potential V1 . V1 is the part of the applied potential that appears across the junction depletion region in semiconductor 1. Following Problem 9, the current may be written, in terms of the effective conduction band density of states NC1 and a momentum-space averaged emission transmission probability T12 , as s kT qφB0 qV1 exp − exp . (4.59) J12 = NC1 T 12 2πm∗1 kT kT Similarly, for the conduction from material 2 the small bandgap material to material 1 (the large bandgap material), this current (J21 ) is given by the integral R∞ R∞ R∞ qT21 ND2 vz exp −m∗2 vx2 + vy2 + vz2 /2kT dvx dvy dvz −vzmin −∞ −∞ R∞ R∞ R∞ exp −m∗2 /2kT vx2 + vy2 + vz2 dvx dvy dvz −∞ −∞ −∞ (4.60) where the minimum velocity, in a way similar to the previous case, is determined by the condition 1 ∗ 2 m v = qφB2 − qV2 , (4.61) 2 2 zmin where V2 is the part of the applied potential V that appears across semiconductor 2. This may be simplified to s kT qφB0 qV2 J21 = NC2 T 21 exp − exp . (4.62) 2πm∗2 kT kT The net current, which is the difference between these two components across the junction, is s " qV1 qφB0 kT J = q exp − T 12 NC1 exp − kT 2πm∗1 kT s # qV2 kT T 21 NC2 exp . (4.63) 2πm∗2 kT In thermal equilibrium, detailed balance in the above implies the condition T 12 NC1 T 21 NC2 p ∗ = p ∗ . m1 m2 (4.64) This condition is, within our approximations, a mathematical abstraction of the requirement of zero current in thermal equilibrium conditions. It should be viewed only as such, that the coefficient in the transmission of the hot carriers across a heterojunction discontinuity adjusts itself to allow the balance at thermal equilibrium. The consequences of the approximation of a Maxwell– Boltzmann distribution function as opposed to the hemi-Maxwellian distribution 208 4 Transport Across Junctions that may actually be more appropriate at the junction, and the self-adjustment of carrier distribution in order to account for current continuity, are all lumped into this phenomenological coefficient. Note that the current varies exponentially with bias and its magnitude depends on how the division of applied voltage occurs on the two sides of the junction. The division of voltage is related by Maxwell’s first equation, which relates the displacement vector with the interface charge. Problems 8 and 9 consider this example with its associated bias voltage partitioning. As can be seen, this behavior for a semiconductor–semiconductor heterojunction is considerably more complicated than that of the metal–semiconductor junction. Fortunately, many heterojunctions of interest are highly asymmetric in doping, and in cases where there exists a sufficiently large barrier, the problem reduces to the metal–semiconductor junction–like situation. An example is a larger barrier with high doping in the smaller bandgap semiconductor. For this problem, the smaller bandgap semiconductor behaves quite similar to the metal, and a thermionic equation based on the Richardson’s constant determined from the large bandgap semiconductor parameters suffices. Quite often, though, the dopings on both sides of junction are high; these are the basis for some of the ohmic contacts. In these cases, however, tunneling effects dominate. We now return to the question of thermal equilibrium in this problem and the proper form of Richardson’s constant.6 This question can be resolved by considering conservation laws of energy and momentum for the carrier emission at the interface. When an electron transits from one semiconductor to another, across the band discontinuity, it occupies different conduction band states determined by the band structure of the new semiconductor. In the process of doing so, assuming that this transit occurs without involvement of any scattering mechanisms that lead to energy loss or momentum change, energy and momentum must be conserved. Continuity of the wave function parallel to the interface actually requires a stricter condition of conservation of momentum parallel to the interface (kk ). The equation for conservation of energy, considering the transit across a discontinuity of ∆Ec, implies 2 2 h̄2 kk2 h̄2 kk2 h̄2 k⊥1 h̄2 k⊥2 + = ∆E + + . c 2m∗1 2m∗1 2m∗2 2m∗2 (4.65) For m∗1 < m∗2 , the constant energy surface for allowed wave vector components is an ellipsoid given by m∗1 2m∗1 ∆Ec m∗1 2 2 k⊥1 + 1 − ∗ kk2 = + ∗ k⊥2 . (4.66) m2 m2 h̄2 The selection criterion described by this conservation equation is shown in Figure 4.13. This matching implies that for thermionic injection from material 1 to 2, there exists a non-zero minimum in energy Emin , which is different from 6 This question has been discussed in detail in A. A. Grinberg, “Thermionic Emission in Heterosystems with Different Effective Electronic Masses,” Phys. Rev. B, 33, No. 10, p. 7256, 1986. Our arguments follow this analysis. 209 4.3 Heterojunctions Figure 4.13: A surface plot showing the allowed wave vectors that satisfy the conditions for conservation of thermionic emission energy and momentum during injection from a low mass m∗1 material across a discontinuity of ∆Ec into a larger mass m∗2 material. the value of energy discontinuity. This minimum is obtained from the matching condition for minimum energy Emin = ∆Ec − (m∗2 − m∗1 )Ek . m∗1 (4.67) With this minimum, the thermionic current is given by the integral Z ∞ Z ∞ Ek qm∗1 E⊥ qVn J= exp − exp − dE exp − dE⊥ . k kT kT kT 2π 2 h̄3 0 Emin (4.68) The integral for emission in the other direction is identical, and hence the apparent discrepancy is resolved. There exists one unique Richardson’s constant that describes the thermionic transport at the heterojunction. The ambiguity arises because of a simplified choice of minima for evaluation of the integral. Hence, the thermionic injection current for flow of carriers in the two directions is equal in thermal equilibrium. Also, it follows that the Richardson’s constant is determined by the smaller effective mass. 4.3.2 Tunneling We ignored tunneling in the above analysis. In the discussion of metal–semiconductor junctions, we included tunneling effects in the thermionic field emission theory 210 4 Transport Across Junctions for the junction. For transport at metal–semiconductor junctions, we treated thermionic emission as the dominant process of current flow, and field emission as a perturbation to the thermionic emission that increases the current. In our treatment of tunneling effects in heterojunctions, we will discuss the tunneling current by itself, because very often it is the dominating means of current flow in the heterojunction, owing to their smaller barriers and barrier widths. The discussion to this point has assumed that the electron energy is conserved during the tunneling transition, although we alluded to the possibility of inelastic processes also. Inelastic interactions can occur between the electrons and phonons, plasmons, etc. Tunneling in p–n junctions, with non-Γ conduction minima, such as in silicon and germanium, occur predominantly with phononassisted processes. This is necessary to allow for the change in the momentum. Optical phonon interaction occurs with a change in energy of h̄ωq . At low temperatures, phonon emission may still occur, but phonon absorption processes disappear because of the freeze-out of phonons. Also, for biases smaller than this threshold (h̄ωq /q), neither emission nor absorption can occur at very low temperatures. Thus at these low biases, phonon-assisted tunneling should be very temperature sensitive. This is unlike the temperature insensitivity of most tunneling processes in semiconductors because bandgaps and effective masses are very weakly temperature dependent. We briefly discuss tunneling in an indirect semiconductor versus a direct semiconductor to show the considerable variety one observes in tunneling in compound semiconductors of various thicknesses and barrier compositions. Consider the prototypical GaAs/Ga1−xAlx As/GaAs structure of Figure 4.14. This structure occurs in various forms in many devices both in field effect transistors (e.g., in SISFETs) and in coupled barriers. Tunneling may take place through processes based on Γ electrons alone, together with conservation of the energy of the electron. This would be most likely if the Ga1−x Alx As had a composition in the direct bandgap region. Even in the direct bandgap region, an electron in the Γ valley in GaAs may tunnel via the L or X valley in Ga1−x Alx As, together with the involvement of an inelastic scattering process. This means that the Γ valley electron may tunnel into the GaAs collector by coupling through the Γ barrier, the L barrier, or the X barrier. Up to a mole-fraction close to 0.4, the Γ barrier is the lowest, and most likely it would dominate the tunneling. But beyond that, the inelastic processes should dominate, since the material becomes indirect. For indirect bandgap Ga1−x Alx As, direct transitions would require the cold electrons in the Γ valley of GaAs to tunnel through a higher barrier unlike the indirect tunneling which occurs through a lower barrier. This makes it far less likely than the other inelastic processes. For increasing molefraction of aluminum arsenide, initially the L valley is lower, and finally the X valley is the lowest. Thus, at the highest mole-fractions, the X barrier may be the dominant cause of tunneling, barrier width permitting, even though the X valley is the third-highest valley in GaAs, and very few electrons start out from it. The larger the barrier width, the higher the likelihood of scattering, and hence the higher the likelihood of inelastic scattering in such structures. This is of importance to SISFETs as well as to coupled tunneling structures which we 4.3 Heterojunctions 211 Figure 4.14: Tunneling of a Γ electron by inelastic (a) and elastic process (b) in a GaAs/Ga1−xAlx As/GaAs structure. The spheres shown are in the constant energy surfaces for the tunneling electron; the differences in the radius represent the change in potential energy during tunneling. In (b), the parallel momentum remains constant while the perpendicular momentum changes. 212 4 Transport Across Junctions will discuss later in this book. Tunneling in indirect parts of the structure can be quite complicated because equi-energy surfaces are anisotropic, and depending on the orientation, they may not even be equivalent. Thus carriers occupying different energy surfaces may behave differently. As an example, consider Ga1−x Alx As at high AlAs molefractions, similar to silicon, for tunneling in the h100i direction. X valleys are the conduction band minima and the constant energy surfaces are as shown in Figure 2.26. A set of two ellipsoids and a set of four ellipsoids are equivalent for the purposes of tunneling, and the four-ellipsoid set is favored in tunneling because it has a lower transverse mass. Tunneling from the GaAs primary valley to these surfaces will still require the involvement of transfer of energy through scattering, and may occur with phonons, plasmons, interface scattering, etc. This problem of tunneling in semiconductor heterostructures for such situations will be revisited during our discussion of coupled barrier structures. We now consider the methods of analysis for determining the current densities in tunneling processes.7 We will consider the problem of a triangular barrier, which has already occurred as part of field emission in the metal–semiconductor junction, first. This is also among the earliest of tunneling problems to have been analyzed. It is related to emission from metal surfaces into vacuum, a reverse of the field emission problem from the semiconductor into the metal. An early theory for tunneling was developed by Fowler and Nordheim assuming a triangular potential barrier for the emission into vacuum. This theory, in a modified form, is relevant to semiconductor structures also. First, we will consider the exact solution to the problem of tunneling transmission through a triangular barrier; then we will use a simpler technique that can be the basis for more general solutions. Consider the triangular potential barrier shown in Figure 4.15. The Schrödinger equation for this single-body problem is − h̄2 2 ∇ ϕ + (V − E) ϕ = 0, 2m∗ (4.69) where ϕ is the eigenfunction and E the eigenenergy. For z < 0, V = 0, and for the triangular barrier, the barrier V is described by V = ξf + qφB − qEz (4.70) for z > 0, where E is the electric field, ξf the Fermi energy, and qφB the barrier height. The eigenfunction and the derivative of the eigenfunction are continuous. This is the statement of continuity of the probability of finding a carrier as a function of position and the continuity of the carrier’s momentum as a function of position. Mathematically, this means that at the classical turning 7 Tunneling is a very rich and diverse phenomenon. Two books, C. B. Duke, Tunneling in Solids in Solid State Physics—Advances in Research and Applications, Academic Press, N.Y. (1969) and E. Burstein and S. Lundqvist, Ed., Tunneling Phenomena in Solids, Plenum Press, N.Y. (1969), which are also general references for this chapter and Chapter 8, give a detailed account of this. Some of our discussion here and in Chapter 8 draws from these. 213 4.3 Heterojunctions Figure 4.15: Part (a) of this figure shows tunneling through a triangular barrier for an electron with energy less than the barrier height. Part (b) shows the classical turning points for this electron. points z = 0 and z = zT , ϕ(z = 0− ) = ∂ϕ = ∂z z=0− and ϕ(z = zT− ) = ∂ϕ = ∂z z=z− T ϕ(z = 0+ ), ∂ϕ , ∂z z=0+ ϕ(z = zT+ ), ∂ϕ . ∂z z=z+ (4.71) T The linear dependence of potential on z appears in a number of semiconductor problems; the one here is an example of a barrier, it also shows up as a well at a heterostructure interface in the small bandgap material. This differential equation, with a linear dependence on z for the term with the zero’th order derivative, is an example of Airy equation. The eigenfunction solution is ϕ(z) = A exp (jkx x + jky y) [exp (jkz z) + % exp (−jkz z)] (4.72) for z < 0, and ϕ(z) = B [Bi(η) + jAi(η)] for z > 0. Here, the normalized factor η is 1/3 2m∗ qE qφB + ξf − Ez η=− z− , qE h̄2 (4.73) (4.74) and Ai(η) and Bi(η) are Airy functions. For z < 0, there is no barrier, and the eigenfunction describes a plane wave. For z > 0, the eigenfunction is described as a linear combination of Airy functions. In these equations, A is an amplitude normalization factor for the plane wave eigenfunction, % is the reflection coefficient at the first classical turning point, and B is the amplitude normalization 214 4 Transport Across Junctions factor for the eigenfunction in the region z > 0. For values of z sufficiently farther than the first classical turning point, the Airy function solution has an asymptotic form, ϕ(z) = π2 |η| −1/4 π 2 3/2 B exp j exp j |η| . 4 3 (4.75) This is the transmitted wave at large distances. The probability current associated with this is 1/3 h̄ dϕ∗ h̄ 2m∗ qE 2 ∗ dϕ J=j ϕ −ϕ = |B| . (4.76) 2m∗ dz dz πm∗ h̄2 The transmission probability Tt can now be found because the incident wave was a plane wave of probability current h̄k/m∗ . For this barrier, #2 1/3 " 1/3 4 1 2m∗ qE 1 2m∗ qE Bi(η0 ) − Ȧi(η0 ) + Tt = πk k h̄2 h̄2 " #2 1/3 1 2m∗ qE Ai(η0 ) + Ḃi(η ) , (4.77) 0 k h̄2 where 1/3 2m∗ qE (qφB + ξf − Ez ) . (4.78) h̄2 This is a general result for the tunneling transmission probability in a triangular barrier, assuming a constant effective mass, and only elastic processes. We can, however, derive a simpler form based on expansion of the Airy functions, discarding the smaller terms of the series expansion. The asymptotic form of the barrier transmission probability, derived in this way (see Problem 10), is η0 = 1 qE 1/2 Tt = (ξf + qφB − Ez ) Ez 1/2 × ξf + qφB " r 3/2 # 4 2m∗ qE | qφB + ξf − Ez | exp − . 3 qE h̄2 4 (4.79) Knowing the tunneling transmission probability Tt , we can now derive the tunneling current. The current density in a small energy range dE, at the energy E, due to tunneling, is a function of the number of carriers available for tunneling described by a source function S(Ez ) which is related to the distribution function and the density of states, the tunneling transmission probability Tt , the charge, and the velocity of the carriers. Thus, the tunneling current density is given by Z ∞ h̄kz J =q Tt (E)S(Ez )dEz . (4.80) m∗ 0 215 4.3 Heterojunctions For an arbitrary problem, current density due to tunneling can be determined knowing the source function, which depends on the distribution function and the density of states, and integrating over the appropriate energy range. This integral could also be written in the momentum space as J= 2q 3 (2π) h̄ Z f(E)Tt (Ez ) ∂E dkz d2 kk, ∂kz (4.81) where the explicit dependence of the tunneling transmission probability on the perpendicular momentum is included. This calculation can now be performed exactly for our problem. First we determine the source function. The source function is directly related to the occupation probability related to Fermi–Dirac statistics and can be written as S(Ez ) = = 2 Z ∞ dkx Z ∞ dky f(E) (2π)3 h̄ −∞ −∞ 4πm∗ kT ξf − Ez ln 1 + exp . h3 kT (4.82) The tunneling transmission probability is given following Equation 4.79, and hence the tunnel current follows by integration of the product. For a triangular barrier, " √ # q 2 m0 E 2 4 2m∗ (qφB )3/2 J= exp − . (4.83) 16π 2 m∗ φB 3qh̄E Perhaps the most complicated step in this calculation was the determination of tunneling transmission probability. The source function or supply function can be quite easily determined because the occupation statistics and the density of states are known for the problems of interest. The characteristic of the barrier is what we are usually interested in determining since we do not know it as well. An approach similar to the above would be difficult for arbitrary cases. A simple example of this is a parabolic barrier. Metal-semiconductor junctions, p–n junctions, etc., all exhibit a parabolic barrier at the interface, if depletion approximation is applicable. The differential equation related to that is even more difficult to handle analytically, and perhaps a faster way would be to solve it numerically. This is at the expense of an intuitive insight that most analytical techniques provide. A common procedure to still handle these problems in closed form is to resort to the WKB approximation. Tunneling through the barrier results in an evanescent wave characterized by an imaginary momentum h̄k. The wave function during transmission through the barrier, therefore, has an exponential decay of the form exp(−jkz z), where the term within the brackets is real negative. The probability of finding the particle at any position z is proportional to the square of the accumulated decay of the eigenfunction. Thus, it stands to reason that the tunneling transmission probability, through a barrier whose 216 4 Transport Across Junctions classical turning points are zT 1 and zT 2 , is approximately given by Z zT 2 Tt (Ez ) ≈ exp −2 kz dz zT 1 s Z zT 2 ∗ (V (z) − E ) 2m z = exp −2 dz . h̄2 zT 1 (4.84) This is the WKB approximation that we had used earlier in the calculation of field emission current in a metal–semiconductor junction. The application of this to a triangular barrier where V decreases linearly with distance is straightforward. Indeed, the tunneling transmission probability is identical to the asymptotic approximation determined before (see Problem 10), and likewise the tunneling current density is determined as " √ # 3/2 4 2m∗ (qφB ) q 2 m0 E 2 exp − J = 16π 2 m∗ φB 3qh̄E " √ # 2 ∗ (qφ )3/2 mE 4 2m B = 1.54 × 10−6 exp − m∗ φB 3qh̄E E0 = αE 2 exp − , (4.85) E where E0 = √ 3/2 4 2m∗ (qφB ) . 3qh̄ (4.86) This can also be rewritten as ln J E0 . 2 = ln α − E E (4.87) This form of the tunneling current equation is called the Fowler–Nordheim equation. Tunneling current occurs in this form in a variety of problems where energy losses during tunneling are small and a triangular barrier is a valid approximation. Recall that we arrived at this form assuming elastic processes. Small losses in energy, e.g., through a single phonon process for carriers that are otherwise high in energy, also follow this behavior. Note that tunneling of higher energy carriers is favored because they encounter a smaller barrier. This functional relationship of current and field is encountered as an approximation in a variety of problems in semiconductor devices. Tunneling through insulators such as SiO2 is one common example, tunneling through larger bandgap barriers at heterojunctions is another example, and finally Zener tunneling where the barrier at a p–n junction can be idealized as a triangular barrier is another example. Note the lack of strong temperature dependence in all these cases because the effective mass is the strongest source for it. Tunneling current is a sensitive function of the field parameter E 0 . Let us consider some simple examples to show this sensitivity, assuming a barrier 4.3 Heterojunctions 217 Table 4.1: Characteristic field for tunneling for triangular barriers of various parameters. Barrier Height= Barrier Height= 0.8 eV 0.3 eV m∗ = m∗ = m∗ = m∗ = 0.067m0 0.5m0 0.067m0 0.5m0 E 0 (V.cm−1 ) 1.26 × 107 3.5 × 107 2.9 × 106 7.9 × 106 height of 0.8 eV to represent metal–semiconductor junctions and 0.3 eV to represent heterojunctions. We consider two effective masses, 0.067m0 to represent electron processes, and 0.5m0 to represent hole processes. Table 4.1 shows the magnitude of the field E 0 for these conditions. The smaller the characteristic field the larger the tunneling current density. Thus, factors-of-10 differences in electron tunneling current result from changes in barrier height typical of heterojunctions. This emphasizes the importance of tunneling currents in heterostructures. 4.3.3 Resonant Fowler–Nordheim Tunneling We now use an example where the WKB approximation is not a good predictor because it is a simplification of the description of wave propagation. Note that the exponential relationship only considers propagating waves in the direction of tunneling. Wave nature, however, can result in effects related to the interferences from reflections that occur at all the semiconductor discontinuities. Resonant Fowler–Nordheim tunneling is such an example resulting from the interference of the waves. Figure 4.16 shows a schematic of this in the triangular well formed at a triangular barrier when it is biased appropriately. Electrons that tunnel into the conduction band of the barrier can suffer quantum-mechanical reflection at the discontinuity, and hence can interfere constructively or destructively depending on the wave propagation properties. These interferences are directly related to the tunneling transmission probability, and appear as a modulation in the current–voltage behavior at low temperatures where elastic processes dominate and other current components can be suppressed. Such interferences can be observed in many of the heterojunction tunneling structures at low temperatures. Such resonance structures have also been observed in SiO2 /Si systems. This also serves as an example of elastic hot carrier tunneling in that system, because interference requires that the energy be identical. Since the barrier height at a SiO2 /Si interface is large, a large field is required to allow for the occurrence of the resonance condition. Large barrier structures thus exhibit this form of tunneling only at the highest biases. This phenomenon actually was among the earliest unambiguous demonstrations of scattering-free electron transport in semiconductor devices. As elastic processes become less likely, the occurrence of resonant processes also becomes 218 4 Transport Across Junctions Figure 4.16: A schematic example of resonant Fowler–Nordheim tunneling due to interference of the propagating waves. less likely because of its dependence on coherent interference. Even for indirect materials, so long as elastic tunneling can take place, such as in SiO2 /Si junctions, it can be observed. 4.4 Ohmic Contacts Our discussion of transport across junctions formed using metals with semiconductors and heterojunctions naturally leads us to a discussion of ohmic contacts. Ohmic contacts are needed in all semiconductor devices in order to allow a link through which current can flow and bias can be applied. Ohmic contacts are generally formed using heavy doping in structures to obtain large current flow without any significant bias drop across the ohmic contact regions. Current flow in these structures may be by any of the transport mechanisms that we have discussed. Ohmicity implies that the current is proportional to voltage, both in sign and magnitude. This can only occur over a limited current or bias range, because of the limitations on linearity. Contacts based on thermionic emission or thermionic field emission exhibit linearity over a smaller range because these processes are strongly non-linear. Tunneling processes exhibit linearity over a larger range. Heavy doping in all these cases serves to increase the currents and hence the current range of ohmicity; it also serves to minimize the potential drop in semiconductors. Heavy doping, therefore, also allows for reducing the effects of non-linearity from transport in the semiconductor itself by keeping the fields low. The ohmic access to a lightly doped region of a semiconductor device from a heavily-doped region, therefore, occurs quite commonly. We considered consequences of quasi-neutrality at such junctions in our discussion of drift-diffusion transport in Chapter 3. Doping changes should occur over length scales that 219 4.4 Ohmic Contacts allow for screening of the background charge, and hence suppression of any barriers caused by the background charge. Exponential changes in doping, such as those that occur in tails of Gaussian profiles or error function profiles, naturally lead to maintaining of quasi-neutrality. If quasi-neutrality is maintained, the current density resulting from majority carrier transport, in steady-state, is a product of charge density and carrier velocity. Since fields are small, and voltage drops across an ohmic region minimal, the time-dependent electric field variations during a transient are also small, and hence the steady-state calculation is also representative of the transient calculation. In compound semiconductor ohmic contacts, these large doping regions are usually implemented together with isotype heterojunctions or with metals. The implementation of the former specifically takes advantage of the lower barrier heights and hence higher tunneling transmission probability of heterojunctions; it is therefore a tunneling-based contact. The implementation of the latter occurs usually with larger barriers, and hence either thermionic field emission emphasizing tunneling near the top of the barrier—a temperature-sensitive process since it depends on electron energy distribution—or tunneling emphasizing processes at the bottom of the barrier—a temperature-insensitive process. Figure 4.17 shows some examples of such contacts. Parts (e) and (f) of this figure demonstrate an interesting variation on the common methods of forming ohmic contact. Fermi level pinning, which usually occurs in the bandgap, can also occur in the conduction or valence band. InAs, e.g., pins in the conduction band, and GaSb pins in the valence band. Such materials, therefore, show direct electronic conduction between the metal and the semiconductor. A suitable grading, following the requirement of quasi-neutrality, or an interface where an additional tunneling process has to be considered, allows one to link this contact region to the semiconductor of interest. Ohmic contacts are usually characterized by the parameters specific contact conductance (σc ), or specific contact resistance (ρc ), and defined by σc = 1 ∂J = ρc ∂V (4.88) where V is the applied bias voltage. We consider these parameters, for metal–semiconductor junctions, for the transport processes that we have analyzed in this chapter. The derivative of the expression for current can be used to show that the specific contact resistances (see Problem 11) are proportional to the exponential factors as ρc ∝ exp for thermionic emission, " qφB kT √ 4π m∗ s φB √ ρc ∝ exp tanh h ND (4.89) hq 4πkT r ND m∗ s !# (4.90) 220 4 Transport Across Junctions Figure 4.17: Band diagrams showing processes of transport at ohmic contacts based on tunneling-dominated transport ((a) and (b)), thermionic field emissiondominated transport ((c) and (d)), and utilizing Fermi level pinning in the bands ((e) and (f)). Parts (a) and (c) utilize metal–semiconductor junctions, (b) and (d) utilize heterojunctions, and (e) and (f) utilize Fermi level pinning in the conduction or valence band. 221 4.4 Ohmic Contacts Table 4.2: Specific contact resistances based on depletion approximation and tunneling through a triangular barrier. Barrier Height= Barrier Height= 0.8 eV 0.3 eV m∗ = m∗ = m∗ = m∗ = 0.067m0 0.5m0 0.067m0 0.5m0 σc (S.cm2 ) 1.26 × 107 3.5 × 107 2.9 × 106 7.9 × 106 for thermionic field emission, and ρc ∝ exp √ 4π m∗ s φB √ h ND (4.91) for field emission in a triangular barrier. Note the general features of these expressions. Thermionic emission processes are temperature-sensitive because they describe current transport due to emission from the hot electron tail of the distribution function. The magnitude of this resistance should be large. The thermionic field emission due to additional tunneling occurring in the higher energy tail of the carrier distribution function is less temperature-sensitive than the thermionic emission, but it is still significant. The tunneling for very thin barriers, assumed to be triangular, leads to least the temperature sensitivity because the thin barriers allow for tunneling of low-energy electrons. The last of these is the basis for many of the metal–semiconductor ohmic contacts. We can use our expression for Fowler–Nordheim tunneling, which is the dominant tunneling process, to derive the complete form of this conductance. Using Equation 4.85, E 0 dE dJ σc = = α (E 0 + 2E) exp − . (4.92) dV E dV The derivative of field with potential follows from the Poisson equation as 1/2 dE 2qND (φB − V ) =− , dV s (4.93) and hence the doping dependence. It is instructive to evaluate the magnitude of this conductance for some examples. We consider barrier heights of 0.6 eV and 0.3 eV, and a doping of 1×1020 cm−3 . The specific contact conductance is shown in Table 4.2. The calculation, although simplistic, is instructive. A smaller barrier, such as in a heterojunction, allows for low specific contact resistance if the semiconductor used in its formation can be accessed with a low specific contact resistance also. Holes, represented here by a larger effective mass, lead to a higher specific contact resistance for similar barrier heights. Light holes exist too, but the density of the light hole states is small and hence tunneling 222 4 Transport Across Junctions to these is less likely. In practice, barrier heights for holes is smaller, and the specific contact resistances for both electrons and holes is similar. The major approximations in the above relate to the exact determination of the fields, interface roughness that significantly enhances the field and hence the tunneling current, image force lowering which reduces the barrier height, heavy doping effects which introduce both Coulombic fluctuations and other band structure effects, interface oxides, etc. Clearly, depletion approximation is quite inappropriate and others only contribute to making the calculation more inexact. A more general expression of current can be derived for field emission where some of the approximations are relaxed (see Problem 12) as A∗ φB − V exp −q × J = α2 k 2 E00 παkT [1 − exp (−qαV )] − qαV exp [−α (ξf − Ec)] , sin(παkT ) (4.94) where α = ln [4 (qφB − qV ) /ξf ] /2E00 . In deriving this expression, we have assumed that 1/2 1 1 − αkT > kT . (4.95) 2E00 ξf The expression for specific contact resistance, assuming further that ξf − Ec − qV > 3kT and αV 1 (see Problem 12), is ρc = (k/qA∗ ) exp (qφB /E00) . (πT / sin(πα∗ kT )) − (1/α∗T ) exp [−α∗ (ξf − Ec)] (4.96) where α∗ is the magnitude of α at zero bias. The functional form is similar to the earlier field emission description in a triangular barrier. Isotype heterojunctions with large dopings on both sides of the junction and a metal–semiconductor junction with large doping in the semiconductor are two of the more common methods of forming ohmic contacts. Due to smaller barrier heights or barrier widths, in some of these cases even for moderate doping conditions, the barriers do not substantively impede the flow of current. One such example is the access to the two-dimensional electron gas at a heterojunction interface of a heterostructure field effect transistor. A low specific contact resistance can be obtained to the two-dimensional gas even if it is formed in a low-doped substrate. This low contact resistance mainly arises because of the low barrier height and width for carrier tunneling from the large bandgap material to the small bandgap material. The contact is still limited by the features of the barrier, and further lowering of the contact resistance may be achieved by grading of the barrier. Grading of the barrier lowers the barrier height and allows for more field emission. The contacts formed from a semiconductor through a heterojunction to a metal that exploit lower barriers in different semiconductors and their interfaces are particularly interesting in compound semiconductor devices. A set 4.4 Ohmic Contacts 223 Figure 4.18: Metal–semiconductor junctions formed with heterostructures using abrupt interface with Ge (a), abrupt interface with InAs (b), and graded interface with InAs (c). (a) and (b) are two examples where the tunneling theory is suitably applicable. The grading in the InAs contact is shown to occur pseudomorphically to a larger bandgap compound such as Ga1−xInx As or GaAs. 224 4 Transport Across Junctions of examples where this may be relevant is shown Figure 4.18. The choice for interfacial heterojunction is a semiconductor with favorable properties for formation of an ohmic contact. Examples for n-type GaAs are InAs and large InAs mole-fraction Ga1−xInx As which show negative barrier heights for conduction band, and Ge, which shows a low positive barrier height. Both of these contacts show minimal resistances (the sum of the specific contact resistance of the metal–semiconductor and the heterojunction interface). Because of the lower barrier height, heterojunctions may be kept abrupt. Abrupt heterojunctions between semiconductors of low barrier heights can be treated in a manner that we have already described. In these cases, the junction current as described by the tunneling current is simply Z 4πm∗ qkT ∞ Tt S(E)dE, (4.97) J= h3 Ec where the source function is S(E) = ln 1 + exp [(ξf − E) /kT ] 1 + exp [(ξf − E − qV ) /kT ] . (4.98) Ohmic contacts can also be formed using other techniques. Disorder at the interface, e.g., can lead to states in the band that allow hopping conduction leading to bias-symmetric conduction. One of the more common methods for forming ohmic contacts in GaAs utilizes a eutectic of gold and germanium. Thermal processing of this structure is commonly believed to lead to islands where an inter-metallic forms an ohmic contact to highly n+ doped regions of compound semiconductor, Ge providing the doping by substituting on the Group III element site. These islands provide conduction by lateral spreading of the current; the contact is non-uniform because it has spreading effects from the islands. Very small area contacts will not follow large area behavior. More importantly, the square root dependence on doping that one expects from the tunneling behavior is not followed. Instead, one sees an inverse dependence (see Problem 13) of the specific contact resistance. 4.5 p–n Junctions We discussed in chapter 3, transport in p–n junctions using the BTE approach, and we also discussed boundary conditions for p–n junctions in both low injection conditions and high injection conditions. Our analysis and discussion here will develop the necessary junction parameters, emphasize limitations of depletion approximation, discuss voltage drop across the quasi-neutral region in high level injection conditions, and develop a general charge control approach to analyze transport in p–n junctions. The latter approach, called Gummel– Poon model after its originators, is applied to a variety of conditions including recombination, a variety of doping profiles, and heavy doping conditions, to demonstrate the transport effects in p–n junctions. 225 4.5 p–n Junctions 4.5.1 Depletion Approximation We first consider, within depletion approximation, junction parameters of interest, and then we will consider limitations of the assumption of complete carrier depletion in the junction space charge region. Figure 4.19 shows band edges and carrier densities for a GaAs p–n junction.8 In the quasi-neutral part of either the p-type or the n-type material, N d2 ψ = −q = 0, dz 2 s (4.99) where ψ is the electrostatic potential. The sign of the charge used in the above equation corresponds to that of donors. In the quasi-neutral region, there exists no net charge density, and hence the electric field is constant. Since the electric field is negligible at the ohmic contact, electric field is negligible in the quasineutral region, and hence the electrostatic potential ψ is constant. In depletion approximation, i.e., ignoring the mobile carrier charge, in the depletion region on the n side, the electric field is given by E=− dψ qND = z + A. dz s (4.100) Electric field is zero at the edge of the depletion region (z = wn ) of the n-type semiconductor, hence the constant A=− qND wn , s (4.101) and ND (wn − z) (4.102) s in the depletion region. This expression is similar to that for a metal–semiconductor diode. Integrating again, Z ND z2 ψ = − Edz = q wn z − + B. (4.103) s 2 E = −q Using the boundary condition for the electrostatic potential in the n-type material, ψ = ψn at z = wn , we obtain ψ = ψn − qND 2 (wn − z) . 2s (4.104) qNA 2 (z + wp ) , 2s (4.105) Similarly, on the p-side we have ψ = ψp + 8 For the calculation of the depletion region widths, etc., we will assume origin to be at the metallurgical junction with the depletion region edge in the p-type material at z = −wp and in the n-type material at z = wn . 226 4 Transport Across Junctions Figure 4.19: Band bending and quasi-Fermi levels (a), and electron and hole densities (b) at a p–n homojunction in GaAs in thermal equilibrium. 227 4.5 p–n Junctions where depletion region edge is assumed to occur at z = −wp . For a homogeneous material, with no interface charge, both the electric field and the electrostatic potential are continuous at the junction (z = 0), i.e., ψp + and qNA 2 w 2s p qNA wp s 2ND 2 w 2s n = ψn − = qND wn . s (4.106) This allows us to write the charge on each side of the depletion region as 1/2 ND NA Q = qNA wp = qND wn = 2qs (ψn − ψp ) , ND + NA (4.107) where (ψn − ψp ) is the total band bending of the junction which is the built-in potential ψj0 , ND NA kT ln (4.108) ψj0 = q ni 2 in the Boltzmann approximation. We can also write the two depletion widths as 1/2 1/2 √ 2s ψj0 NA qψj0 NA wn = = 2λDn , (4.109) q (ND + NA ) ND kT (NA + ND ) and wp = 2s ψj0 ND q (ND + NA ) NA 1/2 = √ 2λDp qψj0 ND kT (NA + ND ) 1/2 , (4.110) where λDn and λDp are the Debye lengths in the n-type and p-type regions. Also, the total depletion region width is W = wn + wp = 2s ψj0 qND NA / (ND + NA ) 1/2 . (4.111) These expressions simplify for one-sided junctions because the effective doping is the geometric mean and it becomes the smaller doping for one-sided junctions. In reality, a mobile charge exists at the junction edges and under larger forward bias, and a significant mobile charge may exist within the depletion region. Close to the flat-band conditions of the junction, this charge can be considerable. Depletion region, therefore, is a misnomer for such conditions. The term space charge region is more appropriate. In this text, both are used interchangeably. Consider the inclusion of this charge at the edges of the junction depletion region, d2 ψ q (ND − n) q qψ = − = − N − n exp . (4.112) D i dz 2 s s kT 228 4 Transport Across Junctions If we consider the deviation of electrostatic potential from ψn given by ∆ψ = ψn − ψ, d2 ∆ψ q ψn − ∆ψ = ND − ni exp q dz 2 s kT qND q∆ψ = 1 − exp − . (4.113) s kT In the small region at the junction edge, with ∆ψ << kT /q, we may expand the exponential in a Taylor series expansion, and if we include only the first perturbation term, we obtain d2 ∆ψ q 2 ND ∆ψ . = ∆ψ = dz 2 s kT λD 2 (4.114) So, electrostatic potential actually deviates exponentially with a characteristic length given by the Debye length at the edge of the depletion region. Consequently the mobile charge density falls off in significance exponentially. The significance of this exponential fall-off is that we may use its characteristic length, the Debye length, to judge the appropriateness of the use of depletion approximation. If the depletion region width on either side is comparable to the Debye length, then the depletion approximation is clearly invalid. We have and wn λDn = wp λDp = 2qψj0 ND kT (NA + ND ) 2qψj0 NA kT (NA + ND ) 1/2 1/2 , . (4.115) Consider an abrupt one-sided GaAs n+ –p junction with dopings of 5 × 10 cm−3 and 5 × 1014 cm−3 . The built-in voltage for this junction kT ND NA ln ψj0 = = 1.19 V, (4.116) q ni 2 17 and hence, wn /λDn = .3, and wp /λDp = 9.6. On the higher-doped side, the depletion approximation is poor, because a substantial electron density occurs throughout the depletion region in this n-type region. On the other hand, for a symmetric junction of 1 × 1016 cm−3 doping, the built-in voltage of the junction is 1.16 V, and wn /λDn and wp /λDp are ≈ 6.7, making the depletion approximation a good one on both sides of the junction. Similarly, for a large doping symmetric junction of 5 × 1017 cm−3 , ψj0 = 1.36 V, and wn /λDn and wp /λDp are ≈ 7.3, a good depletion approximation. Thus, one-sided junctions lead to breakdown of the depletion approximation in the higher-doped side. The approximation is poorest because potential drop across the heavily doped layer is lower due to asymmetry and hence the depletion width in the higher-doped side is smaller. 229 4.5 p–n Junctions 4.5.2 High-Level Injection We considered the low-level injection behavior of p–n junctions quite extensively during the discussion of Shockley, Fletcher, and Misawa boundary conditions. We will analyze the problem further by considering the behavior of p–n junction in high-level injection. In particular, we are interested in determining the voltage drops across the n-side and the p-side. Let J be the total current through the device. Our transport equation for the n-side is ∂nn , ∂z (4.117) Dn ∂nn Jn − . qµn nn µn nn ∂z (4.118) Jn = qµn nn E + qDn and hence E= Particle current flows both as electron and hole current, therefore, Jn (z) = J − Jp (z), (4.119) and hence we get the expression for the electric field as E(z) = J Jp (z) kT ∂nn − − . qµn nn (z) qµn nn (z) qnn ∂z (4.120) On the n-side again, we may express the hole current directly, and substitute the above for the electric field. This allows us to express the hole current density as Jp (z) = = ∂pn qµp pn E(z) − qDp ∂z J Jp (z) kT ∂nn − − qµp pn (z) − qµn nn (z) qµn nn (z) qnn ∂z ∂pn (z) qDp . ∂z (4.121) Since charge neutrality implies ∂pn (z) ∂nn (z) = , ∂z ∂z we can simplify this to yield µp pn (z) pn (z) ∂pn (z) 1 Jp (z) = J − qDp 1 + µn nn (z) nn (z) ∂z µ p (z) 1+ p n µn nn (z) (4.122) (4.123) as the expression for hole current, and, substituting back in the electric field expression, E(z) = J Dn − Dp ∂pn (z) − q(µn nn (z) + µp pn (z)) (µn nn (z) + µp pn (z)) ∂z (4.124) 230 4 Transport Across Junctions as the expression for the electric field. Note that this actually follows from the the total current relation dpn (z) dpn (z) − qDp , (4.125) dz dz where σ is the conductivity of the material which also includes high-level injection effects. We can now determine the voltage drop across either of the semiconductor regions. Let Vn be the change in electrostatic potential on the n-side; it is given by Z J = σE(z) + qDn zn Vn = − wn E(z)dz, where zn is the position of the ohmic contact to the n-type material. neutrality and the junction boundary conditions allow us to write z , pn (z) = pn0 + ∆pn exp − Lp z nn (z) = nn0 + ∆nn exp − , Lp ∆pn = ∆nn , qVj and ∆pn = pn0 exp −1 , kT and hence Vn = (4.126) Charge (4.127) (4.128) (4.129) (4.130) Z J zn 1 dz − q wn (µn nn0 + µp pn0 ) + (µn + µp )∆pn exp (−z/Lp ) Z pn0 (Dn − Dp ) dpn . (µ n + µ p ) + (µn + µp )∆pn exp (−z/Lp ) n n0 p n0 pn (wn ) (4.131) This may be written in the form of the integrable expression Z J zn 1 Vn = dz − q wn (µn nn0 + µp pn0 ) + (µn + µp )∆pn exp (−z/Lp ) Z pn0 1 (Dn − Dp ) dpn , (µ n − µ p ) + (µn + µp )pn (z) n n0 n n0 pn (wn ) (4.132) and finally, following integration, Vn = J(zn − wn ) JLp + × q(µn nn0 + µp pn0 ) q(µn nn0 + µp pn0 ) (µn nn0 + µp pn0 ) + (µn + µp )∆pn exp [− (wn − zn ) /Lp] log − (µn nn0 + µp pn0 ) + (µn + µp )∆pn Dn − Dp (µn nn0 + µp pn0 ) log . (4.133) µn + µp (µn nn0 + µp pn0 ) + (µn + µp )∆pn 231 4.5 p–n Junctions This describes completely, in terms of known prameters, the total voltage drop across the n-side of the junction. Its simplification, at low level injection (i.e., nn0 >> pn0 , ∆pn ) where the logarithmic terms are negligible, is simply Vn = J(zn − wn ) , qµn nn0 (4.134) or E = = Vn zn − wn J , qµn nn0 (4.135) which is Ohm’s Law because the denominator is the conductivity of the semiconductor. A similar expression may be found for the p-side. Usually, though, junctions are one-sided and the high-level injection effects need to be included on only one side of the junction. These relations relate the current density to the voltage drop in the quasi-neutral region. The relationship between the current and electrostatic potential at the junction is known from Chapter 3. The applied voltage is partitioned between the junction and the quasi-neutral region at highlevel injection. These form a complete set of equations to determine the current for the applied bias at the device terminals. Figure 4.20 shows the characteristics of a symmetric p–n junction under conditions of medium- and high-level injection. The diode in this example is a short diode, where the diffusion length is larger than the base width—the width of the quasi-neutral region. Depletion approximation is quite valid at low-level injection conditions, and the exponential drop in the carrier concentration is also demonstrated under these conditions. The potential drop is negligible in the low-level injection conditions, and all the applied potential drops at the junction. Figure 4.20 shows the changes from this at medium- and high-level injection. At medium-level injection conditions, some deviation in majority carrier concentration occurs because the minority carrier concentration is becoming significant, and the change maintains quasi-neutrality away from the junction. Almost all of the voltage still drops across the junction. Under high-level injection conditions, a significant injection of minority carriers occurs, and an equal change in majority carrier concentration occurs to re-establish quasi-neutrality. The electric field needed to maintain this gradient in the majority carriers is now clear in the variation of the conduction band edge as a function of position. Also note from this variation of the conduction band edge, and the variation of the quasi-Fermi level, that both diffusion and drift current flow now occurs in the base of the p–n junction. The low and medium injection conditions show current transport only through diffusion. Figure 4.21 shows the current–voltage behavior of a GaAs diode; this example assumes a large lifetime and diffusion length. At the lowest biases the current 232 4 Transport Across Junctions Figure 4.20: Band edges and electron and hole concentration in a symmetric GaAs p–n junction under medium- (a), and high-level (b) injection. The thermal equilibrium conditions for this junction are shown in the previous figure. Figure 4.21: Current-voltage characteristics of an idealized one-sided n+ –p GaAs junction as a function of applied bias. The n+ -type doping is 5×1018 cm−3 and the p-type doping is varied between 1017 cm−3 and 1018 cm−3 . 4.5 p–n Junctions 233 increases exponentially, at the rate of 60 mV/decade in current. This increase is characteristic of the exponential current–voltage relationship that characterizes transport in an ideal p–n junction. It occurs because the flat quasi-Fermi level at the low-level injection condition relates the carrier concentration at the edges of the depletion region by the Boltzmann factor. Therefore, in the presence of diffusion-dominated transport in the low-level injection condition, and with low recombination effects so that electron and hole current densities are constant in the depletion region, the current also varies exponentially. Deviation from this behavior at the higher-level injection condition comes about because now the junction voltage is smaller than the applied voltage, and because of the high injection, both diffusive and drift transport occur. Note also that in the exponential region the current is only very weakly dependent on the doping of the lighter doped side. It is the strongest function of the built-in voltage which is only a weak function of doping. This discussion assumed transport with perfect ohmic contacts, i.e., contacts where the excess carrier concentration was zero. We have discussed modelling of contacts by a surface recombination velocity that relates this excess carrier concentration above its value at thermal equilibrium. Problem 29 considers incorporation of such boundary conditions in analyzing the behavior of p–n junction diodes. 4.5.3 Gummel–Poon Quasi-Static Model The Gummel–Poon model implementation9 for p–n junctions and bipolar transistors is a useful approach for predicting the the quasi-static transport behavior of an arbitrary device. In our discussion of p–n junctions to this point, we have only considered uniform dopings. It may be desirable in certain structures to have varying doping profiles. p–n junctions with large dopings occur with bandgap grading due to bandgap shrinkage. Alloy grading of heterostructures occurs with bandgap grading also. These devices can, thus, have varying quasifields in the base either with a doping gradient or an alloy gradient. Gummel– Poon modelling is a convenient mechanism to precisely predict the quasi-static behavior for such a variety of structures. It is also useful for complex recombination situations. Our model is a simple extension of the homojunction model to include the heterostructure and the bandgap grading in the base. It is useful at both low and medium current densities. Consider the references and charge parameters for an arbitrary p–n junction as described in Figure 4.22. Qp and Qn describe the integrated charge due to majority carriers in the quasi-neutral region on both sides of the junction, while Qpn and Qnp are the corresponding integrated minority carrier charge densities. The ohmic contacts are located at z = −zp and z = zn for the p-type and n-type regions, and z = −wn and z = wp are the positions of the edges of the depletion region. 9 H. K. Gummel and H. C. Poon, “An Integral Charge Control Model of Bipolar Transistors,” The Bell System Technical Journal, p. 827, May-June 1960, discusses the application of the approach in bipolar transistors. 234 4 Transport Across Junctions Figure 4.22: References for analysis of p–n junctions using the quasi-static Gummel–Poon approach; Qp and Qn are the integrated majority carrier charge densities in the p-type and n-type quasi-neutral regions, Qpn and Qnn are the integrated minority carrier charge densities in the quasi-neutral regions. 235 4.5 p–n Junctions The continuity equations for steady-state are ∂Jn = q [R(z) − G(z)] ∂z (4.136) ∂Jp = −q [R(z) − G(z)] ∂z (4.137) for the electron current and for the hole current. We will employ these equations, which describe the positional change of the current density, to write equations for the current density as a function of its magnitude at the contacts. Since current continuity requires the current at the two contacts to be the same, this will allow us, by referencing to either of the contacts, to write an equation for the current in terms of the changes in the quasi-Fermi level which may then be related to the voltage for different injection conditions, just as we did in the boundary condition analysis. In doing this, several well-defined integrals occur, which are variously referred to as Gummel or modified Gummel numbers. The origin of these integrals can be traced to the charge in the quasi-neutral regions, modified by factors such as alloy grading, bandgap changes, and differing diffusivities or mobilities, all of which affect current transport. In low-level injection, for uniformly-doped short diodes, the minority carrier current is proportional to the minority carrier density at the edges of the depletion region, and inversely proportional to the width because these two parameters define the gradient of the minority carrier charge density. The minority carrier charge density is directly related to the exponential of the junction bias—the Boltzmann factor—and the minority carrier density at thermal equilibrium. The minority carrier density, thus, is inversely related to the majority carrier density, which is a constant for a uniformly-doped and uniform-alloy composition junction in low-level injection. Under these conditions, the current density is inversely proportional to the majority carrier charge density and the width of the quasi-neutral region, i.e., the integrated majority carrier charge densities Qn and Qp . These are the simplest forms of Gummel numbers applicable if alloy grading, bandgap changes, diffusivity or mobility changes as well as other injection effects are negligible, and the p–n junction is a short junction. Our derivation allows for the inclusion of these, and hence we generate modified Gummel numbers,10 which are more complex in form, but more generally applicable. Our major limitation will be that current transport is considered by drift-diffusion alone. Thus, it is not applicable to devices with any rapid changes in alloy composition that lead to band edge discontinuities and thermionic transport. In the absence of recombination, current density for electrons and holes is constant in the junction region, the sum of which is the total current in the 10 For a basis of this modification, see A. H. Marshak and K. M. Van Vliet, “Carrier Densities and Emitter Efficiency in Degenerate Materials with Position-Dependent Band Structure,” Solid-State Electronics, 21, p. 429 (1978), and A. H. Marshak and C. M. Van Vliet, “Electrical Current and Carrier Density in Degenerate Materials with Non-Uniform Band Structure,” Proc. of IEEE, 72, No. 2, p. 148 (1984). 236 4 Transport Across Junctions device. This constant current density in the junction region for both carriers is used as the basis for the calculation of total current density in the simpler diode problem. It allows us to determine the minority carrier current density at the junction edges and hence the current density of the diode. These minority currents are diffusive, i.e., there exists a gradient in the minority carrier density in the quasi-neutral region. The current supports this carrier distribution. The converse is also true: the carrier distribution supports this current. If we integrate the current continuity equation from the contacts, the electron current density at any position z may be written w.r.t. its magnitude at one of the contacts as Z zn Jn (z) = Jn (zn ) − q [R(z) − G(z)] dz, (4.138) z and Jn (z) = Jn (−zp ) + q Z z −zp [R(z) − G(z)] dz. (4.139) The first term in the former equation is related to the injected or extracted electron current density and the second is related to generation–recombination current. The second term relates the exchange between the minority and majority carrier current density. A decrease in minority carrier current occurs with an increase in majority carrier current, and in the process, the total current remains constant. A similar set of equations for the hole current density are Z z Jp (z) = Jp (−zp ) − q [R(z) − G(z)] dz, (4.140) −zp and Jp (z) = Jp (zn ) + q Z z zn [R(z) − G(z)] dz. (4.141) Electron current is injected through the n-type region, and hole current through the p-type region, thus, the terms Jn (zn ) and Jp (−zp ) are the injected electron and hole current densities. The total current density remains constant in this one-dimensional analysis, and at any cross-section, the total current density is given by J(z) = = Jn (z) + Jp (z) Z zn Jn (zn ) − q [R(z) − G(z)] dz + Jp (−zp ) − z Z z q [R(z) − G(z)] dz −zp = Jn (zn ) + Jp (−zp ) − Jgr (−zp ). (4.142) The current density Jgr (z) is the integral of the charge generation–recombination rate from any position z in the diode to the end of the device defined by the n-side ohmic contact, Z zn Jgr (z) = q [R(z) − G(z)] dz. (4.143) z 237 4.5 p–n Junctions This definition allows us to write more succinct forms of the spatial dependence of the current density as Jn (z) = Jn (zn ) − Jgr (z) (4.144) Jp (z) = Jp (zn ) + Jgr (z). (4.145) and Both electron and hole current densities are the largest at the ohmic contacts of their respective majority carrier regions. The hole current density decreases from the p-contact to the n-contact, while a corresponding increase occurs in the electron current density. The decrease in hole current density appears as an increase in the electron current density and vice-versa. An equation, similar to Equation 4.142, can be written by using the opposite references. This equation is therefore written in terms of the minority current densities at the contacts instead of the majority current densities. J(z) = Jn (−zp ) + Jp (zn ) + Jgr (−zp ). (4.146) This equation may be viewed as being in terms of collected currents since the minority carriers are injected by majority carrier regions. The total current is the sum of the minority carrier current at the contacts and the Jgr (−zp ) term due to generation–recombination effects that characterizes the exchange current of carriers. The carrier transport can now be written using drift-diffusion formalism. We write the currents in terms of the quasi-Fermi potentials φn and φp for electrons and holes, and the electrostatic potential ψ. We have Jn = −qµn n where ∂φn , ∂z q(ψ − φn ) n = ni exp . kT For hole current density, we have Jp = qµp p where (4.148) (4.149) q(φp − ψ) . (4.150) kT Using the Einstein relation, and quasi-Fermi potentials instead of carrier densities as the variable, current density can be written as q(ψ − φn ) ∂φn Jn = qµn ni exp kT ∂z kT qψ ∂ qφn = qµn ni exp exp − q kT ∂z kT qψ ∂ qφn = qDn ni exp exp − . (4.151) kT ∂z kT p = ni exp ∂φp , ∂z (4.147) 238 4 Transport Across Junctions This relates the change of quasi-Fermi levels for electrons to the electron current density as ∂ qφn Jn (z) exp − = . (4.152) ∂z kT qDn ni exp (qψ/kT ) We may now relate the changes in quasi-Fermi potential to its magnitude at the contacts. Integrating from the p-type ohmic contact to the n-type ohmic contact (−zp to zn ), Z zn qφn (zn ) qφn (−zp ) Jn (z) exp − − exp − = dz. (4.153) kT kT qD n exp (qψ/kT ) n i −zp The current density at any position is related to the current density at the contact and the generation–recombination term through the identity Jn (z) = Jn (zn ) − Jgr (z). Thus, qφn (zn ) qφn (−zp ) exp − − exp − = kT kT Z zn Z zn 1 Jgr Jn (zn ) dz − dz, −zp qDn ni exp (qψ/kT ) −zp qDn ni exp (qψ/kT ) (4.154) and hence, the majority carrier current at the contact at z = zn can be written as "Z #−1 zn 1 Jn (zn ) = dz × −zp qDn ni exp (qψ/kT ) qφn (zn ) qφn (−zp ) exp − − exp − + kT kT ) Z zn Jgr (z) dz . (4.155) qD n exp (qψ/kT ) n i −zp The total change in the quasi-Fermi potential between the two ohmic contacts is the applied voltage V across the diode, i.e., V = φn (−zp ) − φn (zn ) . (4.156) This assumes a perfect ohmic contact with no voltage drop across it; more complicated conditions, e.g., using finite surface recombination velocity, can also be incorporated. For now, we consider ideal contacts. We multiply and divide by the factor exp [qφn (−zp )/kT ], giving (Z )−1 zn exp [q (φn (−zp ) − ψ) /kT ] Jn (zn ) = dz × qDn ni −zp qV exp −1 + kT 239 4.5 p–n Junctions Z zn −zp ) Jgr (z) φn (−zp ) − ψ exp q dz . qDn ni kT (4.157) This is a general form of the expression for electron current density for arbitrary situations with doping, alloy composition, and bias variations in a onedimensional geometry. It is a complicated form, which relates the currents through integrals of terms involving elementary charge, the diffusion coefficient, and the majority charge density. These integrals are the various forms of modified Gummel numbers. Equation 4.157 is the basic expression that we will refer to in complicated problems, but to demonstrate its utility even in simpler forms, we will consider homojunction structures. A convenient form, then, is qni 2 qV Jn (zn ) = exp −1 + Γn kT Z zn 1 Jgr (z)ni φn (−zp ) − ψ exp q dz, (4.158) Γn −zp Dn kT where Γn = Z zn −zp ni φn (−zp ) − ψ exp q dz Dn kT (4.159) is one form of the Gummel number for electrons. Following similar procedures, an expression may be written for hole current (see Problem 14) for the general case as "Z #−1 zn 1 dz Jp (zn ) = × −zp qDp ni exp (−qψ/kT ) qφp (−zp ) qφp (zn ) exp − exp − kT kT ) Z zn Jgr (z) dz , (4.160) −zp qDn ni exp (−qψ/kT ) which, under the restricted condition of no alloy grading, reduces to qni 2 qV Jp (zn ) = exp −1 − Γp kT Z zn 1 Jgr (z)ni ψ − φp (zn ) exp q dz, Γp −zp Dp kT where Γp = Z zn −zp ni ψ − φp (zn ) exp q dz Dp kT (4.161) (4.162) is a Gummel number for holes. These expressions for Gummel numbers have been written in terms of the quasi-Fermi potentials, the electrostatic potential, and the intrinsic carrier concentration. They are in a general form that is 240 4 Transport Across Junctions applicable to high-level injection or long base conditions. Under these arbitrary conditions, the total current, a constant at any bias, flowing in the diode can be written as J(z) = = Jn (zn ) + Jp (zn ) 1 1 qV qni 2 + exp −1 + Γn Γp kT Z zn Jgr (z)ni φn (−zp ) − ψ 1 exp q dz − Γn −zp Dn kT Z zn 1 Jgr (z)ni ψ − φn (−zp ) exp q dz. Γp −zp Dp kT (4.163) We continue to assume perfect ohmic contacts with quasi-Fermi level position defined by the majority carrier, the excess minority carrier concentration going to zero, and the voltage drop at the contact negligible. The assumption of perfect ohmic contacts implies φp (−zp ) = φn (−zp ) (4.164) φp (zn ) = φn (zn ) . (4.165) and We now restrict our discussion to applications involving low-level injection. Under these conditions, the quasi-Fermi potentials φn and φp remain approximately constant in the quasi-neutral regions and the junction space charge region. The Gummel number for electrons can then be written as Z zn ni φn (−zp ) − ψ Γn = exp q dz kT −zp Dn Z zn ni φp (−zp ) − ψ ≈ exp q dz. (4.166) kT −zp Dn The Gummel number can be evaluated by integrating over the device depth. The carriers are majority carriers in part of the device; the integrand in this region is large. In the space charge region, and in the region where they are minority carriers, this magnitude is usually small in low-level injection. Using references from Figure 4.22, we have Z −wp Z zn p ni φp (−zp ) − ψ Γn = dz + exp q dz, (4.167) kT −zp Dn −wp Dn where the integral is related to majority carrier density (holes) in the p-type region, and the last term is in a region where the integrand is small. Usually, therefore, in low-level injection, the last term is small, and we obtain Z −wp p Γn ≈ dz. (4.168) −zp Dn 241 4.5 p–n Junctions Similarly, we may find the hole Gummel number, whose major term is due to the electron charge density in the n-type region, i.e., Z zn n dz. (4.169) Γp ≈ D p wn In their original formulation, Gummel and Poon considered the integrated charge as the basis for the integral equations. These unmodified Gummel numbers were defined as Z zn Qn GNn = = ndz (4.170) q wn and GNp = Qp =q q Z −wp pdz. (4.171) −zp If the diffusivity is constant, intrinsic carrier concentration is constant, and lowlevel injection conditions exist, then the Gummel numbers of Equation 4.159 and 4.162 are equivalent to these. The effect of varying diffusivity of carriers is effectively incorporated in the unmodified Gummel–Poon approach by using the weighted diffusion coefficients D n and Dp . We may write these relationships as and 1 Γn = qDn Qp 1 Γp = qDp , Qn where and Dn = Dp = R −wp −zp (4.172) pdz R −wp (p/Dn ) dz R zn ndz R zn wn . (n/Dp ) dz wn −zp (4.173) Our expressions for electron and hole current densities at z = zn can be rewritten in terms of these integrated charge numbers as q 2 ni 2 D n qV Jn (zn ) = exp −1 + Qp kT Z zn qDn Jgr (z)ni φn (−zp ) − ψ exp q dz (4.174) Qp −zp Dn kT and Jp (zn ) = q 2 ni 2 D p qV exp −1 − Qn kT Z qDp zn Jgr (z)ni ψ − φp (zn ) exp q dz. Qn −zp Dp kT (4.175) 242 4 Transport Across Junctions The total current density for this homojunction, under conditions of low-level injection and with ideal ohmic contacts, is qDn qDp qV + exp −1 + J(z) = qni 2 Qp Qn kT Z zn qDn φn (−zp ) − ψ Jgr (z)ni exp q dz − Qp −zp Dn kT Z qDp zn Jgr (z)ni ψ − φp (zn ) exp q dz. (4.176) Qn −zp Dp kT This was derived from first principles including both drift and diffusion terms for the minority carriers since the quasi-Fermi potentials were used as a basis for the derivation. Thus, it does apply to conditions where the doping may be a function of position and where drift effects may be also be important. The geometrically weighted diffusivities D n and D p contain the contribution due to drift current. The effect of motion of minority carriers is related to their motion parameters of effective diffusivity. The expressions indicate that this parameter is dependent on the material properties related to diffusivity and intrinsic carrier concentration, and to the integrated majority carrier charge density. This dependence was discussed on the basis of intuitive arguments at the beginning of this section. Thus, the contribution of electrons is related to ni , Dn , and Qp , and the generation–recombination effects. The voltage V in these equations is the total potential drop in the semiconductor from one ohmic contact edge to the other, i.e., V = Vp + Vj + Vn , where Vp is the voltage drop across the p-side, Vj the voltage drop at the junction, and Vn the voltage drop across the n-side. Let us now apply this approach to the simple situation of low-level injection in a short diode with generation–recombination considered negligible and with a uniform doping profile. We have Qp Qn = = Jgr (z) Dp and Dn = = = q(zp − wp)pp0 , q(zn − wn )nn0 , 0, Dp , Dn . (4.177) This results in the following: Jn (zn ) = = = q 2 ni 2 D n qV exp −1 Qp kT 2 qni Dn qV exp −1 (zp − wp )pp0 kT qnp0 Dn qV exp −1 , zp − wp kT (4.178) 243 4.5 p–n Junctions and Jp (zn ) qV q 2 ni 2 D p exp −1 Qn kT 2 qV qni Dp exp −1 (zn − wn )nn0 kT qpn0 Dp qV exp −1 . zn − wn kT = = = (4.179) The total current, constant and independent of position in the device structure is qnp0 Dn qpn0 Dp qV J(z) = + exp −1 . (4.180) zp − wp zn − wn kT This is the common expression for a short, uniformly-doped, homojunction diode in low-level injection, ignoring generation–recombination contributions. It is the sum of diffusion currents on either side of the junction, which is related to the gradients of the minority carrier densities which are constant in the absence of generation–recombination. Now consider the same example with a varying doping profile to show the more general applicability in cases where the generation–recombination effects may still be ignored (by definition, the generation–recombination effects may not be ignored in a long diode). We consider a short diode with an exponential doping profile in one of the base regions. Consider the example of Figure 4.23 . The diode has a uniformly doped p-type region with a doping NA on one side of an abrupt junction and an exponentially increasing doping ND (z) on the other side of the junction given by z − zn . (4.181) ND (z) = ND0 exp ` Such a retrograde doping profile commonly occurs in devices where constant capacitance is desired. An example is the varactor diode used for frequency multiplication in microwave applications. Because of the non-uniform doping, a built-in field exists in the n-type region, and both diffusion and drift currents occur in this region. These are included in the weighted diffusion coefficient Dp . For the doping profile shown, we have Qp = Qn = = and Jgr = Dp = Dn = q(zp − wp )NA , Z zn q ND (z)dz wn zn − wn q`ND0 1 − exp − , ` 0, R zn ndz R zn wn , (n/Dp ) dz wn Dn . (4.182) 244 4 Transport Across Junctions Figure 4.23: Example of a short p–n diode with an exponentially varying profile in one of the base regions. The top half of the figure shows the band edges and the bottom half shows the carrier density as a function of position. 245 4.5 p–n Junctions The expression for the diffusivity Dp , thus, weights the contribution of the highest doping that occurs at the ohmic contact, and not at the edge of the junction depletion region. The drift effect is incorporated in this effective coefficient. Using the expression for current, under these conditions, J = qni 2 Dn qni 2 D p + (zp − wp )NA `ND0 {1 − exp [− (zn − wn ) /`]} qVj −1 , exp kT × (4.183) a considerably more complex expression, but obtained in a fairly straightforward manner. The first part of this expression, due to electron transport in the short uniformly-doped p-type region, is the same as in the previous example. The second part of the expression is the variation introduced by non-uniform doping, and the drift and diffusion current contribution of the hole current. These examples ignore recombination effects, usually a poor assumption in materials with short lifetimes such as compound semiconductors. We will therefore show the applicability of our derivation of the Gummel–Poon model to these by including simpler forms of generation–recombination effects in examples. Consider HSR-dominated generation–recombination processes, in a uniformlydoped long abrupt diode. The generation–recombination rates in the quasineutral regions are characterized by a lifetime, τn for electrons, τp for holes; and let −Uscr represent the net generation–recombination rate in the space charge region. Following our discussion of recombination processes, the former would be equally applicable for Auger processes due to heavy doping effects, the latter, however, is a complicated quantity because it exhibits a position-dependent variation within the space charge region of the junction. These net generation– recombination rates, for uniform doping in various parts of the diode, are given by np0 qVj z + wp R(z) − G(z) = exp − 1 exp (4.184) τn kT Ln in the p-type region (−zp ≤ z ≤ −wp ), R(z) − G(z) = Uscr (4.185) due to HSR recombination in the space charge region (−wp ≤ z ≤ wn ), and pn0 qVj z − wn R(z) − G(z) = exp − 1 exp − (4.186) τp kT Lp in the n-type region (wn ≤ z ≤ zn ). We wish to evaluate the integral containing the generation–recombination current term where the expression for the generation–recombination current is Z zn Jgr (z) = [R(z) − G(z)] dz. (4.187) z 246 4 Transport Across Junctions Let Jscr represent the contribution of the generation–recombination in the space charge region, i.e., Z wn Jscr = qUscr (z)dz. (4.188) −wp Using our simplified equation for electron current at the n-region contact, qni 2 qV Jn (zn ) = exp −1 + Γn kT Z zn φn (−zp ) − ψ 1 Jgr (z)ni exp q dz Γn −zp Dn kT Z −wp qni 2 qVj 1 Jgr (z)pp0 ≈ exp −1 + dz. Γn kT Γn −zp Dn (4.189) The latter follows from the assumption of perfect ohmic contacts, which allows us to substitute φn (−zp ) = φp (−zp ); the integral is therefore dominated by the contribution of the p-type region. We can evaluate this resulting integral involving recombination current by considering the three sections (p-type region, space charge region, and n-type region) contributing to it, and, in view of the above, we will consider the contribution of Jgr (z) in the p-type region only. The effect of the generation–recombination term, due to Jgr (z), is the most complicated in form in the p-type region since the limits of integration for the generation–recombination rate are from this to zn , which includes contributions from both the space charge region and the quasi-neutral n-type region. Let us consider this term first, i.e., the contribution of the quasi-neutral p-region of the device (−zp ≤ z ≤ −wp ) Jgr (z) = Jscr + qpn0 Lp qV zn − wn exp − 1 1 − exp − + τp kT Lp qnp0 Ln qV z + wp exp − 1 1 − exp . (4.190) τn kT Ln In a long diode, and zn − wn zp − wp Lp Ln , (4.191) and, therefore, the exponential in the second term is negligible. Also, by definition, and Lp τp Ln τn = = Dp Lp Dn , Ln (4.192) 247 4.5 p–n Junctions yielding Jn (zn ) = qni 2 qV exp −1 + Γn kT 1 qpn0 Dp qnp0 Dn qV + exp − 1 + Jscr × Γn Lp Ln kT (zp − wp )pp0 − Dn 2 np0 Dn qV zp − wp Ln exp − 1 1 − exp − . Γn L n kT Ln (4.193) Again, the device being a long diode, the exponent in the last equation is negligible, and since (zp − wp )pp0 Γn ≈ (4.194) Dn for a uniformly doped device, we obtain qpn0 Dp qnp0 Dn qVj Jn (zn ) = + exp − 1 + Jscr . Lp Ln kT (4.195) This is the electron current at the n-type contact in the long diode. In deriving this we consider the recombination perturbation as coming about only due to the recombination current integral in the p-type region. The basis of this is that this integral is a product of the hole density and the recombination current integral; therefore, the space charge region and the n-type region contribute little to the perturbation. Intuitively, also, since this is a long diode, all the current at the n-type contact must be electron current, since all excess holes injected in the n-type region must recombine before reaching the contact. The above expression, therefore, must also give the total current for a long diode. Let us show this by considering the hole current at the n-type contact at z = zn . We may evaluate this hole current at zn Jp (zn ) = ≈ qni 2 qV exp −1 − Γp kT Z zn 1 Jgr (z)ni ψ − φn (zn ) exp dz Γp −zp Dp kT Z zn qni 2 qV 1 Jgr (z)nn0 exp −1 − dz. Γp kT Γp wn Dp (4.196) Since the recombination perturbation is an integral involving the product of the hole density and the generation–recombination integral, it is dominated by the 248 4 Transport Across Junctions contribution from the quasi-neutral n-type region. This contribution is given by Z zn qpn0 qV z − wn Jgr (z) = exp − 1 exp − dz τp kT Lp z qpn0 qV Lp exp −1 × = τp kT z − wn zn − wn exp − − exp − Lp Lp qpn0 qV z − wn ≈ Lp exp − 1 exp − . (4.197) τp kT Lp We have again used the inequality (zn − wn ) << Lp , and hence dropped the last exponential. We can now evaluate the hole current at zn , Jp (zn ) qV qni 2 exp −1 − ≈ Γp kT Z zn 1 qpn0 Lp nn0 qV z − wn exp − 1 exp − dz Γp −wn τp Dp kT Lp qV qni 2 ≈ exp −1 − Γp kT 2 qni qV zn − wn exp − 1 1 − exp − Γp kT Lp ≈ 0. (4.198) As expected, the hole current is negligible at the n-region contact for this example of long diode. The total diode current density, therefore, is J(zn ) = Jn (zn ) + Jp (zn ) = Jn (zn ) qpn0 Dp qnp0 Dn qV + exp − 1 + Jscr . Lp Ln kT = (4.199) The first term of this expression is the familiar form of the long diode expression for uniform doping. The second term in this expression of Jscr is the contribution of the space charge layer. The conventional expression ignores the space charge region contribution to generation–recombination, while this expression was derived considering contributions from all the regions. The contribution Jscr , therefore, arrived naturally in our expression instead of through perturbative iterations of the derivation. Since our control equations are linear differential equations, it occurs as a superposition term, as expected. 249 4.5 p–n Junctions The evaluation of Jscr follows directly from the evaluation of the integral in Equation 4.188. Space charge recombination usually arises from HSR recombination. Hence, following our discussion in Chapter 3, we employ the simplified equation np − n2i , (4.200) U= τ0 {n + p + 2ni cosh [(ET − Ei ) /kT ]} where we have assumed the trap to have identical τn0 and τp0 given by τ0 . Such traps are efficient recombination centers. However, differing values are the norm and can be treated numerically. Given this assumption, another characteristic of the net recombination rate is that a maximum in it occurs when ET = Ei . A differing τn0 and τp0 changes this conclusion only slightly. So, deep traps are responsible for the generation-recombination effects. The np product is known in the space charge region since quasi-Fermi levels are assumed constant in lowlevel injection. We will evaluate this integral for these most efficient traps, i.e., for ET = Ei . The contribution of the space charge region recombination current is Z wn 2 ni [exp (qV /kT ) − 1] Jscr = dz. (4.201) τ0 (n + p + 2ni ) −wp Since the maximum contribution to this integral occurs from the region of maximum net recombination rate, we can approximate this integral as a product of the width of the space charge region W = (wn − wn ) and the maximum of the net recombination rate. n and p are know as a function of the displacement between the quasi-Fermi levels and intrinsic energy level. Hence, a maximum in Uscr can be shown to occur when Ei = ξn + ξp 2 (4.202) in the space charge region. This occurs where qV n = p = ni exp , 2kT (4.203) yielding the approximate relationship for space region current as Jscr = qW ni exp (qV /kT ) − 1 . 2τ0 exp (qV /2kT ) + 1 (4.204) In forward bias, this reduces to Jscr qW ni ≈ exp 2τ0 qV 2kT . (4.205) In reverse bias, this reduces to Jscr ≈ − qW ni . 2τ0 (4.206) 250 4 Transport Across Junctions The derivation for current in a long diode assumed a uniform doping density. Our Gummel–Poon equations are more general than that. Problem 15 discusses the long diode case with a non-uniform doping, similar to our short diode example. In these examples of Gummel–Poon modelling, we made a simplifying assumption by restricting the exposition to homojunctions. This allowed us to move the term ni outside the integral. In general, it may be position-dependent, such as when heavy doping effects or alloy grading effects predominate. We will now establish the expressions for these conditions. The derivation only needs to include the fact that the intrinsic carrier concentration may be positiondependent. Our derivation will be in terms of the current density at the edges of the depletion region, and hence, in general, use of this procedure will require the determination of both the hole current density and the electron current density. The general expression for current density at the n-type contact (z = zn ), as a simple extension of the earlier derivation is, (see Problem 16) Jn (−wp ) = (Z −wp 1 dz qD n exp {q [ψ − φn (−zp )] /kT } n i −zp Vp + Vj exp q −1 + kT ) Z −wp p Jgr (z) dz , −zp qDn ni exp {q [ψ − φn (zp )] /kT } where p Jgr (z) = Z )−1 × (4.207) −wp q [R(z) − G(z)] dz. z (4.208) This equation is in a general form, applicable also for high-level injection, since we have only equated the differences in the quasi-Fermi potentials to the change in the electrostatic potential that they correspond to. A similar expression may be written for the hole current density, and is given as Z zn −1 1 Jp (wn ) = dz × wn qDn ni exp {q [φp (zn ) − ψ] /kT } Vn + Vj exp q −1 + kT Z zn n Jgr (z) dz , (4.209) wn qDp ni exp {q [φp (zn ) − ψ] /kT } where n Jgr (z) = Z z wn q [R(z) − G(z)] dz. (4.210) 251 4.5 p–n Junctions Assuming perfect ohmic contacts under low-level injection, we obtain !−1 Z −wp p Jn (−wp ) = dz × 2 −zp qDn ni ) ( Z −wp p pJgr (z) qV −1 + dz (4.211) exp 2 kT −zp qDn ni for the electron current. This equation may be written in a form similar to the earlier equation for diodes using an effective Gummel number, qDn ni 2 qV Jn (−wp ) = exp −1 , (4.212) 0 kT GNp where the effective Gummel number is R −wp p −1 pJgr (z)/qDn ni 2 dz 0 Qp −zp 1+ . GNp = q exp (qV /kT ) − 1 (4.213) Likewise, the expression for hole current at the n-type contact (z = zn ) is Jp (wn ) = Z −1 n dz × 2 wn qDp ni Z zn n nJgr (z) qV exp −1 + dz . 2 kT wn qDp ni zn (4.214) Writing this equation in a form similar to the expression for the electron current density, we obtain qV qDp ni 2 Jp (wn ) = exp − 1 , (4.215) 0 kT GNn where the effective electron Gummel number is given by ( )−1 R zn n nJgr (z)/qDp ni 2 dz 0 Qn wn GNn = 1+ . q exp (qV /kT ) − 1 (4.216) These expressions are cast in a form similar to our expressions for the long diode and short diode expressions. They reduce directly to the short diode expression since the effective Gummel number is then the majority charge divided by the electronic charge. The form of these expressions is chosen to directly show this relationship, and the perturbative effect of alloy compositional changes, large doping effects,and recombination effects. Note that the majority charge densities Qn and Qp and the effective diffusivities Dn and Dp continue to directly influence the current transport. The perturbation due to the recombination effect is generally small because the dividing factor is exponentially 252 4 Transport Across Junctions proportional to the applied voltage. The expressions also directly show that the recombination current density increases the current through the device, and 0 0 the corresponding Gummel numbers GNn and GNp are decreased. The effect of changes in bandgap, such as through the alloy composition variation, occur through the effect on the intrinsic carrier concentration, an exponential effect. The effect on current under these conditions can thus become large, and is considered in the next sub-section. We now use these expressions in determining the current, with recombination, for the example of varying doping profile. We will assume a long diode, unlike our earlier example that was for a varying doping profile in a short diode and with no recombination. The treatment of the p-side is the same as before for the case of a long diode with uniform doping profile. For the n-side, which is non-uniformly doped, the treatment is different and the expressions need to be reevaluated. The excess minority carrier density on the n-side is qV wn − z 0 p (z) = pn0 (wn ) exp − 1 exp , (4.217) kT Lp assuming the diffusion coefficient to be a constant. The generation–recombination rate in the quasi-neutral n-type region is 0 R(z) − G(z) = p (z) τp (4.218) for wn < z < zn . To determine the effective Gummel number, we need the n magnitude of the recombination current integral Jgr (z) only in this interval. Hence, Z z qpn0 (wn ) qV wn − z n Jgr (z) = exp −1 dz exp τp kT Lp wn qpn0 Lp qV wn − z = exp − 1 1 − exp τp kT Lp qDp pn0 qV wn − z = exp − 1 1 − exp . (4.219) Lp kT Lp To determine the effective Gummel number we need to determine the integral n using this Jgr (z), i.e., the effective Gummel number for calculation of the hole current is ( R zn n )−1 2 dz 0 Qn wn nJgr (z)/qDp ni GNn = 1+ q exp (qV /kT ) − 1 Qn pn0 (wn ) ≈ 1+ × q ni 2 L p −1 Z zn wn − z z − zn 1 − exp − ND (0) exp dz Lp ` wn 253 4.5 p–n Junctions ≈ Qn pn0 (wn ) wn − zn 1+ `N (0) 1 − exp − + D q ni 2 L p ` pn0 (wn ) `Lp ND (0) ni 2 L p ` − L p −1 wn − zn wn − zn − exp . exp Lp ` (4.220) Since (wn − zn ) << Lp , the exponential involving this factor can be ignored, and the effective Gummel number is Qn pn0 (wn )ND (0) wn − zn 0 GNn = 1+ ` 1 − exp − − q ni 2 L p ` −1 `Lp wn − zn exp . (4.221) ` − Lp ` Since the effective Gummel number is known, the hole current density at the edge of the depletion region follows. The electron current can be similarly derived, indeed it is the analog of this with ` → ∞. In a long diode, the total width of the depletion region is relatively short compared to the two bases of the diode. Therefore, we may ignore it, and hence determine the total current density (see Problem 17). 4.5.4 Abrupt and Graded Heterojunction p–n Diodes Use of p–n heterojunctions is central to the operation of both the heterostructure bipolar transistor and the heterostructure laser. In these structures, the injection of carriers occurs through a heterojunction with the heterojunction aiding in the selective suppression of the injection process of one of the carriers. In abrupt heterojunctions, it occurs due to the existence of the discontinuity in the conduction and valence bands, and in the graded heterojunction diode, it occurs because the difference in bandgap appears predominately as a barrier to injection of one of the carrier types. Examples of some variations of the heterojunctions due to abruptness and grading of the alloy composition at one-sided junctions are shown in Figure 4.24. This example considers the Ga.7 Al.3 As/GaAs junction; the doping for the larger bandgap Ga.7 Al.3 As is identified by the capital N or P for n-type and p-type doping. The graded structures are formed using a grading length of 200 Å evenly distributed at the metallurgical junction. The effect of this grading is to distribute the bandgap change at the junction between the conduction and the valence band edges, whose extreme example is the case of the abrupt heterojunction under similar doping conditions, i.e., the band edges in this graded case show a smaller deviation then that caused by abrupt heterojunctions. We need to establish how this band variation description comes about. Maxwell’s equations continue to be valid, and to this point, we have only added 254 4 Transport Across Junctions Figure 4.24: Band edges in thermal equilibrium for one-sided abrupt and graded heterojunctions of Ga.7Al.3 As/GaAs, drawn to scale for various combinations of doping on either side of the junction. The chained lines show the band edges for the graded heterojunction with a linear alloy grading over 200 Å. 4.5 p–n Junctions 255 the requirement that abrupt heterojunctions discontinuities in the conduction and valence band edges have to be established experimentally. Thus, Poisson’s equation, which is a restatement of Maxwell’s second equation, continues to be valid, and we have to incorporate variation in the dielectric constant. Gauss’s law, which is a restatement of Maxwell’s second equation applied at the interface, states that the difference in the displacement vector normal to the interface must differ by the interface charge density. For heterojunctions of interest, abrupt and graded, this is negligible. Thus, the displacement vector normal to the interface is continuous. We have thus established three rules for describing the electronic behavior of abrupt heterojunctions: Poisson’s equation, Gauss’s Law, and the band edge discontinuities at the interface. These, together with the boundary conditions at the edges of the depletion region and the constancy of the Fermi level in thermal equilibrium, are sufficient to determine the band edge for abrupt heterojunctions in thermal equilibrium. These rules were used in determining the abrupt heterojunction band edges in Figure 4.24. As we remarked earlier, in the discussion of isotype heterojunctions, there will exist in these structures a discontinuity in the vacuum level and the electrostatic potential at the interface. The discontinuity in the vacuum level indicates that electrons at the band edge on either side of the interface require different energy to be removed into vacuum. The materials have different characteristics and this discontinuity is not unexpected. The difference in electrostatic potential has the same cause— it comes about because the electrochemical potential includes the effect of the material in the term that we have referred to as alloy potential. The band edge variation changes when a bias is applied to the abrupt heterojunction. Under these conditions, the transport process has to be included together with the rules of Poisson’s equation, Gauss’s Law, and band edge discontinuity to determine the new variation. If, e.g., transport is by drift-diffusion, then we may continue to use the concept of quasi-Fermi energy as applied to a displaced Maxwell–Boltzmann distribution, and the quasi-Fermi energies stay continuous at the interface. The argument here is similar to the discussion of isotype heterojunctions. The carrier distribution at either side of the interface is very similar because of the small difference between drift and diffusion flux. With the large mobility of electrons in most compound semiconductors of interest, however, the transport of electrons at the interface is limited by thermionic emission and the higher-energy field emission current. Thus, similar to our discussion of isotype heterojunctions, the concept of quasi-Fermi energy is not strictly valid within a few kT ’s of changes in band edge energy at the interface. These must therefore be treated as fitting parameters in this region. Knowing the transport mathematics, however, we may include the other rules from the above and again derive the band edge variation in the abrupt heterojunction. We have discussed the transport equations in slowly graded heterostructures, where the grading lengths are such that any band edge discontinuities can be ignored and all compositional variations can be directly included in the bandgap changes, in Chapter 3. Using this treatment of transport in graded heterostructures, Poisson’s equation, and the boundary conditions at the edges 256 4 Transport Across Junctions of the depletion region, the band edge variation can be derived for the slowly graded heterojunctions. So, the transport through such graded heterojunctions, is determined using the modified drift-diffusion equation. The last of our Gummel–Poon quasi-static model derivation can be applied to such graded structures because it included variations in ni , variations which result from alloy composition variation. Thus, the slowly graded heterojunction case is fairly straightforward and follows our discussion of homojunctions quite closely. We will return to analysis of slowly graded heterojunctions later in this section. First, we consider the transport through the anisotype abrupt heterojunctions. In our discussion of isotype abrupt heterojunctions, we discussed the thermionic emission behavior. This analysis can be extended for the case of anisotype heterojunction diodes also. Consider the example of abrupt N–p+ junction shown in case (b) of Figure 4.24. It is chosen because it occurs in the emitter-base junction of an abrupt heterostructure bipolar transistor. The base in these structures is more heavily doped and takes advantage of the suppression of hole injection current. Our discussion follows a similar argument as in the case of abrupt isotype heterojunctions. We will therefore be brief, with the intent of considering the problem for practical application. The injected carriers thermalize over few mean free paths in the base and then drift-diffuse to the contact. In the analysis of which conduction mechanism is dominant, we must consider the ability of the junction to thermionically emit the carriers over the barrier and the ability of the semiconductor bulk in the emitting and collecting regions to supply and collect these carriers. Due to the use of a heterojunction, the ability to inject carriers has decreased by the increase in the built-in junction voltage for that carrier without affecting other transport characteristics. Therefore, it is this barrier transport that limits the current across the junction. In our analysis of the isotype heterojunction, we derived this thermionic current in a form where we can now ignore the component from the smaller bandgap material. A significant barrier continues to exist for the injection from the small bandgap material to the large bandgap material throughout the bias range. In a first-order analysis, this injection from the small bandgap material may be ignored. We can determine it, if needed, by considering the transport via thermionic–drift-diffusion theory as well as via field emission. This thermionically injected current is given by m∗ 2 q Eg + ∆Ec + (1 ND /2 NA ) Vn − Vp T exp − × |Jth | = A m0 kT 1 + 1 ND /2 NA q V kT exp −1 for V , kT 1 + 1 ND /2 NA q (4.222) where we have parameterized the pre-factor. In this equation, Jth is the thermionic current density, A is the Richardson’s constant for a free electron whose magnitude is 120 A.cm−2 .K−2 , m∗e and m0 are the effective and free electron masses, ∆EC is the conduction band edge discontinuity, 1 and ND and 2 4.5 p–n Junctions 257 and NA are the permittivity and doping of the two semiconductors, Vn and Vp are the differences in potential between the Fermi levels and the conduction and the valence band edge in the two semiconductors, and V is the applied potential at the junction. The ratio 1 ND /2 NA in this equation accounts for the partitioning of the electrostatic potential across the depletion region. This does not have to be considered in metal–semiconductor junctions where the thermionic emission theory is usually applied. This is a simplified equation; more rigorous equations similar in form to the metal–semiconductor thermionic field emission and thermionic–drift-diffusion equations can also be applied. Indeed, since those equations were derived by considering the transport only in the semiconductor, they are well applicable here for the specific transport directions if the correct meaning are ascribed to the parameters. As an example of the thermionic–drift-diffusion equation applied to this problem, the effective mass is for the correct orientation in the large bandgap material, the effective density of states is the effective density of states of the large bandgap material, the barrier height is the difference between the Fermi level and the top of the conduction band edge, and the potential V is the value of the partitioned quantity that occurs across the large bandgap material. Similar comments apply to the modification of the thermionic field emission equation for this problem. Figure 4.25 shows behavior of the conduction band edge under forward bias conditions for a graded junction at two different doping levels in the n-type injector/emitter region. The higher doped emitter is well behaved in the band edge while the lower doped emitter shows a barrier at the higher injection conditions. The formation of the barrier, due to variation in composition and associated alloy potential, will be subject of further discussion later in this chapter and in Chapter 7. Our treatment here assumes that the conditions of monotonic variation in band edge hold. This is usually the case for low-level injection. Let us now consider the determination of the current in such graded anisotype heterojunctions. The application of the modified drift-diffusion equation follows in a similar manner as the simpler form of the drift-diffusion equation for transport. We will use a simple example of a heterojunction formed by compositional grading within the junction depletion region, and apply the modified drift-diffusion equation and the extended Gummel–Poon model to evaluate the currents. Consider the analysis in one dimension of a short N–p heterojunction in low-level injection, whose band edge schematic and some parameters are shown in Figure 4.26. The composition in the quasi-neutral region is a constant in this example, and like the homojunction in low-level injection, the quasi-Fermi levels remain constant through the bulk of the device and the current transport is limited by diffusion of minority carriers in the quasi-neutral regions. The device is a short device, and we also consider recombination as being absent. Thus, to determine the current, we need minority carrier current at the edge of the depletion regions. In the absence of recombination, this current density stays constant in the depletion region, and the total current is the sum of these minority carrier current densities. 258 4 Transport Across Junctions Figure 4.25: Conduction band edge energy diagram of an N–p+ Ga.7 Al.3 As/GaAs heterojunction diode under low (V = 1.0 V), medium (V = 1.2 V), and high (V = 1.4 V) forward bias. Two n-type dopings are shown; the solid lines are for 8 × 1017 cm−3 doping and the dashed lines are for 2 × 1017 cm−3 doping. The p+ doping is 5 × 1018 cm−3 . 4.5 p–n Junctions 259 Figure 4.26: A graded p–N heterojunction formed using a large bandgap material (identified by 1), and a small bandgap material (identified by 2). The alloy grading occurs within the junction depletion region, and like the homojunction analysis in low-level injection, the transport in the junction region is not a limiting transport mechanism. 260 4 Transport Across Junctions The Shockley boundary conditions describe the minority carrier densities at the edges of the depletion region as qV np (−wp ) = np0 exp kT qV , (4.223) and pn (wn ) = pn0 exp kT where np0 and pn0 are the concentrations of minority carriers in thermal equilibrium in the two different materials. The current density due to electron and hole transport in the junction quasi-neutral regions is described by the modified drift-diffusion equations dψ φCn dn Jn = qnµn − − + qDn dz dz dz dψ φV p dp and Jp = qpµp − − − qDp . (4.224) dz dz dz From these, Jn (−wp ) = and Jp (wn ) = qV qnp0 Dn exp −1 zp − wp kT qpn0 Dp qV exp −1 , zn − wn kT (4.225) and hence the total current is qpn0 Dp qnp0 Dn qV J = Jn (−wp ) + Jp (wn ) = + exp − 1 . (4.226) zn − wn zp − wp kT The equation has the same form as our earlier example of a homojunction, but with the major difference that the thermal equilibrium minority carrier concentration is different in a heterojunction. Thus, if ND and NA represented the donor and acceptor doping densities, Eg1 and Eg2 the two bandgaps (Eg1 > Eg2 in this example), NC1 and NC2 the effective conduction band density of states, NV 1 and NV 2 the effective valence band density of states, and ni1 and ni2 the intrinsic carrier concentrations in the two materials, then these are related in the Boltzmann approximation as and np0 = pn0 = n2i1 = n2i2 = n2i2 , NA n2i1 , ND Eg1 NC1 NV 1 exp − , kT Eg2 NC2 NV 2 exp − . kT (4.227) 4.5 p–n Junctions 261 The hole concentration in thermal equilibrium in the larger bandgap material is significantly smaller compared to the electron concentration in thermal equilibrium in the smaller bandgap material. This ratio is pn0 NA n2i1 NA NC2 NV 2 Eg1 − Eg2 = = exp − . (4.228) np0 ND n2i2 ND NC1 NV 2 kT The difference in bandgap decreases this minority carrier concentration exponentially with the bandgap change. The corresponding hole current density also decreases by the same exponential factor. On the other hand, the electron current and the electron transport are not influenced by the presence of the heterojunction. Another way of looking at this follows arguments based on built-in voltages. In Figure 4.26, the flat quasi-Fermi levels and bandgap grading leave the barrier for injection of electrons unchanged from the homojunction case except for the second order effects related to the effective density of states and its influence on position of the Fermi level in the quasi-neutral region. However, the hole barrier increases by this increase in the bandgap, and hence hole injection is suppressed by a corresponding amount. Thus, the presence of a heterojunction causes the built-in junction voltages for the electrons and the holes to be different. The built-in voltage now represents the sum of two effects, the electrostatic potential, which we may still define in terms of the variation of the vacuum level, and the alloy potential. The latter changes at the junction due the compositional changes. These built-in voltages follow from the drift-diffusion equations, applied at thermal equilibrium where each of the current densities is zero and the Fermi level is flat. For electrons, the junction built-in voltage is Z kT n(wn ) dn kT ND NA ψjn = = ln , (4.229) q n(−wp ) n q n2i2 and for holes, the junction built-in voltage is Z kT p(−wp ) dp kT ND NA ψjp = = ln . q p(wn ) p q n2i1 (4.230) The junction built-in voltage for holes increased by the difference in the bandgap. Here, only low-level injection was considered. A high current density across heterojunctions presents a particularly interesting problem because it is concomitant with a smaller space charge region (due both to the larger doping that a larger current capability requires and to the forward biasing of the junction). The smaller space charge region and decreased electrostatic field lead naturally to alloy potential effects appearing in the conduction band. One may see this as an example of the mixing of case (b) and case (d) for the graded case of Figure 4.24. A small electrostatic field at the junction occurs near flat band conditions. When this happens, the difference in alloy potential appears partially in the conduction band and partially in the valence band. Looking at the graded heterojunction examples of Figure 4.24, the difference in the alloy 262 4 Transport Across Junctions potential appears in the valence band edge in case (a) and case (b), and in the conduction band edge for case (c) and case (d). The magnitude and direction of the electrostatic field force the alloy potential effects to appear in the conduction or the valence band, and when the electrostatic field becomes small, such as in large forward bias, they cause the alloy effects to appear in both the band edges. Appearance of the resulting barrier limits the current density in the structure, and the junctions need to be designed to prevent this. The alloy grading length needed to prevent barrier-limited transport effects in the depletion approximation limit can be derived by consideration of the electrostatic and alloy potential variation. If the electrostatic field remains larger than the alloy field, the band bending remains monotonic, and no barrier exists. Mathematically, this requirement can be summarized as dψall < Ees , (4.231) dz where Ees is the local electrostatic field and ψall is the alloy potential. For a one sided p–n junction, this results in (see Problem 18), ∆Eg zg > p >> λD , 2kT (Eg − qV − 2kT ) (4.232) where zg is the grading length, ∆Eg the total bandgap change, q the electronic charge, Eg the bandgap in the narrow bandgap material, V the applied bias, and λD the extrinsic Debye length. The expression is derived assuming the depletion approximation, and hence is inaccurate at high forward bias conditions, where the mobile charge should be taken into consideration. Graded heterojunctions are convenient to analyze using the extended Gummel– Poon model. The derivation for current in the heterojunction example follows directly; it is the same as the expression derived in our homojunction short diode example using the Gummel–Poon model. We consider another short diode example with a change in the alloy composition in one of the bases of the diode to show the breadth of this approach. This example is similar to the example of varying doping in the base of a short diode, except here doping is constant and the intrinsic carrier concentration is allowed to change exponentially as z − wn 2 2 ni = ni0 exp for z > wn ` and n2i = n2i0 for − zp < z ≤ wn . (4.233) Figure 4.27 shows a schematic of this problem. The general expressions for the electron and hole currents at the edges of the junction are given by !−1 Z −wp p Jn (−wp ) = dz × 2 −zp qDn ni ( ) Z −wp p pJgr (z) qV exp −1 + dz , (4.234) 2 kT −zp qDn ni 263 4.5 p–n Junctions Figure 4.27: Band diagram of a p–n heterojunction with a base region with exponentially decreasing intrinsic carrier concentration. and Jp (wn ) −1 n dz × = 2 wn qDp ni Z zn n nJgr (z) qV exp −1 + dz . 2 kT wn qDp ni Z zn (4.235) Ignoring recombination in the short diode, and assuming low-level injection and a hole diffusion coefficient that is a weighted constant Dp , we can evaluate these currents. The minority carrier electron current density is −1 NA (zp − wp ) qV Jn (−wp ) = exp − 1 , (4.236) qDn n2i0 kT an expression identical to the earlier expression. The minority carrier hole current in the bandgap grading region is modified, and given by −1 ND ` zn − wn qV Jp (wn ) = exp −1 exp −1 , (4.237) ` kT qDp n2i0 and the total current, which is the sum of the above two expressions, is given by qDn n2i0 qDp n2i0 qV J= + exp −1 . NA (zp − wp ) ND ` [exp [(zn − wn )/`] − 1] kT (4.238) 264 4 Transport Across Junctions The drift current due to the quasi-field for holes in the n-type bandgap graded region is included in the above expressions. This drift field opposes the motion of holes and hence suppresses the hole current as drawn in Figure 4.27. Note that the hole concentration and the electron concentration at the edges of the junction depletion region are still identical to the homojunction example since we chose the bandgap change to occur only in the quasi-neutral n-type region. Also, in the limit of ` → ∞, i.e., no bandgap and intrinsic carrier concentration variation, this expression reduces to the expression for a short uniformly-doped homojunction diode. More examples of the application of the extended Gummel–Poon model are considered in the Problems, and we will also consider it again in our discussion of heterostructure bipolar transistors. 4.6 Summary This chapter developed the concepts and mathematical framework for treatment of transport across junctions. We considered junctions between different materials, i.e., junctions formed between metals and semiconductors or two different semiconductors, as well as junctions formed by a change in the type of doping, i.e., p–n junctions. For the metal–semiconductor and heterojunctions, we considered the contributions due to thermionic emission and field emission in the region at the interface as well as due to other restrictions placed by drift-diffusion transport in the bulk. We showed how, in the case of thermionic emission, the consequences of Bethe condition relating the collision-less emission of carriers at the interface and the momentum matching condition lead to an unambiguous effective mass for the Richardson’s constant. In considering the specialized case of heterojunctions, we also reviewed tunneling: the conventional Fowler–Nordheim tunneling that considers wave function decay in a trapezoidal barrier, and resonant Fowler–Nordheim tunneling, important at low temperatures, and involving additional wave interference effects in the barrier region. These processes are important in the near-ideal heterojunctions of compound semiconductors for a variety of devices. As an extension of the analysis we considered the formation of ohmic contacts, contacts that allow low resistance bi-directional current flow in device structures. We also considered in this chapter the approximations of p–n junction analysis and described the bulk effects occurring at high level injection conditions. For graded p–n junctions, i.e., those lacking an abrupt barrier at the interfaces, we developed an appropriate criterion for grading. For predicting the current, we developed a formal method of quasi-static analysis, the Gummel– Poon method, that allows a description of diode behavior in a variety of practical circumstances. This was applied to cases involving doping variation as well as composition variation. General References 265 General References 1. E. H. Rhoderick and R. H. Williams, Metal-Semiconductor Contacts, Clarendon Press, Oxford (1988). 2. H. K. Henisch, Semiconductor Contacts—An Approach to Ideas and Models, Clarendon Press, Oxford (1984). 3. F. A. Padovani and R. Stratton, in R. K. Willardson and A. C. Beer, Eds., Semiconductor and Semimetals, 7A, Academic Press, N.Y. (1971). 4. R. Stratton, “Diffusion of Hot and Cold Electrons in Semiconductor Barriers,” Phys. Rev., 126, No. 6, p. 2002, 1962. 5. A. G. Milnes and D. L. Feucht, Heterojunctions and Metal–semiconductor Junctions, Academic Press, N.Y. (1972). 6. S. M. Sze, Physics of Semiconductor Devices, John Wiley, N.Y. (1981). 7. S. S. Cohen and G. Sh. Gildenblat, Metal–Semiconductor Contacts and Devices, in N. G. Einspruch, Ed., VLSI Electronics and Microstructure Science, V 13, Academic Press, FL (1986). 8. C. B. Duke, Tunneling in Solids, in F. Seitz, D. Turnbull, and H. Ehrenreich, Eds., Solid State Physics, Suppl. 10, Academic Press, N.Y. (1969). 9. E. Burstein and S. Lundqvist, Ed., Tunneling Phenomena in Solids, Plenum Press, N.Y. (1969). Problems 1. Problems of thermionic injection encountered in metal–semiconductor junctions involve injection from many complicated situations. Injection in metal/n-Ga1−xAlx As junctions, e.g., involves electrons in the anisotropic L and X valleys. Injection in metal–p-Ga1−xAlx As junctions, e.g., occurs from valence bands with light and heavy hole mass. Consider the electron and hole injection problem and determine the mass appropriate to the determination of Richardson’s constant for (a) injection from the L valley on (100), (110), and (111) surfaces, (b) injection from the X valley on (100), (110), and (111) surfaces, and (c) injection from valence bands. 2. We have considered the thermionic injection component and the tunneling component of injection at a metal–semiconductor junction separately. In a metal–semiconductor junction, thermionic injection occurs together with tunneling of carriers. The tunneling of higher-energy carriers is favored because these encounter smaller barrier energies and width. Show that 266 Transport Across Junctions when both of these processes dominate, the current can be expressed in the form shown in Equation 4.37. 3. Show that the low temperature limit of thermionic field emission in a metal–semiconductor junction can be expressed as # " 3/2 2 (2qφB ) ∗ E00 qφB − qV − qVn √ . (4.239) J=A exp − k2 qφB 3E00 qφB + qV − qVn 4. Plot the carrier concentration and the velocity as a function of position between z = 0 and z = zc for a GaAs metal–semiconductor junction on 1×1016 cm−3 doped material at thermal equilibrium at 300 K. The barrier height from the metal to the semiconductor is 0.8 eV. 5. What is the ratio of the carrier concentration in the semiconductor at the metal–semiconductor junction, if the Bethe condition is satisfied, and if the quasi-Fermi level is assumed to be flat? 6. Show that Equation 4.57 follows from the application of current continuity to the boundary of regions dominated by drift-diffusion transport and thermionic emission transport. 7. Consider the application of Equation 4.57 to the metal–semiconductor junction formed on 1 × 1016 cm−3 n-type GaAs. Consider a metal barrier height of 0.8 eV, and an operating temperature of 300 K. Plot the current density of this thermionic–drift-diffusion expression, as well as its thermionic and drift-diffusion limit. Which component dominates? Now consider the same structure at 77 K, and plot the three current densities. Which component dominates? 8. Consider the application of the thermionic–drift-diffusion theory to an n–n heterojunction. Compared to the metal–semiconductor junction the differences include the partitioning of the electrostatic potential on the two sides of the heterojunction and the injection of carriers of differing effective mass, and requiring appropriate momentum matching as they traverse the junction. Taking into account these differences, find an expression similar to Equation 4.57, and derive the current voltage relationship for thermionic–drift-diffusion transport. 9. An alternate, but simplistic, way of analyzing Problem 8 is to consider transport as emission of a Maxwell–Boltzmann distribution across a barrier with transmission coefficients T12 and T21 which are functions of energy. Using detailed balance, derive an expression for current transport and compare it with the thermionic emission limit of Problem 8. 10. Using the complete solution of the triangular barrier tunneling transmission probability (Equation 4.77), derive the asymptotic form of Equation 4.79. Show that this asymptotic form follows directly from the use of the WKB approximation. 267 Problems 11. Using the current voltage relationships due to thermionic emission and thermionic field emission of a metal–semiconductor junction, and field emission in a triangular barrier, derive the expressions for the contact resistance together with their pre-factors. Apply the appropriate relationship to an n-type metal–semiconductor junction on GaAs. Assume a temperature of 300 K, a barrier height of 0.8 eV, and n-type dopings of 1 × 1016 cm−3 , 1 × 1017 cm−3 , 1 × 1018 cm−3 , 1 × 1019 cm−3 , and 5 × 1019 cm−3 . 12. For a field emission-dominated region of transport across a metal–semiconductor junction, show that the current can be expressed as shown by Equation 4.94 and that the contact resistance follows as Equation 4.96. Estimate the contact resistance resulting from this for Problem 11 at the highest doping. 13. Consider the practical contact as a distribution of point contacts on the semiconductor surface. Show that, if the spreading resistance of these point contacts dominates, then the contact resistance must vary inversely with doping. 14. Derive the expression for hole current density at zn (Equation 4.160) using the hole quasi-Fermi level as basis for the calculation of current. 15. Consider a n+ –p diode with a long p-type region where the doping varies as ∆NA exp(z/`)+NA0 . Derive the expression for electron current in such a structure using the Gummel–Poon model. 16. Derive Equation 4.207 for electron current at the p-type contact using the Gummel–Poon model. 17. Derive the current in a long diode by considering both the electron and the hole current and ignoring the recombination in the depletion region. 18. Show that the requirement that the alloy field be maintained smaller than the electrostatic field results in the following condition zg > p ∆Eg >> λD 2kT (Eg − qV − 2kT ) (4.240) to obtain an alloy-barrier free transport in a p–n junction. 19. Consider a uniformly-doped GaAs p–n junction with a doping of 1 × 1017 cm−3 on either side. Assuming depletion approximation, what is the junction depth in thermal equilibrium? Plot the capacitance C and 1/C 2 as functions of reverse bias for the junction. Now consider a deep donor trap density of 1 × 1016 cm−3 uniformly distributed throughout the semiconductor. The trap energy is 0.75 eV below the conduction band edge, and the degeneracy is 2. How does the junction depth change in thermal equilibrium and what is the behavior of capacitance C and 1/C 2 268 Transport Across Junctions Figure 4.28: Schematic of the Poole-Frenkel process. with reverse bias? Can one determine the position and density of the donor trap using such a measurement technique? 20. Solve Laplace’s equation in the presence of a conducting plane to show that the lowering of energy described by the image charge leads to an identical result for the energy of a charged carrier as a function of position from the conducting plane. 21. The Poole-Frenkel effect is the lowering of barrier energy at a defect in a dielectric, e.g., at a positively charged defect that can capture an electron and has related Coulombic effects. The effect has parallels with the image force lowering with the major difference being the absence of the conducting plane. Find an expression for the amount of barrier lowering due to the Poole-Frenkel process described in Figure 4.28. 22. Following the previous problem, what electric field will give rise to a PooleFrenkel barrier lowering effect equal to the donor ionization energy in GaAs (typically 6 meV)? 23. Barrier heights may be changed by incorporation of a limited amount of dopants. The region of incorporated dopants is depleted under the biasing conditions applied to the semiconductor junction. This can be employed to either increasing or forming a low-energy barrier such as in planar doped diodes, as well as to lowering barrier heights of metal–semiconductor junctions. (a) Consider a metal–semiconductor junction where the donor density is increased to a value of ND2 in a region of width ` from the donor density of ND1 . Let ` be less than the Debye length. What is the electric field as a function of position and the magnitude of image force lowering? 269 Problems (b) Consider the same metal–semiconductor junction with an acceptor layer of width ` and doping NA at the junction. What is the electric field as a function of position and the magnitude of image force lowering due to the changed electric field at the interface? 24. Consider a GaAs n-type material of doping 1 × 1017 cm−3 . What is the barrier energy if one places a plane of acceptors of sheet density, 1 × 1010 cm−2 , 5×1010 cm−2 , 1×1011 cm−2 , 5×1011 cm−2 , and 1×1012 cm−2 in it? 25. Consider a GaAs p+ –n junction doped 2×1018 cm−3 in the p+ region and 1 × 1017 cm−3 in the n region. For base widths of 1 µm, at what lifetime is the simplified expression that ignores recombination current suspect? 26. Consider an electric dipole layer of moment δ per unit area on either side of a junction. Show that this results in a discontinuous change in the electrostatic potential of δ. 27. A problem of particular interest in high-level injection is that of transport and storage in a p–i–n diode. The i-region is doped lightly n-type and the high injection condition exists in this lightly-doped region. Considering the electron and hole carrier concentration to be similar in the i-region, show that the carrier concentration at any position z in the i-region referenced to one of the junctions, for an i-region of width Wi , at a current density J, is LJ 1 cosh(z/L) 1 cosh[(Wi − z)/L] n(z) = + . (4.241) 2q Dn sinh(Wi /L) Dp sinh(Wi /L) √ In this equation, the diffusion length L = Dτ where D is the ambipolar diffusion length given as 2Dn Dp , (4.242) D= Dn + Dp and τ is the high-level injection lifetime given by τ = τn0 + τp0 . 28. What is the ratio between the diffusion capacitances of one-sided widebase and narrow-base p–n junction diodes in terms of time constants? 29. Consider the analysis of p–n junctions, in low-level injection, but with the Dirichlet boundary conditions at the ohmic contacts. Find the minority carrier distribution for the homogeneously doped abrupt junctions. In the p-type region, the electron concentration, e.g., is given by n(z) = np0 + Sτn sinh [(z + zp )/Ln ] + Ln cosh [(z + zp )/Ln ] . (4.243) Sτn sinh [(zp − wp )/Ln ] + Ln cosh [(zp + wp )/Ln ] In short devices, i.e., with (zp −wp )/Ln 1, show that the ohmic contacts are inefficient and lead to increased storage and smaller current if S< Dn . zp − wp (4.244) 270 Transport Across Junctions Chapter 5 Metal–Semiconductor Field Effect Transistors 5.1 Introduction The simplest and most common form of a field effect transistor in GaAs utilizes a metal gate to control the transport through the channel, and is called the metal–semiconductor field effect transistor (MESFET). It is a close analog of the junction field effect transistor and operationally similar in principle. The depletion region of the metal–semiconductor junction is used as a means to control the conductivity of the channel region. Since the extent of the depletion region can be modulated, the channel current can be modulated. It thus uses a capacitive coupling between the metal gate and the conducting channel for the modulation. Carriers flow from the source of the transistor to the drain of the transistor. With increasing drain bias, for a gate bias that allows for channel conduction, channel current and drain current saturate or change slowly. For large gate-length devices, with relatively low fields, this current saturation is associated with the pinching of the channel due to a gate-to-drain voltage that depletes the doped channel region. For short gate-length devices, saturation of the velocity of carriers is responsible for the current saturation. In either of the cases, a drain current that is weakly dependent on the drain bias, i.e., exhibiting a high output resistance or a low output conductance, occurs. This allows for a nearly constant drain current drive under quasi-static conditions that can be modulated by a gate voltage. Capacitive coupling allows for high input impedance, and current saturation results in a desirable current source. The device can therefore be used in analog and digital applications, with the compound semiconductors providing an improvement in the transport characteristics of the carriers, generally electrons. In all these, the device is operationally similar to the junction field effect transistor. The metal gate, or the characteristics of the semiconductor, bring perturbations which are of significance in the behavior of the device, and ulti271 272 5 Metal–Semiconductor Field Effect Transistors mately in our use of the device. Many effects are common between the MESFET and the other field effect transistor of interest in compound semiconductors— the heterostructure field effect transistor (HFET). Our discussion of many of the characteristics, therefore, overlaps, and hence a few of the common phenomena have been chosen for emphasis in the discussion here, and a few of these will be discussed in the context of HFETs in Chapter 6. Detailed differences in operational characteristics of different field effect transistors result from differences in junction characteristics, transport characteristics, and characteristics of control of mobile charge in the channel. Examples of differences in characteristics due to junctions include those due to the metal– semiconductor junction for the MESFET, p–n junction for the junction FET, or metal–insulator–semiconductor junction for the MISFET. Metal-semiconductor junctions, e.g., have a lower built-in junction voltage, and hence begin to conduct current at smaller forward biases than either the p–n junction or the metal– insulator–semiconductor junction. Examples of transport characteristics relate to differences in low field and high field behavior of carriers. Electrons in compound semiconductors generally exhibit large mobilities and, at low dopings, negative differential velocities. The former causes increased emphasis on effects related to saturation of velocity, and the latter leads to formation of accumulation and depletion regions of carriers along the channel because of the decrease in velocity with increasing longitudinal channel fields. Thus, a MESFET, which is based on a doped channel, and a MISFET, which is based on carrier transfer to a low doped channel region, exhibit differences resulting from the above. Examples of control of mobile charge are more immediate. A MESFET, e.g., is based on removal of carriers which would otherwise be present under quasineutral conditions in the material, while HFETs include examples of devices where this conducting charge may be induced. The effect of this basis of operation on parasitic resistances as well as on current continuity is very direct. One important consequence, e.g., is that MESFETs tend to have a saturated drain current that is closer in dependence to the square of the gate voltage while HFETs have a closer to a linear dependence. Two additional and particularly important effects unique to compound semiconductors that will be discussed are that of sidegating (also called backgating), which is the ability of a potential distant from the device, arising from the trapping characteristics of the substrate, the substrate surface, and the interfaces, to influence the channel current; and the piezoelectric effect, which is the creation of a position-dependent charge density due to stress (e.g., from metallurgies and dielectrics) and the ionic character of compound semiconductors—an effect which again results in shifts in the electrical characteristics. We will also emphasize some of the interesting aspects and implications of the accumulation and depletion region that forms in the channel due to current continuity as well as due to negative differential mobility. First, however, we will discuss quasi-static models, useful in predicting current– voltage characteristics and commonly applied in computer-aided design. We will discuss the principles that these are based on to understand their limitations, and we will selectively use rigorous small-signal high-frequency and two- 5.2. ANALYTIC QUASI-STATIC MODELS 273 dimensional analyses to emphasize their approximations. We will also discuss the off-equilibrium and transient behavior of devices, both in the short-channel limit, and emphasize the non–quasi-static aspects of operation in transient conditions. The appeal of the computer-aided design models is their analytic or numerical simplicity, which brings together with it a more intuitive insight. However, these models must always be used with caution and with an understanding of their limitations. We will discuss these models in order of increasing complexity and generality. Our discussion, therefore, extends beyond the simplest of these models to predict and evaluate the quasi-static behavior more accurately, and in the process also assimilate the limitations of simpler models. We will begin our discussion of computer-aided design models by discussing the long-channel device limit where constant mobility is an adequate approximation, then discuss the short-channel device limit where velocity is approximated as being constant along the channel, and then develop a model where both of these limits are included. 5.2 Analytic Quasi-Static Models We have remarked that the appeal of computer-aided design models is their analytic or numerical simplicity, which brings together with it a more intuitive insight. The simplest form of such a model assumes a constant mobility operation of the transistor. Thus, for a practical semiconductor, it implies operating in a bias region where the electric fields remain low and approximately in the constant mobility region of the semiconductor velocity-field characteristics. Most semiconductors exhibit deviation from this behavior at electric fields exceeding 1 × 103 V.cm−1. For operating voltages of a few volts, this requires the device gate-length to be larger than 20 µm. This electric field, the channel electric field, can of course be much smaller than the field in the depletion region that modulates the channel width and hence conductance. A particularly useful simplification in the analysis under conditions of a large difference in the electric field between the depletion and the channel region is the gradual channel approximation. 5.2.1 Gradual Channel Approximation Since the current flow in the FET occurs due to application of drain-to-source voltage across the channel with the modulation of channel conductance by the gate-to-source voltage, one would expect the problem to be complicated with electric fields being two-dimensional in the structure. Real situations quite often lend themselves to approximations which ease the description of the physical problem. Figure 5.1 shows underneath the gate of a MESFET, in the mirrored part of a symmetric configuration, the conduction band edge and the velocity of carriers in the conducting part of the channel. The channel current flow occurs between the source and the drain, and the gate potential controls the 274 5 Metal–Semiconductor Field Effect Transistors Figure 5.1: Surface plot of the conduction band edge of a 5 µm gate length GaAs MESFET is shown in (a). (b) shows the band edge and the velocity of carriers at a cross-section in the conducting part of the channel. 5.2 Analytic Quasi-Static Models 275 Figure 5.2: A schematic of a long-channel device with geometric parameters used in the long-channel model. constriction of the channel and hence the conductance. The channel current flow occurs in the z-direction, with the channel cross-section and the electric field Ez varying with z. In addition, there is a component of the electric field Ey due to the gate potential. In a symmetric structure, Ey goes to zero at the center (shown at the 0.25 µm in in Figure 5.1(a)), but increases towards the surface. If, in the conducting part of the channel, this electric field stays very much smaller than Ez , then the equi-potential surfaces are planes nearly orthogonal to z. The problem now reduces to one dimension, in the z-direction of the channel, and in the y-direction in the depleted region underneath the gate. An accompanying relationship of this one-dimensional framework, which is referred to as the gradual channel approximation, is that the electric field Ez should vary in the channel region slowly with z, and hence the carrier density should also vary slowly in the channel. 5.2.2 Constant Mobility Model We first consider a geometry where this approximation is very accurate, the case of a device with a long gate-length, i.e., a long-channel device where the fields are sufficiently small that a constant mobility may be assumed. Figure 5.2 shows variation of the depletion region in our device. The figure also shows geometric parameters to be used in our analysis. In the long-channel model, the gradual channel approximation is valid because while the gate and drain voltages are comparable, the channel length is significantly larger than the thickness of the conducting layer. We can get closed-form solutions if we further assume abrupt depletion and ignore diffusive current. The latter follows from a small channel electric field, which implies small deviations from quasi-neutrality and therefore a small gradient in carrier concentration. The depletion layer width h(z) varies slowly along the channel. The electric field in the depletion region is along the y-axis and the electric field in the channel region along the z-axis. In the depletion region, using depletion approximation, − d2 V ρ(y) qND = = dy2 s s (5.1) 276 5 Metal–Semiconductor Field Effect Transistors for uniform doping, and hence the depletion region width h(z) at any position z along the channel is given by h(z) = 2s [V (z) + VG + ψj0 ] qND 1/2 , (5.2) where V (z) is the channel voltage at z w.r.t. the source, ψj0 is the built-in voltage of the metal–semiconductor junction (ψj0 = φM − Vn ), and VG is the absolute gate voltage. The square-root dependence in voltage above, or other similar parametric dependence in voltage, occurs quite often in these analytic models in field effect transistors. We will encounter a similar form in cubic root in our analysis of HFETs. These parameters form a convenient basis for deriving and writing expressions for current. These parameters characterize identifiable features of the device or their normalizations. h(z) can be used as a parameter itself, or in its normalized form u(z) = h(z)/a, they are related to the width of the depletion region underneath the gate. We have h(z = 0) = 2s (VG + ψj0 ) qND 1/2 (5.3) at the source end, and h(z = L) = 2s (VD + VG + ψj0 ) qND 1/2 (5.4) at the drain end. In a constant mobility long-channel model, the highest electric fields are limited. For example, 5 V across a 100 µm channel leads to an average field of 500 V.cm−1 , which is sufficiently small that a constant mobility may be assumed throughout the device. The saturation of the current in such a device occurs when the drain end of the gate pinches off, and is depleted of carriers. This condition, termed channel pinch-off, occurs when 2(VD + VG + ψj0 ) h(z = L) = a = qND 1/2 . (5.5) The pinch-off voltage therefore, is defined as the parameter Vp , where Vp = qND a2 . 2s (5.6) This is the magnitude of the voltage between gate and source to shut off current flow in the channel, since the extent of the gate-source depletion width is now a, and hence carriers do not enter the channel. It is also the voltage between the gate and the drain when current saturation occurs, because it pinches off the drain opening in the channel. These voltages are identical due to constant mobility and gradual channel approximation. In general, such as for the models we discuss later, these voltages can be different. The gate voltage required 277 5.2 Analytic Quasi-Static Models to shut off current flow is usually referred to as the threshold voltage, and the voltage required to saturate the current is usually referred to as pinch-off voltage. We will return to the questionable practice of referring to this as a pinch-off voltage, later in our discussion of the combined constant mobility and constant velocity model. In a first-order approximation, at any position z along the channel, we can evaluate the drain current assuming that the diffusion current is negligible. This is quite valid over much of the channel, but not at the drain end of the gate. A pinch-off of the channel maintains current continuity because a large diffusion current flows through this region. The gradient of carrier concentration is large at the drain end. We assume that this condition is met to satisfy current continuity. In other parts of the device under the gate, drift current is dominant, and hence one may write dV dz (5.7) 2s (V + VG + ψj0 ) , qND (5.8) 2s dV, qND (5.9) ID = qND µW [a − h(z)] where the drain current enters the device. Since h2 (z) = we obtain 2hdh = and hence ID = W qND µ(a − h) qND dh h . s dz (5.10) We now employ the continuity of this current in the channel to eliminate the position-dependent variable h(z) by integrating over the local variable. This is a common technique that is useful in problems involving current continuity, e.g., it will also be applied in HFETs and in the collector depletion region of a bipolar transistor. Application of it along a path where current continuity is maintained allows for elimination of a local variable. Continuity allows one to obtain as a result the current in terms of variables at the source or drain end in this problem. Integrating, Z 2 L ID dz = 0 (qND ) µW s Z h(L) h(0) (a − h)hdh, (5.11) and ID W µq 2 ND 2 a3 = 6s L 3 2 2 3 2 3 h (L) − h (0) − 3 h (L) − h (0) . a2 a (5.12) This is the form of the current, in constant mobility and long-channel approximation, in terms of structural variables and h(0) and h(L), which depend on biases applied at the terminals and parameters of the device. 278 5 Metal–Semiconductor Field Effect Transistors The expression above can be written in terms of voltages and other normalized parameters, to make it appear more direct. Using the normalizations, Inorm = W µq 2 ND 2 a3 , 6s L (5.13) and and u = u(0) = u(L) = 1/2 V + VG + ψj0 , Vp 1/2 h(0) VG + ψj0 = , a Vp 1/2 h(L) VD + VG + ψj0 = , a Vp h(z) = a (5.14) we can express the drain current as ID = Inorm 3 u2 (L) − u2 (0) − 2 u3 (L) − u3 (0) ( ) i VD 2 h 3/2 3/2 = Inorm 3 − 3/2 (VD + VG + ψj0 ) − (VG + ψj0 ) . Vp Vp (5.15) These expressions relate the current up to the point of pinch-off of the channel. At this bias, which occurs when h(z = L) = a or equivalently u(y = L) = 1, the drain current saturates and then remains constant independent of the drain bias. This current IDSS is given by " 3/2 # VG + ψj0 VG + ψj0 IDSS = Inorm 1 − 3 +2 , (5.16) Vp Vp which occurs at a drain-to-source voltage VDSS given by VDSS = Vp − VG − ψj0 = qND a2 kT − VG − φM + ln 2 q NC ND . (5.17) The quasi-static expression for drain current in terms of the gate and drain biases is complete, and we may determine the quasi-static device parameters using these expressions. As an example, the transconductance follows from this analysis as: 2W µqaND ∂ID gm = = [u(L) − u(0)] , (5.18) ∂VG L and the output conductance follows as gd = ∂ID 2W µqaND = [1 − u(L)] ∂VD L (5.19) 5.2 Analytic Quasi-Static Models 279 in the bias region before the channel pinches off. This region is sometimes referred to as the triode region of operation because of its poorer output conductance. For biases beyond channel pinch-off, i.e., for drain voltages exceeding VDSS (VDSS being dependent on the gate bias), the transconductance in this model stays constant, and the output conductance is zero. Because of the latter, the output characteristics beyond current saturation are said to be pentode-like. The transconductance can be found by finding its magnitude at VDSS . So, in the triode region, the transconductance " 1/2 1/2 # 2W µqaND VD + VG + ψj0 VG + ψj0 gm = − , (5.20) L Vp Vp and in the pentode region, the transconductance " 1/2 # 2W µqaND VG + ψj0 gm = 1− . L Vp (5.21) Note that in the constant mobility assumption, the derivation of the behavior is quite straightforward, and even for complicated impurity distribution functions (e.g., Gaussian, complementary error function, etc.) simple results can be derived. However, these are valid only as long as the constant mobility assumption is a good one. For GaAs devices, this requires maintaining electric fields below 1000 V/cm. So for a device with 5 V drain bias the gate-length should be maintained at 5/1000 = 50 µm. Devices used in circuits are significantly smaller than this. We will therefore consider the other limit of the behavior of devices—that based on a constant high field velocity throughout the channel. This follows our discussion in the introduction. 5.2.3 Constant Velocity Model For shorter gate-lengths, with average fields exceeding 3 × 103 V.cm−1, the velocity of the carriers is similar to or larger than the saturation velocity vs , as shown in Figure 5.3. Thus, carriers transit with a velocity that is on an average higher than the saturated velocity. The simplest method of analyzing this prob0 lem would be to assume a source end velocity vs , which is close to the saturation velocity or slightly exceeding it, because the field is the smallest at the source end and below the peak-velocity field. We may also ignore diffusive currents because the gradient in carrier concentration remains low; velocity saturation in a constant-channel cross-section requires the absence of gradient in carrier concentration. The consequence of this nearly constant carrier concentration is that even though this velocity occurs in a region where the linear velocity–field relationship is largely maintained, since it does not change appreciably any fur0 ther, we may incorporate a constant velocity vs in evaluating the current. Thus, for gate-lengths ≈ 1µm of interest, instead of a constant mobility assumption, 280 5 Metal–Semiconductor Field Effect Transistors Figure 5.3: Surface plot of the conduction band edge in a 1 µm gate length 5 × 1017 cm−3 doped GaAs MESFET is shown in (a). The conduction band edge and the velocity of carriers is shown in (b) in a conducting part of the channel. This figure should be compared with the 5 µm gate length MESFET shown in Figure 5.1. Both devices are biased under identical conditions and have similar threshold voltages. 281 5.2 Analytic Quasi-Static Models we now resort to a constant velocity assumption to crudely estimate the current. This current I is 0 I ≈ qnvs [a − h(0)] W. (5.22) Under quasi-static conditions this particle current is continuous, and hence this is also the drain current of the device. IDS ≈ ∝ 0 qW vs [a − h(0)] ND " 1/2 # V . Inorm 1 − Vp (5.23) This expression is appealing in simplicity and extendable to obtain the transconductance of the device, since the dependence of the source-end depletion width h(0) is known as a function of gate-source bias. Note that the current changes with a square-root power dependence on voltage because of the direct effect of the modulation of the width of the channel. We have assumed that a field exists at the source end that is sufficient to cause a large velocity, comparable to the saturated velocity, even though it is largely in the constant mobility region of the device. The accuracy of this constant velocity model is limited by the extent of this constant mobility section. So long as it is short, the analysis is meaningful. However, if the extent of this region is large, the velocity in the drift current expression is an abstraction of a hypothetical average, meaningful only as a fitting parameter following an experiment, and limited in the predictive ability desired from models. So, this is an approximate relationship, and is only applicable in the region of device operation where the drain current has saturated. However, it serves well to relate the approximate variation expected in the drain current in response to a change in gate voltage for an arbitrary doping profile within the channel, or for variations 0 of other parameters such as the velocity vs ≈ vs . For many digital circuits, there is a preference to have devices with constant but large transconductance. Hence, there has historically been an interest in doping profiles that give linear IDS –VG characteristics. From the above relationship, it can be seen that this is connected with how the depletion width h(0) changes with the gate voltage. A smaller change in the depletion width with bias leads to a smaller change in the transconductance also. As we shall see later, HFETs based on inducing the conducting charge in a two-dimensional electron gas channel come quite close to having a constant transconductance because of the nearly constant depth and the linear dependence of this charge through capacitive coupling of the gate. For MESFETs, this would require a large doping of small width at the edge of the depletion region with a small doping everywhere else. This kind of doping pattern is referred to as planar doping. The device is fully turned on when this region is undepleted and turned off when it is depleted. Since the position of the depletion edge does not change substantially between these two,1 the 1 Screening is of particular importance to this problem. It was been shown earlier that a plane of doping leads to a carrier distribution with exponential tails characterized by the Debye length. This Debye length also characterizes the shape of the carrier distribution at 282 5 Metal–Semiconductor Field Effect Transistors transconductance is nearly constant. Problem 2 considers the behavior of the transconductance for various channel doping profiles. Because of the constant velocity assumption, different doping profiles in the channel should lead to a transconductance–voltage relationship which follows the behavior of capacitance–voltage relationship, which relates the controlled charge to the gate bias. Thus, the gate-to-source capacitance dependence on gate bias is related to the transconductance behavior or the dependence of drain current on the gate bias. A constant capacitance implies a linear charge control in voltage, and hence when the charge moves with a constant velocity, a linear IDS -VG characteristic is obtained. The example of planar doping pins the depletion region at the doping plane and hence leads to the nearly constant capacitance–voltage and transconductance–voltage behavior. In order to assure pinch-off of the channel of the device, only a limited amount of charge compatible with the breakdown voltage of the gate can be placed in the doped region. The drawback of such a profile is that it leads to large source and drain resistance because the undoped region cladding the doped planar region makes it difficult to form low access regions to the source and drain of the device. HFETs, which we commented on as another example of linear transconductance devices, have the desired attribute of forming this planar region using a two-dimensional carrier gas, along with a simplified low resistance implementation. 5.3 Constant Mobility with Saturated Velocity Model We have now developed an approximate description of the behavior of the MESFET under two conditions: under a low longitudinal electric field in the channel where we applied the constant mobility model together with the gradual channel approximation, and under a high longitudinal electric field in the channel where we applied a constant velocity model. To develop a general framework we must include both of these in a unified model so that it may have a general applicability for various gate-lengths as well as for various bias conditions. Even for small gate-lengths our approximate constant velocity model is still limited to conditions of high fields and hence large drain bias conditions in the device. It does not, therefore, predict the current–voltage relationship before the onset of current saturation. At low voltages and hence low electric fields, the constant mobility model would be more appropriate. So, we now go a step further and combine the constant mobility and constant velocity assumptions in a single device. Since this would develop a model that incorporates both the low-field constant mobility feature and the high-field constant velocity feature of carrier transport, it should have more general application. We now consider the entire velocity–field behavior of the carrier by making a constant mobility and constant velocity approximation of the two limits of the the edge of the depletion region. Hence the order of change in the depletion width between the on and off conditions for planar doping is of the order of Debye screening length. 5.3 Constant Mobility with Saturated Velocity Model 283 Figure 5.4: Device cross-section (a) and the assumed velocity–field curve (b) for the PHS model as an approximation to the velocity–field curve at typical channel dopings exceeding mid-1017 cm−3 in GaAs. In region I of both parts, constant mobility is assumed. In region II of both parts, a constant velocity is assumed. behavior. This approximation of the velocity–field curve and transport behavior in the channel is shown in Figure 5.4. Thus, we will assume the constant mobility to be an adequate approximation in the part of the device channel at the source end where the fields are low, and we will assume the constant velocity to be an adequate approximation at the drain end of the channel where the fields are high. Our discussion follows the analysis of Pucel, Haus, and Statz, and will be referred to as the PHS model.2 The saturation in channel current occurs when the field towards the drain end becomes high enough that the carriers begin moving with a constant high field limit velocity—the saturated velocity. The channel current saturation, or equivalently the drain current saturation, occurs due to the saturation in the velocity of carriers. Recall that in the constant mobility model it occurs due to the pinching of the channel. These are quite different in nature. Current saturation, with a constant cross-section for flow of carriers, implies a constant carrier distribution for current continuity in the former and a constant carrier gradient in the latter. The latter is important in long gate2 R. A. Pucel, H. A. Haus, and H. Statz, “Signal and Noise Properties of Gallium Arsenide Microwave Field-Effect Transistors,” in Advances in Electronics and Electron Physics, 38, Academic Press, N.Y. (1975) also has a treatment of noise and a historic introduction to early MESFET models for computer-aided design. The PHS model is an example of quasi-static model. For a lucid discussion of the general approach that is the basis of PHS model see the treatment on junction field effect transistors in R. S. C. Cobbold, Theory and Applications of Field-Effect Transistors, Wiley-Interscience, N.Y. (1970). Cobbold’s book also contains a detailed treatment of small-signal modelling. 284 5 Metal–Semiconductor Field Effect Transistors length devices where the current density is small and hence the gradient in carrier concentration is feasible without violating the particle velocity limits from the characteristics of the semiconductor. In small gate-length devices, the fields at the drain end are large enough, the gradual channel approximation is no longer applicable, and the carriers move with velocities close to the saturated velocity. Once this channel current saturation occurs, the gate depletion width accommodates itself longitudinally, towards the source and the drain, to allow for the drain current to flow through the undepleted part of the channel. We will consider the device geometry shown in part (a) of Figure 5.4. We ignore the current in the substrate of the device as well as its effect on the flow in the channel itself by considering a symmetric section of a device with the second half being a mirror reflection of the bottom edge of the device. In our earlier analysis, we had ignored the substrate boundary; implicitly, this is the geometry that we analyzed. Our velocity–field curve is a two section model (Figure 5.5) that is an approximation of the semiconductor velocity–field curve. This figure also shows the variation in channel opening, Here, at low fields a constant mobility is used, and at fields E > Es a constant velocity is used. We obtain continuity in the slope of the derived characteristics by matching the boundary conditions at the point at which E = Es . This will also serve for us as a demonstration of the use of boundary conditions in matching sections with the constraint of current continuity. Among other parameters for the device, a is the channel thickness, b is the channel opening, and V is the a normalized potential. In the region of length L1 , where E < Es , gradual channel approximation is assumed to be valid; this field is low enough that it is significantly smaller than the transverse gate field and we employ a constant mobility. In the region beyond, of length L2 , the carriers are assumed to move with their limit velocity, the saturated velocity velocity vs . The point L1 , therefore, defines the spatial point of onset of velocity saturation. We will denote the potential of this point by Vp , in conformity with the earlier analysis, since drain current saturation is intimately related to this velocity saturation.3 We assume the source at ground potential. The potential of the channel referred to the gate is V(z) = Vsg + φM − V (z). (5.24) This is a translated variable, whose magnitude at the source end, the drain end, and the point at which the carrier velocity saturates are Vs and Vd Vp = Vsg + φM , = Vsg + φM − Vsd , = Vsg + φM − Vp . (5.25) 3 In the constant mobility model, the current saturation occurs due to a pinch-off of the channel where few carriers exist, and current transport occurs via diffusion in this pinched region. In the constant velocity model, the channel does not physically pinch off. The velocity saturates and a large carrier density exists that supports the drift current. These are distinctly different. The subscript p, whose origin is in this “pinch-off ” term, should not be confused with a physical pinch-off of the channel. 5.3 Constant Mobility with Saturated Velocity Model 285 Figure 5.5: (a) shows the channel opening (ξ(z)) as a function of channel position, (b) shows the electric field (E(z)) as a function of position, (c) shows the velocity of carriers (v(z)) as a function of position, and (d) shows the normalized potential (V(z)) as a function of position along the channel. These figures are shown schematically for a doping of 2.5 × 107 cm.s−1 . 286 5 Metal–Semiconductor Field Effect Transistors In the constant mobility model, we employed a variable h proportional to the square root of potential—this term represented the depletion depth. It is useful to employ a similar square-root term here. We will employ a normalization factor of the channel thickness a. These normalization factors, the reduced potentials,4 are the following at the source end, the drain end, and at the point of velocity saturation: ξs and = ξd = ξp = Vs V00 Vd V00 Vp V00 1/2 1/2 1/2 , , , (5.26) with the reduced potential at any position z along the channel as ξ(z) = V(z) V00 1/2 . (5.27) In these expressions, the normalization potential is the potential V00 = qND 2 a , 2s (5.28) which is the potential associated with full channel depletion in gradual channel approximation. Note that because of the square root of V, the terms ξs , ξd , ξp , and ξ(z) correspond to the depletion region width normalized by the channel thickness, since, in the depletion region, the fields largely terminate on the gate electrode irrespective of the behavior in the channel region. The parameter ξ, therefore, corresponds to the parameter h used in our earlier constant mobility calculations. The manner in which we assure current continuity, and include velocity saturation and hence the existence of large longitudinal fields in the channel, prevents it from being identical, and allows us to include the velocity saturation effect. In the constant mobility section of the device, using gradual channel approximation, 2 b(z) V(z) = V00 1 − (5.29) a and ξ(z) = 1 − b(z) . a (5.30) 4 We employ the symbol ξ for this. It should not be confused with the symbol for quasiFermi energy. 5.3 Constant Mobility with Saturated Velocity Model 287 Also, at any cross-section, the current I, which is also the drain current ID because of current continuity, is given by I = ID = b(z)W qµ0 ND ∂V , ∂z (5.31) where W is the gate width. This gives, in the constant mobility section of the device, Z L1 Z ξp ID dz = 2aqµ0 ND W V00 (1 − ξ)ξdξ. (5.32) 0 ξs Note, b(z) and so ID = 2ξ(z)dξ(z) = a [1 − ξ(z)] , dV(z) , = V00 aqµ0 ND W V00 2 ξp 2 − ξs 2 − ξp 3 − ξs 3 . L1 3 (5.33) (5.34) This relationship is identical to that derived for the constant mobility model since it is based on identical assumptions. The difference between the present model and the constant mobility model is that the latter assumes constant mobility is valid over the entire channel length. We may introduce go as a conductance parameter per unit width, go = aqµ0 ND , giving ID g0 W V00 2 3 3 2 2 = ξp − ξs − ξp − ξs . L1 3 (5.35) (5.36) In the second region, where the constant velocity assumption is applied, vs = µ0 Es . (5.37) Since velocity is constant and the field in the conducting section is longitudinal, in the presence of a constant channel thickness and hence constant depletion region width, current continuity can only be maintained by a constant carrier concentration. The current at the point of velocity saturation is ID = = qµ0 Es ND W a(1 − ξp ) = go W Es (1 − ξp ) Inorm (1 − ξp ). (5.38) The normalized current Inorm = qvs ND W a is the drain current if the channel is completely open and carriers move at saturated velocity. This is the maximum current that can be obtained from the device. Current continuity between the constant mobility and constant velocity sections implies go W V00 2 ξp 2 − ξs 2 − ξp 3 − ξs 3 = go W Es (1 − ξp ), (5.39) L1 3 288 5 Metal–Semiconductor Field Effect Transistors and hence the length L1 is given by V00 2 2 2 3 3 ξp − ξs − ξp − ξs . L1 = Es (1 − ξp ) 3 (5.40) 2 1 2 2 3 3 ξp − ξs − ξp − ξs , L1 = L α(1 − ξp ) 3 (5.41) We write this as where α= Es L V00 (5.42) is a dimensionless potential parameter that the PHS model calls saturation index. It is inversely related to the degree of importance of saturation of velocity in the determination of the device behavior. Recall that V00 , for a constant mobility model, is the voltage for current saturation. For large α, the parameter V00 Es L; hence typically applied voltages are less than the voltages required to achieve velocity saturation across a significant fraction of the channel lengths. So, a large α results in constant mobility–dominated behavior of the device. If α is small, Es L < V00 , and hence, for potentials typical of current saturation, in a substantial part of the device, the carriers travel at saturated velocities. Let us now consider the channel potential for a given current ID through the device. Consider the first section of the device, where the gradual channel approximation is applicable. The potential in the channel at the point of onset of velocity saturation is Vp = = −(Vp − Vs ) −V00 (ξp 2 − ξs 2 ). (5.43) The field in the depleted region is transverse, and the field in the channel with a constant mobility conduction is longitudinal. In the second section, both in the depleted and constant velocity conduction region, the fields are two-dimensional. For this section, the potentials can not be derived in as straightforward a fashion, since gradual channel approximation is no longer applicable. We may not use the one-dimensional Poisson’s equation applied in the conducting region of the first section, which followed from the existence of only a longitudinal field in the constant mobility section. In the constant velocity section, the fields are two-dimensional, and the electrostatic potential ψ is a function of both y and z. A rigorous solution would require us to solve the problem subject to the boundary conditions of continuity in potential and field at the intersection of the constant mobility and constant velocity regions for all y’s and also to satisfy the appropriate approximations of boundary conditions at the gate–semiconductor interface, at the drain contact interface with the second region, and at the line of mirror symmetry at the bottom. Our solution will be approximate. We break the problem in two parts, emphasizing the two electrostatically distinct parts. Let ψ2 be the electrostatic 289 5.3 Constant Mobility with Saturated Velocity Model potential associated with the large charge density qND of the depletion region lacking in mobile charge, and let ψ1 be the electrostatic potential associated with the conducting region filled with mobile charge. The superposition of these two potentials, ψ = ψ1 + ψ2 , is the electrostatic potential of the second region with ψ1 dominating in the conducting channel part and ψ2 in the depletion region part. The potential ψ2 is still approximately parabolic in y because the depletion charge still largely terminates on the gate electrode. In the conducting region of the channel, carriers move at the constant saturated velocity, carrier concentration is constant to maintain current continuity, and hence the longitudinal electric field is associated with charge at the drain electrode. So, in the conducting part of the second region, −∇2 ψ1 = q (ND − n) ≈ 0 for L1 < z < L, (5.44) i.e., ψ1 satisfies Laplace’s equation. We employ the boundary conditions of continuous longitudinal electric field and potential at z = L1 , and vanishing transverse field at y = 0, the central cross-section of the device. Mathematically, and ψ1 (z = L− ) 1 ∂ψ1 ∂z z=L− 1 = = ψ1 (z = L+ 1) ∂ψ1 . ∂z z=L+ (5.45) 1 For the general case, the solution to Poisson’s equation for the above problem is the sum of the solution to Laplace’s equation (ψ1 ) and the solution to Poisson’s equation with fixed ionized charge (ψ2 ). The solution to Laplace’s equation is a sum of products of exponentials in the two orthogonal directions. Since, in the y-direction, the field vanishes at the surface, and since it builds up towards the drain electrode (the charge on the drain electrode sustains this field), intuitively one would expect the solution to be a harmonic function that peaks at y = a and vanishes at y = 0, i.e., a cosine function, and an exponential function in the z direction. The solution for potential should be of the form ψ1 (y, z) = m=±∞ X m=0 Am (−1)2m+1 cos mπ(z − L1 ) mπ(y − a) exp − + B, 2a 2a (5.46) where the Am ’s and B are constants. Strictly speaking, we should have tried to force the cosine function to zero at the depletion region edge since the mobile charge nearly vanishes there. This would lead to a very complex analytic formulation. In this approximate solution we wish to emphasize the accuracy at y = a so that we may calculate the potential accurately along this line of symmetry. The calculation of the potential at y = a does not get severely affected by the approximation in the cosine function. So, an approximate result for the potential drop and length of the region can be found by considering the behavior at y = a. In the above series, the terms corresponding to m = 0 and m = ±1 have the largest contribution 290 5 Metal–Semiconductor Field Effect Transistors for this cross-section of symmetry. This contribution, π(y − a) π(z − L1 ) 2a ψ1 (y, z) = − Es cos sinh + ψ(L1 ), π 2a 2a (5.47) where ψ(L1 ) is the potential of the channel derived as a solution from the analysis of first region, may be seen as the part of the solution that corresponds to a point drain contact at y = a and z = L, and the resultant variation in ψ(y, z) is most accurate at the cross-section of symmetry with large deviations occurring further away. At y = a and z = L1 , the longitudinal electric field is Es and the potential is ψ(L1 ). Since the potential is symmetric in the y-direction around y = a, the transverse field vanishes at y = a. Also, because of the cosine term, the longitudinal field drops off towards the depletion region edge and into the depletion region. The approximation here is clear; in the conducting region, while we actually expect the potential variation in the y-direction to be negligible, this potential describes it as changing appreciably. However, at y = a, this potential is quite accurate. So, this potential should be considered as the approximate solution in the conducting undepleted region at y = a, and we will make appropriate evaluations of voltage drops, etc., at y = a only. In the depletion region, the electric field is mostly transverse, the charge is + ND , and the total potential (sum of contribution from the depletion region and the conducting region) increases parabolically towards the gate. Our rationale in adopting the above approach to obtain relatively simple results is that if we model behavior at y = a accurately enough, maintaining current continuity, then the results will not be too different from an analysis considering more terms in the harmonic series expansion. Were we to adopt the latter approach, we could also consider the potential contribution of the charge in the depletion region too, by considering the boundary conditions in terms of equi-potential surface at the gate, no orthogonal field at y = a, continuity of potential and electric field at z = L1 , and equi-potential surface at the drain electrode. This would be unwieldy. The longitudinal channel voltage drop in our present approximation can now be obtained as follows 2 a πL2 VII = −V00 α sinh , (5.48) π L 2a hence, Vsd 2 a πL2 = −V00 (ξp − ξs ) − V00 α sinh π L 2a a 2 πL2 2 2 = −V00 (ξp − ξs ) + α sinh , π L 2a 2 where L1 = L 2 ξp 2 − ξs 2 − 23 (ξp 3 − ξs 3 ) , α(1 − ξp ) (5.49) (5.50) 5.3 Constant Mobility with Saturated Velocity Model 291 and L2 = L − L1 . (5.51) Given Vsd , Vsg , and L, we know the source end opening a(1 − ξs ). Device and material parameters imply knowledge of the long-channel pinch-off normalized potential V00 , the saturation index α, and the channel thickness a. This allows us to determine the drain end opening a(1−ξp ). From this the device characteristics follow. Figure 5.6 shows the output characteristics of GaAs MESFETs with 1µm and 10 µm gate-lengths. The dashed lines of this figure show the output characteristics in the constant mobility limit for zero gate bias. The PHS model shows the lowest current and a finite output conductance throughout the bias range. The constant mobility model shows zero output conductance in the current saturation region, and a much higher current. Since this model ignores any velocity saturation effect, it overestimates the velocity at this short gate-length and hence overestimates the current too. Clearly, a self-consistent inclusion of constant mobility and constant velocity conduction is important in predicting the device characteristics. Let us now look at some of the device parameters and get a feel for the degree of importance and implications of the saturation of velocity. A plot of opening in the channel at the source and drain ends (a(1 −ξs ) and a(1 −ξp )) as functions of the drain current is shown in Figure 5.7. In this figure, at a constant current, the openings are a function of the aspect ratio (L/a). Small aspect ratios and small gate-lengths mean nearly identical source and drain openings (the source opening is slightly larger because of smaller velocities) because carriers transit at saturated velocities through much of the device. Note that because of velocity saturation, the channel can be fully open at high gate biases even when high drain biases occur. The saturated velocity forces the drain end of the channel to remain significantly open even at high drain biases in order to maintain the large drain currents. The source opening is bigger but not significantly. At 1/10th the full channel current, it may be about 30–40% percent bigger for the longest aspect ratio device of L/a = 10. For a smaller aspect ratio, e.g., a 1.0 µm gate-length with a 0.3 µm channel thickness, the source opening is within 5% of the drain opening. The depletion region is essentially parallel to the surface—which also indicates the quite good validity of gradual channel approximation. While the differences in fractional openings at source and drain ends are insensitive to the current being driven or the drain voltage, the fractional length of the velocity saturated region is very sensitive, with L2 /L increasing rapidly with Vsd . Figure 5.8 shows an example of this dependence for our model device at various aspect ratios, with the smaller aspect ratio showing the larger effect. The smaller the aspect ratio of the device, the less is this region—but for shorter gate-lengths at a potential equal to the long-channel pinch-off potential V00 , e.g., for the device with L/a = 3, almost the whole longitudinal section may have carrier transport at saturated velocity. This is also seen from a plot with α as a variable shown in Figure 5.9. Notice that as the saturation index decreases. 292 5 Metal–Semiconductor Field Effect Transistors Figure 5.6: Output characteristics for a 1 µm gate length GaAs MESFET are shown in (a) following the PHS analysis. (b) shows the output characteristics for a 10 µm gate length GaAs MESFET following the PHS analysis. Both figures show, using dashed lines, the current for zero gate bias assuming no velocity saturation, i.e., assuming that a constant mobility is valid throughout the operation. 5.3 Constant Mobility with Saturated Velocity Model 293 Figure 5.7: Source (solid lines) and drain (dashed line) end openings of MESFET channel derived from the PHS model at different aspect ratios with Vsd /V00 = 1 and α = 0.1. The normalization parameter for current is Inorm . After R. A. Pucel, H. A. Haus, and H. Statz, “Signal and Noise Properties of Gallium Arsenide Microwave Field-Effect Transistors,” in Advances in Electronics and Electron Physics, 38, Academic Press, N.Y. (1975). 294 5 Metal–Semiconductor Field Effect Transistors Figure 5.8: Relative length of the velocity saturated region L2 /L as a function of the normalized source-to-drain voltage Vsd /V00 for different aspect ratios, ID /Inorm = 0.5, and α = 0.1. After R. A. Pucel, H. A. Haus, and H. Statz, “Signal and Noise Properties of Gallium Arsenide Microwave Field-Effect Transistors,” in Advances in Electronics and Electron Physics, 38, Academic Press, N.Y. (1975). 5.3 Constant Mobility with Saturated Velocity Model 295 Figure 5.9: The normalized length of the saturated velocity region L2 /a, as a function of the aspect ratio L/a for varying saturation parameters. Vsd /V00 = 1, and ID /Inorm = 0.5. After R. A. Pucel, H. A. Haus, and H. Statz, “Signal and Noise Properties of Gallium Arsenide Microwave Field-Effect Transistors,” in Advances in Electronics and Electron Physics, 38, Academic Press, N.Y. (1975). the transport effects in the saturated region become dominant. Since we can predict the output current–voltage relationship, we can also derive secondary parameters of interest (such as transconductance, output conductance, etc.) in the quasi-static approximation. We can also derive simplified limits of the capacitances by considering the electrostatics of the problem. These are considered next. 5.3.1 Transconductance We again use quasi-static approximation and find gm through perturbation of the drain current. gm = ∂ID − ∂Vsg Vsd ∂ξp ∂Vsg Vsd = g o Es W = go Es W dξp . 2ξs V00 dξs (5.52) 296 5 Metal–Semiconductor Field Effect Transistors This gives gm = Inorm (1 − ξs ) cosh (πL2 /2a) − (1 − ξp ) . V00 [2ξp (1 − ξp ) + α (L1 /L) cosh (πL2 /2a) − 2ξp (1 − ξp )] (5.53) Note when L2 → 0, i.e., when there is no velocity saturated region, gm ≈ go W (ξp − ξs ), L (5.54) which is our earlier long-channel expression. In the other limit of L2 → L, i.e., velocity saturated conduction throughout the channel, ξp ≈ ξs , and gm ≈ Inorm 1 , V00 2ξp (5.55) because the cosh term dominates, and gm ≈ Inorm 1 . 2V00 1 − ID /Inorm (5.56) This follows from our constant velocity expression (see Problem 1). Note that these expressions predict an increasing transconductance at smaller gatelengths. 5.3.2 Output Conductance The output conductance is defined as gsd ∂ID =− . ∂Vsd Vsg (5.57) Following our expression for current, this can be derived as gds = Inorm 1 − ξp . V00 [2ξp (1 − ξp ) + α (L1 /L)] cosh (πL2 /2a) − 2ξp (1 − ξp ) (5.58) When, L2 → 0, i.e., no velocity saturated region, gds = = Inorm V00 (1 − ξp ) V00 Es L go (1 − ξp )W . L (5.59) When the aspect ratio L/a gets smaller, the output conductance increases and the output characteristics of the device show higher slope. This was shown in the two separate plots for the long-channel and short-channel devices of Figure 5.6. For short gate-length structures, gds ≈ α a Inorm 1 , π L |Vsd | ξp (5.60) 297 5.3 Constant Mobility with Saturated Velocity Model from our expressions. The most inaccurate small-signal parameter in this model for predicting characteristics of real devices is this resistance, because the idealized geometry does not include injection into the substrate and modifications resulting from that in the device—a very important consideration under shortchannel conditions. We show implications of some of these effects in later sections. 5.3.3 Gate-to-Source Capacitance Since the depletion region charge also responds to changes in bias, this calculation is quite complicated. The total gate charge Qg is (see Problem 3) Qg ≈ 2qND aW α a2 π L " 2 (ξ 3 − ξs 3 ) − 12 (ξp 4 − ξs 4 ) 3 p (ξp 2 − ξs 2 ) − 23 (ξp 3 − ξs 3 ) + ξp L2 + πL2 cosh −1 , 2a and the gate-to-source capacitance, following definition, is ∂Qg Cgs = . ∂Vsg Vsd (5.61) (5.62) The gate-to-source capacitance increases with increased current. 5.3.4 Gate-to-Drain Capacitance In our analysis of device behavior at biases beyond those at which the channel current saturates, we obtained an output conductance that came about because essentially the device acts as if it has a shorter gate-length which has a higher current capability. This “shortening” of gate-length, in the case of long devices where the electric field does not reach the values necessary to achieve velocity saturation, occurs via channel pinch-off. We encountered this phenomenon in our long-channel constant mobility analysis. The effects that give rise to channel length shortening also give rise to drain-to-gate capacitance effects. First consider the non–current-saturation region of operation. The charge underneath the gate terminates at the gate, and the depletion region edge responds to both the source and the drain bias. If the two are at identical potentials, the depletion region is symmetric in both source and drain and the gate-to-source and gate-to-drain capacitances are identical. If, now, a drain bias is applied in excess of the source bias, the depletion region at the drain extends farther, and at the source end it responds to the requirements of conserving channel current for the quasi-static conditions. As a result of application of drain bias in excess of source bias, however, the capacitance and the charge that can directly be modulated by the drain decrease. The source capacitance increases because a larger part of the charge underneath the gate can be directly 298 5 Metal–Semiconductor Field Effect Transistors Figure 5.10: The equi-potential lines in a very lightly doped GaAs substrate due to bias applied between two metal electrodes on the surface. Electric field lines are orthogonal to these equi-potential lines. modulated. Another way of viewing this is that a higher electric field that naturally forms towards the drain as a result of the application of this drain bias results in screening of the channel and source regions. As a result, a larger and larger fraction of the depletion region underneath the gate can be associated with the source electrode and hence the gate-to-source capacitance. The net consequence, irrespective of the reason for channel current saturation, is that the drain-to-gate capacitance decreases. If there were no conducting channel, there would still be a capacitance associated with the drain-to-gate as well as the drain-to-source electrodes because of mutual termination of fields (see Figure 5.10). This capacitance really can not be calculated independently because the presence of a conducting channel changes the field profile. However, a calculation based on a semi-insulating medium with planar electrodes on the surface gives a lower bound for the capacitance of the structure. This capacitance Cdg,si is approximately given by Cdg,si = (s + 0 ) W K √ 1 − k2 , K (k) (5.63) √ where K(k) and K( 1 − k 2 ) are Elliptic integrals of the first kind, and k is given as 1/2 Ldg k= . (5.64) Ldg + L 5.4. ACCUMULATION–DEPLETION OF CARRIERS 299 In these expressions, Ldg is is the drain-to-gate spacing and the drain length is assumed to be the same as that of the gate. 5.3.5 Drain-to-Source Capacitance The drain-to-source capacitance is generally the smallest of capacitances and occurs to a large extent due to the fields through the substrate. The drain is usually isolated from the source by the high field regions in the channel. Hence, the approximation above for inter-electrode capacitance gives a better approximation for this capacitance. √ K 1 − k2 , (5.65) Cds,si = (s + 0 ) W K (k) √ where K(k) and K( 1 − k 2 ) are Elliptic integrals of first kind, and k is given as 1/2 (2Ls + Lds ) Lds k= , (5.66) Ls + Lds where Ls is the source length assumed to be the same as the gate and Lds is the drain-to-source spacing. We have now determined a number of elements associated with the ports of the MESFET using perturbation on the quasi-static analysis: gm to represent the variation of drain current with gate bias, Cdg to represent the change in associated storage between drain and gate electrodes, Cgs to represent the change in storage associated with gate-to-source electrode, Cds for the fringing effects between drain and source electrodes, and gds for output effects. The channel region charging the capacitance Cgs has associated with it a finite resistance. Later on, we will see how this naturally appears as a result of a direct smallsignal analysis from the small-signal transport equations. Here we will introduce it ad hoc as a resistance Ri that represents the intrinsic resistance associated with the integrated effect of channel conductance in the gate-source region. The resulting equivalent circuit, a quasi-static equivalent circuit, is shown in Figure 5.11. This figure includes three resistances, Rs , Rd , and Rg , to represent the ohmic effects in the extrinsic regions of the device.5 5.4 Accumulation–Depletion of Carriers In the PHS model, a nearly flat depletion region occurs as a consequence of velocity saturation, and the carrier concentration in the conducting region is nearly constant to maintain current continuity. This is not a good general description of real devices. The most important reason for this inadequacy is that the analysis entirely ignores diffusive currents, a current component that can be quite important. For example, in the long gate-length limit, this is the 5 In equivalent circuit representation, we adopt the use the hat symbol to represent smallsignal. Thus, V̂gs is the small-signal gate-to-source voltage. 300 5 Metal–Semiconductor Field Effect Transistors Figure 5.11: Quasi-static small-signal equivalent circuit for a MESFET based on elements derived as part of perturbation analysis on the PHS model. dominant current in the pinched region of the channel. It can be important in short gate-length devices also, depending on the design of the device and the bias conditions. Large electric fields exist in this region; they are the reason for velocity saturation, and hence these large electric fields can support and exist with deviations from quasi-neutrality. Models incorporating diffusion current can be quite complicated. We will consider a model that includes diffusion current in the analysis of HFETs in Chapter 6. Here, a more suitable way of exemplifying the deviations from quasineutrality in the form of an accumulation-depletion region is by considering a full two-dimensional model based on drift-diffusion transport6 of our 1 µm with a 5 × 1017 cm−3 doped channel MESFET example. Results of the variation in electric field and the carrier density along the channel are shown in Figure 5.12. Note that diffusion currents tend to be small at the source end but get larger in the high field region because of the rapid changes in the carrier concentration. There are two other important features in the results associated with this phenomenon. One is that the depletion region is not entirely flat in the high field region where carriers do move with essentially a constant velocity (see Figure 5.1). This is connected to the changes in the diffusion current. Current continuity requires that the sum, drift and diffusion, be a constant following integration over the cross-section. A changing cross-section can still accommodate current continuity with diffusion currents present. The presence of diffusion current also implies the presence of a concentration gradient in the conducting region with high fields. Thus, depletion depth changes, carrier concentration 6 i.e., the use of a two-dimensional simulator that finds the solution of the drift-diffusion equation, the continuity equation, and Poisson’s equation throughout the device cross-section subject to the boundary conditions. Such simulators are usually based on finite element analysis. They solve by dividing the device into many small but finite sized elemental volumes and by assuring continuity at their interfaces and with the device surfaces. Simulators can also be based on the use of the BTE approach or the Monte Carlo approach as discussed in Chapter 3. 5.4 Accumulation–Depletion of Carriers 301 Figure 5.12: Electric field and carrier density for a 1 µm gate-length GaAs MESFET with a 5 × 1017 cm−3 doped channel biased into current saturation. The formation of the accumulation-depletion region is shown in proximity of the drain electrode. changes, and diffusion currents can all be present in MESFETs, and the PHS model does not include them. However, its inclusion would be very difficult numerically within the framework of the model. Indeed, making it significantly more complex would remove its attractiveness as an intuitive model. One might as well, then, employ a complete two-dimensional model. The change in carrier concentration, shown in Figure 5.12 is of particular interest since it brings out an additional consideration. Current continuity, in the presence of a decreasing channel cross-section and high electric fields, results in an accumulation of carriers. If the change in channel cross-section takes place over a sufficiently large distance, then the associated diffusion current is small, and the accumulation of carriers is a direct consequence of current continuity alone. Eventually, when the drain is reached, the conducting channel may expand and hence a depletion of carriers may also occur. So, the large longitudinal field in the region of velocity-saturated transport occurs together with a change in the net charge density. For most short gate-length structures, employing relatively large channel dopings, current continuity is the main source of this accumulation–depletion. It occurs in all materials at appropriately short gate-lengths where velocity saturation may occur.7 A phenomenon similar to this, of accumulation–depletion, also occurs due to the negative differential mobility in the velocity–field characteristics of electrons 7 i.e., it occurs in silicon FETs also; see D. P. Kennedy and R. R. O’Brien, “Computer-Aided Two-Dimensional Analysis of the Junction Field-Effect Transistor,” IBM J. of Research and Development, 14, No. 2, p. 95, 1970. 302 5 Metal–Semiconductor Field Effect Transistors in a variety of compound semiconductors. An example is GaAs. But, for this negative differential mobility to be significant, the channel doping has to be kept low—in the low-1017 cm−3 range for GaAs. This formation of an accumulationdepletion of charge in the channel region of the GaAs MESFET is shown in Figure 5.13 for a low-doped GaAs MESFET of 1 µm gate length. As carriers travel along from the source edge of the channel to the drain they encounter higher fields beyond the field corresponding to peak velocity. Following the velocity–field curve, this initially leads to a decrease in velocity and hence an increase in carrier density, the channel cross-section effects being secondary. As the carriers move further down the channel, near the drain, they encounter lower electric fields. The carriers accelerate and hence a depletion of charge occurs to maintain current continuity. Thus, along the channel, an accumulation and depletion region forms in the conducting channel region. In PHS model, a constant velocity is assumed in the high field region. This accumulationdepletion region would have formed in this part of the device underneath the drain edge of the gate, had we included the specific velocity–field curve with negative differential mobility. Short gate-length devices are usually made with channel dopings in the range of mid-1017 cm−3 ; at such doping levels, the effect of negative differential mobility is weaker since peak velocity is smaller, however, the similar effect of current continuity is larger. Note that a nearly constant channel cross-section is important to arguments regarding this dipole. The PHS model considers a symmetric cross-section for the device and entirely ignores substrate injection effects, a reason why it is inadequate in modelling output conductance features. Substrate injection is also important because of its effect on the formation of the dipole. If carriers can spill over into the substrate, the cross-section can stay larger. Large electric fields from drain-to-source, both transverse and longitudinal, aid this injection into the substrate and hence mitigate substantially the formation of dipole layers. Figure 5.14 shows an example similar to Figure 5.13 in the presence of substrate injection. Note the decrease in the dipole formation. The effect is much more substantial in the case of the first type of dipole because channel cross-section is very central to the dipole’s formation. Substrate and back interfaces are usually designed to suppress injection away from the gatechannel region. Any current path farther away from the gate leads to poorer control by the gate. So, for most designs of MESFETs, irrespective of the cause, some dipole effect is present in the high field region of the conducting channel. The effect is larger at smaller doping levels, and its implications are significant at very high frequencies because its principle consequence is a capacitive feedback from the output. For computer-aided design models of current–voltage characteristics, this may be neglected with an acceptable error; for quasi-static capacitance models, this may or may not be acceptable depending on the doping level and other structural features of the device. A complete inclusion of the implications of the accumulation-depletion requires an elaborate numerical calculation, since the complex velocity–field curve does not allow for analytic or simple numerical analysis. We will, however, see how a simpler analysis may be used to incorporate first-order effects of this 5.4 Accumulation–Depletion of Carriers 303 Figure 5.13: Surface plot of the conduction band edge for a 1 µm GaAs MESFET with a 1 × 1017 cm−3 doped channel biased into current saturation. (b) shows the electric field and the carrier concentration as a function of position along a conducting cross-section of the channel. 304 5 Metal–Semiconductor Field Effect Transistors Figure 5.14: Surface plot of the conduction band edge is shown in part (a) for a 1 µm GaAs MESFET with a 1 × 1017 cm−3 doped channel biased into current saturation. This example allows for injection into the substrate. Part (b) shows the electric field and the carrier concentration as a function of position along a conducting cross-section of the channel. This figure should be compared with the previous figure which assumed a symmetric boundary condition at the interface between the channel and the substrate. 5.4 Accumulation–Depletion of Carriers 305 dipole region, by considering the negative differential mobility–induced dipole as an example. The objective of this exercise is to serve as an example of how a complex phenomenon may be analyzed within a section of a device in order to include its important consequences for device behavior. As we have remarked before, though, this particular source of dipole is relatively weak in the short gate-length heavily-doped channels. Mathematically, the current continuity equation for the channel carrier transport8 is d (nD(E)) J = q nv(E) + , (5.67) dz where D(E) is the diffusion coefficient of electrons as a function of electric field. If ND is the background donor concentration, q dE = − (n − ND ) , dz s (5.68) and just outside the dipole region, where the channel is quasi-neutral, J = qND v1 , (5.69) s nv(E) − ND v1 d(nD) = . dE q n − ND (5.70) giving Here we have utilized the approximations of the velocities in the high field region of the device. The solution of this differential equation is found as follows, with the perturbation of the diffusive term, a small term, ignored: Z n ND or Z 0 n − ND 0 s E v − ND v1 /n 0 dn = dE , 0 n0 q E1 D(E ) Z E n − ND n − ND s v − ND v1 /n 0 − ln 1 + = dE . 0 ND ND qND E 1 D(E ) (5.71) (5.72) We now consider only limited deviation from quasi-neutrality, i.e., |n − ND | /ND 1, (5.73) appropriate for low-1017 cm−3 or higher doped devices in GaAs. If the dipole forms over a region of many Debye lengths, i.e., exceeding 0.1 µm, then the limited deviation from quasi-neutrality also implies a diffusion current density 8 Here we follow arguments discussed in detail in T. J. Fjeldy, “Analytical Modeling of the Stationary Domain in GaAs MESFETs,” IEEE Trans. on Electron Devices, ED-33, No. 7, p. 874, July, 1986. We stress, however, that at doping levels of interest in practical MESFETs, this is of secondary, not primary importance. It occurs together with the other cause of dipole already discussed. It is probably of larger significance in HFETs where the background doping is much lower and hence the negative differential mobility is significantly stronger. 306 5 Metal–Semiconductor Field Effect Transistors much smaller than drift current density. This justifies the prior assumption of this analysis. 2 Z E 0 n − ND 2s 1 ND = v− v1 (5.74) 0 dE . ND qND E 1 n D(E ) At the peak field Em in the domain, Z Em v − v1 0 0 dE = 0, E 1 D(E ) (5.75) because n = ND . This allows us to determine the maximum field Em —the maximum electric field in the dipole region—and hence a reduction of variables. The total voltage drop in the dipole region Vdip , assuming symmetric accumulation and depletion, is Vdip = 2 = 2 Z Em E1 Z Em E1 (E − E 1 )dz (E − E 1 ) s dE, q(n − ND ) (5.76) using Poisson’s Equation. The total sheet charge density in the dipole region Qdip , using Gauss’s Law, is Qdip = s (Em − E 1 ), and hence the capacitance associated with this charge, Cdip , is −1 ∂Vdip ∂Qdip Cdip = = s . ∂Vdip ∂ (Em − E 1 ) (5.77) (5.78) In the limit of large field in this dipole domain region, one can determine a parameter R for a given D(E) and v(E) characteristic, whose magnitude in the high field or high voltage limit is given by R = ≈ Z Em v(E) − v1 dE D(E) E1 Z ∞ v(E ) − vs dE, D(E) Es (5.79) since, at the high field end (Em → ∞), v1 approaches the saturated velocity vs . At the low field end E → Es = vs /µ0 , because a constant mobility may be assumed. Under this assumption of a large dipole domain voltage, it can be shown that the dipole voltage reduces to (see Problem 4) √ 1/2 4 2 µ0 2 Vdip = λD (Em − Es ) . (5.80) 3 D0 R 5.4 Accumulation–Depletion of Carriers 307 Figure 5.15: The origin of elements of a quasi-static small-signal MESFET model (a) including intrinsic and extrinsic elements derived in the quasi-static approximations. The developed model is shown in (b). where R is a constant ≈ 5.5 × 107 V.cm−2 for a doping ND = 1017 cm−3 in GaAs and D0 is the diffusion coefficient in the absence of field. The dipole capacitance follows as 1/2 3 D0 R 1 . (5.81) Cdip = 8λD 2µ0 Em − Es Based on this analysis, we may now infer a quasi-static equivalent circuit model for the GaAs MESFET, by including in it the features related to current– voltage dependence, the parasitic resistances and capacitances, and the intrinsic resistances and capacitances. A model with a broad range of applicability under quasi-static conditions is shown in Figure 5.15. The equivalence between the cross-sectional parameters and the equivalent circuit elements is quite intuitive. The intrinsic device is the part of the device used in the analysis of channel charge transport and control. Extrinsic elements are those required to link this intrinsic device to the stimulus we apply to or sample from the device. Source resistance Rs , drain resistance Rd, and gate resistance Rg (which is usually negligible due to high metal conductivity but non-negligible at very short gate-lengths due to small cross-section area) are examples of extrinsic resistances. Pads used to connect the device are also extrinsic elements. The intrinsic elements are related to the functioning of the device whose operational basis is incorporated in our model. Ri is the resistance that results from conductance effects of the channel region, and it emphasizes in a lumped element the effects of the source end of the channel. The gate-to-source capacitance Cgs , the drain-to-gate capacitance Cdg , and the drain-to-source capacitance Cds have been derived before. The capacitance due to accumulation and depletion of the charge in the channel Cdip is incorporated 308 5 Metal–Semiconductor Field Effect Transistors in the channel path between the drain and the source. The output resistance Rds is incorporated to account for effects of channel modulation by the drain bias, and the transconductance gm is incorporated through the current source. This is a quasi-static equivalent circuit model, and we will show later that it is useful up to moderate frequencies. Significantly more complex circuits, or even network parameters, based on a direct small-signal analysis or experimental measurements at the frequencies of interest, are necessary for modelling effects at higher frequencies. This model will also be used as a basis in HFETs, the operation of the devices being similar in basis. The variation in magnitudes of the elements, may, however, be significantly different because of the nature of the charge control process itself. The model itself is quite similar and shows very similar current gain–frequency dependence and other features of interest. 5.5 Sub-Threshold and Substrate Injection Effects The bias-dependent high fields result in injection of carriers into the substrate. This is certainly very strong in the sub-threshold region where most conduction takes place due to injection of carriers from the passive regions related to access to the channel. This injection region, with lower carrier densities, also has large changes in carrier densities. Thus, diffusive effects are large in this bias region of device operation. Since the injection is over a barrier, it has a characteristic exponential behavior with the gate bias. This sub-threshold behavior is quite similar in all FETs irrespective of how they operate in the conducting region. The reason for this is behavior is that sub-threshold conduction largely takes place in the substrate and injection and collection occur in the access regions of the source and the drains. All these regions are quite identical in FETs. We will discuss sub-threshold current in more detail in Chapter 6. The injection of carriers into the substrate can also be very strong even when the channel is conducting. This injection is particularly strong when the device is in the saturated current mode of operation. The high fields push the conduction towards the channel–substrate interface and beyond from the doped region of the device, and the high field region related to formation of the dipole domain can make this effect stronger. Injection into the substrate occurs along longer path lengths and further away from the gate. It acts effectively as a large gate-length parasitic device and hence results in a device that is intrinsically slower and has poorer operational characteristics, such as transconductance, output conductance, etc. Band bending in the substrate is dependent on the characteristics of the substrate material; the electric fields in the device together with this barrier result in the injection into the substrate. The problem is therefore complicated and intrinsically two-dimensional in nature. It also becomes particularly strong at small gate-lengths. Our discussion in the following section, coupled with the sub-threshold and injection behavior, addresses this in more detail, together 5.6. SIDEGATING EFFECTS 309 with analytic and one-dimensional models for intuitive understanding and twodimensional solutions for rigorous understanding of the injection problem. 5.6 Sidegating Effects We now look at important problems in the use of compound semiconductor FETs—HFETs and MESFETs—in circuits. The first of these is the phenomenon of backgating or sidegating—a general term describing a change in device characteristics caused by changes in applied potentials at other than the device terminals themselves. An example of this is the effect of logic signals carried by metal lines in the vicinity of a device. Ideally, any signals other than those applied to the device should have no effect on the device characteristics because the substrate, such as that of GaAs, is semi-insulating. Semi-insulating substrates should be expected to effectively shielded at distances of µm’s away from the line, resulting in very small effects on the characteristics. Without specific precautions in the technology, however, it can actually be quite substantial. We will call the collection of such effects sidegating effects since we are most interested in those resulting from biases on lines, etc., on the same surface. These effects are also sometimes referred to in the literature as backgating effects. Sidegating effects can result from causes related to the semiconductor surface as well as the substrate. The direct effect of sidegating on the device occurs through changes in the depletion region at the substrate–channel interface, but effects can also occur, if device geometrical and functional considerations allow, due to changes in surface–channel interfaces. A change in the depletion region does not require any significant current flow because significant changes in device currents can occur with small changes in the depletion region, both for moderately forward biased and reverse biased substrate–channel interfaces. These small changes in the depletion region occur with small changes in the bias voltage across it. Thus, the important cause of sidegating is changes in the bias voltages across the substrate and surface junctions. These small changes in potential drops can occur without need for significant conduction, and the propagation of the voltage via the substrate is a requisite to sidegating. It should be emphasized that this propagation can also occur via surface effects because of local changes in trap concentrations in the surface region as well as at the surface itself. The subject is complicated because such propagation is two-dimensional in origin, and because this electrostatic voltage propagation in a semi-insulating substrate depends on the mechanism that leads to the semiinsulating character, this may, in reality, be position-dependent because of the processes involved in fabrication of structures. Our discussion therefore looks at conduction mechanisms in semi-insulating material first, both without and with the deep traps and shallow levels that occur in a balance, which result in the semi-insulating character of the substrate. Most device structures are designed so that there is no source of holes, and hence unipolar considerations are sufficient in a preliminary analysis. However, hole effects can occur from small-barrier metals or the presence of p-type regions 310 Metal–Semiconductor Field Effect Transistors due to thermally-induced conversion of the surface, and hence may need to be included too. We will do this using only illustrative examples. In all such structures, where a source of holes may exist, bipolar transport considerations will apply. Using these, we will study the propagation of voltages in the presence of traps and relate it to the behavior of currents in devices. 5.6.1 Injection and Conduction Effects As a preliminary exercise, we will look at conduction currents in one dimension in semi-insulating substrates for both trap-free and trap-dominated cases. The former is a case study for a very pure material such as that grown epitaxially, intrinsic GaAs, e.g., is semi-insulating. The latter is, however, more generally the case of substrate material. Quite often, here, the semi-insulating character is achieved by over-compensating the residual shallow acceptors, such as carbon, by a deep donor, such as a trap level called the EL2 level. EL2 is believed to be a native defect in GaAs. The semi-insulating material is obtained without intentionally introducing an impurity in the crystal. Shallow donors and other deep traps, both acceptor-like and donor-like, may also exist in GaAs, and these may be employed to obtain, by alternate means, semi-insulating GaAs. An example is that of obtaining semi-insulating GaAs through compensation of shallow donors and a deep acceptor such as chromium. In this latter case, the densities of traps and shallow levels are larger because these are intentionally introduced into the crystal. The energy band schematic for these various means of achieving semi-insulating GaAs is shown in Figure 5.16. The EL2 compensation scheme relies on a dominant shallow acceptor (e.g., C, Be, Mg, Mn) being present, while the chromium compensation scheme relies on a dominant shallow donor (e.g., S, Si, Se, Te, Ge) being present. We will discuss our trap model using a shallow acceptor and deep donor example; its implications can be derived using symmetry arguments for the shallow donor and deep acceptor case. The causes of sidegating can vary depending on the behavior of these traps. We will discuss some of these unusual characteristics that result due to the propagation of electrostatic potential to the device junctions in a later section. Before that, we will discuss the behavior of current in the presence of deep donor traps with larger electron capture rates than hole capture rates. These characteristics are important, since, at thermal equilibrium, the substrate is semi-insulating, and the bulk currents that flow under bias are space charge–limited. First consider a trap-free n+ –ν–n+ structure as shown in Figure 5.17 and its behavior with and without bias; the current transport in this structure is largely by electrons, because the contacts, with a mid-gap barrier height, can only provide electrons in significant numbers assuming that avalanching does not occur in these structures. The current in the structure, carried by the electrons injected and collected at the contacts, is largely by drift in the constant mobility regime; we are restricting applied voltages to less than Es L for a sample of length L. For the 5 µm sample of Figure 5.17, this would mean that for voltages less 311 Sidegating Effects Figure 5.16: An energy-band model for obtaining semi-insulating GaAs using shallow donor and deep acceptor (Cr) is shown in (a) and using shallow acceptors, shallow donors, and deep donor (EL2) is shown in (b). than 1.5 V, this current is given by J = qµnE = µs E dE . dz (5.82) The field is negligible at z = 0 at the edge of the depletion region of the injecting contact, and hence s 2Jz E(z) = , (5.83) µs the potential is V (z) = − Z 0 z s Edz = − 8J 3/2 z , 9s µ (5.84) and hence the relationship in terms of terminal parameters is 9 V2 J = − µs 3 . 8 L (5.85) The current in trap-free material, in the constant mobility drift-dominated region, follows a direct dependence on the square of the applied voltage and an inverse dependence on the cube of the sample length. This is sometimes referred to as the trap-free square law or the Mott-Gurney law. Figure 5.17 shows the dependence on a wider voltage range than the limit of validity of this law. Now consider this problem in the presence of shallow acceptors and deep donors as shown in Figure 5.18. This problem analyzes a geometry similar to that of Figure 5.17. Poisson’s equation for this problem is 312 Metal–Semiconductor Field Effect Transistors Figure 5.17: The band edges and electron quasi-Fermi level of a n+ –ν–n+ structure in GaAs with and without bias is shown in (a). (b) shows the associated electron densities as a function of position. (c) shows the current–voltage characteristics of the structure. Sidegating Effects 313 Figure 5.18: The band edges and electron quasi-Fermi levels of a n+ –ν–n+ structure containing shallow acceptors and deep donors (1015 cm−3 ) in GaAs is shown in (a) with and without bias. (b) shows the associated trap density that is charged as a function of bias. (c) shows the current–voltage characteristics of the structure. This figure should be compared with the previous figure where no traps were present. 314 Metal–Semiconductor Field Effect Transistors − d2 V q =− n + NA − NT+ . 2 dz s (5.86) Using a convention similar to that in the HSR recombination problem, with nT as an electron concentration when the quasi-Fermi level coincides with the trap level, and with the assumption that the shallow acceptor concentration is smaller than the deep donor concentration, thus imparting the semi-insulating character, we obtain nT NC exp [− (Ec − ET ) /kT ] ET − ξn = = exp . (5.87) n NC exp [− (Ec − ξn ) /kT ] kT Since NT+ 1 = , NT 1 + exp [− (ET − ξn ) /kT ] (5.88) we can write the identities under the Boltzmann approximation of nT = nNT+ , NT − NT+ (5.89) NT nT . n + nT (5.90) and NT+ = In thermal equilibrium, for semi-insulating material with low carrier concentration (i.e., neglecting the carrier concentration w.r.t. the acceptor concentration or nT ), we obtain NT − NA . (5.91) n0 = nT NA + nT We can now solve Poisson’s equation, again assuming constant mobility transport and neglecting the nT carrier term w.r.t. the free carrier term, d2 V q nT NT = n + NA − . (5.92) dz 2 s n The first term in this equation, which is associated with the free carrier charge, leads to the square-law behavior that we have already discussed for the trapfree case. The second term, due to the ionized acceptor charge, gives a constant term for the definite integral of voltage; this constant is given by VT F L = qL2 NA , 2s (5.93) a parabolic voltage term similar to that of the p–n junction problem. It corresponds to the contribution of the ionized acceptor charge of density NA throughout the insulating region. The last term results in n(z) = − J n0 = , qµdV /dz 1 − [1 − n0 /n(0)] exp (−z/LT ) (5.94) 315 Sidegating Effects and V (z) = − J qn0 µ n0 z z − LT 1 − 1 − exp − , n(0) LT (5.95) with n0 ≈ nT NT /NA because NT NA nT , and LT = − Js . 0 NA q 2 µn (5.96) In these equations, the carrier density at z = 0 is written explicitly to account for carrier enhancement provided by the contacts beyond the thermal equilibrium value. The constant potential term due to the ionized acceptors becomes important when the other charge terms are either insignificant or closely neutralize each other. For low bias voltages, i.e., with very small injected carrier density (electrons in our example) sufficient number of deep donors ionize to compensate for the acceptor charge, the injected electron charge, and to support the applied bias. The ionized donor density is approximately the same as the acceptor charge density. The rest of the deep donor traps are neutral in much of the semi-insulating region. At a bias of VT F L , sufficient electron charge density has been injected in the semi-insulating region to saturate the deep donor levels, most of which are now in the neutral state, and hence the ionized acceptors provide the net resultant charge, and the corresponding potential term is parabolic in length akin to the depletion region of a p–n junction. The significance of this potential VT F L is that at higher biases the deep donors remain neutral due to the filling of the trap with electrons, and hence the term trap-filled limit used as a subscript to this voltage. At higher biases, the material can be treated as being trap-free, and should follow the square law in voltage. Figure 5.18 demonstrates the break point that this trap-filling provides, as well as the power law relationship following that. We can make further analytic approximations in the analysis of this problem. For large current densities, i.e., a significant enhancement of carriers at z = 0, i.e., n0 n(0) and z/LT 1, the applied potential VA can be expressed using the first term of the expansion of the exponential as 2n0 qµVT F L , (5.97) VA = V (z = L) = VT F L 1 + 3LT J and hence the current density under these approximations is J=− 2n0 qµVT2F L . 3LT (VT F L − VA ) (5.98) This equation is very approximate; however, it serves well to indicate that a sudden rise in current should be expected at biases corresponding to the trapfilled limit voltage. In the example of Figure 5.18, the acceptor doping was 1 × 1015 cm−3 , and sample length 5 µm, corresponding to a VT F L of 20 V. The exact number is different because of the Debye tailing effect in the low-doped 316 Metal–Semiconductor Field Effect Transistors region and drift approximation in the calculation. Figure 5.18 also shows that in addition to this threshold behavior at the trap-filled voltage, a significant voltage drop can occur in the space charge region and a small voltage does drop at the other junction. We would therefore expect sidegating effects to occur due this conduction mechanism. In deriving these analytic relations, and in analyzing the space charge effect, we have considered unipolar transport even when traps were present. We have mentioned that conditions may exist where hole transport may also occur in addition to electron transport. In such situations, the capture characteristics of the traps themselves become very important, since they are important to the residual space charge in the “semi-insulating” region. Consider the characteristics of the EL2 level: since it is a deep donor it has a significant electron cross-section and a small hole cross-section. The consequence of this can be that an EL2 trap can be compensated by electrons, and a simultaneous hole conduction can lead to a very efficient propagation of electrostatic potential, as shown in Figure 5.19. We will visit this condition in greater detail later. Here, we emphasize that there is now a negligible drop in the space-charge region. Most of the voltage drop occurs at the junction, specifically at the reverse biased junction. If this reverse biased junction corresponded to the channel-substrate interface of an FET, clearly there would be a significant sidegating effect. These two mechanisms of conduction and electrostatic propagation are quite different. The first relies on trap filling at a threshold voltage for the propagation of electrostatic potential, while the second relies on the significant differences in the capture cross-sections for the two types of carriers. The second mechanism propagates electrostatic potential extremely efficiently. It also does not have a threshold voltage associated with it. Our discussion of the bulk-dominated behavior of sidegating will be based on these two mechanisms. 5.6.2 Bulk-Dominated Behavior We reiterate the basis of the semi-insulating character of GaAs substrates: it occurs because of the presence of compensating acceptors and donors, both shallow and deep, in the ≈ 1014 to ≈ 1016 cm−3 concentration range. Since the traps are larger in concentration and are deep, the Fermi level is in the middle of the semiconductor, and semi-insulating characteristics result because of the relatively large bandgap of GaAs. However, this technique of obtaining semiinsulating characteristics relies on compensation by traps that have differing electron and hole capture cross-sections. In the case of trap-filled conduction whose one-dimensional and single carrier theory we have looked at, the potential drop occurs both in the bulk and at the substrate–channel junction. This leads to one possible means of electrostatic propagation, and should have a threshold feature associated with it corresponding to the trap-filled voltage. Although we looked at a single carrier theory for this, it should also occur in ambipolar conduction, provided the capture cross-sections are similar for both the carriers. In the case of large differences in capture cross-sections of the carriers, and provided both carriers are available, propagation of potential can occur due to Sidegating Effects 317 Figure 5.19: (a) shows the energy band diagram under bias for the n+ –ν– n+ example with bipolar transport. The trap is assumed to have significantly different electron and hole capture cross-section. (b) shows the carrier densities as a function of position. 318 Metal–Semiconductor Field Effect Transistors equilibrium between one carrier and the trap—e.g., electrons and donor traps— with the current being carried by the other carrier.9 Since the current density is small, this allows most of the electrostatic potential drop to occur at the substrate–channel interface, hence resulting in efficient sidegating. This is the second possible mechanism for sidegating. We discuss the first mechanism and possible means of reducing its impact first. The effect of a sidegate leading to a perturbation of electric fields in the vicinity of a device is shown in Figure 5.20. In this example, once sufficient voltage is applied across the material, so that injected carriers saturate the donor trap, ambipolar conduction determines the transport across the material. The required voltage to fill the traps is the trap-filled voltage VT F L . We derived an expression for this. In general, this is proportional to the nth power of the spacing between the device and the sidegate where n is generally larger than 3/2, depending on the characteristics of the trap. Once this trap-filled voltage is reached, conduction occurs and the depletion width at the channel substrate interface begins getting modulated, giving rise to a modulation of the channel current of the FET. The current–voltage characteristics show a decrease in current with the sidegate bias. A reverse bias is required for this conduction process to begin. Figure 5.20 shows the onset of substrate conduction and how it is affected by other potentials applied under different conditions. The two cases show the signature of a rapid rise in sidegating current when a trap-filled voltage is reached. The rapid increase in current in this example occurs at the VT F L and following this rapid rise the current remains larger. It is also following this rise that the drain current changes rapidly, hence the leakage current through the substrate and associated potential propagation is directly responsible for the sidegating effect. If sidegating were to occur through this particular mechanism, one could envision controlling it by providing a shielding of the sidegate potential and modulation of the leakage current. Such a shielding could be provided by applying an additional potential between the sidegate and the device using an ohmic contact, a n+ region, or a metal–semiconductor junction, all of which are reverse biased. In the ohmic and n+ region–based structures, since there is no voltage drop across the contact—the current being small—all the voltage drop occurs across the semi-insulating substrate and the channel–semi-insulating substrate interface. This leads to a decrease in the device channel saturation current due to the application of this shielding bias itself. The shield itself acts as an additional sidegate, acting as a remote gate. It reduces the current flowing in the device; since it now isolates the device from the actual sidegate potential, it also reduces the effect of the sidegate voltage. In this case, the shield at the channel interface acts just like a remote gate because of the depletion region for this applied voltage. However, it shields the other sidegate voltage applied through other metal lines. A more efficient means of providing a shielding for this sidegating mechanism is through a metal–semiconductor barrier—similar to the metal lines 9 For a discussion of this type of propagation, with one specific trap characteristic, see N. Goto, Y. Ohno, and H. Yano, “Two-Dimensional Numerical Simulation of Sidegating Effect in GaAs MESFETs,” IEEE Trans. on Electron Devices, ED-37, No. 8, p. 1821, Aug. 1990. Sidegating Effects 319 Figure 5.20: (a) shows a surface plot of the conduction band edge of a MESFET in the presence of modulation by a sidegate. The source of the device is located near the origin, followed by the drain and the sidegate. The sidegate has the large bias applied. (b) shows the current–voltage characteristics (drain-to-source current (IDS ) and sidegate current (ISG )) as a function of applied voltage at the sidegate. Results due to two different trap densities are shown; these result in different current–voltage response. 320 Metal–Semiconductor Field Effect Transistors Figure 5.21: Example of shielding of sidegating effect using a metal– semiconductor junction. The figure shows a surface plot of the conduction band edge. The source is at the origin, followed by the drain, the shield electrode, and the sidegate electrode. The shield is shown to reduce the electrostatic potential propagation from a sidegate. that caused this problem in the first place. The metal–semiconductor diode has a voltage drop across the junction and the semi-insulating regon instead of the channel-substrate interface region (see Figure 5.21, which should be compared with Figure 5.20). This capacitive shielding (ohmic and n+ contacts provide resistive shielding) occurs without the modulation of the channel-substrate interface, and hence the channel current continues to stay large. The use of a metal–semiconductor diode does not change the device saturation current appreciably, although it shifts the onset of backgating considerably. With an ohmic shield, the saturation current changes substantially because of its conduction and proximity to the channel. Similarly, the doped region shield also reduces the channel current. There is another means by which this sidegating mechanism can be reduced in useful circuits. This employs generation of a high concentration of traps, such as by ion implanting in the vicinity of the device, since it would raise the trap-filled voltage. The defects may be native defects, e.g., those created by implanting ionized hydrogen (i.e. protons), isoelectronic species such as boron, or inert species such as helium, argon, etc. In addition to native defects, one may generate extrinsic deep levels by implanting other impurities such as oxygen. This allows annealing away of the native defects while still maintaining the efficacy of additional deep levels. Of the species mentioned, oxygen is among Sidegating Effects 321 the heaviest, and is apparently among the most effective because of the nature of the deep traps generated. The trap-fill–limited sidegating phenomenon is dependent on the spacing of the sidegate. None of these techniques is completely effective in suppressing sidegating at the device-to-device spacings one would like to use in circuits, which is approximately the pitch of metal lines. This dimension is too small for the above techniques to be completely effective. In practice, with implantation isolation, one employs a sufficiently large device-to-device spacing to limit the worst-case drain current variations to an acceptable range; or, equivalently, the threshold voltage and other device parameters to an acceptable range. Another possible solution of this problem is the use of a sufficiently p-doped layer to isolate devices by junction isolation. However, this also leads to an increase in capacitance to the substrate and reduces the speed of circuits. The trap-fill–limited conduction discussed so far depends on the distance between the sidegating electrode and the device. Quite often, one encounters instances where sidegating is not dependent on the distance, and a large modulation of the channel can occur over very large distances, such as from the back of the substrate. Such cases involve sidegating through a mechanism that is obviously very different, because for substrate thickness, which is usually about 500 µm, the trap-fill–limited voltage would be very high. Here, the likelihood of the second sidegating mechanism discussed in the beginning of this section is most likely. In these cases the trap characteristics of large asymmetry between the capture cross-sections for electrons and holes plays a very important role and leads to the behavior of an otherwise semi-insulating material acting like a conductor of the potential, although very little actual current flow occurs. The reason is that electron and hole concentrations are very low for this conduction, or for contribution towards band bending. The substrate potential distribution is related to the charge on the trap, e.g., the deep donor trap due to EL2. This charge depends on the statistics of occupation and is related to the capture crosssections. The deep donor trap has a significantly larger electron cross-section and a small electron lifetime (≈ 10−9 s), and a small hole capture cross-section and a large hole lifetime (≈ 2 × 10−5 s). This leads to local neutralization of the trap throughout the substrate except at the channel-substrate interface. The potential drop occurs at the channel-substrate interface, and hence, significant sidegating that is independent of the distance occurs. Note that in this instance the semi-insulating material acts as an n–p junction. An example of this propagation of electrostatic potential is shown in Figure 5.22 for the deep acceptor shallow donor case. An example of a deep acceptor is Cr, together with Si or other shallow donor species. So, in this case, the conduction occurs due to electrons, and the trap compensation is by holes. This mechanism shows no threshold behavior. Cr, e.g., is one of the deep acceptors in Cr-doped semi-insulating substrates, where the substrate will behave like a p-type region. The converse of this occurs with deep-donor EL2 and a shallow acceptor. Additional extensions of these occur at the surface due to temperature-induced changes in the deep and shallow level densities, and we consider an example with EL2 compensated material for this variation. 322 Metal–Semiconductor Field Effect Transistors Figure 5.22: Surface plot of conduction band edge showing electrostatic potential propagation for a semi-insulating substrate consisting of a deep acceptor and shallow donor due to local neutralization of acceptors by holes. The current is carried by electrons. The figure, unlike the earlier surface plots, shows the applied sidegate bias appearing nearly entirely at the channel-substrate interface. . 5.7. PIEZOELECTRIC EFFECTS 5.6.3 323 Surface-Dominated Behavior During the high temperature processing for fabrication of devices, EL2 depletion can occur at the surface together with an accumulation of acceptors (such as boron and carbon). This can lead to a very lightly compensated or even a p-type layer at the surface. If the material is entirely p-type, electrostatic propagation could occur with a process that is complementary of the previous example. Now, the holes will carry the current and the electrons will equilibrate with the traps. A surface can play a role in other ways, too. Due to the Fermi level pinning at the surface, unoccupied trap concentration can become lower than in the bulk, leading to a lowering of the trap-filled voltage limit, and hence to the mechanism that we discussed earlier. We have emphasized the role of traps and trap statistics in our discussion. The role of carriers and carrier injection is also important, since the equilibrium is achieved with carriers available. Avalanching at a large biased junction can, e.g., cause both electrons and holes to be available. So, results from metal electrodes, even if they are poor sources of holes at low bias, can be different at high bias. Both these cases will show different sidegating behavior. It should be clear from our discussion that sidegating can occur by a variety of means in different materials due to differing compensation and surface conditions brought about by the traps, the processing, and the geometry. The sidegating thresholds can be raised by increased trap concentrations in some of the cases where trap-filling is the dominant mechanism; these traps can be introduced using damage implantation. However, these may have little effect in other cases where electrostatic propagation occurs because of the trap characteristics and the polarity of the material. In all these cases, one possible solution is to use sufficiently p-type doped material so that junction isolation is achieved. This would isolate the sidegating voltage from the substrate–channel interface by dropping across the sidegate–substrate junction, but at the expense of an increase in capacitance. 5.7 Piezoelectric Effects A second problem, unique to compound semiconductors, is related to their ionic character. This ionic character leads to a piezoelectric nature of the crystal, and an effect resulting from stress that is termed the piezoelectric effect. The basis of this effect lies in stress-induced polarization in the crystal because of the ionic charge and distortion of the lattice. The polarization can be viewed to result in additional charge because ∇.(s E + P) = ρ, (5.99) where P is the polarization vector and ρ is the charge density. The polarization results in additional charge and hence device parameter variation because of stress10 in the material. This stress can occur in devices 10 The problem of determining stress and its piezoelectric consequences is a subject intimately related to finite element analysis and the theory of elasticity of solids. This section is written as an introduction without undue reliance on the mathematical details of the de- 324 Metal–Semiconductor Field Effect Transistors Figure 5.23: Polarization effect in GaAs as a result of compressive stress. The atoms are shown in one plane viewed from h111i direction. because of different expansion coefficients of the materials employed; it may result from the dielectric films employed on semiconductor surfaces or the metallizations of the gate and ohmic contacts which are in proximity to the device active region. We first show in a simple way how this polarization occurs in GaAs as shown schematically in Figure 5.23. This figure is drawn in one plane. When a compressive stress is applied, the angle between the bonds for the atoms away from the center section increases and there is a net displacement of the positive charge to the left and the negative charge to the right. Consequently, there is now a net dipole moment in the crystal pointing towards the right and the crystal is polarized. A shear stress, instead of compressive stress, would have similarly resulted in a net dipole moment pointing upwards. This polarization, caused by stress, can be determined in general by tensor analysis as P = d × σ, (5.100) scription of the problem. The interested reader is referred to S. P. Timoshenko and J. N. Goodier, Theory of Elasticity, McGraw–Hill, N.Y. (1970); P. M. Asbeck, C. P. Lee, and M. F. Chang, “Piezoelectric Effects in GaAs FETs and Their Role in Orientation-Dependent Device Characteristics,” IEEE Trans. on Electron Devices, ED-31, p. 1377, 1984; J. C Ramirez, P. J. McNally, L. S. Cooper, J. J. Rosenberg, L. B. Freund, and T. N. Jackson, “Development and Experimental Verification of a Two-Dimensional Numerical Model of Piezoelectrically Induced Threshold Voltage Shifts in GaAs MESFETs,” IEEE Trans. on Electron Devices, ED-35, p. 1232 1988; and T. Onodera and H. Nishi, “Theoretical Study of Piezoelectric Effect on GaAs MESFETs on (100), (011), (111)Ga, and (111)As,” IEEE Trans. on Electron Devices, ED-36, p. 1580, 1989, for further details. Piezoelectric Effects 325 Figure 5.24: Orientation nomenclature. We have treated y axis as pointed towards the substrate. Thus, the surface of GaAs is (010). The figure also shows the gate orientations in MESFETs. where d is the piezoelectric tensor and σ is the stress tensor. There is an additional requirement for this polarization to lead to a cumulative charge effect and hence a macroscopic variation with position. This is that the crystal be non-centro-symmetric. Non-centro-symmetry leads to the accumulation of the polarization of the unit cells because the polarizations are additive and have the same direction. Centro-symmetric crystals do not accumulate the polarization of unit cells since they oppose in alternate unit cells. Most of the elements of d are zero for compound semiconductors, except the ijth component for which i 6= j. This results in a polarization vector Px σxy P y = d 1 (σxx − σzz ) , (5.101) 2 σyz Pz where d is the magnitude of the equal non-zero components, the x subscript denotes the h101i direction, the y subscript denotes the h010i direction, and the z subscript denotes the h101i direction, as shown in Figure 5.24. Since the strongest effect occurs due to the surface dielectric and metal films in close vicinity to the active region of the device, we need to assess the effect of stress in geometries such as those shown in Figure 5.25. The effect from stress due to the gate and the dielectric films may be present simultaneously. Both the gate and the dielectric films can be under compressive or tensile stress, and hence the effect can cause electric parameter (e.g., threshold voltage) change of both signs. In addition, depending on the orientation of the gate or dielectric lines, the polarization results are different. Si3 N4 , one of the dielectric films 326 Metal–Semiconductor Field Effect Transistors Figure 5.25: Two common sources of piezoelectric effects due to stress generated by the mismatch of materials. (a) shows the effect occuring from the gate of a MESFET, while (b) shows that due to dielectric films. Both of these effects may be present simultaneously. employed, is usually under compressive stress, while amorphous SiO2 , another dielectric employed, is usually under tensile stress. The resulting polarization from the dielectric film is therefore of the opposite sign, and hence threshold voltage variation is opposite. Using the stress tensor we can determine the polarization. Knowing the polarization, ρpol = ∇.P, (5.102) the charge density associated with the polarization can be found for the bulk. At the surface of the crystal, a surface charge density of Qpol is also induced, Qpol = n b.P, (5.103) where n b is the unit vector normal to the surface. For a h010i surface, this results in Qpol = Py . As an example, consider the geometry of Figure 5.25. The maximum stress occurs at the corner of the substrate and the film. For gates and dielectric films, the two corners are the logical choice for a coordinate system (r1 , r2), where the radial distance is measured from the the points of highest stress. The resulting stress components can be written as 2 z1 z2 σxx = − νσf t 2 − 2 , π r r2 12 2 z1 y z2 y2 σyy = − σf t − , π r14 r24 3 2 z z3 σzz = − σf t 14 − 24 , π r r2 12 2 z y z2y and σzy = − σf t 14 − 24 , (5.104) π r1 r2 Piezoelectric Effects 327 where t is the film thickness, which has also been assumed to be much smaller than the substrate, ν is the Poisson ratio, and σf is the stress in the film. Note that the maximum stress occurs at the substrate–film interface and that it disappears for large distances into the substrate. This gives for the polarization charge density in the bulk and at the surface: ( ) z1 y z12 − βy2 z2 y z22 − βy2 ρpol = γb σf t − r16 r26 1 1 − . (5.105) and Qpol = γs σf t z1 z2 The magnitudes, for GaAs, are ν = 0.31, γb = 2d(4 + ν)/π ≈ 390 electron charges per dyne, β = (2 + ν)/(4 + ν) = 0.53, and γs = d(1 − ν)/π ≈ 40 electron charges per dyne. An example of the piezoelectric charge distribution for the h101i oriented device in compressive stress is shown in Figure 5.26. The piezo-charge gets stronger towards the center of the gate and away from the surface, and is dependent on the angle. Near the tail of the doping density, its effect can be substantial because of a reduction in dopant charge. It can, therefore, significantly disturb the low current behavior of devices, i.e., it affects parameters such as threshold voltage and conductance at low biases. The effect is strongly dependent on the orientation. For a device perpendicular to this direction, the charge sign will actually reverse, and hence the electric parameters will change in the opposite direction. This leads to the problem of changes in threshold voltage in devices that are oriented differently on the same wafer—a significant design constraint. In the example that we have looked at, the threshold voltage shifts negative, and the device is more conductive at any given bias because of the piezoelectric effect. However, devices perpendicular to this device have a threshold voltage shift that is positive, with the device being less conductive. The threshold shift also becomes more pronounced with a decrease in dimensions, i.e., shortening of the gate length. Shortening of the gate-length naturally leads to an increase in the stress underneath the gate due to stress from dielectric films. This gate-length effect is in addition to the effect of the short-channel phenomenon. Figure 5.27 shows the threshold variation in an example of GaAs MESFETs. Note the rapid increase in the shifts in the sub-5 µm range of gate lengths. Thicker films lead to larger stress, and hence stronger shifts. While these results are for compressive Si3 N4 films, the results for SiO2 are similar but of the opposite sign because those films are usually tensile in nature. Interestingly, it turns out that variations due to such stress effects on (101) oriented substrates with h101i or h101i oriented FETs are minimal because of the symmetry of the piezoelectric charge distribution. It changes sign at the center of the gate on either side of the plane through the substrate. Figure 5.28 shows the piezoelectric charge distribution effects due to stress in gate metallurgy placed on a (101) surface of GaAs. This results in a significantly lower threshold voltage dependence on the gate-length for this substrate orientation. 328 Metal–Semiconductor Field Effect Transistors Figure 5.26: Normalized piezoelectric charge distribution due to compressive Si3 N4 film is shown in (a). (b) shows the charge density at the center of gate and going into the substrate. After P. M. Asbeck, C. P. Lee, and M. F. Chang, “ Piezoelectric Effects in GaAs FETs and Their Role in Orientation-Dependent Device Characteristics,” IEEE Trans. on Electron Devices, ED-31, p. 1377, c 1984 IEEE. 5.8. SIGNAL DELAY ALONG THE GATE 329 Figure 5.27: A schematic variation of the threshold voltage shift due to compressive stress in dielectric films as a function of gate-length for GaAs MESFETs. Note the differing effect on two different orientations. In GaAs, the (100) family of substrate surfaces is among the most difficult surfaces to work with, due to the large piezoelectric effect. All other major orientations show periodic modulation of charge, as in the above example, leading to smaller threshold voltage shifts. Figure 5.29 shows the gate orientation dependence of threshold voltage with various crystallographic surfaces due to stress caused by gate metallurgy. Effects similar to dielectric stress effects occur due to gate stress. In addition, these stress effects show up as a function of temperature, even if a device is fabricated to have a negligible stress for any specific temperature of operation. 5.8 Signal Delay along the Gate We now return to the modelling of the devices at high frequencies. Our quasistatic analysis is strictly true only for moderate and low frequencies since it ignores all dispersive effects and treats the problem as a steady-state problem. The discussion in this and the following sections is related to understanding the device operation from a high frequency perspective. MESFETs are high frequency devices, and we have been analyzing them, in quasi-static approximation, for phenomena underneath the gate between the source and the drain. We have assumed the gate to be an equi-potential region because it is usually made of metal. Both at high frequencies and for unusually wide gate structures, these approximations break down. A metal line, such 330 5 Metal–Semiconductor Field Effect Transistors Figure 5.28: Piezoelectric charge distribution for a h101i oriented gate on a (101) substrate. Contours correspond to electron density of 1015 , 1016 , and 1017 cm−3 . After T. Onodera and H. Nishi, “Theoretical Study of Piezoelectric Effect on GaAs MESFETs on (100), (011), (111)Ga, and (111)As,” IEEE Trans. c on Electron Devices, ED-36, p. 1580, 1989 IEEE. 5.8 Signal Delay along the Gate 331 Figure 5.29: Threshold voltage shift as a function of gate orientation on various GaAs substrate surfaces. The angles are w.r.t. h101i orientation. The open circles are for (010) surface, the squares are for (101) surface, the normal triangles are for (111) Ga surface, and the inverted triangles are for 111) As surface. The periodic changes in the threshold voltage are the largest for the (010) substrate. After T. Onodera and H. Nishi, “Theoretical Study of Piezoelectric Effect on GaAs MESFETs on (100), (011), (111)Ga, and (111)As,” IEEE Trans. on c Electron Devices, ED-36, p. 1580, 1989 IEEE. 332 5 Metal–Semiconductor Field Effect Transistors Figure 5.30: A schematic for transmission of signal along the gate for a long gate-width MESFET together with